# Solution manual to materials science and engineering an intro 6E callister ( PDFDrive ) ```SOLUTIONS TO PROBLEMS
PREFACE
This section of instructor's resource materials contains solutions and answers to
all problems and questions that appear in the textbook. My penmanship leaves
something to be desired; therefore, I generated these solutions/answers using
computer software so that the resulting product would be &quot;readable.&quot; Furthermore, I
endeavored to provide complete and detailed solutions in order that: (1) the instructor,
without having to take time to solve a problem, will understand what principles/skills are
to be learned by its solution; and (2) to facilitate student understanding/learning when
the solution is posted.
I would recommend that the course instructor consult these solutions/answers
before assigning problems and questions. In doing so, he or she ensures that the
students will be drilled in the intended principles and concepts. In addition, the
instructor may provide appropriate hints for some of the more difficult problems.
With regard to symbols, in the text material I elected to boldface those symbols
that are italicized in the textbook. Furthermore, I also endeavored to be consistent
relative to symbol style. However, in several instances, symbols that appear in the
textbook were not available, and it was necessary to make appropriate substitutions.
These include the following: the letter a (unit cell edge length, crack length) is used in
place of the cursive a. And Roman E and F replace script E (electric field in Chapter
18) and script F (Faraday's constant in Chapter 17), respectively.
I have exercised extreme care in designing these problems/questions, and then
in solving them. However, no matter how careful one is with the preparation of a work
such as this, errors will always remain in the final product. Therefore, corrections,
suggestions, and comments from instructors who use the textbook (as well as their
teaching assistants) pertaining to homework problems/solutions are welcomed. These
may be sent to me in care of the publisher.
1
CHAPTER 2
ATOMIC STRUCTURE AND INTERATOMIC BONDING
PROBLEM SOLUTIONS
2.1 (a) When two or more atoms of an element have different atomic masses, each is termed an
isotope.
(b) The atomic weights of the elements ordinarily are not integers because: (1) the atomic masses
of the atoms generally are not integers (except for
12
C), and (2) the atomic weight is taken as the
weighted average of the atomic masses of an atom's naturally occurring isotopes.
2.2 Atomic mass is the mass of an individual atom, whereas atomic weight is the average (weighted) of
the atomic masses of an atom's naturally occurring isotopes.
2.3 (a) In order to determine the number of grams in one amu of material, appropriate manipulation of
the amu/atom, g/mol, and atom/mol relationships is all that is necessary, as
⎛
⎞ ⎛ 1 g / mol ⎞
1 mol
⎟
# g/amu = ⎜
⎟⎜
23
⎝ 6.023 x 10
atoms ⎠ ⎝ 1 amu / atom ⎠
= 1.66 x 10-24 g/amu
(b) Since there are 453.6 g/lbm,
(
)(
23
1 lb - mol = 453.6 g/lbm 6.023 x 10
)
atoms/g - mol
= 2.73 x 1026 atoms/lb-mol
2.4 (a) Two important quantum-mechanical concepts associated with the Bohr model of the atom are
that electrons are particles moving in discrete orbitals, and electron energy is quantized into shells.
(b) Two important refinements resulting from the wave-mechanical atomic model are that electron
position is described in terms of a probability distribution, and electron energy is quantized into both
shells and subshells--each electron is characterized by four quantum numbers.
2.5 The n quantum number designates the electron shell.
2
The l quantum number designates the electron subshell.
The m quantum number designates the number of electron states in each electron subshell.
l
The m quantum number designates the spin moment on each electron.
s
2.6 For the L state, n = 2, and eight electron states are possible. Possible l values are 0 and 1, while
1
possible ml values are 0 and &plusmn;1. Therefore, for the s states, the quantum numbers are 200 ( ) and
2
1
1
1
1
1
2
2
2
2
200 (− ) . For the p states, the quantum numbers are 210 ( ) , 210 (− ) , 211 ( ) , 211 (− ) ,
2
1
1
2
2
21(-1 )( ) , and 21(-1 )(− ) .
For the M state, n = 3, and 18 states are possible. Possible l values are 0, 1, and 2;
1
possible ml values are 0, &plusmn;1, and &plusmn;2; and possible ms values are &plusmn; . Therefore, for the s states,
2
1
1
1
1
1
2
2
1
2
1
2
1
2
2
the quantum numbers are 300 ( ) , 300 (− ) , for the p states they are 310 ( ) , 310 (− ) , 311 ( ) ,
2
1
1
1
2
1
2
1
2
1
1
1
1
1
2
2
2
2
2
2
2
311 (− ) , 31(-1 )( ) , and 31(-1 )(− ) ;
for the d states they are 320 ( ) , 320 (− ) , 321 ( ) ,
2
321 (− ) , 32(-1 )( ) , 32(-1 )(− ) , 322 ( ) , 322 (− ) , 32(-2) ( ) , and 32(-2) (− ) .
2.7 The electron configurations of the ions are determined using Table 2.2.
2+
2 2 6 2 6 6
Fe - 1s 2s 2p 3s 3p 3d
3+
2 2 6 2 6 5
Fe - 1s 2s 2p 3s 3p 3d
+
2 2 6 2 6 10
Cu - 1s 2s 2p 3s 3p 3d
2+
2 2 6 2 6 10 2 6 10 2 6
Ba - 1s 2s 2p 3s 3p 3d 4s 4p 4d 5s 5p
2 2 6 2 6 10 2 6
Br - 1s 2s 2p 3s 3p 3d 4s 4p
22 2 6 2 6
S - 1s 2s 2p 3s 3p
2.8
+
The Na ion is just a sodium atom that has lost one electron; therefore, it has an electron
configuration the same as neon (Figure 2.6).
The Cl ion is a chlorine atom that has acquired one extra electron; therefore, it has an
electron configuration the same as argon.
2.9 Each of the elements in Group IIA has two s electrons.
2 2 6 2 6 7 2
2.10 (a) The 1s 2s 2p 3s 3p 3d 4s electron configuration is that of a transition metal because of an
incomplete d subshell.
3
2 2 6 2 6
(b) The 1s 2s 2p 3s 3p electron configuration is that of an inert gas because of filled 3s and 3p
subshells.
2 2 5
(c) The 1s 2s 2p electron configuration is that of a halogen because it is one electron deficient
from having a filled L shell.
2 2 6 2
(d) The 1s 2s 2p 3s electron configuration is that of an alkaline earth metal because of two s
electrons.
2 2 6 2 6 2 2
(e) The 1s 2s 2p 3s 3p 3d 4s electron configuration is that of a transition metal because of an
incomplete d subshell.
2 2 6 2 6 1
(f) The 1s 2s 2p 3s 3p 4s electron configuration is that of an alkali metal because of a single s
electron.
2.11 (a) The 4f subshell is being filled for the rare earth series of elements.
(b) The 5f subshell is being filled for the actinide series of elements.
2.12 The attractive force between two ions FA is just the derivative with respect to the interatomic
separation of the attractive energy expression, Equation (2.8), which is just
FA =
dE A
dr
⎛ A⎞
d⎜− ⎟
⎝ r⎠
A
=
= 2
dr
r
The constant A in this expression is defined in footnote 3. Since the valences of the Ca2+ and O2ions (Z1 and Z2) are both 2, then
FA =
(Z1e )(Z2e)
4πεor 2
(
−19
(2)(2 ) 1.6 x 10
=
(
(4)(π) 8.85 x 10
−12
)
C
)(
2
F / m) 1.25 x 10
= 5.89 x 10-10 N
2.13 (a) Differentiation of Equation (2.11) yields
dEN
dr
=
A
−
r(1 + 1)
4
nB
r(n + 1)
= 0
−9
)
m
2
(b) Now, solving for r (= r )
o
A
ro 2
nB
=
ro(n + 1)
or
⎛ A⎞
ro = ⎜ ⎟
⎝ nB ⎠
1/(1 - n)
(c) Substitution for ro into Equation (2.11) and solving for E (= Eo)
Eo = −
= −
A
B
+
r
ron
o
A
⎛ A⎞
⎜ ⎟
⎝ nB ⎠
1/(1 - n)
+
B
⎛ A⎞
⎜ ⎟
⎝ nB ⎠
n/(1 - n)
2.14 (a) Curves of E , E , and E are shown on the plot below.
A R
N
5
(b) From this plot
r = 0.24 nm
o
E = -5.3 eV
o
(c) From Equation (2.11) for E
N
A = 1.436
-6
B = 7.32 x 10
n=8
Thus,
⎛ A⎞
ro = ⎜ ⎟
⎝ nB ⎠
⎡
1.436
⎢
= ⎢
-6
⎢⎣(8) 7.32 x 10
(
1/(1 - n)
1/(1 - 8)
⎤
⎥
⎥
⎥⎦
= 0.236 nm
)
and
Eo = −
1.436
⎡
⎤
1.436
⎢
⎥
⎢ (8) ⎛ 7.32 x 10−6 ⎞ ⎥
⎠⎦
⎣ ⎝
1/(1 − 8)
+
7.32 x 10 −6
⎡
⎤
1.436
⎢
⎥
⎢ (8) ⎛ 7.32 x 10 −6 ⎞ ⎥
⎠⎦
⎣ ⎝
8 /(1 − 8)
= - 5.32 eV
2.15 This problem gives us, for a hypothetical X+-Y- ion pair, values for ro (0.35 nm), Eo (-6.13 eV), and
n (10), and asks that we determine explicit expressions for attractive and repulsive energies of
Equations 2.8 and 2.9. In essence, it is necessary to compute the values of A and B in these
equations. Expressions for ro and Eo in terms of n, A, and B were determined in Problem 2.13,
which are as follows:
⎛ A⎞
ro = ⎜ ⎟
⎝ nB ⎠
6
1/(1 - n)
Eo = −
A
⎛ A⎞
⎜
⎟
⎝ nB ⎠
+
1/(1 - n)
B
⎛ A⎞
⎜
⎟
⎝ nB ⎠
n/(1 - n)
Thus, we have two simultaneous equations with two unknowns (viz. A and B). Upon substitution of
values for ro and Eo in terms of n, these equations take the forms
⎛ A ⎞ 1/(1 - 10)
0.35 nm = ⎜
⎟
⎝ 10B ⎠
− 6.13 eV = −
A
⎛ A ⎞
⎜
⎟
⎝ 10B ⎠
1/(1 − 10)
+
B
⎛ A ⎞
⎜
⎟
⎝ 10B ⎠
10 /(1 − 10)
Simultaneous solution of these two equations leads to A = 2.38 and B = 1.88 x 10-5.
Thus,
Equations (2.8) and (2.9) become
2.38
r
EA = −
ER =
1.88 x 10 −5
r10
Of course these expressions are valid for r and E in units of nanometers and electron volts,
respectively.
2.16 (a) Differentiating Equation (2.12) with respect to r yields
−r / ρ
dE
C
De
=
−
2
ρ
dr
r
At r = ro, dE/dr = 0, and
C
ro 2
=
De
− (ro /ρ)
ρ
Solving for C and substitution into Equation (2.12) yields an expression for Eo as
7
(2.12b)
Eo = De
− (ro/ρ) ⎛
ro ⎞
⎜1 −
⎟
ρ⎠
⎝
(b) Now solving for D from Equation (2.12b) above yields
D =
Cρe
(ro/ρ)
ro2
Substitution of this expression for D into Equation (2.12) yields an expression for Eo as
Eo =
⎞
C⎛ ρ
⎜⎜
− 1⎟⎟
r ⎝r
⎠
o o
2.17 (a) The main differences between the various forms of primary bonding are:
Ionic--there is electrostatic attraction between oppositely charged ions.
Covalent--there is electron sharing between two adjacent atoms such that each atom assumes a
stable electron configuration.
Metallic--the positively charged ion cores are shielded from one another, and also &quot;glued&quot; together
by the sea of valence electrons.
(b)
The Pauli exclusion principle states that each electron state can hold no more than two
electrons, which must have opposite spins.
2.18
Covalently bonded materials are less dense than metallic or ionically bonded ones because
covalent bonds are directional in nature whereas metallic and ionic are not;
when bonds are
directional, the atoms cannot pack together in as dense a manner, yielding a lower mass density.
2.19
The percent ionic character is a function of the electron negativities of the ions XA and XB
according to Equation (2.10). The electronegativities of the elements are found in Figure 2.7.
For MgO, XMg = 1.2 and XO = 3.5, and therefore,
2⎤
⎡
%IC = ⎢1 − e (− 0.25) (3.5 − 1.2) ⎥ x 100 = 73.4%
⎣
⎦
For GaP, XGa = 1.6 and XP = 2.1, and therefore,
8
2⎤
⎡
%IC = ⎢1 − e (− 0.25) (2.1−1.6) ⎥ x 100 = 6.1%
⎣
⎦
For CsF, XCs = 0.7 and XF = 4.0, and therefore,
2⎤
⎡
%IC = ⎢1 − e (− 0.25) (4.0 − 0.7) ⎥ x 100 = 93.4%
⎣
⎦
For CdS, XCd = 1.7 and XS = 2.5, and therefore,
2⎤
⎡
%IC = ⎢1 − e (− 0.25) (2.5 − 1.7 ) ⎥ x 100 = 14.8%
⎣
⎦
For FeO, XFe = 1.8 and XO = 3.5, and therefore,
2⎤
⎡
%IC = ⎢1 − e (− 0.25) (3.5 − 1.8) ⎥ x 100 = 51.4%
⎣
⎦
2.20 Below is plotted the bonding energy versus melting temperature for these four metals. From this
plot, the bonding energy for copper (melting temperature of 1084&deg;C) should be approximately 3.6
eV. The experimental value is 3.5 eV.
9
2 2
2.21 For silicon, having the valence electron structure 3s 3p , N' = 4; thus, there are 8 - N' = 4 covalent
bonds per atom.
2 5
For bromine, having the valence electron structure 4s 4p , N' = 7; thus, there is 8 - N' = 1
covalent bond per atom.
2 3
For nitrogen, having the valence electron structure 2s 2p , N' = 5; thus, there are 8 - N' = 3
covalent bonds per atom.
2 4
For sulfur, having the valence electron structure 3s 3p , N' = 6; thus, there are 8 - N' = 2
covalent bonds per atom.
2.22 For brass, the bonding is metallic since it is a metal alloy.
For rubber, the bonding is covalent with some van der Waals. (Rubber is composed
primarily of carbon and hydrogen atoms.)
For BaS, the bonding is predominantly ionic (but with some covalent character) on the basis
of the relative positions of Ba and S in the periodic table.
For solid xenon, the bonding is van der Waals since xenon is an inert gas.
For bronze, the bonding is metallic since it is a metal alloy (composed of copper and tin).
For nylon, the bonding is covalent with perhaps some van der Waals. (Nylon is composed
primarily of carbon and hydrogen.)
For AlP the bonding is predominantly covalent (but with some ionic character) on the basis
of the relative positions of Al and P in the periodic table.
2.23 The intermolecular bonding for HF is hydrogen, whereas for HCl, the intermolecular bonding is van
der Waals. Since the hydrogen bond is stronger than van der Waals, HF will have a higher melting
temperature.
2.24 The geometry of the H O molecules, which are hydrogen bonded to one another, is more restricted
2
in the solid phase than for the liquid. This results in a more open molecular structure in the solid, and
a less dense solid phase.
10
CHAPTER 3
THE STRUCTURE OF CRYSTALLINE SOLIDS
PROBLEM SOLUTIONS
3.1 Atomic structure relates to the number of protons and neutrons in the nucleus of an atom, as well as
the number and probability distributions of the constituent electrons. On the other hand, crystal
structure pertains to the arrangement of atoms in the crystalline solid material.
3.2 A crystal structure is described by both the geometry of, and atomic arrangements within, the unit
cell, whereas a crystal system is described only in terms of the unit cell geometry. For example,
face-centered cubic and body-centered cubic are crystal structures that belong to the cubic crystal
system.
3.3 For this problem, we are asked to calculate the volume of a unit cell of aluminum. Aluminum has an
FCC crystal structure (Table 3.1). The FCC unit cell volume may be computed from Equation (3.4)
as
VC = 16R
3
(
-9
2 = (16) 0.143 x 10
)
m
3
2 = 6.62 x 10
3.4 This problem calls for a demonstration of the relationship a = 4R
unit cell shown below
Using the triangle NOP
11
-29
3
m
3 for BCC. Consider the BCC
(NP)2 = a 2 + a 2 = 2a 2
And then for triangle NPQ,
(NQ)2 = (QP)2 + (NP)2
But NQ = 4R, R being the atomic radius. Also, QP = a. Therefore,
(4R)2 = a 2 + 2a2 , or
a =
4R
3
3.5 We are asked to show that the ideal c/a ratio for HCP is 1.633. A sketch of one-third of an HCP unit
cell is shown below.
Consider the tetrahedron labeled as JKLM, which is reconstructed as
12
The atom at point M is midway between the top and bottom faces of the unit cell--that is MH = c/2.
And, since atoms at points J, K, and M, all touch one another,
JM = JK = 2R = a
where R is the atomic radius. Furthermore, from triangle JHM,
(JM) 2 = (JH)2 + (MH)2, or
a
2
2
= (JH)
⎛ c⎞
+ ⎜ ⎟
⎝ 2⎠
2
Now, we can determine the JH length by consideration of triangle JKL, which is an equilateral
triangle,
cos 30&deg; =
a/ 2
=
JH
JH =
3
, and
2
a
3
Substituting this value for JH in the above expression yields
2
2
⎛ a ⎞
a2
c2
⎛ c⎞
⎜
⎟
a2 = ⎜
+
=
+
⎟
⎝ 2⎠
3
4
⎝ 3⎠
and, solving for c/a
13
c
=
a
8
= 1.633
3
3.6 We are asked to show that the atomic packing factor for BCC is 0.68. The atomic packing factor is
defined as the ratio of sphere volume to the total unit cell volume, or
APF =
VS
VC
Since there are two spheres associated with each unit cell for BCC
3
⎛ 4πR 3 ⎞
8πR
VS = 2(sphere volume) = 2 ⎜⎜
⎟⎟ =
3
⎝ 3 ⎠
3
Also, the unit cell has cubic symmetry, that is V = a . But a depends on R according to Equation
C
(3.3), and
⎛ 4R ⎞
VC = ⎜
⎟
⎝ 3⎠
3
=
64R 3
3 3
Thus,
APF =
8πR 3 / 3
64R 3 / 3 3
= 0.68
3.7 This problem calls for a demonstration that the APF for HCP is 0.74. Again, the APF is just the total
sphere-unit cell volume ratio. For HCP, there are the equivalent of six spheres per unit cell, and thus
⎛ 4π R3 ⎞
VS = 6 ⎜⎜
⎟⎟ = 8πR 3
3
⎝
⎠
Now, the unit cell volume is just the product of the base area times the cell height, c. This base area
is just three times the area of the parallelepiped ACDE shown below.
14
The area of ACDE is just the length of CD times the height BC . But CD is just a or 2R, and
BC = 2R cos (30&deg;) =
2R 3
2
Thus, the base area is just
⎛ 2R 3 ⎞
2
AREA = (3)(CD)(BC) = (3)(2 R) ⎜
⎟ = 6R 3
2
⎝
⎠
and since c = 1.633a = 2R(1.633)
(
2
2
VC = (AREA)(c) = 6R c 3 = 6 R
)
3 (2)(1.633)R = 12 3 (1.633 )R
3
Thus,
APF =
VS
VC
3
=
8π R
12 3 (1.633 )R 3
= 0.74
3.8 This problem calls for a computation of the density of iron. According to Equation (3.5)
ρ =
nAFe
VC NA
For BCC, n = 2 atoms/unit cell, and
15
⎛ 4R ⎞
VC = ⎜
⎟
⎝ 3⎠
3
Thus,
ρ =
(2 atoms/unit cell)(55.9 g/mol)
3
⎧⎡
⎫
3
⎤
⎪
⎪
-7
23
⎨⎢(4 ) 0.124 x 10 cm / 3 ⎥ /(unit cell)⎬ 6.023 x 10 atoms/mol
⎪⎩⎣
⎪⎭
⎦
(
)
(
)
= 7.90 g/cm3
3
The value given inside the front cover is 7.87 g/cm .
3.9 We are asked to determine the radius of an iridium atom, given that Ir has an FCC crystal structure.
For FCC, n = 4 atoms/unit cell, and V = 16R
C
3
ρ =
2 [Equation (3.4)]. Now,
nAIr
V N
C A
And solving for R from the above two expressions yields
⎛ nA
⎞
Ir
⎟
R = ⎜⎜
⎟
⎝ 16ρN A 2 ⎠
⎡
⎢
= ⎢
⎢⎣
(
1/3
(4 atoms/unit cell)(192.2 g/mol)
2 )(16) 22.4 g/cm3 6.023 x 10 23 atoms/mol
(
)(
⎤
⎥
⎥
⎥⎦
1/3
)
= 1.36 x 10-8 cm = 0.136 nm
3.10 This problem asks for us to calculate the radius of a vanadium atom. For BCC, n = 2 atoms/unit cell,
and
⎛ 4R ⎞
VC = ⎜
⎟
⎝ 3⎠
16
3
=
64R 3
3 3
Since,
ρ =
nAV
V N
C A
and solving for R
⎛ 3 n 3A ⎞
V⎟
R = ⎜
⎜ 64ρN ⎟
A ⎠
⎝
1/3
⎡
3 3 (2 atoms/unit cell)(50.9 g/mol)
⎢
= ⎢
3
23 atoms/mol
⎢⎣ (64) 5.96 g/cm 6.023 x 10
( )
(
)(
⎤
⎥
⎥
⎥⎦
1/3
)
= 1.32 x 10-8 cm = 0.132 nm
3.11 For the simple cubic crystal structure, the value of n in Equation (3.5) is unity since there is only a
single atom associated with each unit cell. Furthermore, for the unit cell edge length, a = 2R.
Therefore, employment of Equation (3.5) yields
ρ =
nA
V N
=
C A
=
nA
(2R )3N
A
(1 atom/unit cell)(74.5 g/mol)
3
⎫⎪
⎪⎧⎡
23
-8
⎤
⎨⎢⎣(2) 1.45 x 10 cm ⎥⎦ /(unit cell)⎬ 6.023 x 10 atoms/mol
⎪⎭
⎪⎩
(
)
(
5.07 g/cm3
3.12. (a) The volume of the Ti unit cell may be computed using Equation (3.5) as
VC =
nATi
ρN
Now, for HCP, n = 6 atoms/unit cell, and for Ti, A
17
A
Ti
= 47.9 g/mol. Thus,
)
VC =
(6 atoms/unit cell)(47.9 g/mol)
23
3
4.51 g/cm 6.023 x 10 atoms/mol
(
)(
)
= 1.058 x 10-22 cm3/unit cell = 1.058 x 10-28 m3/unit cell
(b) From the solution to Problem 3.7, since a = 2R, then, for HCP
VC =
3 3 a 2c
2
but, since c = 1.58a
VC =
3 3 (1.58)a 3
-22
3
= 1.058 x 10
cm /unit cell
2
Now, solving for a
(
⎡ 2 1.058 x 10-22 cm3
⎢( )
a = ⎢
(3 ) 3 (1.58)
⎢⎣
( )
)⎤⎥
1/3
⎥
⎥⎦
= 2.96 x 10-8 cm = 0.296 nm
And finally
c = 1.58a = (1.58)(0.296 nm) = 0.468 nm
3.13 This problem asks that we calculate the theoretical densities of Al, Ni, Mg, and W.
(
Since Al has an FCC crystal structure, n = 4, and VC = 2R 2
)3 .
Also, R = 0.143 nm (1.43
x 10-8 cm) and AAl = 26.98 g/mol. Employment of Equation (3.5) yields
ρ =
(4 atoms/unit cell)(26.98 g/mol)
3
⎧
⎫
-8
23
atoms/mol
⎨ (2)(1.43 x 10 cm) 2 /(unit cell) ⎬ 6.023 x 10
⎩
⎭
[
( )]
(
= 2.71 g/cm3
The value given in the table inside the front cover is 2.71 g/cm3.
18
)
Nickel also has an FCC crystal structure and therefore
ρ =
(4 atoms/unit cell)(58.69 g/mol)
3
⎫
⎧
-8
23
atoms/mol
⎨ (2)(1.25 x 10 cm) 2 /(unit cell )⎬ 6.023 x 10
⎩
⎭
[
( )]
(
)
= 8.82 g/cm3
The value given in the table is 8.90 g/cm3.
Magnesium has an HCP crystal structure, and from Problem 3.7,
3 3 a 2c
2
VC =
and, since c = 1.624a and a = 2R = 2(1.60 x 10-8 cm) = 3.20 x 10-8 cm
(
)
3 3 (1.624) 3.20 x 10-8 cm
VC =
3
2
−22
= 1.38 x 10
3
cm /unit cell
Also, there are 6 atoms/unit cell for HCP. Therefore the theoretical density is
ρ =
nAMg
V N
C A
=
(6 atoms/unit cell)(24.31 g/mol)
23
-22
1.38 x 10
cm3 /unit cell 6.023 x 10 atoms/mol
(
)(
)
= 1.75 g/cm3
The value given in the table is 1.74 g/cm3.
Tungsten has a BCC crystal structure for which n = 2 and a =
and R = 0.137 nm. Therefore, employment of Equation (3.5) leads to
19
4R
; also AW = 183.85 g/mol
3
ρ =
(2 atoms/unit cell)(183.85 g/mol)
(
)
3
⎧⎡
⎫
⎤
-8
⎪⎪⎢(4 ) 1.37 x 10 cm ⎥
⎪⎪
23
/(unit
cell)
⎨⎢
⎬ 6.023 x 10 atoms/mol
⎥
3
⎪⎢
⎪
⎥⎦
⎪⎩⎣
⎪⎭
(
)
= 19.3 g/cm3
The value given in the table is 19.3 g/cm3.
3.14 In order to determine whether Nb has an FCC or BCC crystal structure, we need to compute its
density for each of the crystal structures. For FCC, n = 4, and a = 2 R 2 . Also, from Figure 2.6, its
atomic weight is 92.91 g/mol. Thus, for FCC
ρ =
nA
Nb
3
2R 2 N A
(
)
(4 atoms/unit cell)(92.91 g/mol)
3
⎧⎡
⎫
-8
23
2 ⎤ /(unitcell)⎬ 6.023 x 10 atoms / mol
⎨ (2) 1.43 x 10 cm
⎣
⎦
⎩
⎭
=
(
)( )
(
)
= 9.33 g/cm3
For BCC, n = 2, and a =
=
4R
, thus
3
(2 atoms/unit cell)(92.91 g/mol)
3
⎫
⎧⎡
-8
⎤
⎪
⎪⎢ (4) 1.43 x 10 cm ⎥
⎬ 6.023 x 10 23 atoms/ mol
⎨⎢
/(unitcell)
⎥
3
⎪
⎪⎢
⎥⎦
⎪⎭
⎪⎩⎣
(
)
(
)
= 8.57 g/cm3
which is the value provided in the problem. Therefore, Nb has a BCC crystal structure.
3.15 For each of these three alloys we need to, by trial and error, calculate the density using Equation
(3.5), and compare it to the value cited in the problem. For SC, BCC, and FCC crystal structures,
20
the respective values of n are 1, 2, and 4, whereas the expressions for a (since VC = a3) are 2R,
2 R 2 , and 4R / 3 .
For alloy A, let us calculate ρ assuming a BCC crystal structure.
ρ =
nAA
V N
C A
=
(2 atoms/unit cell)(43.1 g/mol)
3
⎧
⎫
⎡
-8
⎤
⎪⎪⎢ (4) 1.22 x 10 cm ⎥
⎪⎪
/(unit cell)⎬ 6.023 x 1023 atoms/mol
⎨⎢
⎥
3
⎪⎢
⎪
⎥⎦
⎪⎩⎣
⎪⎭
(
)
(
)
= 6.40 g/cm3
Therefore, its crystal structure is BCC.
For alloy B, let us calculate ρ assuming a simple cubic crystal structure.
ρ =
(1 atom/unit cell)(184.4 g/mol)
3
⎫⎪
⎪⎧⎡
23
-8
⎤
⎨⎢⎣(2 ) 1.46 x 10 cm ⎥⎦ /(unit cell)⎬ 6.023 x 10 atoms/mol
⎪⎭
⎪⎩
(
)
(
)
= 12.3 g/cm3
Therefore, its crystal structure is simple cubic.
For alloy C, let us calculate ρ assuming a BCC crystal structure.
ρ =
(2 atoms/unit cell)(91.6 g/mol)
3
⎧
⎫
⎡
-8
⎤
⎪⎪⎢(4) 1.37 x 10 cm ⎥
⎪⎪
/(unit cell)⎬ 6.023 x 1023 atoms/mol
⎨⎢
⎥
3
⎪⎢
⎪
⎥⎦
⎪⎩⎣
⎪⎭
(
)
(
= 9.60 g/cm3
Therefore, its crystal structure is BCC.
21
)
3.16 In order to determine the APF for U, we need to compute both the unit cell volume (VC) which is
just the product of the three unit cell parameters, as well as the total sphere volume (VS) which is
just the product of the volume of a single sphere and the number of spheres in the unit cell (n). The
value of n may be calculated from Equation (3.5) as
ρVC NA
n =
AU
(
)(
(19.05)(2.86)(5.87)(4.95) x10 -24 6.023 x 1023
=
283.03
= 4.01 atoms/unit cell
Therefore
⎛4
⎞
(4) ⎜ π R3 ⎟
⎝3
⎠
APF =
=
VC
(a)(b)(c)
VS
⎡4
3⎤
(4)⎢ (π)(0.1385) ⎥
⎣3
⎦
=
(0.286)(0.587)(0.495)
= 0.536
3.17 (a) From the definition of the APF
APF =
VS
VC
=
⎛4
⎞
n ⎜ πR 3 ⎟
⎝3
⎠
a 2c
we may solve for the number of atoms per unit cell, n, as
2
n =
(APF)a c
4
πR 3
3
22
)
(
(0.693)(4.59)2(4.95) 10 -24 cm3
=
(
)
4
π 1.625 x 10-8 cm
3
3
)
= 4.0 atoms/unit cell
(b) In order to compute the density, we just employ Equation (3.5) as
nAIn
ρ =
a 2 cN
A
=
(4 atoms/unit cell)(114.82 g/mol)
2
⎡
⎤
-8
-8
23
atoms/mol
⎢ 4.59 x 10 cm 4.95 x 10 cm /unit cell ⎥ 6.023 x 10
⎣
⎦
(
)(
(
)
)
= 7.31 g/cm3
3. 18 (a) We are asked to calculate the unit cell volume for Be. From the solution to Problem 3.7
VC = 6R2c 3
But, c = 1.568a, and a = 2R, or c = 3.14R, and
3
VC = (6)(3.14) R
( )[0.1143 x 10-7 cm]
3
= (6) (3.14 ) 3
3
= 4.87 x 10−23 cm3 /unit cell
(b) The density of Be is determined as follows:
ρ =
For HCP, n = 6 atoms/unit cell, and for Be, A
ρ =
nA Be
VC NA
Be
= 9.01 g/mol. Thus,
(6 atoms/unit cell)(9.01 g/mol)
-23
3
23
4.87 x 10
cm /unit cell 6.023 x 10 atoms/mol
(
)(
23
)
= 1.84 g/cm3
3
The value given in the literature is 1.85 g/cm .
3.19 This problem calls for us to compute the atomic radius for Mg. In order to do this we must use
Equation (3.5), as well as the expression which relates the atomic radius to the unit cell volume for
HCP; from Problem 3.7 it was shown that
VC = 6R2c 3
In this case c = 1.624(2R). Making this substitution into the previous equation, and then solving
for R using Equation (3.5) yields
⎡
⎤
nAMg
⎥
R = ⎢
⎢ (1.624) 12 3 ρN ⎥
⎣
A⎦
(
1/3
)
⎡
⎢
(6 atoms/unit cell)(24.31 g/mol )
= ⎢
3
23 atoms/mol
⎢⎣ (1.624) 12 3 1.74 g/cm 6.023 x 10
(
)(
)(
1/3
⎤
⎥
⎥
⎥⎦
)
= 1.60 x 10-8 cm = 0.160 nm
3.20 This problem asks that we calculate the unit cell volume for Co which has an HCP crystal structure.
In order to do this, it is necessary to use a result of Problem 3.7, that is
VC = 6R2c 3
The problem states that c = 1.623a, and a = 2R. Therefore
VC = (1.623)(12 3 ) R 3
(
= (1.623)(12 3) 1.253 x 10
-8
cm
)
3
= 6.64 x 10
24
-23
cm
3
= 6.64 x 10
-2
3
nm
3.21 (a) The unit cell shown in the problem belongs to the tetragonal crystal system since a = b = 0.35
nm, c = 0.45 nm, and α = β = γ = 90&deg;.
(b) The crystal structure would be called body-centered tetragonal.
(c) As with BCC, n = 2 atoms/unit cell. Also, for this unit cell
(
VC = 3.5 x 10
−8
= 5.51 x 10
cm
−23
) (4.5 x 10−8 cm)
2
3
cm /unit cell
Thus,
ρ =
=
nA
VC NA
(2 atoms/unit cell)(141 g/mol )
-23
3
23
5.51 x 10
cm /unit cell 6.023 x 10
atoms/mol
(
)(
)
= 8.50 g/cm3
3.22 First of all, open ‘Notepad” in Windows. Now enter into “Notepad” commands to generate the
AuCu3 unit cell. One set of commands that may be used is as follows:
[DisplayProps]
Rotatez=-30
Rotatey=-15
[AtomProps]
Gold=LtRed,0.14
Copper=LtYellow,0.13
[BondProps]
SingleSolid=LtGray
[Atoms]
Au1=1,0,0,Gold
Au2=0,0,0,Gold
Au3=0,1,0,Gold
Au4=1,1,0,Gold
Au5=1,0,1,Gold
Au6=0,0,1,Gold
25
Au7=0,1,1,Gold
Au8=1,1,1,Gold
Cu1=0.5,0,0.5,Copper
Cu2=0,0.5,0.5,Copper
Cu3=0.5,1,0.5,Copper
Cu4=1,0.5,0.5,Copper
Cu5=0.5,0.5,1,Copper
Cu6=0.5,0.5,0,Copper
[Bonds]
B1=Au1,Au5,SingleSolid
B2=Au5,Au6,SingleSolid
B3=Au6,Au2,SingleSolid
B4=Au2,Au1,SingleSolid
B5=Au4,Au8,SingleSolid
B6=Au8,Au7,SingleSolid
B7=Au7,Au3,SingleSolid
B8=Au3,Au4,SingleSolid
B9=Au1,Au4,SingleSolid
B10=Au8,Au5,SingleSolid
B11=Au2,Au3,SingleSolid
B12=Au6,Au7,SingleSolid
Under the &quot;File&quot; menu of &quot;Note Pad,&quot; click &quot;Save As&quot;, and then assign the file for this figure a name
followed by a period and &quot;mdf&quot;; for example, “AuCu3.mdf”. And, finally save this file in the “mdf” file
inside of the “Interactive MSE” folder (which may be found in its installed location).
Now, in order to view the unit cell just generated, bring up “Interactive MSE”, and then
open any one of the three submodules under “Crystallinity and Unit Cells” or the “Ceramic
Structures” module. Next select “Open” under the “File” menu, and then open the “mdf” folder.
Finally, select the name you assigned to the item in the window that appears, and hit the “OK”
button. The image that you generated will now be displayed.
3.23 First of all, open ‘Notepad” in Windows.. Now enter into “Notepad” commands to generate the AuCu
unit cell. One set of commands that may be used is as follows:
[DisplayProps]
Rotatez=-30
Rotatey=-15
[AtomProps]
Gold=LtRed,0.14
Copper=LtYellow,0.13
[BondProps]
SingleSolid=LtGray
[Atoms]
Au1=0,0,0,Gold
Au2=1,0,0,Gold
Au3=1,1,0,Gold
Au4=0,1,0,Gold
Au5=0,0,1.27,Gold
Au6=1,0,1.27,Gold
26
Au7=1,1,1.27,Gold
Au8=0,1,1.27,Gold
Cu1=0.5,0.5,0.635,Copper
[Bonds]
B1=Au1,Au2,SingleSolid
B2=Au2,Au3,SingleSolid
B3=Au3,Au4,SingleSolid
B4=Au1,Au4,SingleSolid
B5=Au5,Au6,SingleSolid
B6=Au6,Au7,SingleSolid
B7=Au7,Au8,SingleSolid
B8=Au5,Au8,SingleSolid
B9=Au1,Au5,SingleSolid
B10=Au2,Au6,SingleSolid
B11=Au3,Au7,SingleSolid
B12=Au4,Au8,SingleSolid
Under the &quot;File&quot; menu of &quot;Note Pad,&quot; click &quot;Save As&quot;, and then assign the file for this figure a name
followed by a period and &quot;mdf&quot;; for example, “AuCu.mdf”. And, finally save this file in the “mdf” file
inside of the “Interactive MSE” folder (which may be found in its installed location).
Now, in order to view the unit cell just generated, bring up “Interactive MSE”, and then
open any one of the three submodules under “Crystallinity and Unit Cells” or the “Ceramic
Structures” module. Next select “Open” under the “File” menu, and then open the “mdf” folder.
Finally, select the name you assigned to the item in the window that appears, and hit the “OK”
button. The image that you generated will now be displayed.
3.24 A unit cell for the face-centered orthorhombic crystal structure is presented below.
3.25 This problem asks that we list the point coordinates for all of the atoms that are associated with the
FCC unit cell. From Figure 3.1b, the atom located of the origin of the unit cell has the coordinates
27
000.
Coordinates for other atoms in the bottom face are 100, 110, 010, and
11
2 2
coordinate for all these points is zero.)
0.
11
For the top unit cell face, the coordinates are 001, 101, 111, 011, and
2 2
(The z
1.
(These
coordinates are the same as bottom-face coordinates except that the “0” z coordinate has been
replaced by a “1”.)
Coordinates for only those atoms that are positioned at the centers of both side faces, and
centers of both front and back faces need to be specified. For the front and back-center face atoms,
the coordinates are 1
11
22
and 0
the respective coordinates are
1 1
, respectively. While for the left and right side center-face atoms,
22
1 1
2
0
2
and
1 1
1 .
2 2
3.26 (a) Here we are asked list point coordinates for both sodium and chlorine ions for a unit cell of the
sodium chloride crystal structure, which is shown in Figure 12.2.
In Figure 12.2, the chlorine ions are situated at all corners and face-centered positions.
Therefore, point coordinates for these ions are the same as for FCC, as presented in the previous
problem—that is, 000, 100, 110, 010, 001, 101, 111, 011,
1 1
11
2 2
0,
11
2 2
1, 1
11
22
, 0
1 1
22
,
1
2
0
1
2
, and
1 .
2 2
Furthermore, the sodium ions are situated at the centers of all unit cell edges, and, in
addition, at the unit cell center. For the bottom face of the unit cell, the point coordinates are as
follows:
1
2
1
1
2
2
00 , 1 0 ,
1
10 , 0 0 . While, for the horizontal plane that passes through the center of
2
1
1
111
2
2
2 22
the unit cell (which includes the ion at the unit cell center), the coordinates are 0 0 , 1 0 ,
1
1
1
2
2
2
11 , and 01 . And for the four ions on the top face
1
1
2
2
01 , 1 1 ,
1
,
11 , and 0 1 .
2
(b) This portion of the problem calls for us to list the point coordinates of both the zinc and sulfur
atoms for a unit cell of the zinc blende structure, which is shown in Figure 12.4.
First of all, the sulfur atoms occupy the face-centered positions in the unit cell, which from
the solution to Problem 3.25, are as follows: 000, 100, 110, 010, 001, 101, 111, 011,
1
11
22
,0
1 1
22
,
1
2
0
1
2
, and
1 1
11
2 2
0,
11
2 2
1,
1 .
2 2
Now, using an x-y-z coordinate system oriented as in Figure 3.4, the coordinates of the zinc
atom that lies toward the lower-left-front of the unit cell has the coordinates
situated toward the lower-right-back of the unit cell has coordinates of
that resides toward the upper-left-back of the unit cell has the
3 1 1
4 44
13 1
4 44
113
4 44
, whereas the atom
. Also, the zinc atom
coordinates.
coordinates of the final zinc atom, located toward the upper-right-front of the unit cell, are
28
And, the
3 33
4 44
.
3.27 A tetragonal unit in which are shown the 11
1
2
and
111
2 42
point coordinates is presented below.
3.28 This portion of the problem calls for us to draw a [12 1 ] direction within an orthorhombic unit cell (a
≠ b ≠ c, α = β = γ = 90&deg;). Such a unit cell with its origin positioned at point O is shown below. We
first move along the +x-axis a units (from point O to point A), then parallel to the +y-axis 2b units
(from point A to point B). Finally, we proceed parallel to the z-axis -c units (from point B to point C).
The [12 1 ] direction is the vector from the origin (point O) to point C as shown.
We are now asked to draw a (210) plane within an orthorhombic unit cell. First remove the three
indices from the parentheses, and take their reciprocals--i.e., 1/2, 1, and ∞. This means that the
29
plane intercepts the x-axis at a/2, the y-axis at b, and parallels the z-axis. The plane that satisfies
these requirements has been drawn within the orthorhombic unit cell below.
3.29 (a) This portion of the problem asks that a [0 1 1] direction be drawn within a monoclinic unit cell (a
≠ b ≠ c, and α = β = 90&deg; ≠ γ). One such unit cell with its origin at point O is sketched below. For this
direction, there is no projection along the x-axis since the first index is zero; thus, the direction lies in
the y-z plane. We next move from the origin along the minus y-axis b units (from point O to point R).
Since the final index is a one, move from point R parallel to the z-axis, c units (to point P). Thus, the
[0 1 1] direction corresponds to the vector passing from the origin to point P, as indicated in the
figure.
30
(b) A (002) plane is drawn within the monoclinic cell shown below. We first remove the parentheses
and take the reciprocals of the indices; this gives ∞, ∞, and 1/2. Thus, the (002) plane parallels
both x- and y-axes, and intercepts the z-axis at c/2, as indicated in the drawing.
3.30 (a) We are asked for the indices of the two directions sketched in the figure. For direction 1, the
projection on the x-axis is zero (since it lies in the y-z plane), while projections on the y- and z-axes
are b/2 and c, respectively. This is an  direction as indicated in the summary below
Projections
x
y
z
0a
b/2
c
0
1/2
1
0
1
2
Projections in terms of a, b,
and c
Reduction to integers
Enclosure

Direction 2 is [112 ] as summarized below.
Projections
x
y
z
a/2
b/2
-c
1/2
1/2
-1
1
1
-2
Projections in terms of a, b,
and c
Reduction to integers
31
Enclosure
[112 ]
(b) This part of the problem calls for the indices of the two planes which are drawn in the sketch.
Plane 1 is an (020) plane. The determination of its indices is summarized below.
x
y
z
∞a
b/2
∞c
Intercepts in terms of a, b,
and c
∞
1/2
∞
Reciprocals of intercepts
0
2
0
Intercepts
Enclosure
(020)
Plane 2 is a (22 1) plane, as summarized below.
x
y
z
Intercepts
a/2
-b/2
c
Intercepts in terms of a, b,
and c
1/2
-1/2
1
2
-2
1
Reciprocals of intercepts
Enclosure
(22 1)
3.31 The directions asked for are indicated in the cubic unit cells shown below.
32
3.32 Direction A is a [ 1 10] direction, which determination is summarized as follows. We first of all
position the origin of the coordinate system at the tail of the direction vector; then in terms of this
new coordinate system
Projections
x
y
z
-a
b
0c
-1
1
0
Projections in terms of a, b,
and c
Reduction to integers
not necessary
Enclosure
[ 1 10]
Direction B is a  direction, which determination is summarized as follows. The vector
passes through the origin of the coordinate system and thus no translation is necessary. Therefore,
x
Projections
y
a
b
2
Projections in terms of a, b,
33
z
c
2
and c
Reduction to integers
1
1
1
2
1
2
2
Enclosure
1

Direction C is a [0 1 2 ] direction, which determination is summarized as follows. We first of
all position the origin of the coordinate system at the tail of the direction vector; then in terms of this
new coordinate system
x
y
b
0a
−
and c
0
-
Reduction to integers
0
-1
Projections
Projections in terms of a, b,
Enclosure
2
z
-c
1
-1
2
-2
[0 1 2 ]
Direction D is a [12 1] direction, which determination is summarized as follows. We first of all
position the origin of the coordinate system at the tail of the direction vector; then in terms of this
new coordinate system
x
Projections
Projections in terms of a, b,
and c
Reduction to integers
y
a
z
c
-b
2
1
2
1
-1
2
1
2
-2
Enclosure
1
[12 1]
3.33 Direction A is a [331 ] direction, which determination is summarized as follows. We first of all
position the origin of the coordinate system at the tail of the direction vector; then in terms of this
new coordinate system
Projections
x
y
a
b
Projections in terms of a, b,
34
z
-
c
3
and c
1
1
Reduction to integers
3
3
Enclosure
-
1
3
-1
[331 ]
Direction B is a [4 03 ] direction, which determination is summarized as follows. We first of
all position the origin of the coordinate system at the tail of the direction vector; then in terms of this
new coordinate system
x
Projections
2a
-
3
Projections in terms of a, b,
and c
Reduction to integers
y
-
2
3
-4
Enclosure
z
c
0b
-
0
-
0
-3
2
1
2
[4 03 ]
Direction C is a [3 61] direction, which determination is summarized as follows. We first of
all position the origin of the coordinate system at the tail of the direction vector; then in terms of this
new coordinate system
x
Projections
-
Projections in terms of a, b,
and c
-
Reduction to integers
y
a
z
c
b
2
1
6
1
1
2
-3
6
6
Enclosure
1
[3 61]
Direction D is a [ 1 1 1 ] direction, which determination is summarized as follows. We first of
all position the origin of the coordinate system at the tail of the direction vector; then in terms of this
new coordinate system
Projections
-
x
y
a
b
2
2
Projections in terms of a, b,
35
z
-
c
2
and c
1
1
2
2
-1
1
-
Reduction to integers
Enclosure
-
1
2
-1

3.34 For tetragonal crystals a = b ≠ c and α = β = γ = 90&deg;; therefore, projections along the x and y axes
are equivalent, which are not equivalent to projections along the z axis.
(a) Therefore, for the  direction, equivalent directions are the following: , [ 1 0 1] , [ 1 01 ] ,
[10 1] , [01 1 ] , [0 1 1] , and [0 1 1 ] .
(b) Also, for the  direction, equivalent directions are the following: [ 1 00] , , and [0 1 0 ] .
3.35 (a) We are asked to convert  and  directions into the four- index Miller-Bravais scheme for
hexagonal unit cells. For 
u' = 1,
v' = 0,
w' = 0
From Equations (3.6)
u =
n
n
2n
(2u ' − v ' ) =
(2 − 0) =
3
3
3
v =
n
n
n
(2v ' − u' ) =
(0 − 1) = 3
3
3
n
⎛ 2n n ⎞
t = - (u + v) = - ⎜
− ⎟=⎝ 3
3
3⎠
w = nw' = 0
If we let n = 3, then u = 2, v = -1, t = -1, and w = 0. Thus, the direction is represented as [uvtw] =
[2 1 1 0 ] .
For , u' = 1, v' = 1, and w' = 1; therefore,
u =
v =
n
n
(2 − 1) =
3
3
n
n
(2 − 1) =
3
3
36
2n
⎛n n⎞
t =-⎜ + ⎟= ⎝ 3 3⎠
3
w=n
If we again let n = 3, then u = 1, v = 1, t = -2, and w = 3. Thus, the direction is represented as
[112 3] .
(b) This portion of the problem asks for the same conversion of the (010) and (101) planes. A plane
for hexagonal is represented by (hkil) where i = - (h + k), and h, k, and l are the same for both
systems. For the (010) plane, h = 0, k = 1, l = 0, and
i = - (0 + 1) = -1
Thus, the plane is now represented as (hkil) = (01 1 0) .
For the (101) plane, i = - (1 + 0) = -1, and (hkil) = (10 1 1) .
3.36 For plane A we will leave the origin at the unit cell as shown. If we extend this plane back into the
plane of the page, then it is a (11 1 ) plane, as summarized below.
Intercepts
x
y
z
a
b
-c
1
1
-1
1
1
-1
Intercepts in terms of a, b,
and c
Reciprocals of intercepts
Reduction
not necessary
Enclosure
(11 1 )
For plane B we will leave the origin of the unit cell as shown; this is a (230) plane, as
summarized below.
Intercepts
x
y
a
b
2
3
Intercepts in terms of a, b,
37
z
∞c
and c
Reciprocals of intercepts
1
1
2
3
2
3
Enclosure
∞
0
(230)
3.37 For plane A we will move the origin of the coordinate system one unit cell distance to the right along
the y axis; thus, this is a (1 1 0 ) plane, as summarized below.
x
Intercepts
Intercepts in terms of a, b,
and c
y
a
-
2
1
-
2
b
2
1
2
z
∞c
∞
Reciprocals of intercepts
2
-2
0
Reduction
1
-1
0
Enclosure
(1 1 0 )
For plane B we will leave the origin of the unit cell as shown; thus, this is a (122) plane, as
summarized below.
x
Intercepts
a
Intercepts in terms of a, b,
and c
Reciprocals of intercepts
1
1
y
z
b
c
2
2
1
1
2
2
2
2
Reduction
not necessary
Enclosure
(122)
3.38 For plane A since the plane passes through the origin of the coordinate system as shown, we will
move the origin of the coordinate system one unit cell distance vertically along the z axis; thus, this
is a (21 1 ) plane, as summarized below.
38
x
Intercepts
Intercepts in terms of a, b,
and c
Reciprocals of intercepts
a
2
1
2
2
y
z
b
-c
1
-1
1
-1
Reduction
not necessary
Enclosure
(21 1 )
For plane B, since the plane passes through the origin of the coordinate system as shown,
we will move the origin one unit cell distance vertically along the z axis; this is a (02 1 ) plane, as
summarized below.
x
Intercepts
y
∞a
Intercepts in terms of a, b,
and c
Reciprocals of intercepts
b
2
1
∞
2
0
2
Reduction
not necessary
Enclosure
(02 1 )
z
-c
-1
-1
3.39 The (01 1 1) and (2 1 1 0 ) planes in a hexagonal unit cell are shown below.
39
3.40 (a) For this plane we will leave the origin of the coordinate system as shown; thus, this is a (12 11)
plane, as summarized below.
a1
a2
Intercepts
a
-
Intercepts in terms of a's and c
1
-
Reciprocals of intercepts
1
-2
a
2
1
2
a3
z
a
c
1
1
1
1
Reduction
not necessary
Enclosure
(12 11)
(b) For this plane we will leave the origin of the coordinate system as shown; thus, this is a
(2 1 1 2) plane, as summarized below.
a1
a2
a3
z
Intercepts
a/2
-a
-a
c/2
Intercepts in terms of a's and c
1/2
-1
-1
1/2
2
-1
-1
2
Reciprocals of intercepts
Reduction
not necessary
Enclosure
(2 1 1 2)
3.41 The planes called for are plotted in the cubic unit cells shown below.
40
3.42 (a) The atomic packing of the (100) plane for the FCC crystal structure is called for. An FCC unit
cell, its (100) plane, and the atomic packing of this plane are indicated below.
(b) For this part of the problem we are to show the atomic packing of the (111) plane for the BCC
crystal structure. A BCC unit cell, its (111) plane, and the atomic packing of this plane are indicated
below.
41
3.43 (a) The unit cell in Problem 3.21 is body-centered tetragonal. Only the (100) (front face) and (0 1 0)
(left side face) planes are equivalent since the dimensions of these planes within the unit cell (and
therefore the distances between adjacent atoms) are the same (namely 0.45 nm x 0.35 nm), which
are different than the (001) (top face) plane (namely 0.35 nm x 0.35 nm).
(b) The equivalent planes are (101), (011), and (1 01) ; the dimensions of these planes within the
[
2
unit cell are the same--that is 0.35 nm x (0.35 nm)
+ (0.45 nm)2
]
1/ 2
.
(c) All of the (111), (1 1 1) , (11 1) , and (1 1 1 ) planes are equivalent.
3.44 (a) The intersection between (110) and (111) planes results in a [ 1 10] , or equivalently, a [1 1 0]
direction.
(b) The intersection between (110) and (1 1 0) planes results in a , or equivalently, a [00 1 ]
direction.
(c) The intersection between (11 1 ) and (001) planes results in a [ 1 10] , or equivalently, a [1 1 0]
direction.
3.45 (a) In the figure below is shown a  direction within an FCC unit cell.
For this  direction there is one atom at each of the two unit cell corners, and, thus, there is
the equivalent of 1 atom that is centered on the direction vector. The length of this direction vector is just
the unit cell edge length, 2R 2 [Equation (3.1)]. Therefore, the expression for the linear density of this
plane is
LD100 =
number of atoms centered on  direction vector
length of  direction vector
=
1 atom
1
=
2R 2
2R 2
An FCC unit cell within which is drawn a  direction is shown below.
42
For this  direction, the vector shown passes through only the centers of the single atom at each
of its ends, and, thus, there is the equivalence of 1 atom that is centered on the direction vector. The
length of this direction vector is denoted by z in this figure, which is equal to
z=
2
2
x +y
where x is the length of the bottom face diagonal, which is equal to 4R. Furthermore, y is the unit
cell edge length, which is equal to 2R 2 [Equation (3.1)]. Thus, using the above equation, the
length z may be calculate as follows:
z=
(4R)2
(
+ 2R 2
)
2
=
24R2 = 2R 6
Therefore, the expression for the linear density of this plane is
LD111 =
number of atoms centered on  direction vector
length of  direction vector
=
1 atom
1
=
2R 6
2R 6
(b) From the table inside the front cover, the atomic radius for copper is 0.128 nm. Therefore, the
linear density for the  direction is
LD100 (Cu) =
1
1
−1
−9 −1
=
= 2.76 nm = 2.76 x 10 m
2R 2
(2)(0.128 nm) 2
While for the  direction
43
LD111(Cu) =
1
1
−1
−9 −1
=
= 1.59 nm = 1.59 x 10 m
2R 6
(2)(0.128 nm) 6
3.46 (a) In the figure below is shown a  direction within a BCC unit cell.
For this  direction there is one atom at each of the two unit cell corners, and, thus, there is the
equivalence of 1 atom that is centered on the direction vector. The length of this direction vector is
denoted by x in this figure, which is equal to
x=
2
2
z −y
where y is the unit cell edge length, which, from Equation (3.3) is equal to
4R
. Furthermore, z is
3
the length of the unit cell diagonal, which is equal to 4R Thus, using the above equation, the length x
may be calculate as follows:
x =
(4R)2
⎛ 4R ⎞ 2
⎟ =
− ⎜
⎝ 3⎠
2
32R
3
= 4R
2
3
Therefore, the expression for the linear density of this direction is
LD110 =
number of atoms centered on  direction vector
length of  direction vector
=
1 atom
4R
2
3
=
3
4R 2
A BCC unit cell within which is drawn a  direction is shown below.
44
For although the  direction vector shown passes through the centers of three atoms, there is an
equivalence of only two atoms associated with this unit cell—one-half of each of the two atoms at the
end of the vector, in addition to the center atom belongs entirely to the unit cell. Furthermore, the
length of the vector shown is equal to 4R, since all of the atoms whose centers the vector passes
through touch one another. Therefore, the linear density is equal to
LD111 =
number of atoms centered on  direction vector
length of  direction vector
=
2 atoms
1
=
4R
2R
(b) From the table inside the front cover, the atomic radius for iron is 0.124 nm. Therefore, the
linear density for the  direction is
LD110 (Fe) =
3
4R 2
=
3
(4)(0.124 nm) 2
= 2.47 nm−1 = 2.47 x 10 −9 m−1
While for the  direction
LD111(Fe) =
1
1
=
= 4.03 nm−1 = 4.03 x 10−9 m−1
2R (2)(0.124 nm)
3.47 (a) In the figure below is shown a (100) plane for an FCC unit cell.
45
For this (100) plane there is one atom at each of the four cube corners, each of which is shared with
four adjacent unit cells, while the center atom lies entirely within the unit cell. Thus, there is the
equivalence of 2 atoms associated with this FCC (100) plane. The planar section represented in the
above figure is a square, wherein the side lengths are equal to the unit cell edge length, 2R 2
(
[Equation (3.1)]; and, thus, the area of this square is just 2 R 2
)2 = 8R2.
Hence, the planar density
for this (100) plane is just
PD100 =
number of atoms centered on (100) plane
area of (100) plane
=
2 atoms
8 R2
=
1
4R 2
That portion of an FCC (111) plane contained within a unit cell is shown below.
There are six atoms whose centers lie on this plane, which are labeled A through F. One-sixth of
each of atoms A, D, and F are associated with this plane (yielding an equivalence of one-half atom),
with one-half of each of atoms B, C, and E (or an equivalence of one and one-half atoms) for a total
equivalence of two atoms. Now, the area of the triangle shown in the above figure is equal to onehalf of the product of the base length and the height, h. If we consider half of the triangle, then
46
(2R)2 + h 2 = (4R)2
which leads to h = 2 R 3 . Thus, the area is equal to
Area =
(
)
4R(h) (4R) 2R 3
2
=
= 4R
2
2
3
And, thus, the planar density is
number of atoms centered on (111) plane
area of (111) plane
PD111 =
=
2 atoms
=
4R 2 3
1
2R2
3
(b) From the table inside the front cover, the atomic radius for aluminum is 0.143 nm. Therefore, the
planar density for the (100) plane is
PD100 (Al) =
1
4 R2
=
1
4(0.143 nm)2
= 12.23 nm−2 = 1.223 x 10 −17 m−2
While for the (111) plane
PD111(Al) =
1
2R2
3
=
1
2
3 (0.143 nm) 2
= 14.12 nm−2 = 1.412 x 10 −17 m−2
3.48 (a) A BCC unit cell within which is drawn a  plane is shown below.
For this (100) plane there is one atom at each of the four cube corners, each of which is shared with
four adjacent unit cells. Thus, there is the equivalence of 1 atom associated with this BCC (100)
plane. The planar section represented in the above figure is a square, wherein the side lengths are
47
equal to the unit cell edge length,
⎛ 4R ⎞
⎟
⎜
⎝ 3⎠
2
=
4R
[Equation (3.3)]; and, thus, the area of this square is just
3
16 R 2
. Hence, the planar density for this (100) plane is just
3
PD100 =
number of atoms centered on (100) plane
area of (100) plane
=
1 atom
16 R2
=
3
16 R2
3
A BCC unit cell within which is drawn a  plane is shown below.
For this (110) plane there is one atom at each of the four cube corners through which it passes, each
of which is shared with four adjacent unit cells, while the center atom lies entirely within the unit cell.
Thus, there is the equivalence of 2 atoms associated with this BCC (110) plane. The planar section
represented in the above figure is a rectangle, as noted in the figure below.
48
From this figure, the area of the rectangle is the product of x and y. The length x is just the unit cell
4R
. Now, the diagonal length z is equal to 4R. For
3
edge length, which for BCC [Equation (3.3)] is
the triangle bounded by the lengths x, y, and z
y=
2
2
z −x
Or
y =
⎛ 4R ⎞ 2
4R 2
⎟ =
(4R) − ⎜
3
⎝ 3⎠
2
Thus, in terms of R, the area of this (110) plane is just
⎛ 4 R ⎞ ⎛ 4R 2 ⎞ 16R2
⎟⎜
⎟ =
Area(110) = xy = ⎜
3
3 ⎠
⎝ 3⎠⎝
2
And, finally, the planar density for this (110) plane is just
PD110 =
number of atoms centered on (110) plane
area of (110) plane
=
2 atoms
16R2
2
=
3
8R 2 2
3
(b) From the table inside the front cover, the atomic radius for molybdenum is 0.136 nm. Therefore,
the planar density for the (100) plane is
PD100 (Mo) =
3
16R2
=
3
16(0.136 nm)2
= 10.14 nm−2 = 1.014 x 10−17 m −2
While for the (110) plane
PD110 (Mo) =
3
8R 2 2
=
3
8 (0.136 nm) 2
2
= 14.34 nm−2 = 1.434 x 10−17 m −2
3.49 (a) A (0001) plane for an HCP unit cell is show below.
49
Each of the 6 perimeter atoms in this plane is shared with three other unit cells, whereas the center
atom is shared with no other unit cells; this gives rise to three equivalent atoms belonging to this
plane.
In terms of the atomic radius R, the area of each of the 6 equilateral triangles that have been
2
drawn is R
3 , or the total area of the plane shown is 6R
2
3 . And the planar density for this
(0001) plane is equal to
PD0001 =
number of atoms centered on (0001) plane
area of (0001) plane
=
3 atoms
6R2
3
=
1
2R2
3
(b) From the table inside the front cover, the atomic radius for titanium is 0.145 nm. Therefore, the
planar density for the (0001) plane is
PD0001(Ti) =
1
2R2
3
=
1
2
3 (0.145 nm) 2
= 13.73 nm−2 = 1.373 x 10 −17 m −2
3.50 Unit cells are constructed below from the three crystallographic planes provided in the problem.
50
(a) This unit cell belongs to the tetragonal system since a = b = 0.40 nm, c = 0.55 nm, and α = β = γ
= 90&deg;.
(b) This crystal structure would be called body-centered tetragonal since the unit cell has tetragonal
symmetry, and an atom is located at each of the corners, as well as the cell center.
3.51 The unit cells constructed below show the three crystallographic planes that were provided in the
problem.
(a) This unit cell belongs to the orthorhombic crystal system since a = 0.25 nm, b = 0.30 nm, c =
0.20 nm, and α = β = γ = 90&deg;.
(b)
This crystal structure would be called face-centered orthorhombic since the unit cell has
orthorhombic symmetry, and an atom is located at each of the corners, as well as at each of the
face centers.
(c) In order to compute its atomic weight, we employ Equation (3.5), with n = 4; thus
51
A =
ρVCN A
n
18.91 g/cm3 )(2.0)(2.5)(3.0) (x 10-24 cm3 /unit cell)(6.023 x 1023 atoms/mol)
(
=
4 atoms/unit cell
= 42.7 g/mol
3.52 Although each individual grain in a polycrystalline material may be anisotropic, if the grains have
random orientations, then the solid aggregate of the many anisotropic grains will behave
isotropically.
3.53W From the table, aluminum has an FCC crystal structure and an atomic radius of 0.1431 nm. Using
Equation (3.1), the lattice parameter a may be computed as
a = 2 R 2 = (2)(0.1431 nm) 2 = 0.4048 nm
Now, the interplanar spacing d110 maybe determined using Equation (3.3W) as
d110 =
a
2
(1)
2
+ (1)
2
=
+ (0)
0.4048 nm
= 0.2862 nm
2
3.54W We must first calculate the lattice parameter using Equation (3.3) and the value of R cited in Table
3.1 as
4R (4)(0.1249 nm)
=
= 0.2884 nm
3
3
a=
Next, the interplanar spacing may be determined using Equation (3.3W) according to
d 310 =
a
2
(3)
2
+ (1)
2
=
+ (0)
And finally, employment of Equation (3.2W) yields
52
0.2884 nm
= 0.0912 nm
10
sin θ =
nλ (1)(0.0711 nm)
=
= 0.390
2d (2)(0.0912 nm)
θ = sin-1(0.390) = 22.94&deg;
And
2θ = (2)(22.94&deg;) = 45.88&deg;
3.55W From the table, α-iron has a BCC crystal structure and an atomic radius of 0.1241 nm. Using
Equation (3.3) the lattice parameter, a, may be computed as
a=
4R (4)(0.1241 nm)
=
= 0.2866 nm
3
3
Now, the d111 interplanar spacing may be determined using Equation (3.3W) as
a
d111 =
2
(1)
2
+ (1)
2
=
0.2866 nm
= 0.1655 nm
3
=
0.2866 nm
= 0.1170 nm
6
+ (1)
And, similarly for d211
a
d 211 =
(2)2 + (1)2 + (1)2
3.56W (a) From the data given in the problem, and realizing that 36.12&deg; = 2θ, the interplanar spacing for
the (311) set of planes may be computed using Equation (3.3W) as
d 311 =
nλ
(1)(0.0711 nm)
=
= 0.1147 nm
36.12&deg; ⎞
2 sin θ
⎛
(2) ⎜ sin
⎟
2 ⎠
⎝
(b) In order to compute the atomic radius we must first determine the lattice parameter, a, using
Equation (3.3W), and then R from Equation (3.1) since Rh has an FCC crystal structure. Therefore,
2
a = d 311 (3)
2
+ (1)
2
+ (1) = (0.1147 nm)
53
( 11)= 0.3804
nm
And
R =
a
0.3804 nm
=
= 0.1345 nm
2 2
2 2
3.57W. (a) From the data given in the problem, and realizing that 75.99&deg; = 2θ, the interplanar spacing for
the (211) set of planes may be computed using Equation (3.2W) as
d 211 =
nλ
(1)(0.1659 nm)
=
= 0.1348 nm
75.99&deg;⎞
2 sin θ
⎛
(2)⎜ sin
⎟
2 ⎠
⎝
(b) In order to compute the atomic radius we must first determine the lattice parameter, a, using
Equation (3.3W), and then R from Equation (3.3) since Nb has a BCC crystal structure. Therefore,
2
2
a = d 211 (2)
+ (1)
2
+ (1) = (0.1347 nm)
( 6 ) = 0.3300
nm
And
R=
a 3 (0.3300 nm) 3
=
= 0.1429 nm
4
4
3.58W The first step to solve this problem is to compute the interplanar spacing using Equation (3.2W).
Thus,
d hkl
(1)(0.1542 nm)
nλ
=
= 0.2035 nm
44.53&deg; ⎞
⎛
2 sin θ
(2)⎜ sin
⎟
2 ⎠
⎝
Now, employment of both Equations (3.3W) and (3.1), and the value of R for nickel from Table 3.1
h
2
+ k
2
2
+ l =
a
d
hkl
=
(2)(0.1246 nm) 2
(0.2035 nm)
This means that
54
=
2R
2
d
hkl
= 1.732
h2 + k2 + l2 = (1.732)2 = 3.0
By trial and error, the only three integers which are all odd or even, the sum of the squares of which
equals 3.0 are 1, 1, and 1. Therefore, the set of planes responsible for this diffraction peak is the
(111) set.
3.59W For each peak, in order to compute the interplanar spacing and the lattice parameter we must
employ Equations (3.3W) and (3.2W), respectively. For the first peak which occurs at 31.3&deg;
d111 =
nλ
(1)(0.1542 nm)
=
= 0.2858 nm
31.3&deg; ⎞
2 sin θ
⎛
(2)⎜ sin
⎟
2 ⎠
⎝
And
a = dhkl (h)2 + (k)2 + (l)2 = d111 (1)2 + (1)2 + (1)2
= (0.2858 nm) 3 = 0.4950 nm
Similar computations are made for the other peaks which results are tabulated below:
Peak Index
2θ
dhkl(nm)
a (nm)
200
36.6
0.2455
0.4910
220
52.6
0.1740
0.4921
311
62.5
0.1486
0.4929
222
65.5
0.1425
0.4936
3.60W The first four diffraction peaks that will occur for BCC consistent with h + k + l being even are
(110), (200), (211), and (220).
3.61W (a) Since W has a BCC crystal structure, only those peaks for which h + k + l are even will
appear. Therefore, the first peak results by diffraction from (110) planes.
(b) For each peak, in order to calculate the interplanar spacing we must employ Equation (3.2W).
For the first peak which occurs at 40.2&deg;
55
d110 =
nλ
(1)(0.1542 nm)
=
= 0.2244 nm
40.2&deg; ⎞
2 sin θ
⎛
(2)⎜ sin
⎟
2 ⎠
⎝
(c) Employment of Equations (3.3W) and (3.3) is necessary for the computation of R for W as
R =
=
a
3
4
(dhkl )( 3)
=
(0.2244 nm)(
3
)
(h)2 + (k)2 + (l) 2
4
(1)2 + (1)2 + (0)2
4
= 0.1374 nm
3.62
A material in which atomic bonding is predominantly ionic in nature is less likely to form a
noncrystalline solid upon solidification than a covalent material because covalent bonds are
directional whereas ionic bonds are nondirectional; it is more difficult for the atoms in a covalent
material to assume positions giving rise to an ordered structure.
56
CHAPTER 4
IMPERFECTIONS IN SOLIDS
PROBLEM SOLUTIONS
4.1 In order to compute the fraction of atom sites that are vacant in lead at 600 K, we must employ
Equation (4.1). As stated in the problem, Q = 0.55 eV/atom. Thus,
v
⎡
⎤
⎛ Q ⎞
0.55 eV / atom
⎢
⎥
= exp ⎜ − V ⎟ = exp ⎢−
−5
N
kT
⎝
⎠
eV / atom -K (600 K) ⎥⎥
⎢⎣ 8.62 x 10
⎦
NV
(
)
= 2.41 x 10
-5
4.2 Determination of the number of vacancies per cubic meter in gold at 900&deg;C (1173 K) requires the
utilization of Equations (4.1) and (4.2) as follows:
NA ρ Au
⎛ Q ⎞
⎛ Q ⎞
NV = N exp ⎜ − V ⎟ =
exp ⎜ − V ⎟
AAu
⎝ kT ⎠
⎝ kT ⎠
=
(6.023
)(
x 10 23 atoms/ mol 19.32 g / cm3
)exp ⎢⎡−
⎢
⎢⎣
196.9 g / mol
⎤
⎥
−5
8.62 x 10
eV / atom − K (1173 K) ⎥⎥
⎦
(
0.98 eV / atom
)
= 3.65 x 1018 cm-3 = 3.65 x 1024 m-3
4.3
This problem calls for the computation of the energy for vacancy formation in silver. Upon
examination of Equation (4.1), all parameters besides Q are given except N, the total number of
v
atomic sites. However, N is related to the density, (ρ), Avogadro's number (N ), and the atomic
A
weight (A) according to Equation (4.2) as
N =
=
(6.023
x 10
23
NA ρ Ag
A
Ag
)(
atoms / mol 10.49 g / cm
107.87 g / mol
57
3
)
= 5.86 x 1022 atoms/cm3 = 5.86 x 1028 atoms/m3
Now, taking natural logarithms of both sides of Equation (4.1), and, after some algebraic
manipulation
⎛ NV ⎞
QV = − RT ln ⎜
⎟
⎝ N ⎠
⎡ 3.60 x 10 23 m−3 ⎤
= − 8.62 x 10-5 eV/atom - K (1073 K) ln ⎢
⎥
⎢⎣ 5.86 x 1028 m −3 ⎥⎦
(
)
= 1.11 eV/atom
4.4 In this problem we are asked to cite which of the elements listed form with Cu the three possible solid
solution types. For complete substitutional solubility the following criteria must be met: 1) the
difference in atomic radii between Cu and the other element (ΔR%) must be less than &plusmn;15%, 2) the
crystal structures must be the same, 3) the electronegativities must be similar, and 4) the valences
should be the same, or nearly the same. Below are tabulated, for the various elements, these
criteria.
Element
ΔR%
Cu
Crystal
ΔElectro-
Structure
negativity
FCC
Valence
2+
C
-44
H
-64
O
-53
Ag
+13
FCC
0
1+
Al
+12
FCC
-0.4
3+
Co
-2
HCP
-0.1
2+
Cr
-2
BCC
-0.3
3+
Fe
-3
BCC
-0.1
2+
Ni
-3
FCC
-0.1
2+
Pd
+8
FCC
+0.3
2+
Pt
+9
FCC
+0.3
2+
Zn
+4
HCP
-0.3
2+
58
(a) Ni, Pd, and Pt meet all of the criteria and thus form substitutional solid solutions having complete
solubility.
(b) Ag, Al, Co, Cr, Fe, and Zn form substitutional solid solutions of incomplete solubility. All these
metals have either BCC or HCP crystal structures, and/or the difference between their atomic radii
and that for Cu are greater than &plusmn;15%, and/or have a valence different than 2+.
(c)
C, H, and O form interstitial solid solutions.
These elements have atomic radii that are
significantly smaller than the atomic radius of Cu.
4.5 In the drawing below is shown the atoms on the (100) face of an FCC unit cell; the interstitial site is
at the center of the edge.
The diameter of an atom that will just fit into this site (2r) is just the difference between the unit cell
edge length (a) and the radii of the two host atoms that are located on either side of the site (R); that
is
2r = a - 2R
However, for FCC a is related to R according to Equation (3.1) as a = 2R 2 ; therefore, solving for
r gives
r =
a − 2R
2R 2 − 2R
=
= 0.41R
2
2
A (100) face of a BCC unit cell is shown below.
59
The interstitial atom that just fits into this interstitial site is shown by the small circle. It is situated in
the plane of this (100) face, midway between the two vertical unit cell edges, and one quarter of the
distance between the bottom and top cell edges. From the right triangle that is defined by the three
arrows we may write
⎛ a⎞
⎜ ⎟
⎝ 2⎠
However, from Equation (3.3), a =
⎛ 4R ⎞
⎜
⎟
⎝2 3⎠
2
⎛a⎞
+ ⎜ ⎟
⎝ 4⎠
2
=
(R
+ r)
2
4R
, and, therefore, the above equation takes the form
3
2
⎛ 4R ⎞
+ ⎜
⎟
⎝ 4 3⎠
2
= R2 + 2R r + r 2
After rearrangement the following quadratic equation results:
r 2 + 2Rr − 0.667R 2 = 0
And upon solving for r, r = 0.291R.
60
Thus, for a host atom of radius R, the size of an interstitial site for FCC is approximately 1.4
times that for BCC.
4.6 (a) This problem asks that we derive Equation (4.7a). To begin, C1 is defined according to Equation
(4.3) as
m1
C1 =
m + m
1
x 100
2
or, equivalently
m1'
C1 =
m1' + m2'
x 100
where the primed m's indicate masses in grams. From Equation (4.4) we may write
m1' = nm1 A 1
m 2' = nm2 A2
And, substitution into the C1 expression
C1 =
nm1 A1
x 100
nm1A 1 + nm2 A 2
From Equation (4.5) it is the case that
( m1 +
C' n
nm1 =
1
m2
)
100
( m1 +
C' n
nm2 =
n
2
n
m2
)
100
And substitution of these expressions into the above equation leads to
61
C1' A 1
C1 =
C1' A 1 + C 2' A 2
x 100
which is just Equation (4.7a).
(b) This problem asks that we derive Equation (4.9a). To begin, C1'' is defined as the mass of
component 1 per unit volume of alloy, or
C1'' =
m1
V
If we assume that the total alloy volume V is equal to the sum of the volumes of the two constituents-i.e., V = V1 + V2--then
C1'' =
m
1
V + V
1
2
Furthermore, the volume of each constituent is related to its density and mass as
V1 =
V2 =
m1
ρ
1
m2
ρ
2
C1'' =
m
m1
ρ
1
1
+
m2
ρ
2
From Equation (4.3), m1 and m2 may be expressed as follows:
m1 =
(
C1 m1 + m 2
100
62
)
(
C2 m1 + m2
m2 =
)
100
Substitution of these equations into the preceding expression yields
C1'' =
(
)
)
(
C1 m1 + m 2
100
C1 m1 + m2
C 2 m1 + m 2
100
100
+
ρ1
ρ2
(
=
)
C1
C1
ρ
+
C2
1
ρ
2
If the densities ρ1 and ρ2 are given in units of g/cm3, then conversion to units of kg/m3 requires that
we multiply this equation by 103, inasmuch as
103 g/cm3 = 1 kg/m3
Therefore, the previous equation takes the form
C1'' =
C1
C1
ρ
+
1
3
C2
ρ
x 10
2
which is the desired expression.
(c) Now we are asked to derive Equation (4.10a). The density of an alloy ρave is just the total alloy mass
M divided by its volume V
ρ ave =
Or, in terms of the component elements 1 and 2
63
M
V
m1 + m2
ρ ave =
V + V
1
2
Here it is assumed that the total alloy volume is equal to the separate volumes of the individual
components, which is only an approximation; normally V will not be exactly equal to (V1 + V2).
Each of V1 and V2 may be expressed in terms of its mass density, which when substituted into the
above equation
m1 + m2
ρ ave =
m1
ρ
+
1
m2
ρ
2
Furthermore, from Equation (4.3)
m1 =
m2 =
(
)
(
)
C1 m1 + m 2
100
C2 m1 + m2
100
Which, when substituted into the above ρave expression yields
ρ ave =
m1 + m2
(1
C m + m
1
2
)
100
ρ1
=
2
+
(m1 +
m
2
)
100
ρ2
100
C1
ρ1
(d)
C
+
C2
ρ2
And, finally, the derivation of Equation (4.11b) for Aave is requested.
The alloy average
molecular weight is just the ratio of total alloy mass in grams M' and the total number of moles in the
alloy Nm. That is
A ave =
m1' + m 2'
M'
=
N
n
+ n
m
m1
64
m2
But using Equation (4.4) we may write
m1' = nm1 A 1
m2' = nm2 A 2
Which, when substituted into the above Aave expression yields
A ave =
n A + nm2 A 2
M'
= m1 1
n
+ n
Nm
m1
m2
Furthermore, from Equation (4.5)
( m1 +
C' n
1
nm1 =
n
m2
)
100
( m1 +
C' n
2
nm2 =
n
m2
)
100
Thus
(
C1' A 1 nm1 + nm2
100
A ave =
)+
n
m1
=
(
C2' A 2 nm1 + n m2
100
+ n
)
m2
C1' A1 + C 2' A 2
100
which is the desired result.
4.7 In order to compute composition, in atom percent, of a 92.5 wt% Ag-7.5 wt% Cu alloy, we employ
Equation (4.6) as
C 'Ag =
C AgA
C
A
Ag Cu
Cu
+C
65
A
Cu Ag
x 100
(92.5)(63.55 g / mol)
x 100
(92.5)(63.55 g/ mol) + (7.5)(107.87g / mol)
=
= 87.9 at%
'
=
CCu
C
C
A
Cu Ag
A
Ag Cu
+C
A
x 100
Cu Ag
(7.5)(107.87 g / mol)
x 100
(92.5)(63.55 g/ mol) + (7.5)(107.87g / mol)
=
= 12.1 at%
4.8 In order to compute composition, in weight percent, of a 5 at% Cu-95 at% Pt alloy, we employ
Equation (4.7) as
C' A
C Cu =
Cu Cu
C'
A
Cu Cu
=
+C' A
x 100
Pt Pt
(5)(63.55 g / mol)
x 100
(5)(63.55 g / mol) + (95)(195.08 g / mol)
= 1.68 wt%
C' A
CPt =
Pt Pt
C' A
Cu Cu
=
+ C' A
x 100
Pt Pt
(95)(195.08 g / mol)
x 100
(5)(63.55 g / mol) + (95)(195.08 g / mol)
= 98.32 wt%
4.9
The concentration, in weight percent, of an element in an alloy may be computed using a
modification of Equation (4.3). For this alloy, the concentration of iron (C ) is just
Fe
66
mFe
CFe =
=
mFe + mC + mCr
x 100
105 kg
x 100 = 98.87 wt%
105 kg + 0.2 kg + 1.0 kg
Similarly, for carbon
CC =
0.2 kg
x 100 = 0.19 wt%
105 kg + 0.2 kg + 1.0 kg
CCr =
1.0 kg
x 100 = 0.94 wt%
105 kg + 0.2 kg + 1.0 kg
And for chromium
4.10 The concentration of an element in an alloy, in atom percent, may be computed using Equation
(4.5). With this problem, it first becomes necessary to compute the number of moles of both Cu and
Zn, for which Equation (4.4) is employed. Thus, the number of moles of Cu is just
nm
m'
Cu
=
A
Cu
=
Cu
33 g
= 0.519 mol
63.55 g / mol
Likewise, for Zn
nm
=
Zn
47 g
= 0.719 mol
65.39 g / mol
Now, use of Equation (4.5) yields
n
'
C Cu
=
=
m
n
m
Cu
Cu
+n
x 100
m
Zn
0.519 mol
x 100 = 41.9 at%
0.519 mol + 0.719 mol
Also,
67
0.719 mol
x 100 = 58.1 at%
0.519 mol + 0.719 mol
'
C Zn
=
4.11 In this problem we are asked to determine the concentrations, in atom percent, of the Ag-Au-Cu
alloy. It is first necessary to convert the amounts of Ag, Au, and Cu into grams.
'
mAg
= (44.5 lbm )(453.6 g/lbm ) = 20,185 g
'
mAu
= (83.7 lbm )(453.6 g/lb m ) = 37,966 g
'
mCu
= (5.3 lbm )(453.6 g/lbm ) = 2,404 g
These masses must next be converted into moles [Equation (4.4)], as
nm
'
mAg
=
AAg
Ag
nm
=
37, 966 g
= 192.8 mol
196.97 g / mol
=
Au
nm
20,185 g
= 187.1 mol
107.87 g / mol
=
Cu
2,404 g
= 37.8 mol
63.55 g / mol
Now, employment of a modified form of Equation (4.5)
n
m
'
C Ag =
=
+n
n
m
Ag
Ag
m
+ n
Au
x 100
m
Cu
187.1 mol
x 100 = 44.8 at%
187.1 mol + 192.8 mol + 37.8 mol
C 'Au =
'
CCu
=
192.8 mol
x 100 = 46.2 at%
187.1 mol + 192.8 mol + 37.8 mol
37.8 mol
x 100 = 9.0 at%
187.1 mol + 192.8 mol + 37.8 mol
68
4.12 We are asked to compute the composition of an alloy in atom percent. Employment of Equation
'
CPb
=
=
CPb ASn
CPb ASn + CSn APb
x 100
5.5(118.69 g / mol)
x 100
5.5 (118.69 g / mol) + 94.5(207.2 g / mol)
= 3.2 at%
'
C Sn
=
=
CSn APb
C SnAPb + CPb ASn
x 100
94.5 (207.2 g / mol)
x 100
94.5(207.2 g / mol) + 5.5(118.69 g / mol)
= 96.8 at%
4.13 This problem calls for a conversion of composition in atom percent to composition in weight percent.
The composition in atom percent for Problem 4.11 is 44.8 at% Ag, 46.2 at% Au, and 9.0 at% Cu.
Modification of Equation (4.7) to take into account a three-component alloy leads to the following
C Ag =
' A
C Ag
Ag
C' A
Ag Ag
=
+ C' A
Au Au
+ C' A
x 100
Cu Cu
(44.8)(107.87 g / mol)
x 100
(44.8)(107.87 g / mol) + (46.2)(196.97 g / mol) + (9.0)(63.55 g / mol)
= 33.3 wt%
C Au =
=
' A
C Au
Au
' A
' A
' A
CAg
+ C Au
+ CCu
Ag
Au
Cu
x 100
(46.2)(196.97 g / mol)
x 100
(44.8)(107.87 g / mol) + (46.2)(196.97 g / mol) + (9.0)(63.55 g / mol)
69
= 62.7 wt%
CCu =
=
' A
C Cu
Cu
' A
' A
C 'AgAAg + C Au
+ CCu
Au
Cu
x 100
(9.0)(63.55 g / mol)
x 100
(44.8)(107.87 g / mol) + (46.2)(196.97 g / mol) + (9.0)(63.55 g / mol)
= 4.0 wt%
4.14 This problem calls for a determination of the number of atoms per cubic meter for aluminum. In
order to solve this problem, one must employ Equation (4.2),
N =
NA ρ Al
A
Al
3
The density of Al (from the table inside of the front cover) is 2.71 g/cm , while its atomic weight is
26.98 g/mol. Thus,
N =
(6.023
23
x 10
)(
atoms/ mol 2.71 g / cm
3
)
26.98 g / mol
= 6.05 x 1022 atoms/cm3 = 6.05 x 1028 atoms/m3
4.15 In order to compute the concentration in kg/m3 of Si in a 0.25 wt% Si-99.75 wt% Fe alloy we must
employ Equation (4.9) as
''
CSi
=
CSi
CSi
ρSi
+
CFe
x 103
ρFe
From inside the front cover, densities for silicon and iron are 2.33 and 7.87 g/cm3, respectively; and,
therefore
''
CSi
=
0.25
0.25
2.33 g / cm3
+
70
99.75
7.87 g / cm3
x 103
= 19.6 kg/m3
4.16 We are asked in this problem to determine the approximate density of a high-leaded brass that has
a composition of 64.5 wt% Cu, 33.5 wt% Zn, and 2 wt% Pb. In order to solve this problem, Equation
(4.10a) is modified to take the following form:
ρ ave =
C Cu
ρ Cu
100
C
Zn +
ρZn
+
CPb
ρPb
And, using the density values for Cu, Zn, and Pb that appear inside the front cover of the text, the
density is computed as follows:
ρ ave =
64.5 wt%
8.94 g / cm3
+
100
33.5 wt%
7.13 g / cm 3
+
2 wt%
11.35 g / cm3
= 8.27 g/cm3
4.17 This problem asks that we derive Equation (4.17), using other equations given in the chapter. The
concentration of component 1 in atom percent (C1' ) is just 100 c 1' where c 1' is the atom fraction of
component 1. Furthermore, c 1' is defined as c 1' = N1/N where N1 and N are, respectively, the
number of atoms of component 1 and total number of atoms per cubic centimeter. Thus, from the
above the following holds:
N1 =
C1' N
100
Substitution into this expression of the appropriate form of N from Equation (4.2) yields
N1 =
C1' N A ρave
100 A ave
71
Finally, substitution into this equation expressions for C1' [Equation (4.6a)], ρave [Equation (4.10a)],
Aave [Equation (4.11a)], realizing that C2 = (C1 - 100), and after some algebraic manipulation we
obtain the desired expression:
NA C1
N1 =
C1 A 1
ρ
+
1
A1
ρ
(100 −
2
C1
)
4.18 This problem asks us to determine the number of molybdenum atoms per cubic centimeter for a
16.4 wt% Mo-83.6 wt% W solid solution. To solve this problem, employment of Equation (4.17) is
necessary, using the following values:
C1 = CMo = 16.4 wt%
ρ1 = ρMo = 10.22 g/cm3
ρ2 = ρW = 19.3 g/cm3
A1 = AMo = 95.94 g/mol
Thus
NMo =
NA CMo
CMo A Mo
A Mo
+
ρ
ρ
Mo
=
(6.023
W
(100
− CMo
)
)
x 10 23 atoms/ mol (16.4)
(16.4)(95.94 g / mol)
(10.22 g / cm 3 )
+
95.94 g / mol
19.3 g / cm 3
(100
− 16.4 )
= 1.73 x 1022 atoms/cm3
4.19 This problem asks us to determine the number of niobium atoms per cubic centimeter for a 24 wt%
Nb-76 wt% V solid solution. To solve this problem, employment of Equation (4.17) is necessary,
using the following values:
C1 = CNb = 24 wt%
ρ1 = ρNb = 8.57 g/cm3
ρ2 = ρV = 6.10 g/cm3
72
A1 = ANb = 92.91 g/mol
Thus
NNb =
=
NACNb
CNb ANb
ANb
+
100 − CNb
ρNb
ρV
(
(6.023 x 1023
(24)(92.91 g / mol)
(8.57 g / cm 3 )
)
atoms / mol (24)
92.91 g / mol
+
)
6.10 g / cm3
(100
− 24)
= 1.02 x 1022 atoms/cm3
4.20 This problem asks that we derive Equation (4.18), using other equations given in the chapter. The
number of atoms of component 1 per cubic centimeter is just equal to the atom fraction of
component 1 (c 1' ) times the total number of atoms per cubic centimeter in the alloy (N). Thus,
using the equivalent of Equation (4.2), we may write
c1' NA ρave
N1 = c1' N =
A ave
Realizing that
c1' =
C1'
100
and
C '2 = 100 − C1'
and substitution of the expressions for ρave and Aave, Equations (4.10b) and (4.11b) leads to
N1 =
c1' N Aρ ave
Aave
73
=
N AC1' ρ1 ρ 2
⎞
⎛
C1' ρ2 A1 + ⎜100 − C1' ⎟ ρ1A 2
⎠
⎝
And, solving for C1'
C1' =
100 N ρ A
1 1 2
NAρ1 ρ2 − N1ρ 2 A 1 + N1 ρ1 A 2
Substitution of this expression for C1' into Equation (4.7a)
C1 =
C' A
1 1
'
1 1 + C 2A 2
C' A
C' A
1 1
=
⎛
⎞
'
1 1 + 100⎜⎝ 1 − C1⎟⎠ A 2
C' A
yields
C1 =
1+
100
NA ρ 2
N1 A1
−
ρ2
ρ1
the desired expression.
4.21 This problem asks us to determine the weight percent of Au that must be added to Ag such that the
resultant alloy will contain 5.5 x 1021 Au atoms per cubic centimeter. To solve this problem,
employment of Equation (4.18) is necessary, using the following values:
N1 = NAu = 5.5 x 1021 atoms/cm3
ρ1 = ρAu = 19.32 g/cm3
ρ2 = ρAg = 10.49 g/cm3
A1 = AAu = 196.97 g/mol
A2 = Ag = 107.87 g/mol
74
Thus
C Au =
1+
100
NAρ Ag
N
A
−
Au Au
=
1+
(6.023
ρ Ag
ρ
Au
100
)
x 10 23 atoms / mol (10.49 g / cm3 )
(5.5 x 10 21 atoms / cm3 )(196.97 g / mol)
⎛ 10.49 g / cm 3 ⎞
− ⎜
⎟
⎜
3⎟
⎝ 19.32 g / cm ⎠
= 15.9 wt%
4.22 This problem asks us to determine the weight percent of Ge that must be added to Si such that the
resultant alloy will contain 2.43 x1021 Ge atoms per cubic centimeter. To solve this problem,
employment of Equation (4.18) is necessary, using the following values:
N1 = NGe = 2.43 x 1021 atoms/cm3
ρ1 = ρGe = 5.32 g/cm3
ρ2 = ρSi = 2.33 g/cm3
A1 = AGe = 72.59 g/mol
A2 = ASi = 28.09 g/mol
Thus
C Ge =
1+
100
N Aρ Si
N GeA Ge
−
ρSi
ρ Ge
100
=
(6.023 x10 atoms/ mol)(2.33 g / cm 3 ) − ⎛⎜ 2.33 g/ cm 3 ⎞⎟
(2.43 x10 21 atoms / cm3 )(72.59 g / mol) ⎜⎝ 5.32 g/ cm 3 ⎟⎠
23
1+
= 11.7 wt%
4.23 This problems asks that we compute the unit cell edge length for a 95 wt% Pt-5 wt% Cu alloy. First
of all, the atomic radii for Cu and Pt (Table 3.1) are 0.1278 and 0.1387 nm, respectively. Also, using
75
Equation (3.5) it is possible to compute the unit cell volume, and inasmuch as the unit cell is cubic,
the unit cell edge length is just the cube root of the volume. However, it is first necessary to
calculate the density and atomic weight of this alloy using Equations (4.10a) and (4.11a). For the
density
ρ ave =
100
C Cu
ρ Cu
=
CPt
+
ρPt
100
5 wt%
8.94 g / cm3
+
95 wt%
21.45 g / cm 3
= 20.05 g/cm3
And for the atomic weight
Aave =
100
C Cu
A Cu
=
+
CPt
APt
100
5 wt%
95 wt%
+
63.55 g / mole
195.08 g / mol
= 176.79 g/mol
Now, VC is determined from Equation (3.5) as
VC =
=
nA ave
ρave NA
(4 atoms / unitcell)(176.79 g / mol)
(20.05 g / cm 3 )(6.023 x1023
= 5.856 x 10-23 cm3/unit cell
And, finally
76
)
atoms / mol
( )
a = VC
(
= 5.856x10
− 23
1/ 3
3
cm /unit cell
)
1/3
= 3.883 x 10-8 cm = 0.3883 nm
4.24 The Burgers vector and dislocation line are perpendicular for edge dislocations, parallel for screw
dislocations, and neither perpendicular nor parallel for mixed dislocations.
4.25 (a) The Burgers vector will point in that direction having the highest linear density. From Section
3.11, the linear density for the  direction in FCC is 1/2R, the maximum possible; therefore for
FCC
b =
a

2
From Problem 3.46 the linear density for the  direction in BCC is also 1/2R, and
therefore for BCC
b =
a

2
For simple cubic, a unit cell of which is shown in Figure 3.19, the atom spheres touch one
another along the cube edges (i.e., in  directions) and therefore, the atomic packing is greatest
in these directions. Therefore, the Burgers vector is
b =
a

2
(b) For Cu which has an FCC crystal structure, R = 0.1278 nm (Table 3.1) and a = 2R 2 =
0.3615 nm [Equation (3.1)]; therefore
b =
=
0.3615 nm
2
a
2
h 2 + k 2 + l2
(1 )2 + (1 )2 + (0) 2 = 0.2556 nm
77
For Fe which has a BCC crystal structure, R = 0.1241 nm (Table 3.1) and a =
4R
= 0.2866
3
nm [Equation (3.3)]; hence
b =
0.2866 nm
2
(1) 2 + (1) 2 + (1) 2 = 0.2482 nm
4.26 (a) The surface energy of a single crystal depends on crystallographic orientation because the
atomic packing is different for the various crystallographic planes, and, therefore, the number of
unsatisfied bonds will vary from plane to plane.
(b) The surface energy will be greater for an FCC (100) plane than for a (111) plane because the
(111) plane is more densely packed (i.e., has more nearest neighbor atoms in the plane)—see
Problem 3.47; as a consequence, more atomic bonds will be satisfied for the (111) plane, giving rise
to a lower surface energy.
4.27 (a) The surface energy will be greater than the grain boundary energy since some atoms on one
side of the boundary will bond to atoms on the other side--i.e., there will be fewer unsatisfied bonds
along a grain boundary.
(b) The small angle grain boundary energy is lower than for a high angle one because more atoms
bond across the boundary for the small angle, and, thus, there are fewer unsatisfied bonds.
4.28 (a) A twin boundary is an interface such that atoms on one side are located at mirror image
positions of those atoms situated on the other boundary side. The region on one side of this
boundary is called a twin.
(b) Mechanical twins are produced as a result of mechanical deformation and generally occur in
BCC and HCP metals. Annealing twins form during annealing heat treatments, most often in FCC
metals.
4.29 (a) The interfacial defect that exists for this stacking sequence is a twin boundary, which occurs at
the following position
78
The stacking sequence on one side of this position is mirrored on the other side.
(b) The interfacial defect that exists within this FCC stacking sequence is a stacking fault, which
occurs over the region indicated
For this region, the BCBC stacking sequence is HCP.
4.30
(a) This problem calls for a determination of the average grain size of the specimen which
microstructure is shown in Figure 4.12b. Seven line segments were drawn across the micrograph,
each of which was 60 mm long. The average number of grain boundary intersections for these lines
was 8.7. Therefore, the average line length intersected is just
60 mm
= 6.9 mm
8.7
Hence, the average grain diameter, d, is
d =
ave. line length int er sec ted
6.9 mm
=
= 6.9 x 10 −2 mm
magnification
100
(b) This portion of the problem calls for us to estimate the ASTM grain size number for this same
material. The average grain size number, n, is related to the number of grains per square inch, N, at
a magnification of 100x according to Equation 4.16. Inasmuch as the magnification is 100x, the
value of N is measured directly from the micrgraph, which is approximately 12 grains. Rearranging
Equation 4.16 and solving for n leads to
n=
=
log N
+1
log 2
log 12
+ 1 = 4.6
log 2
4.31 (a) This portion of the problem calls for a determination of the average grain size of the specimen
which microstructure is shown in Figure 9.22a.
79
Seven line segments were drawn across the
micrograph, each of which was 60 mm long. The average number of grain boundary intersections
for these lines was 6.3. Therefore, the average line length intersected is just
60 mm
= 9.5 mm
6.3
Hence, the average grain diameter, d, is
d =
ave. line length int er sec ted
9.5 mm
=
= 0.106 mm
magnification
90
(b) This portion of the problem calls for us to estimate the ASTM grain size number for this same
material. The average grain size number, n, is related to the number of grains per square inch, N, at
a magnification of 100x according to Equation 4.16. However, the magnification of this micrograph is
not 100x, but rather 90x. Consequently, it is necessary to use the following equation:
2
⎛ M ⎞
n−1
⎟ =2
NM ⎜
⎝ 100 ⎠
where NM = the number of grains per square inch at magnification M, and n is the ASTM grain size
number. (The above equation makes use of the fact that, while magnification is a length parameter,
area is expressed in terms of units of length squared. As a consequence, the number of grains per
unit area increases with the square of the increase in magnification.) Solving the above expression
⎛ M ⎞
⎟
log NM + 2 log ⎜
⎝ 100⎠
n=
+1
log 2
From Figure 9.22a, NM is measured to be approximately 4, which leads to
⎛ 90 ⎞
⎟
log 4 + 2 log ⎜
⎝ 100⎠
n=
+1
log 2
= 2.7
80
4.32 (a) This part of problem asks that we compute the number of grains per square inch for an ASTM
grain size of 6 at a magnification of 100x. All we need do is solve for the parameter N in Equation
4.16, inasmuch as n = 6. Thus
N = 2 n− 1
=2
6 −1
= 32 grains/in.2
(b) Now it is necessary to compute the value of N for no magnification. In order to solve this
problem it is necessary to use the following equation:
2
⎛ M ⎞
n−1
⎟ =2
NM ⎜
⎝ 100 ⎠
where NM = the number of grains per square inch at magnification M, and n is the ASTM grain size
number. (The above equation makes use of the fact that, while magnification is a length parameter,
area is expressed in terms of units of length squared. As a consequence, the number of grains per
unit area increases with the square of the increase in magnification.) Without any magnification, M
in the above equation is 1, and therefore,
2
⎛ 1 ⎞
6 −1
⎟ =2
N1 ⎜
= 32
⎝ 100⎠
And, solving for N1, N1 = 320,000 grains/in.2.
4.33 This problem asks that we determine the ASTM grain size number if 30 grains per square inch are
measured at a magnification of 250. In order to solve this problem we make use of the equation
cited in Problem 4.31b—i.e.,
2
⎛ M ⎞
n−1
⎟ =2
NM ⎜
⎝ 100 ⎠
where NM = the number of grains per square inch at magnification M, and n is the ASTM grain size
number. Solving the above equation for n, and realizing that NM = 30, while M = 250, we have
81
⎛ M ⎞
⎟
log NM + 2 log ⎜
⎝ 100⎠
n=
+1
log 2
⎛ 250 ⎞
⎟
log 30 + 2 log ⎜
⎝ 100 ⎠
=
+ 1 = 2.5
log 2
4.34 This problem asks that we determine the ASTM grain size number if 25 grains per square inch are
measured at a magnification of 75. In order to solve this problem we make use of the equation cited
in Problem 4.31b—i.e.,
2
⎛ M ⎞
n−1
⎟ =2
NM ⎜
⎝ 100 ⎠
where NM = the number of grains per square inch at magnification M, and n is the ASTM grain size
number. Solving the above equation for n, and realizing that NM = 25, while M = 75, we have
⎛ M ⎞
log NM + 2 log ⎜
⎟
⎝ 100⎠
+1
n=
log 2
⎛ 75 ⎞
⎟
log 25 + 2 log ⎜
⎝ 100 ⎠
=
+ 1 = 4.8
log 2
Design Problems
4.D1 This problem calls for us to compute the concentration of lithium (in wt%) that, when added to
aluminum, will yield an alloy having a density of 2.55 g/cm3. Solution of this problem requires the
use of Equation (4.10a), which takes the form
ρ ave =
CLi
ρ Li
+
100
100 − CLi
ρ Al
inasmuch as CLi + CAl = 100. According to the table inside the front cover, the respective densities
of Li and Al are 0.534 and 2.71 g/cm3. Upon solving for C from the above equation
Li
82
(
ρave (ρ Al −
100 ρ Li ρAl − ρ ave
CLi =
(
(100) 0.534 g / cm
=
(
3
ρLi
)
)(2.71 g / cm3 −
)
2.55 g / cm
2.55 g/ cm3 2.71 g / cm3 − 0.534 g / cm3
)
3
)
= 1.537 wt%
4.D2 This problem asks that we determine the concentration (in weight percent) of V that must be added
to Fe so as to yield a unit cell edge length of 0.289 nm. To begin, it is necessary to employ Equation
(3.5), and solve for the unit cell volume, VC, as
nA ave
VC =
ρave NA
where Aave and ρave are the atomic weight and density, respectively, of the Fe-V alloy. Inasmuch
as both of these materials have the BCC crystal structure, which has cubic symmetry, VC is just the
cube of the unit cell length, a. That is
VC = a3 = (0.289 nm)3
(2.89 x 10 −8 cm) = 2.414 x 10−23 cm 3
3
It is now necessary to construct expressions for Aave and ρave in terms of the concentration of
vanadium, CV using Equations (4.11a) and (4.10a). For Aave we have
Aave =
=
100
CV
(100 − C V )
+
AFe
AV
100
CV
50.94 g / mol
+
whereas for ρave
83
(100 − CV )
55.85 g / mol
ρ ave =
=
100
(100 − C V )
+
ρFe
ρV
CV
100
CV
6.10 g / cm 3
+
(100 − C V )
7.87 g / cm 3
Within the BCC unit cell there are 2 equivalent atoms, and thus, the value of n in Equation (3.5) is 2;
hence, this expression may be written in terms of the concentration of V in weight percent as follows:
VC = 2.414 x 10-23 cm3
=
nAave
ρaveN A
⎡
⎤
⎢
⎥
100
⎥
(2 atoms / unit cell) ⎢
CV
(100 − CV ) ⎥
⎢
+
⎢
⎥
55.85 g/ mol ⎦
⎣ 50.94 g / mol
=
⎡
⎤
⎢
⎥
100
23
⎢
⎥
atoms / mol
6.023 x 10
⎢
(100 − C V ) ⎥
CV
+
⎢
⎥
7.87 g / cm3 ⎥⎦
⎢⎣ 6.10 g / cm3
(
And solving this expression for CV leads to CV = 12.9 wt%.
84
)
CHAPTER 5
DIFFUSION
PROBLEM SOLUTIONS
5.1 Self-diffusion is atomic migration in pure metals--i.e., when all atoms exchanging positions are of the
same type. Interdiffusion is diffusion of atoms of one metal into another metal.
5.2 Self-diffusion may be monitored by using radioactive isotopes of the metal being studied. The motion
of these isotopic atoms may be monitored by measurement of radioactivity level.
5.3 (a) With vacancy diffusion, atomic motion is from one lattice site to an adjacent vacancy. Selfdiffusion and the diffusion of substitutional impurities proceed via this mechanism. On the other
hand, atomic motion is from interstitial site to adjacent interstitial site for the interstitial diffusion
mechanism.
(b) Interstitial diffusion is normally more rapid than vacancy diffusion because: (1) interstitial atoms,
being smaller, are more mobile; and (2) the probability of an empty adjacent interstitial site is greater
than for a vacancy adjacent to a host (or substitutional impurity) atom.
5.4 Steady-state diffusion is the situation wherein the rate of diffusion into a given system is just equal to
the rate of diffusion out, such that there is no net accumulation or depletion of diffusing species--i.e.,
the diffusion flux is independent of time.
5.5 (a) The driving force is that which compels a reaction to occur.
5.6 This problem calls for the mass of hydrogen, per hour, that diffuses through a Pd sheet. It first
becomes necessary to employ both Equations (5.1a) and (5.3). Combining these expressions and
solving for the mass yields
M = JAt = − DAt
ΔC
Δx
⎡ 0.6 − 2.4 kg / m 3 ⎤
= − 1.0 x 10-8 m2 /s 0.2 m2 (3600 s/h) ⎢
⎥
⎢⎣ 5 x 10 −3 m ⎦⎥
(
)(
)
85
= 2.6 x 10-3 kg/h
3
5.7 We are asked to determine the position at which the nitrogen concentration is 2 kg/m . This problem
is solved by using Equation (5.3) in the form
C − C
B
J = − D A
x − x
A
B
3
If we take C to be the point at which the concentration of nitrogen is 4 kg/m , then it becomes
A
necessary to solve for x , as
B
⎡ C − CB ⎤
xB = x A + D ⎢ A
⎥
J
⎣
⎦
Assume x is zero at the surface, in which case
A
(
-11
xB = 0 + 6 x 10
)(
⎡ 4 kg / m3 − 2 kg / m3
⎢
m /s ⎢
−7 kg / m2 - s
⎢⎣ 1.2 x 10
2
)⎤⎥
⎥
⎦⎥
= 1 x 10-3 m = 1 mm
5.8 This problem calls for computation of the diffusion coefficient for a steady-state diffusion situation.
Let us first convert the carbon concentrations from wt% to kg C/m3 using Equation (4.9a). For 0.012
wt% C
''
CC
=
CC
CC
ρC
=
3
CFe
+
x 10
ρ Fe
0.012
0.012
2.25 g / cm3
+
99.988
7.87 g / cm3
0.944 kg C/m3
86
x 10 3
Similarly, for 0.0075 wt% C
0.0075
''
CC
=
0.0075
2.25 g / cm3
+
99.9925
x 103
7.87 g/ cm3
= 0.590 kg C/m3
Now, using a form of Equation (5.3)
⎡ x − xB ⎤
D = − J ⎢ A
⎥
⎢⎣C A − CB ⎥⎦
−3
⎡
⎤
− 10
m
= − 1.40 x 10-8 kg/m2 - s ⎢
⎥
3
3
⎢⎣0.944 kg / m − 0.590 kg / m ⎥⎦
(
)
= 3.95 x 10-11 m2/s
5.9 This problems asks for us to compute the diffusion flux of hydrogen gas through a 1-mm thick plate of
iron at 250&deg;C when the pressures on the two sides are 0.15 and 7.5 MPa. Ultimately we will employ
Equation (5.3) to solve this problem.
However, it first becomes necessary to determine the
concentration of hydrogen at each face using Equation (5.11). At the low pressure (or B) side
(
CH(B) = 1.34 x 10-2
27, 200 J / mol
⎤
) 0.15 MPa exp ⎢⎣⎡− (8.31 J / molK)(250 + 273 K) ⎥⎦
9.93 x 10-6 wt%
Whereas, for the high pressure (or A) side
(
CH(A) = 1.34 x 10-2
) 7.5
⎡
27,200 J/ mol
⎤
MPa exp ⎢−
⎣ (8.31 J/ mol- K)(250 + 273 K) ⎥⎦
7.02 x 10-5 wt%
87
We now convert concentrations in weight percent to mass of hydrogen per unit volume of solid. At
face B there are 9.93 x 10-6 g (or 9.93 x 10-9 kg) of hydrogen in 100 g of Fe, which is virtually pure
iron. From the density of iron (7.87 g/cm3), the volume iron in 100 g (VB) is just
VB =
100 g
7.87 g / cm 3
= 12.7 cm3 = 1.27 x 10-5 m3
Therefore, the concentration of hydrogen at the B face in kilograms of H per cubic meter of alloy
''
] is just
[ CH(B)
''
CH(B)
=
=
9.93 x 10−9 kg
1.27 x 10−5 m3
C
H(B)
V
B
-4
= 7.82 x 10
kg/m
3
At the A face the volume of iron in 100 g (VA) will also be 1.27 x 10-5 m3, and
''
CH(A)
=
=
7.02 x 10−8 kg
1.27 x 10−5 m3
C
H(A )
V
A
-3
= 5.53 x 10
3
kg/m
Thus, the concentration gradient is just the difference between these concentrations of hydrogen
divided by the thickness of the iron membrane; that is
− C ''
C ''
ΔC
H(B)
H(A)
=
Δx
x − x
B
=
A
7.82 x 10 −4 kg / m3 − 5.53 x 10−3 kg / m 3
10 −3 m
= − 4.75 kg/m4
At this time it becomes necessary to calculate the value of the diffusion coefficient at 250&deg;C using
Equation (5.8). Thus,
88
⎛ Q ⎞
D = D o exp ⎜ − o ⎟
⎝ RT ⎠
(
= 1.4 x 10
)
⎛
⎞
13, 400 J / mol
2
m / s exp ⎜ −
⎟
(8.31
J
/
mol
−
K)(250
+
273
K)
⎝
⎠
−7
= 6.41 x 10-9 m2/s
And, finally, the diffusion flux is computed using Equation (5.3) by taking the negative product of this
diffusion coefficient and the concentration gradient, as
J =−D
(
-9
= − 6.41 x 10
2
ΔC
Δx
)(
4
m /s − 4.75 kg/m
)= 3.05 x 10-8 kg/m2 - s
5.10 It can be shown that
⎛ x2 ⎞
⎟⎟
exp − ⎜⎜
Dt
⎝ 4 Dt ⎠
B
Cx =
is a solution to
∂C
∂2C
= D 2
∂t
∂x
simply by taking appropriate derivatives of the C expression. When this is carried out,
x
2
∂C
∂ C
B
= D
=
2
1/
∂t
2 D 2t 3 / 2
∂x
5.11
⎛ x2
⎞
− 1⎟⎟ exp
⎜⎜
⎝ 2 Dt
⎠
⎛ x2 ⎞
⎜⎜ −
⎟⎟
⎝ 4Dt ⎠
We are asked to compute the diffusion time required for a specific nonsteady-state diffusion
situation. It is first necessary to use Equation (5.5).
⎛ x ⎞
= 1 − erf ⎜
⎟
C −C
⎝ 2 Dt ⎠
s
o
C x − Co
89
-3
wherein, C = 0.45, C = 0.20, C = 1.30, and x = 2 mm = 2 x 10 m. Thus,
x
o
s
C x − Co
C −C
s
o
=
⎛ x ⎞
0.45 − 0.20
= 0.2273 = 1 − erf ⎜
⎟
1.30 − 0.20
⎝ 2 Dt ⎠
or
⎛ x ⎞
erf ⎜
⎟ = 1 − 0.2273 = 0.7727
⎝ 2 Dt ⎠
By linear interpolation from Table 5.1
z
erf(z)
0.85
0.7707
z
0.7727
0.90
0.7970
z − 0.850
0.7727 − 0.7707
=
0.900 − 0.850 0.7970 − 0.7707
From which
z = 0.854 =
x
2 Dt
Now, from Table 5.2, at 1000&deg;C (1273 K)
(
)
⎡
⎤
148, 000 J/ mol
D = 2.3 x 10-5 m2 /s exp ⎢−
⎥
⎣ (8.31 J / mol-K)(1273 K) ⎦
-11 2
= 1.93 x 10
m /s
Thus,
0.854 =
(
2 x 10−3 m
)
(2) 1.93x10−11 m2 / s (t)
90
Solving for t yields
4
t = 7.1 x 10 s = 19.7 h
5.12 This problem asks that we determine the position at which the carbon concentration is 0.25 wt%
after a 10-h heat treatment at 1325 K when Co = 0.55 wt% C. From Equation (5.5)
C x − Co
C −C
s
o
=
⎛ x ⎞
0.25 − 0.55
= 0.5455 = 1 − erf ⎜
⎟
0 − 0.55
⎝ 2 Dt ⎠
Thus,
⎛ x ⎞
erf ⎜
⎟ = 0.4545
⎝ 2 Dt ⎠
Using data in Table 5.1 and linear interpolation
z
erf (z)
0.40
0.4284
z
0.4545
0.45
0.4755
z − 0.40
0.4545 − 0.4284
=
0.45 − 0.40 0.4755 − 0.4284
And,
z = 0.4277
Which means that
x
2 Dt
= 0.4277
And, finally
x = 2(0.4277) Dt = (0.8554)
(4.3 x 10−11 m2 / s)(3.6 x 104 s )
= 1.06 x 10-3 m = 1.06 mm
91
5.13 This problem asks us to compute the nitrogen concentration (C ) at the 1 mm position after a 10 h
x
diffusion time, when diffusion is nonsteady- state. From Equation (5.5)
C x − Co
C −C
s
⎛ x ⎞
= 1 − erf ⎜
⎟
0.1 − 0
⎝ 2 Dt ⎠
Cx − 0
=
o
⎡
⎢
= 1 − erf ⎢
⎢ (2)
⎣
⎤
⎥
⎥
−11 2
2.5 x 10
m / s (10 h)(3600 s / h) ⎥
⎦
−3
10
(
m
)
= 1 - erf (0.527)
Using data in Table 5.1 and linear interpolation
z
erf (z)
0.500
0.5205
0.527
y
0.550
0.5633
0.527 − 0.500
y − 0.5205
=
0.550 − 0.500
0.5633 − 0.5205
from which
y = erf (0.527) = 0.5436
Thus,
Cx − 0
0.1 − 0
= 1.0 − 0.5436
This expression gives
C = 0.046 wt% N
x
5.14 (a) The solution to Fick's second law for a diffusion couple composed of two semi-infinite solids of
the same material is as follows:
92
⎛ C1 + C 2 ⎞
⎛ C1 − C2 ⎞ ⎛ x ⎞
Cx = ⎜
⎟
⎟ − ⎜
⎟ erf ⎜
2
2
⎠
⎠ ⎝ 2 Dt ⎠
⎝
⎝
for the boundary conditions
C = C1 for x &lt; 0, and t = 0
C = C2 for x &gt; 0, and t = 0
(b) For this particular silver-gold diffusion couple for which C1 = 5 wt% Au and C2 = 2 wt% Au, we
are asked to determine the diffusion time at 750&deg;C that will give a composition of 2.5 wt% Au at the
50 μm position. Thus, the equation in part (a) takes the form
⎛ 50 x 10 −6 m ⎞
⎛ 5 + 2⎞
⎛ 5 − 2⎞
2.5 = ⎜
⎟ − ⎜
⎟ erf ⎜⎜
⎟⎟
⎝ 2 ⎠
⎝ 2 ⎠
2 Dt
⎝
⎠
It now becomes necessary to compute the diffusion coefficient at 750&deg;C (1023 K) given that Do = 8.5
x 10-5 m2/s and Qd = 202,100 J/mol. From Equation (5.8) we have
⎛ Q ⎞
D = D oexp ⎜ − d ⎟
⎝ RT ⎠
(
-5
= 8.5 x 10
)
⎤
⎡
202,100 J / mol
2
m /s exp⎢−
⎥
⎣ (8.31J / mol − K)(1023 K) ⎦
= 4.03 x 10-15 m2/s
Substitution of this value into the above equation leads to
⎡
⎢
5
+
2
5
−
2
⎛
⎞
⎛
⎞
2.5 = ⎜
⎟ − ⎜
⎟ erf ⎢
⎝ 2 ⎠
⎝ 2 ⎠
⎢2
⎣
This expression reduces to the following form:
93
⎤
⎥
⎥
−15 2
4.03 x 10
m / s (t) ⎥
⎦
−6
(
50 x 10
m
)
⎛ 393.8 s ⎞
0.6667 = erf ⎜
⎟
t
⎝
⎠
Using data in Table 5.1 and linear interpolation
z
erf (z)
0.650
0.6420
y
0.6667
0.700
0.6778
y − 0.650
0.6667 − 0.6420
=
0.700 − 0.650
0.6778 − 0.6420
from which
y = 0.6844 =
393.8 s
t
And, solving for t gives
t = 3.31 x 105 s = 92 h
5.15 This problem calls for an estimate of the time necessary to achieve a carbon concentration of 0.45
wt% at a point 5 mm from the surface. From Equation (5.6b),
x2
= constant
Dt
But since the temperature is constant, so also is D constant, and
x2
= constant
t
or
x12
t1
=
Thus,
94
x2
2
t2
(2.5 mm)2
(5.0 mm) 2
=
10 h
t
2
from which
t = 40 h
2
5.16 We are asked to compute the diffusion coefficients of C in both α and γ iron at 900&deg;C. Using the
data in Table 5.2,
(
)
80,000 J/ mol
⎡
⎤
Dα = 6.2 x 10-7 m 2/s exp ⎢−
⎥⎦
(8.31
J/
mol
-K)(1173
K)
⎣
-10 2
= 1.69 x 10
m /s
(
)
148, 000 J/ mol
⎡
⎤
Dγ = 2.3 x 10-5 m2/s exp ⎢−
⎣ (8.31 J/ mol -K)(1173 K) ⎦⎥
-12 2
= 5.86 x 10
m /s
The D for diffusion of C in BCC α iron is larger, the reason being that the atomic packing
factor is smaller than for FCC γ iron (0.68 versus 0.74); this means that there is slightly more
interstitial void space in the BCC Fe, and, therefore, the motion of the interstitial carbon atoms
occurs more easily.
5.17 This problem asks us to compute the magnitude of D for the diffusion of Zn in Cu at 650&deg;C (923 K).
From Table 5.2
(
)
189,000 J/ mol
⎡
⎤
D = 2.4 x 10-5 m2 /s exp ⎢−
⎥
(8.31
J/
molK)(923
K)
⎦
⎣
-16 2
= 4.8 x 10
m /s
5.18 We are asked to calculate the temperature at which the diffusion coefficient for the diffusion of Cu in
-17 2
Ni has a value of 6.5 x 10
m /s. Solving for T from Equation (5.9a)
95
T = −
(
Qd
R ln D − ln D
o
)
and using the data from Table 5.2 for the diffusion of Cu in Ni
T = −
256,000 J/mol
⎡
(8.31 J/mol -K) ln 6.5 x 10-17 − ln 2.7 x 10 -5 ⎤
⎣
⎦
(
)
(
)
= 1152 K = 879&deg;C
5.19 For this problem we are given Do and Qd for the diffusion of Cr in Ni, and asked to compute the
temperature at which D = 1.2 x 10-14 m2/s. Solving for T from Equation (5.9a) yields
T =
=
Qd
(
)
R ln D o − ln D
272,000 J/mol
(
(8.31 J/mol - K)⎡ln 1.1 x 10 -4
⎣
) - ln (1.2 x 10-14 )⎤⎦
= 1427 K = 1154&deg;C
5.20 In this problem we are given Qd for the diffusion of Cu in Ag (i.e., 193,000 J/mol) and asked to
compute D at 1200 K given that the value of D at 1000 K is 1.0 x 10-14 m2/s. It first becomes
necessary to solve for Do from Equation (5.8) as
⎛Q ⎞
Do = D exp ⎜ d ⎟
⎝ RT ⎠
(
= 1.0 x 10
-14
)
⎤
⎡
193, 000 J / mol
2
m /s exp ⎢
⎥
(8.31
J
/
mol
K)(1000
K)
⎦
⎣
= 1.22 x 10-4 m2/s
Now, solving for D at 1200 K gives
96
(
D = 1.22 x 10
-4
)
⎤
⎡
193, 000 J / mol
2
m /s exp ⎢−
⎥
⎣ (8.31 J / mol - K)(1200 K) ⎦
= 4.8 x 10-13 m2/s
5.21 (a) Using Equation (5.9a), we set up two simultaneous equations with Q and D as unknowns.
d
o
-16
Solving for Q in terms of temperatures T and T (1273 K and 1473 K) and D and D (9.4 x 10
d
1
2
1
2
and 2.4 x 10 14 m2/s), we get
Qd = − R
ln D1 − ln D2
1
1
−
T1
T2
(
)
(
)
-16
-14 ⎤
− ln 2.4 x 10
(8.31 J/mol- K)⎣⎡ln 9.4 x 10
⎦
= −
1
1
−
1473 K
1273 K
= 252,400 J/mol
Now, solving for D from Equation (5.8)
o
⎛Q ⎞
Do = D1exp ⎜⎜ d ⎟⎟
⎝ RT1⎠
(
-16
= 9.4 x 10
)
⎤
⎡
252, 400 J / mol
2
m /s exp ⎢
⎥
(8.31
J
/
mol
K)(1273
K)
⎦
⎣
-5 2
= 2.2 x 10 m /s
(b) Using these values of D and Q , D at 1373 K is just
o
d
(
-5
D = 2.2 x 10
)
⎤
⎡
252,400 J / mol
2
m /s exp ⎢ −
⎥
⎣ (8.31 J / mol - K)(1373 K) ⎦
-15 2
= 5.4 x 10
m /s
97
5.22 (a) Using Equation (5.9a), we set up two simultaneous equations with Q and D as unknowns.
d
o
Solving for Q in terms of temperatures T and T (873 K [600&deg;C] and 973 K [700&deg;C]) and D and
d
1
2
1
-14
-13 2
m /s), we get
D (5.5 x 10
and 3.9 x 10
2
Qd = − R
ln D1 − ln D2
1
1
−
T1 T2
(
)
(
)
-14
-13 ⎤
− ln 3.9 x 10
(8.31 J/mol - K)⎣⎡ln 5.5 x 10
⎦
= −
1
1
−
973 K
873 K
= 138,300 J/mol
Now, solving for D from Equation (5.8)
o
⎛Q ⎞
Do = D1exp ⎜⎜ d ⎟⎟
⎝ RT1⎠
(
-14
= 5.5 x 10
)
⎤
⎡
138,300 J / mol
2
m /s exp ⎢
⎥
(8.31
J
/
mol
K)(873
K)
⎦
⎣
-5 2
= 1.05 x 10 m /s
(b) Using these values of D and Q , D at 1123 K (850&deg;C) is just
o
d
(
D = 1.05 x 10
-5
)
⎤
⎡
138, 300 J / mol
2
m /s exp ⎢−
⎥
⎣ (8.31 J / mol - K)(1123 K) ⎦
-12 2
= 3.8 x 10
m /s
5.23 This problem asks us to determine the values of Qd and Do for the diffusion of Au in Ag from the
plot of log D versus 1/T. According to Equation (5.9b) the slope of this plot is equal to - Qd/2.3R
(rather than - Qd/R since we are using log D rather than ln D) and the intercept at 1/T = 0 gives the
value of log Do. The slope is equal to
98
slope =
log D1 − log D 2
Δ (log D)
=
1
1
⎛ 1⎞
−
Δ⎜ ⎟
T2
T1
⎝ T⎠
Taking 1/T1 and 1/T2 as 1.0 x 10-3 and 0.90 x 10-3 K-1, respectively, then the values of log D1 and
log D2 are –14.68 and –13.57, respectively. Therefore,
Qd = − 2.3 R
Δ(log D)
⎛ 1⎞
Δ⎜ ⎟
⎝ T⎠
⎡
⎤
-14.68 − (-13.57)
⎢
⎥
= − (2.3)(8.31 J/mol - K) ⎢
−
3
−
3
−
1
− 0.90 x 10
K ⎥⎥
⎢⎣ 1.0 x 10
⎦
(
)
= 212,200 J/mol
Rather than trying to make a graphical extrapolation to determine Do, a more accurate value is
obtained analytically using Equation (5.9b) taking a specific value of both D and T (from 1/T) from
the plot given in the problem; for example, D = 1.0 x 10-14 m2/s at T = 1064 K (1/T = 0.94 x 10-3).
Therefore
⎛Q ⎞
Do = D exp ⎜ d ⎟
⎝ RT ⎠
(
= 1.0 x 10
-14
)
⎤
⎡
212,200 J / mol
2
m /s exp ⎢
⎥
⎣(8.31 J / mol - K)(1064 K) ⎦
= 2.65 x 10-4 m2/s
5.24
This problem asks that we compute the temperature at which the diffusion flux is 6.3 x 10-10
kg/m2-s. Combining Equations (5.3) and (5.8) yields
⎛ Q ⎞
ΔC
J = − Do
exp ⎜ − d ⎟
Δx
⎝ RT ⎠
Solving for T from this expression leads to
99
⎛ Qd ⎞
T = ⎜
⎟
⎝ R ⎠
⎛ 80, 000 J / mol ⎞
⎟
= ⎜
⎝ 8.31 J / mol- K ⎠
1
⎛ Do ΔC ⎞
ln ⎜ −
⎟
⎝ JΔx ⎠
1
(
(
)(
)⎤⎥
)⎥⎥⎦
⎡ 6.2 x 10 −7 m 2 / s 0.45 kg / m3
ln ⎢⎢
−10
kg / m 2 - s 10 −2 m
⎢⎣ 6.3 x 10
)(
= 900 K = 627&deg;C
5.25 In order to solve this problem, we must first compute the value of Do from the data given at 1200&deg;C
(1473 K); this requires the combining of both Equations (5.3) and (5.8). Solving for Do from these
expressions gives
Do = −
⎛Q ⎞
J
exp ⎜ d ⎟
ΔC / Δx
⎝ RT ⎠
⎛ 7.8 x 10 −8 kg / m2 - s ⎞
⎡
⎤
145,000 J/ mol
⎟⎟ exp ⎢
= − ⎜⎜
⎥
⎣(8.31 J/ mol - K)(1473 K) ⎦
− 500 kg / m4
⎝
⎠
= 2.18 x 10-5 m2/s
The value of the diffusion flux at 1273 K may be computed using these same two equations as
follows:
⎛ Qd ⎞
⎛ ΔC ⎞
J = − Do⎜
⎟ exp ⎜ − RT ⎟
⎝ Δx ⎠
⎝
⎠
(
= − 2.18 x 10
-5
2
)(
4
m /s -500 kg/m
⎤
J / mol
)exp ⎡⎢⎣− (8.31145,000
J / mol - K)(1273 K) ⎥⎦
= 1.21 x 10-8 kg/m2-s
5.26 To solve this problem it is necessary to employ Equation (5.7) which takes on the form
D900t 900 = DT t T
100
At 900&deg;C, and using the data from Table 5.2
(
-5
D900 = 2.3 x 10
)
⎡
⎤
148, 000 J / mol
2
m /s exp ⎢−
⎥
⎣ (8.31 J / mol- K)(900 + 273 K) ⎦
-12 2
= 5.9 x 10
m /s
Thus,
(5.9 x 10-12 m2 /s)(15 h) = DT (2 h)
And
-11
D = 4.43 x 10
T
2
m /s
Solving for T from Equation (5.9a)
T =−
= −
(
Qd
R ln DT − ln D o
)
148, 000 J/mol
⎡
(8.31 J/mol - K) ln 4.43 x 10-11 − ln 2.3 x 10-5 ⎤
⎣
⎦
(
)
(
)
= 1353 K = 1080&deg;C
5.27 (a) We are asked to calculate the diffusion coefficient for Cu in Al at 500&deg;C. Using the data in Table
5.2
⎛ Q ⎞
D = D o exp ⎜ − d ⎟
⎝ RT ⎠
(
-5
= 6.5 x 10
)
⎡
⎤
136, 000 J / mol
2
m /s exp ⎢−
⎥
(8.31
J
/
mol
K)(500
+
273
K)
⎣
⎦
-14 2
= 4.15 x 10
m /s
101
(b) This portion of the problem calls for the time required at 600&deg;C to produce the same diffusion
result as for 10 h at 500&deg;C. Equation (5.7) is employed as
D500t 500 = D600t600
Now, from Equation (5.8)
(
D600 = 6.5 x 10
-5
)
⎡
⎤
136,000 J / mol
2
m /s exp ⎢−
⎥
⎣ (8.31 J / mol - K)(600 + 273 K) ⎦
-13 2
= 4.69 x 10
m /s
Thus,
D500 t500
t 600 =
=
D600
(4.15 x 10−14 m2 / s)(10 h) = 0.88 h
(4.69 x 10 −13 m2 / s)
5.28 In order to determine the temperature to which the diffusion couple must be heated so as to
produce a concentration of 3.0 wt% Ni at the 2-mm position, we must first utilize Equation (5.6b) with
time t being a constant. That is
x2
= constant
D
Or
2
x1000
D1000
2
xT
=
DT
Now, solving for DT utilizing Equation (5.8) in order to compute D1000 yields
⎡
DT =
⎛ Q ⎞⎤
(x2T )⎢⎢⎣D o exp ⎜⎝ − RTd ⎟⎠ ⎥⎥⎦
x2
1000
102
⎡
⎞⎤
236,000 J/ mol
⎟
⎝ (8.31 J/ mol - K)(1273 K) ⎠ ⎥⎦
⎛
(2 mm) 2 ⎢ ⎛⎝ 2.7 x 10 −4 m2 / s⎞⎠ exp ⎜ −
⎣
=
(1mm)2
= 2.21 x 10-13 m2/s
We now need to find the T at which D has this value. This is accomplished by rearranging Equation
(5.9a) and solving for T as
T =
=
Qd
(
R ln D
o
− ln D
)
236,000 J/mol
⎡
(8.31 J/mol - K) ln 2.7 x 10 -4 − ln 2.21 x 10-13 ⎤
⎣
⎦
(
)
(
)
= 1357 K = 1084&deg;C
5.29 In order to determine the position within the diffusion couple at which the concentration of A in B is
2.5 wt%, we must employ Equation (5.6b) with t constant. That is
x2
= constant
D
Or
2
2
x800
=
D800
x1000
D1000
It is necessary to compute both D800 and D1000 using Equation (5.8), as follows:
(
)
⎡
⎤
125, 000 J/ mol
D800 = 1.5 x 10 -4 m2 /s exp ⎢−
⎥
⎣ (8.31 J/ mol -K)(1073 K) ⎦
= 1.22 x 10-10 m2/s
(
)
⎡
⎤
125,000 J/ mol
D1000 = 1.5 x 10-4 m2 /s exp ⎢−
⎥
⎣ (8.31 J/ mol- K)(1273 K) ⎦
= 1.11 x 10-9 m2/s
103
Now, solving for x1000 yields
x1000 = x 800
= (5 mm)
D 1000
D
800
1.11 x 10 −9 m 2 / s
−10
1.22 x 10
2
m /s
= 15.1 mm
5.30 In order to compute the diffusion time at 900&deg;C to produce a carbon concentration of 0.75 wt% at a
position 0.5 mm below the surface we must employ Equation (5.6b) with position constant; that is
Dt = constant
Or
D600t 600 = D900t900
In addition, it is necessary to compute both D600 and D900 using Equation (5.8). From Table 5.2, for
the diffusion of C in α Fe, Qd = 80,000 J/mol and Do = 6.2 x 10-7 m2/s. Therefore,
(
D600 = 6.2 x 10
-7
)
⎡
⎤
80,000 J / mol
2
m /s exp ⎢−
⎥
⎣ (8.31 J / mol - K)(600 + 273 K) ⎦
= 1.01 x 10-11 m2/s
(
)
⎡
⎤
80,000 J / mol
D900 = 6.2 x 10-7 m 2/s exp ⎢−
⎥
⎣ (8.31 J / mol - K)(900 + 273 K) ⎦
= 1.69 x 10-10 m2/s
Now, solving for t900 gives
t 900 =
D600 t600
D900
104
=
(1.01 x 10−11 m2 / s)(100 min)
1.69 x 10 −10 m 2 / s
= 5.98 min
5.31 This problem asks us to compute the temperature at which a nonsteady-state 48 h diffusion anneal
was carried out in order to give a carbon concentration of 0.30 wt% C in FCC Fe at a position 3.5
mm below the surface. From Equation (5.5)
C x − Co
C
s
− C
o
=
⎛ x ⎞
0.30 − 0.10
= 0.2000 = 1 − erf ⎜
⎟
1.10 − 0.10
⎝ 2 Dt ⎠
Or
⎛ x ⎞
erf ⎜
⎟ = 0.8000
⎝ 2 Dt ⎠
Now it becomes necessary to, using the data in Table 5.1 and linear interpolation, to determine the
x
.
value of
2 Dt
z
erf (z)
0.90
0.7970
y
0.8000
0.95
0.8209
y − 0.90
0.8000 − 0.7970
=
0.95 − 0.90
0.8209 − 0.7970
From which
y = 0.9063
Thus,
x
= 0.9063
2 Dt
And since t = 48 h and x = 3.5 mm
105
x2
D =
(4t)(0.9063)2
(3.5 x 10 −3 ) m2
2
=
(4)(172, 800 s)(0.821)
= 2.16 x 10
-11
2
m /s
Now, in order to solve for the temperature at which D has the above value, we must employ
Equation (5.9a); solving for T yields
T =
Qd
(
R ln D − ln D
o
)
From Table 5.2, Do and Qd for the diffusion of C in FCC Fe are 2.3 x 10-5 m2/s and 148,000 J/mol,
respectively. Therefore
T =
148,000 J/mol
⎡
(8.31 J/mol - K) ln 2.3 x 10-5 - ln 2.16 x 10-11 ⎤
⎣
⎦
(
)
(
)
= 1283 K = 1010&deg;C
Design Problems
5.D1 This problem calls for us to ascertain whether or not a hydrogen-nitrogen gas mixture may be
enriched with respect to hydrogen partial pressure by allowing the gases to diffuse through an iron
sheet at an elevated temperature. If this is possible, the temperature and sheet thickness are to be
specified; if such is not possible, then we are to state the reasons why. Since this situation involves
steady-state diffusion, we employ Fick's first law, Equation (5.3). Inasmuch as the partial pressures
on the high-pressure side of the sheet are the same, and the pressure of hydrogen on the low
pressure side is five times that of nitrogen, and concentrations are proportional to the square root of
the partial pressure, the diffusion flux of hydrogen JH is the square root of 5 times the diffusion flux
of nitrogen JN--i.e.
JH =
5 JN
106
Thus, equating the Fick's law expressions incorporating the given equations for the diffusion
coefficients and concentrations in terms of partial pressures leads to the following
JH
1
x
Δx
=
(2.5 x 10 −3 )( 0.1013 MPa −
(
)
⎛ 27.8 kJ ⎞
⎛ 13.4 kJ ⎞
−7 2
0.051MPa exp ⎜ −
⎟
⎟ 1.4 x 10 m / s exp ⎜ −
RT ⎠
RT ⎠
⎝
⎝
)
=
5 JN
5
x
Δx
⎛ 37.6 kJ⎞
⎛ 76.15 kJ⎞
−7 2
0.01013 MPa exp ⎜ −
⎟ 3.0 x 10 m / s exp ⎜ −
⎟
RT ⎠
RT ⎠
⎝
⎝
=
(2.75 x 103 )( 0.1013 MPa −
(
)
)
The Δx's cancel out, which means that the process is independent of sheet thickness. Now solving
the above expression for the absolute temperature T gives
T = 3467 K
which value is extremely high (surely above the vaporization point of iron). Thus, such a diffusion
process is not possible.
5.D2 This problem calls for us to ascertain whether or not an A2-B2 gas mixture may be enriched with
respect to the A partial pressure by allowing the gases to diffuse through a metal sheet at an
elevated temperature. If this is possible, the temperature and sheet thickness are to be specified; if
such is not possible, then we are to state the reasons why. Since this situation involves steady-state
diffusion, we employ Fick's first law, Equation (5.3). Inasmuch as the partial pressures on the highpressure side of the sheet are the same, and the pressure of A2 on the low pressure side is 2.5
times that of B2, and concentrations are proportional to the square root of the partial pressure, the
diffusion flux of A, JA, is the square root of 2.5 times the diffusion flux of nitrogen JB--i.e.
JA =
2.5 JB
107
Thus, equating the Fick's law expressions incorporating the given equations for the diffusion
coefficients and concentrations in terms of partial pressures leads to the following
JA
=
(1.5 x 103 )(
(2.0 x 103 )(
0.1013 MPa −
0.1013 MPa −
1
x
Δx
(
)
(
)
⎛ 20.0 kJ⎞
⎛ 13.0 kJ⎞
−7 2
0.051 MPa exp ⎜ −
m / s exp ⎜ −
⎟ 5.0 x 10
⎟
RT ⎠
RT ⎠
⎝
⎝
)
=
2.5 JB
=
2.5
x
Δx
)
⎛ 27.0 kJ ⎞
⎛ 21.0 kJ ⎞
−6 2
⎟ 3.0 x 10 m / s exp ⎜ −
0.0203 MPa exp ⎜ −
⎟
⎝
⎝
RT ⎠
RT ⎠
The Δx's cancel out, which means that the process is independent of sheet thickness. Now solving
the above expression for the absolute temperature T gives
T = 568 K (295&deg;C)
5.D3 This is a nonsteady-state diffusion situation; thus, it is necessary to employ Equation (5.5), utilizing
the following values for the concentration parameters:
Co = 0.0025 wt% N
Cs = 0.45 wt% N
Cx = 0.12 wt% N
Therefore
C x − Co
C s − Co
=
0.12 − 0.0025
0.45 − 0.0025
⎛ x ⎞
= 0.2626 = 1 − erf ⎜
⎟
⎝ 2 Dt ⎠
108
And thus
⎛ x ⎞
1 − 0.2626 = 0.7374 = erf ⎜
⎟
⎝ 2 Dt ⎠
Using linear interpolation and the data presented in Table 5.1
z
erf (z)
0.7500
0.7112
y
0.7374
0.8000
0.7421
0.7374 − 0.7112
y − 0.7500
=
0.7421 − 0.7112
0.8000 − 0.7500
From which
y =
x
= 0.7924
2 Dt
The problem stipulates that x = 0.45 mm = 4.5 x 10-4 m. Therefore
4.5 x 10 −4 m
= 0.7924
2 Dt
Dt = 8.06 x 10-8 m2
Furthermore, the diffusion coefficient depends on temperature according to Equation (5.8); and, as
stipulated in the problem, Do = 3 x 10-7 m2/s and Qd = 76,150 J/mol. Hence
⎛ Q ⎞
Dt = Doexp ⎜ − d ⎟ (t) = 8.06 x 10-8 m 2
⎝ RT ⎠
J / mol ⎤
(3.0 x 10 -7 m2 /s)exp ⎡⎢⎣− (8.3176,150
⎥(t)
J / mol - K)(T) ⎦
109
= 8.06 x 10
−8
2
m
And solving for the time t
t (in s) =
0.269
⎛ 9163.7 ⎞
exp ⎜ −
⎟
⎝
T ⎠
Thus, the required diffusion time may be computed for some specified temperature (in K). Below are
tabulated t values for three different temperatures that lie within the range stipulated in the problem.
_________________________________
Temperature
(&deg;C)
Time
s
h
_________________________________
500
37,900
10.5
550
18,400
5.1
600
9,700
2.7
__________________________________
5.D4 This is a nonsteady-state diffusion situation; thus, it is necessary to employ Equation (5.5), utilizing
the following values for the following parameters:
Co = 0.15 wt% C
1.2 wt% C ≤ Cs ≤ 1.4 wt% C
Cx = 0.75 wt% C
x = 0.65 mm
Let us begin by assuming a specific value for the surface concentration within the specified range—
say 1.2 wt% C. Therefore
C x − Co
C s − Co
=
0.75 − 0.15
1.20 − 0.15
⎛ x ⎞
= 0.5714 = 1 − erf ⎜
⎟
⎝ 2 Dt ⎠
And thus
110
⎛ x ⎞
1 − 0.5714 = 0.4286 = erf ⎜
⎟
⎝ 2 Dt ⎠
Using linear interpolation and the data presented in Table 5.1
z
erf (z)
0.4000
0.4284
y
0.4286
0.4500
0.4755
0.4286 − 0.4284
y − 0.4000
=
0.4755 − 0.4284
0.4500 − 0.4000
From which
y =
x
= 0.4002
2 Dt
The problem stipulates that x = 0.65 mm = 6.5 x 10-4 m. Therefore
6.5 x 10 −4 m
= 0.4002
2 Dt
Dt = 6.59 x 10-7 m2
Furthermore, the diffusion coefficient depends on temperature according to Equation (5.8); and, as
noted in Design Example 5.1, Do = 2.3 x 10-5 m2/s and Qd = 148,000 J/mol. Hence
⎛ Q ⎞
Dt = Doexp ⎜ − d ⎟ (t) = 6.59 x 10-7 m2
⎝ RT ⎠
148,000 J/ mol ⎤
⎥(t)
(2.3 x 10 -5 m2 /s)exp ⎡⎢⎣− (8.31
J / mol - K)(T) ⎦
And solving for the time t
111
= 6.59 x 10
−7
2
m
−2
t (in s) =
2.86 x 10
⎛ 17,810 ⎞
exp ⎜ −
⎟
T ⎠
⎝
Thus, the required diffusion time may be computed for some specified temperature (in K). Below are
tabulated t values for three different temperatures that lie within the range stipulated in the problem.
_________________________________
Temperature
(&deg;C)
Time
s
h
_________________________________
1000
34,100
9.5
1100
12,300
3.4
1200
5,100
1.4
__________________________________
Now, let us repeat the above procedure for two other values of the surface concentration, say 1.3
wt% C and 1.4 wt% C. Below is a tabulation of the results, again using temperatures of 1000&deg;C,
1100&deg;C, and 1200&deg;C.
Cs
(wt% C)
1.3
1.4
Temperature
Time
(&deg;C)
s
h
1000
26,700
7.4
1100
9,600
2.7
1200
4,000
1.1
1000
21,100
6.1
1100
7,900
2.2
1200
1,500
0.9
112
CHAPTER 6
MECHANICAL PROPERTIES OF METALS
PROBLEM SOLUTIONS
6.1
This problem asks that we derive Equations (6.4a) and (6.4b), using mechanics of materials
principles. In Figure (a) below is shown a block element of material of cross-sectional area A that is
subjected to a tensile force P. Also represented is a plane that is oriented at an angle θ referenced
to the plane perpendicular to the tensile axis; the area of this plane is A' = A/cos θ. In addition, the
forces normal and parallel to this plane are labeled as P' and V', respectively. Furthermore, on the
left-hand side of this block element are shown force components that are tangential and
perpendicular to the inclined plane. In Figure (b) are shown the orientations of the applied stress σ,
the normal stress to this plane σ', as well as the shear stress τ' taken parallel to this inclined plane.
In addition, two coordinate axis systems in represented in Figure (c): the primed x and y axes are
referenced to the inclined plane, whereas the unprimed x axis is taken parallel to the applied stress.
Normal and shear stresses are defined by Equations (6.1) and (6.3), respectively. However,
we now chose to express these stresses in terms (i.e., general terms) of normal and shear forces (P
and V) as
σ=
P
A
τ=
V
A
For static equilibrium in the x' direction the following condition must be met:
113
∑ Fx' = 0
which means that
P' − P cos θ = 0
Or that
P' = P cos θ
Now it is possible to write an expression for the stress σ' in terms of P' and A' using the above
expression and the relationship between A and A' [Figure (a)]:
σ' =
=
P'
A'
P cos θ
P
2
=
cos θ
A
A
cos θ
However, it is the case that P/A = σ; and, after make this substitution into the above expression, we
have Equation (6.4a)--that is
σ' = σ cos2θ
Now, for static equilibrium in the y' direction, it is necessary that
∑ Fy ' = 0
= − V' + P sin θ
Or
V' = P sin θ
We now write an expression for τ' as
114
τ' =
V'
A'
And, substitution of the above equation for V' and also the expression for A' gives
τ' =
=
=
V'
A'
P sin θ
A
cos θ
P
sin θ cos θ
A
= σ sinθ cos θ
which is just Equation (6.4b).
6.2 (a) Below are plotted curves of cos2θ (for σ') and sin θ cos θ (for τ') versus θ.
(b) The maximum normal stress occurs at an inclination angle of 0&deg;.
115
(c) The maximum shear stress occurs at an inclination angle of 45&deg;.
6.3
This problem calls for us to calculate the elastic strain that results for an aluminum specimen
2
stressed in tension. The cross-sectional area is just (10 mm) x (12.7 mm) = 127 mm (= 1.27 x 10-4
2
m2 = 0.20 in. ); also, the elastic modulus for Al is given in Table 6.1 as 69 GPa (or 69 x 109 N/m2).
Combining Equations (6.1) and (6.5) and solving for the strain yields
ε =
F
σ
=
=
E A E
o
6.4
35,500 N
(
)(
1.27 x 10−4 m 2 69 x 109 N/ m 2
= 4.1 x 10-3
)
We are asked to compute the maximum length of a cylindrical titanium alloy specimen that is
deformed elastically in tension. For a cylindrical specimen
⎛ do ⎞
A o = π⎜ ⎟
⎝ 2⎠
where d
o
2
is the original diameter. Combining Equations (6.1), (6.2), and (6.5) and solving for lo
lo =
E π d2
oΔ l
4F
(107 x 109 N / m2 )(π)(3.8 x 10 −3 m) (0.42 x 10−3 m)
2
=
(4)(2000 N)
= 0.25 m = 250 mm (10 in.)
6.5 This problem asks us to compute the elastic modulus of steel. For a square cross-section, A = b2o ,
o
where b is the edge length. Combining Equations (6.1), (6.2), and (6.5) and solving for E, leads to
o
E =
Flo
b 2Δ l
o
(
)
2
(20 x 10−3 m) (0.10 x 10 −3 m)
(89,000 N) 100 x 10 −3 m
=
= 223 x 109 N/m2 = 223 GPa (31.3 x 106 psi)
116
6.6 In order to compute the elongation of the Ni wire when the 300 N load is applied we must employ
Equations (6.1), (6.2), and (6.5). Solving for ∆l and realizing that for Ni, E = 207 GPa (30 x 106 psi)
(Table 6.1),
Δl =
=
Fl o
EAo
=
Flo
⎛ do ⎞
Eπ⎜ ⎟
⎝ 2⎠
(4)(300 N)(30 m)
(
9
2
π 207 x 10 N / m
)(2 x 10 m)
−3
2
2
= 0.0138 m = 13.8 mm (0.53 in.)
6.7 (a) This portion of the problem calls for a determination of the maximum load that can be applied
without plastic deformation (F ). Taking the yield strength to be 345 MPa, and employment of
y
(
Fy = σ y A o = 345 x 10
6
2
N/m
)(130 x 10-6 m2 )
= 44,850 N (10,000 lbf)
(b) The maximum length to which the sample may be deformed without plastic deformation is
determined from Equations (6.2) and (6.5) as
σ⎞
⎛
li = l o ⎜1 + ⎟
⎝
E⎠
⎡
345 MPa ⎤
= (76 mm) ⎢1 +
⎥ = 76.25 mm (3.01 in.)
⎢⎣
103 x 10 3 MPa ⎥⎦
6.8 This problem asks us to compute the diameter of a cylindrical specimen to allow an elongation of
0.50 mm. Employing Equations (6.1), (6.2), and (6.5), assuming that deformation is entirely elastic
σ =
F
=
Ao
F
⎛ d2 ⎞
π⎜ o⎟
⎜ 4 ⎟
⎝
⎠
117
= E
Δl
lo
Or
4 loF
do =
(
π E Δl
(4) 380 x 10
(
=
−3
)
)(
m (6660 N)
)
(π) 110 x 109 N/ m 2 0.5 x 10 −3 m
= 7.65 x 10-3 m = 7.65 mm (0.30 in.)
6.9
This problem asks that we calculate the elongation ∆l of a specimen of steel the stress-strain
behavior of which is shown in Figure 6.24. First it becomes necessary to compute the stress when a
load of 65,250 N is applied as
σ =
F
=
Ao
F
⎛ do ⎞
π⎜ ⎟
⎝ 2⎠
2
=
65, 250 N
⎛ 8.5 x 10 −3 m⎞
π⎜
⎟⎟
⎜
2
⎝
⎠
2
= 1150 MPa (170, 000 psi)
Referring to Figure 6.24, at this stress level we are in the elastic region on the stress-strain curve,
which corresponds to a strain of 0.0054. Now, utilization of Equation (6.2) yields
Δ l = ε lo = (0.0054)(80 mm) = 0.43 mm (0.017 in.)
6.10 (a) This portion of the problem asks that the tangent modulus be determined for the gray cast iron,
the stress-strain behavior of which is shown in Figure 6.25. The slope (i.e., ∆σ/∆ε) of a tangent
drawn through this curve at 25 MPa (3625 psi) is about 90 GPa (15 x 106 psi).
(b) The secant modulus taken from the origin is calculated by taking the slope of a secant drawn
from the origin through the stress-strain curve at 35 MPa (5,000 psi). When such a secant is drawn,
a modulus of approximately 100 GPa (14.5 x 106 psi) is obtained.
6.11 We are asked, using the equation given in the problem, to verify that the modulus of elasticity
values along  directions given in Table 3.3 for aluminum, copper, and iron are correct. The α, β,
and γ parameters in the equation correspond, respectively, to the cosines of the angles between the
 direction and ,  and  directions. Since these angles are 45&deg;, 45&deg;, and 90&deg;, the
values of α, β, and γ are 0.707, 0.707, and 0, respectively. Thus, the given equation takes the form
118
1
E&lt;110&gt;
=
⎛
1
1 ⎞
⎟⎟ (0.707) 2(0.707) 2 + (0.707)2 (0)2 + (0)2 (0.707)2
− 3 ⎜⎜
−
E
E
E
⎝ &lt;100&gt;
&lt;100&gt;
&lt;111&gt; ⎠
[
1
=
]
⎛
1
1 ⎞
⎟⎟
− (0.75) ⎜⎜
−
E
⎝ E&lt;100&gt; E&lt;111&gt; ⎠
&lt;100&gt;
1
Utilizing the values of E&lt;100&gt; and E&lt;111&gt; from Table 3.3 for Al
1
E&lt;110 &gt;
=
⎡
⎤
1
1
1
− (0.75) ⎢
−
⎥
63.7 GPa
⎣ 63.7 GPa 76.1 GPa ⎦
Thus, E&lt;110&gt; = 72.6 GPa, which is the value given in the table.
For Cu,
⎡
⎤
1
1
1
1
=
− (0.75) ⎢
−
⎥
E&lt;110 &gt; 66.7 GPa
191.1
GPa
66.7
GPa
⎣
⎦
from which E&lt;110&gt; = 130.3 GPa, which is the value given in the table.
Similarly, for Fe
1
E&lt;110 &gt;
=
⎡
⎤
1
1
1
− (0.75) ⎢
−
⎥
125.0 GPa
⎣125.0 GPa 272.7 GPa ⎦
and E&lt;110&gt; = 210.5 GPa, which is also the value given in the table.
6.12 This problem asks that we derive an expression for the dependence of the modulus of elasticity, E,
on the parameters A, B, and n in Equation (6.36). It is first necessary to take dEN/dr in order to
obtain an expression for the force F; this is accomplished as follows:
119
⎛B⎞
⎛ A⎞
d⎜ ⎟
⎜
⎟
d
−
dEN
⎝ rn ⎠
⎝ r⎠
F =
=
+
dr
dr
dr
=
A
r2
nB
−
r
(n + 1)
The second step is to set this dEN/dr expression equal to zero and then solve for r (= ro). This
procedure is carried out in Problem 2.13, with the result that
⎛ A⎞
ro = ⎜ ⎟
⎝ nB ⎠
1/(1 - n)
Next it becomes necessary to take the derivative of the force (dF/dr), which is accomplished as
follows:
⎛
nB ⎞
⎛ A⎞
⎟
d⎜−
d⎜ ⎟
⎜ (n + 1) ⎟
⎝ r
⎠
⎝ r2 ⎠
dF
=
+
dr
dr
dr
2A (n)(n + 1)B
=− 3 +
(n + 2)
r
r
Now, substitution for ro into this equation yields
⎛ dF ⎞
2A
(n)(n + 1)B
+
⎜
⎟ =−
3
/(1−
n)
(n + 2) /(1− n)
⎝ dr ⎠ r
⎛ A⎞
⎛ A⎞
o
⎜ ⎟
⎜
⎟
⎝ nB ⎠
⎝ nB ⎠
which is the expression to which the modulus of elasticity is proportional.
6.13 This problem asks that we rank the magnitudes of the moduli of elasticity of the three hypothetical
metals X, Y, and Z. From Problem 6.12, it was shown for materials in which the bonding energy is
dependent on the interatomic distance r according to Equation (6.36), that the modulus of elasticity E
is proportional to
120
E ∝ −
2A
3 /(1 − n)
⎛ A⎞
⎜ ⎟
⎝ nB ⎠
+
(n)(n + 1)B
⎛ A⎞
⎜ ⎟
⎝ nB ⎠
(n + 2) /(1 − n)
For metal X, A = 1.5, B = 7 x 10-6, and n = 8. Therefore,
E ∝ −
(
−6
(8)(8 + 1) 7 x 10
(2)(1.5)
3 /(1 − 8)
⎡
⎤
1.5
⎢
⎥
⎢ (8) ⎛ 7 x 10−6 ⎞ ⎥
⎝
⎠⎦
⎣
+
⎡
⎤
1.5
⎢
⎥
⎢
⎥
−6
⎢⎣(8) 7 x 10
⎦⎥
(
)
(8 + 2) /(1 − 8)
)
= 830
For metal Y, A = 2.0, B = 1 x 10-5, and n = 9. Hence
E ∝ −
⎡
⎤
2.0
⎢
⎥
⎢ (9) ⎛1 x 10 −5 ⎞ ⎥
⎝
⎠⎦
⎣
(
(9)(9 + 1) 1 x 10
(2)(2.0)
3 /(1 − 9)
+
⎡
⎤
2.0
⎢
⎥
⎢
⎥
−5
⎢⎣ (9) 1 x 10
⎦⎥
(
−5
)
(9 + 2) /(1 − 9)
)
= 683
And, for metal Z, A = 3.5, B = 4 x 10-6, and n = 7. Thus
E ∝ −
⎡
⎤
3.5
⎢
⎥
⎢ (7) ⎛ 4 x 10−6 ⎞ ⎥
⎝
⎠⎦
⎣
(
(7)(7 + 1) 4 x 10
(2)(3.5)
3 /(1 − 7)
+
⎡
⎤
3.5
⎢
⎥
⎢
−6 ⎥
(7)
4
x
10
⎢⎣
⎥⎦
(
−6
)
(7 + 2) /(1 − 7)
)
= 7425
Therefore, metal Z has the highest modulus of elasticity.
6.14 (a) We are asked, in this portion of the problem, to determine the elongation of a cylindrical
specimen of aluminum. Using Equations (6.1), (6.2), and (6.5)
121
F
⎛ d2 ⎞
π⎜ o⎟
⎜ 4 ⎟
⎝
⎠
=E
Δl
lo
Or
Δl =
4 Flo
π d 2E
o
−3
m)
(
= 0.50 mm (0.02 in.)
−3 2
9
2
(π) (
19 x 10 m) (69 x 10 N/ m )
(4)(48, 800 N) 200 x 10
=
(b) We are now called upon to determine the change in diameter, Δd. Using Equation (6.8)
ε
Δd / d o
ν = − x = −
εz
Δ l/ lo
From Table 6.1, for Al, ν = 0.33. Now, solving for ∆d yields
Δd = −
ν Δ ld o
lo
= −
(0.33)(0.50 mm)(19 mm)
200 mm
= -1.57 x 10-2 mm (-6.2 x 10-4 in.)
The diameter will decrease.
6.15 This problem asks that we calculate the force necessary to produce a reduction in diameter of 3 x
-3
10 mm for a cylindrical bar of steel. Combining Equations (6.1), (6.5), and (6.8), realizing that
Ao =
and
εx =
π do2
4
Δd
do
Now, solving for F leads to
122
d Δd π E
F = − o
4ν
From Table (6.1), for steel, ν = 0.30 and E = 207 GPa. Thus,
−3
−6
9
2
10 x 10 m)(− 3.0 x 10 m)(π) (207 x 10 N / m )
(
F = −
(4)(0.30)
= 16,250 N (3770 lbf)
6.16 This problem asks that we compute Poisson's ratio for the metal alloy. From Equations (6.5) and
(6.1)
εz =
σ F / Ao
=
=
E
E
F
2
⎛d ⎞
π⎜ o ⎟ E
⎝ 2⎠
=
4F
π d2 E
o
Since the transverse strain εx is just
εx =
Δd
do
and Poisson's ratio is defined by Equation (6.8) then
ν = −
=
ε
Δd / d
o
x = −
= −
ε
⎛
⎞
z
4F
⎜
⎟
⎜ π d2E ⎟
⎝ o ⎠
do Δd πE
4F
−3
−6
9
2
10 x 10 m)(−7 x 10 m)(π) (100 x 10 N/ m )
(
−
= 0.367
(4)(15,000 N)
6.17 This problem asks that we compute the original length of a cylindrical specimen that is stressed in
compression. It is first convenient to compute the lateral strain εx as
εx =
Δd 30.04 mm − 30.00 mm
=
= 1.33 x 10-3
30.00 mm
do
123
In order to determine the longitudinal strain εz we need Poisson's ratio, which may be computed
using Equation (6.9); solving for ν yields
3
ν =
65.5 x 10 MPa
E
−1 =
− 1 = 0.289
2G
(2) 25.4 x 1 0 3 MPa
(
)
Now εz may be computed from Equation (6.8) as
ε
1.33 x 10 −3
εz = − x = −
= − 4.60 x 10-3
ν
0.289
Now solving for lo using Equation (6.2)
li
lo =
=
1+ ε
105.20 mm
1 − 4.60 x 10−3
z
= 105.69 mm
6.18 This problem asks that we calculate the modulus of elasticity of a metal that is stressed in tension.
Combining Equations (6.5) and (6.1) leads to
E =
F / Ao
σ
=
=
ε
ε
z
z
F
⎛d ⎞
ε π⎜ o ⎟
z
⎝ 2 ⎠
2
=
4F
ε π d2
z
o
From the definition of Poisson's ratio, [Equation (6.8)] and realizing that for the transverse strain, εx=
Δd
do
ε
Δd
εz = − x = −
d ν
ν
o
Therefore, substitution of this expression for εz into the above equation yields
E =
4F
ε π d2
z o
=
124
4F ν
π d Δd
o
=
(
(4)(1500 N)(0.35)
)(
)
π 10 x 10−3 m 6.7 x 10−7 m
= 1011 Pa = 100 GPa (14.7 x 10 6 psi)
6.19 We are asked to ascertain whether or not it is possible to compute, for brass, the magnitude of the
load necessary to produce an elongation of 7.6 mm (0.30 in.). It is first necessary to compute the
strain at yielding from the yield strength and the elastic modulus, and then the strain experienced by
the test specimen. Then, if
ε(test) &lt; ε(yield)
deformation is elastic, and the load may be computed using Equations (6.1) and (6.5). However, if
ε(test) &gt; ε(yield)
computation of the load is not possible inasmuch as deformation is plastic and we have neither a
stress-strain plot nor a mathematical expression relating plastic stress and strain. We compute
these two strain values as
ε(test) =
and
ε(yield) =
σy
E
Δl
7.6 mm
=
= 0.03
lo
250 mm
=
275 MPa
103 x 10 3 MPa
= 0.0027
6.20 (a) This part of the problem asks that we ascertain which of the metals in Table 6.1 experience an
elongation of less than 0.080 mm when subjected to a stress of 28 MPa. The maximum strain that
may be sustained is just
ε =
Δl 0.080 mm
=
= 3.2 x 10-4
lo
250 mm
Since the stress level is given, using Equation (6.5) it is possible to compute the minimum modulus
of elasticity which is required to yield this minimum strain. Hence
E =
σ
28 MPa
=
= 87.5 GPa
ε
3.2 x 10−4
Which means that those metals with moduli of elasticity greater than this value are acceptable
candidates--namely, brass, Cu, Ni, steel, Ti and W.
125
(b) This portion of the problem further stipulates that the maximum permissible diameter decrease is
1.2 x 10-3 mm. Thus, the maximum possible lateral strain εx is just
εx =
Δd
−1.2 x 10 −3 mm
-5
=
= − 9.45 x 10
d
12.7 mm
o
Since we now have maximum permissible values for both axial and lateral strains, it is possible to
determine the maximum allowable value for Poisson's ratio using Equation (6.8). Thus
ν =−
εx
ε
=−
z
−9.45 x 10−5
3.2 x 10 −4
= 0.295
Or, the value of Poisson's ratio must be less than 0.295. Of the metals in Table 6.1, only W meets
both of these criteria.
6.21 (a) This portion of the problem asks that we compute the elongation of the brass specimen. The
first calculation necessary is that of the applied stress using Equation (6.1), as
σ =
F
=
Ao
F
⎛ do ⎞
π⎜ ⎟
⎝ 2⎠
2
=
10, 000 N
⎛ 10 x 10 −3 m ⎞
π⎜
⎟⎟
⎜
2
⎝
⎠
2
= 127 MPa (17, 900 psi)
From the stress-strain plot in Figure 6.12, this stress corresponds to a strain of about 1.5 x 10-3.
From the definition of strain, Equation (6.2)
(
-3
Δ l = ε lo = 1.5 x 10
)(101.6 mm) = 0.15 mm
(6.0 x 10
-3
in.)
(b) In order to determine the reduction in diameter ∆d, it is necessary to use Equation (6.8) and the
definition of lateral strain (i.e., εx = ∆d/do) as follows
(
Δd = doε x = − d o νε z = − (10 mm)(0.35) 1.5 x 10
= -5.25 x 10-3 mm (-2.05 x 10-4 in.)
126
-3
)
6.22
Elastic deformation is time-independent and nonpermanent, anelastic deformation is timedependent and nonpermanent, while plastic deformation is permanent.
6.23 This problem asks that we assess the four alloys relative to the two criteria presented. The first
criterion is that the material not experience plastic deformation when the tensile load of 35,000 N is
applied; this means that the stress corresponding to this load not exceed the yield strength of the
material. Upon computing the stress
σ =
F
=
Ao
F
⎛ do ⎞
π⎜ ⎟
⎝ 2⎠
2
=
35, 000 N
6
⎛ 15 x 10−3 m ⎞
π⎜
⎟⎟
⎜
2
⎝
⎠
2
2
= 200 x 10 N/m
= 200 MPa
Of the alloys listed in the table, the Al, Ti and steel alloys have yield strengths greater than 200 MPa.
Relative to the second criterion, it is necessary to calculate the change in diameter ∆d for
these two alloys. From Equation (6.8)
ε
Δd / d o
ν = − x = −
εz
σ /E
Now, solving for ∆d from this expression,
Δd = −
νσ d o
E
For the aluminum alloy
Δd = −
(0.33)(200 MPa)(15 mm)
70 x 103 MPa
= − 1.41 x 10-3 mm
Therefore, the Al alloy is not a candidate.
For the steel alloy
Δd = −
(0.27)(200 MPa)(15 mm)
205 x 103 MPa
Therefore, the steel is a candidate.
127
= − 0.40 x 10-2 mm
For the Ti alloy
Δd = −
(0.36)(200 MPa)(15 mm)
= − 1.0 x 10-2 mm
105 x 103 MPa
Hence, the titanium alloy is also a candidate.
6.24
This problem asks that we ascertain which of four metal alloys will 1) not experience plastic
deformation, and 2) not elongate more than 0.9 mm when a tensile load is applied.
It is first
necessary to compute the stress using Equation (6.1); a material to be used for this application must
necessarily have a yield strength greater than this value. Thus,
σ =
F
=
Ao
24,500 N
⎛ 10 x 10−3 m ⎞
π⎜
⎟⎟
⎜
2
⎝
⎠
2
= 312 MPa
Of the metal alloys listed, only brass and steel have yield strengths greater than this stress.
Next, we must compute the elongation produced in both brass and steel using Equations
(6.2) and (6.5) in order to determine whether or not this elongation is less than 0.9 mm. For brass
Δl =
σlo
E
=
(312 MPa)(380 mm)
100 x 10 3 MPa
= 1.19 mm
Thus, brass is not a candidate. However, for steel
Δl =
σ lo
E
=
(312 MPa)(380 mm)
207 x 103 MPa
= 0.57 mm
Therefore, of these four alloys, only steel satisfies the stipulated criteria.
6.25 Using the stress-strain plot for a steel alloy (Figure 6.24), we are asked to determine several of its
mechanical characteristics.
(a) The elastic modulus is just the slope of the initial linear portion of the curve; or, from the inset
and using Equation (6.10)
E =
σ2 − σ1
(1300 − 0 ) MPa
=
= 210 x 103 MPa = 210 GPa (30.5 x 106 psi)
−
3
ε 2 − ε1
6.25 x 10 − 0
(
)
128
The value given in Table 6.1 is 207 GPa.
(b) The proportional limit is the stress level at which linearity of the stress-strain curve ends, which is
approximately 1370 MPa (200,000 psi).
(c)
The 0.002 strain offset line intersects the stress-strain curve at approximately 1570 MPa
(228,000 psi).
(d) The tensile strength (the maximum on the curve) is approximately 1970 MPa (285,000 psi).
6.26
We are asked to calculate the radius of a cylindrical brass specimen in order to produce an
elongation of 5 mm when a load of 100,000 N is applied. It first becomes necessary to compute the
strain corresponding to this elongation using Equation (6.2) as
ε =
Δl
5 mm
=
= 5 x 10-2
l o 100 mm
From Figure 6.12, a stress of 335 MPa (49,000 psi) corresponds to this strain. Since for a cylindrical
specimen, stress, force, and initial radius ro are related as
F
σ =
πr 2
o
then
ro =
F
=
πσ
(
100,000 N
π 335 x 106 N / m2
)
= 0.0097 m = 9.7 mm (0.38 in.)
6.27 This problem asks us to determine the deformation characteristics of a steel specimen, the stressstrain behavior of which is shown in Figure 6.24.
(a) In order to ascertain whether the deformation is elastic or plastic, we must first compute the
stress, then locate it on the stress-strain curve, and, finally, note whether this point is on the elastic
or plastic region. Thus,
σ =
F
=
Ao
140, 000 N
⎛ 10 x 10 −3 m⎞
π⎜
⎟⎟
⎜
2
⎝
⎠
2
= 1782 MPa (250,000 psi)
129
The 1782 MPa point is past the linear portion of the curve, and, therefore, the deformation will be
both elastic and plastic.
(b) This portion of the problem asks us to compute the increase in specimen length. From the
stress-strain curve, the strain at 1782 MPa is approximately 0.017. Thus, from Equation (6.2)
Δ l = ε lo = (0.017)(500 mm) = 8.5 mm (0.34 in.)
6.28 (a) We are asked to compute the magnitude of the load necessary to produce an elongation of 2.25
mm for the steel displaying the stress-strain behavior shown in Figure 6.24. First, calculate the
strain, and then the corresponding stress from the plot.
ε =
Δ l 2.25 mm
=
= 0.006
lo
375 mm
This is within the elastic region; from the inset of Figure 6.24, this corresponds to a stress of about
1250 MPa (180,000 psi). Now,
F = σA o = σb 2
in which b is the cross-section side length. Thus,
(
)(
) = 37, 800 N
F = 1250 x 106 N/m2 5.5 x 10-3 m
2
(8500 lb f )
(b) After the load is released there will be no deformation since the material was strained only
elastically.
6.29 This problem calls for us to make a stress-strain plot for aluminum, given its tensile load-length data,
and then to determine some of its mechanical characteristics.
(a) The data are plotted below on two plots: the first corresponds to the entire stress-strain curve,
while for the second, the curve extends just beyond the elastic region of deformation.
130
(b) The elastic modulus is the slope in the linear elastic region as
E =
Δ σ 200 MPa − 0 MPa
3
=
= 62.5 x 10 MPa = 62.5 GPa
Δε
0.0032 − 0
(9.1 x 106 psi)
(c) For the yield strength, the 0.002 strain offset line is drawn dashed. It intersects the stress-strain
curve at approximately 285 MPa (41,000 psi ).
(d) The tensile strength is approximately 370 MPa (53,500 psi), corresponding to the maximum
stress on the complete stress-strain plot.
131
(e)
The ductility, in percent elongation, is just the plastic strain at fracture, multiplied by one-
hundred. The total fracture strain at fracture is 0.165; subtracting out the elastic strain (which is
about 0.005) leaves a plastic strain of 0.160. Thus, the ductility is about 16%EL.
(f) From Equation (6.14), the modulus of resilience is just
Ur =
σ2
y
2E
which, using data computed in the problem, yields a value of
2
Ur =
(285 MPa)
(
(2) 62.5 x 103 MPa
5
)
3
= 6.5 x 10 J/m
(93.8 in. - lbf /in.3 )
6.30 This problem calls for us to make a stress-strain plot for a magnesium, given its tensile load-length
data, and then to determine some of its mechanical characteristics.
(a) The data are plotted below on two plots: the first corresponds to the entire stress-strain curve,
while for the second, the curve extends just beyond the elastic region of deformation.
132
(b) The elastic modulus is the slope in the linear elastic region as
E =
Δ σ 50 MPa − 0 MPa
=
= 50 x 103 MPa = 50 GPa
Δε
0.001 − 0
(7.3 x 106 psi)
(c) For the yield strength, the 0.002 strain offset line is drawn dashed. It intersects the stress-strain
curve at approximately 150 MPa (21,750 psi).
(d) The tensile strength is approximately 240 MPa (34,800 psi), corresponding to the maximum
stress on the complete stress-strain plot.
(e) From Equation (6.14), the modulus of resilience is just
σ2
Ur =
y
2E
which, using data computed in the problem, yields a value of
(150 x 10 6 N/ m2 ) = 2.25 x 105 J/m3 32.6 in. - lb /in.3
(
)
f
(2) (50 x 10 9 N/ m 2 )
2
Ur =
(f) The ductility, in percent elongation, is just the plastic strain at fracture, multiplied by one-hundred.
The total fracture strain at fracture is 0.110; subtracting out the elastic strain (which is about 0.003)
leaves a plastic strain of 0.107. Thus, the ductility is about 10.7%EL.
133
6.31 This problem calls for ductility in both percent reduction in area and percent elongation. Percent
reduction in area is computed using Equation (6.12) as
2
%RA =
⎛ do ⎞
⎛ df ⎞
π⎜
⎟ − π⎜ ⎟
⎝2⎠
⎝ 2 ⎠
⎛ do ⎞
π⎜
⎟
⎝ 2 ⎠
2
2
x 100
in which d and d are, respectively, the original and fracture cross-sectional areas. Thus,
o
f
2
%RA =
⎛ 12.8 mm ⎞
⎛ 6.60 mm ⎞
π⎜
⎟ − π⎜
⎟
⎝
⎠
⎝
⎠
2
2
⎛ 12.8 mm ⎞
π⎜
⎟
⎝
⎠
2
2
x 100 = 73.4%
2
While, for percent elongation, Equation (6.11) is used as
⎛ l − lo ⎞
%EL = ⎜⎜ f
⎟⎟ x 100
⎝ lo ⎠
=
72.14 mm − 50.80 mm
x 100 = 42%
50.80 mm
6.32 This problem asks us to calculate the moduli of resilience for the materials having the stress-strain
behaviors shown in Figures 6.12 and 6.24. According to Equation (6.14), the modulus of resilience
Ur is a function of the yield strength and the modulus of elasticity as
σ2
Ur =
y
2E
The values for σy and E for the brass in Figure 6.12 are 250 MPa (36,000 psi) and 93.9 GPa (13.6 x
106 psi), respectively. Thus
2
Ur =
(250 MPa)
(
(2) 93.9 x 103 MPa
5
)
= 3.32 x 10 J/m
134
3
(47.6 in. - lbf/in.3 )
Values of the corresponding parameters for the steel alloy (Figure 6.24) are 1570 MPa
(230,000 psi) and 210 GPa (30.5 x 106 psi), respectively, and therefore
Ur =
(1570
(
MPa )
2
(2) 210 x 10 3 MPa
)
6
= 5.87 x 10 J/m
3
(867
in. - lbf /in.
3
)
6.33 The moduli of resilience of the alloys listed in the table may be determined using Equation (6.14).
Yield strength values are provided in this table, whereas the elastic moduli are tabulated in Table
6.1.
For steel
σ2
Ur =
y
2E
6
2
830 x 10 N / m )
(
5
3
3
=
= 16.6 x 10 J/m (240 in. - lbf /in. )
9
2
(2) (207 x 10 N/ m )
2
For the brass
6
2
380 x 10 N / m )
(
5
3
3
Ur =
= 7.44 x 10 J/m (108 in. - lbf /in. )
9
2
(2) (97 x 10 N/ m )
2
For the aluminum alloy
6
2
275 x 10 N / m )
(
Ur =
= 5.48 x 105 J/m3 (80.0
9
2
(2) (69 x 10 N/ m )
2
in. - lbf /in.3
)
And, for the titanium alloy
6
2
690 x 10 N/ m )
(
5
3
3
= 22.2 x 10 J/m (323 in. - lbf /in. )
Ur =
9
2
(2) (107 x 10 N/ m )
2
135
6.34
The modulus of resilience, yield strength, and elastic modulus of elasticity are related to one
another through Equation (6.14); the value of E for steel given in Table 6.1 is 207 GPa. Solving for
σy from this expression yields
σy =
2 UrE =
(
(2) (2.07 MPa ) 207 x 103 MPa
)
= 925 MPa (134,000 psi)
6.35 (a) In the schematic plot shown below, curve (1) represents the tensile true stress-strain behavior
for a typical metal alloy.
(b) The compressive stress-strain behavior is also represented by curve (1), which is virtually the
same as that for the tensile behavior inasmuch as both compressive and tensile true stress take into
account the cross-sectional area over which deformation is occurring (i.e., within the neck region for
tensile behavior).
(c) Curve (2) in this plot represents the compression engineering stress-strain behavior for this
same alloy; this curve lies below curve (1) which is for compression true stress and strain. The
reason for this is that during compression the cross-sectional area is increasing (that is, Ai &gt; Ao),
and since σ = F/Ao and σT = F/Ai, then it follows that σT &lt; σ.
6.36 To show that Equation (6.18a) is valid, we must first rearrange Equation (6.17) as
136
Ai =
Ao lo
li
Substituting this expression into Equation (6.15) yields
σT =
⎛l ⎞
F
F ⎛ li ⎞
⎜⎜ ⎟⎟ = σ ⎜⎜ i ⎟⎟
=
A
A ⎝l ⎠
⎝ lo⎠
i
o o
But, from Equation (6.2)
l
ε = i − 1
l
o
Or
li
l
= ε +1
o
Thus,
⎛l ⎞
σ T = σ⎜⎜ i ⎟⎟ = σ ( ε + 1)
⎝ lo ⎠
For Equation (6.18b)
ε T = ln (1 + ε)
is valid since
⎛l ⎞
ε T = ln ⎜⎜ i ⎟⎟
⎝ lo ⎠
and
li
l
=ε + 1
o
from above.
6.37 This problem asks us to demonstrate that true strain may also be represented by
⎛A ⎞
ε T = ln ⎜⎜ o ⎟⎟
⎝ Ai ⎠
137
Rearrangement of Equation (6.17) leads to
li
lo
=
Ao
Ai
Thus, Equation (6.16) takes the form
⎛l ⎞
⎛A ⎞
ε T = ln ⎜⎜ i ⎟⎟ = ln ⎜⎜ o ⎟⎟
⎝ lo ⎠
⎝ Ai ⎠
⎛A ⎞
o
⎟⎟ is more valid during necking because A is taken as the area of the
The expression ε T = ln ⎜⎜
i
A
⎝ i⎠
neck.
6.38 These true stress-strain data are plotted below.
6.39 We are asked to compute the true strain that results from the application of a true stress of 600 MPa
(87,000 psi); other true stress-strain data are also given. It first becomes necessary to solve for n in
Equation (6.19). Taking logarithms of this expression and after rearrangement we have
138
n =
log σT − log K
log ε
T
=
log (575 MPa) − log (860 MPa)
= 0.250
log (0.2)
Expressing εT as the dependent variable, and then solving for its value from the data stipulated in
⎛ σT ⎞
εT = ⎜
⎟
⎝ K ⎠
1/n
⎛ 600 MPa ⎞
=⎜
⎟
⎝ 860 MPa ⎠
1/0.25
= 0.237
6.40 We are asked to compute how much elongation a metal specimen will experience when a true
stress of 415 MPa is applied, given the value of n and that a given true stress produces a specific
true strain. Solution of this problem requires that we utilize Equation (6.19). It is first necessary to
solve for K from the given true stress and strain. Rearrangement of this equation yields
K =
σT
(ε )n
T
=
345 MPa
(0.02 )0.22
= 816 MPa (118,000 psi)
Next we must solve for the true strain produced when a true stress of 415 MPa is applied, also using
Equation (6.19). Thus
⎛ σT ⎞
εT = ⎜
⎟
⎝ K ⎠
1/n
⎛ 415 MPa ⎞
=⎜
⎟
⎝ 816 MPa ⎠
1/0.22
⎛ li ⎞
= 0.0463 = ln⎜⎜ ⎟⎟
⎝ lo ⎠
Now, solving for li gives
li = lo e0.0463 = (500 mm)e0.0463 = 523.7 mm (20.948 in.)
And finally, the elongation ∆l is just
Δl = li − lo = 523.7 mm − 500 mm = 23.7 mm (0.948 in.)
139
6.41 For this problem, we are given two values of εT and σT, from which we are asked to calculate the
true stress which produces a true plastic strain of 0.25. After taking logarithms of Equation (6.19),
we may set up two simultaneous equations with two unknowns (the unknowns being K and n), as
log (50, 000 psi) = log K + n log (0.10)
log (60, 000 psi) = log K + n log (0.20)
From these two expressions,
n=
log (50,000) − log (60, 000)
= 0.263
log (0.1) − log (0.2)
log K = 4.96 or K = 91,623 psi
Thus, for εT = 0.25
( )0.263 = (91,623 psi)(0.25)0.263 = 63,700 psi
σ T = K εT
(440 MPa)
6.42 For this problem we first need to convert engineering stresses and strains to true stresses and
strains so that the constants K and n in Equation (6.19) may be determined. Since σT = σ(1 + ε)
then
σ T = (315 MPa)(1 + 0.105) = 348 MPa
1
σ T = (340 MPa)(1 + 0.220) = 415 MPa
2
Similarly for strains, since εT = ln(1 + ε) then
ε T = ln (1 + 0.105) = 0.09985
1
ε T = ln (1 + 0.220) = 0.19885
2
Taking logarithms of Equation (6.19), we get
log σ T = log K + n log ε T
140
which allows us to set up two simultaneous equations for the above pairs of true stresses and true
strains, with K and n as unknowns. Thus
log (348) = log K + n log (0.09985)
log (415) = log K + n log (0.19885)
Solving for these two expressions yields K = 628 MPa and n = 0.256.
Now, converting ε = 0.28 to true strain
ε T = ln (1 + 0.28) = 0.247
The corresponding σT to give this value of εT [using Equation (6.19)] is just
σ T = KεnT = (628 MPa)(0.247) 0.256 = 439 MPa
Now converting this σT to an engineering stress
σ =
σT
1+ ε
=
439 MPa
= 343 MPa
1 + 0.28
6.43 This problem calls for us to compute the toughness (or energy to cause fracture). The easiest way
to do this is to integrate both elastic and plastic regions, and then add them together.
Toughness =
0.01
∫
=
0.75
Eε d ε +
0
Eε 2
=
2
∫ σ dε
∫ Kε n dε
0.01
0.01
0.75
K
(n + 1)
+
ε
(n + 1)
0
0.01
141
9
=
2
6
172 x 10 N/ m
6900 x 10 N/m
(0.01)2 +
2
(1.0 + 0.3)
2
[(0.75 )
1.3
- (0.01 )
1.3
]
= 3.65 x 109 J/m3 (5.29 x 105 in.-lbf/in.3)
6.44 This problem asks that we determine the value of εT for the onset of necking assuming that necking
begins when
dσT
dε
T
= σT
Let us take the derivative of Equation (6.19), set it equal to σT, and then solve for εT from the
resulting expression. Thus
( )
n⎤
⎡
d ⎢K ε T ⎥
(n − 1)
⎣
⎦
= Kn ε T
= σT
dε T
( )
However, from Equation (6.19), σT = K(εT)n, which, when substituted into the above expression,
yields
( )(n - 1) = K (ε T )n
Kn ε T
Now solving for εT from this equation leads to
εT = n
as the value of the true strain at the onset of necking.
6.45 This problem calls for us to utilize the appropriate data from Problem 6.29 in order to determine the
values of n and K for this material. From Equation (6.38) the slope and intercept of a log σT versus
log εT plot will yield values for n and log K, respectively. However, Equation (6.19) is only valid in
the region of plastic deformation to the point of necking; thus, only the 7th, 8th, 9th, and 10th data
points may be utilized. The log-log plot with these data points is given below.
142
The slope yields a value of 0.136 for n, whereas the intercept gives a value of 2.7497 for log K, and
thus K = 562 MPa.
6.46 (a) In order to determine the final length of the brass specimen when the load is released, it first
becomes necessary to compute the applied stress using Equation (6.1); thus
σ =
F
=
Ao
F
⎛ do ⎞
π⎜ ⎟
⎝ 2⎠
2
=
11,750 N
⎛ 10 x 10−3 m ⎞
π⎜
⎟⎟
⎜
2
⎝
⎠
2
= 150 MPa (22,000 psi)
Upon locating this point on the stress-strain curve (Figure 6.12), we note that it is in the linear, elastic
region; therefore, when the load is released the specimen will return to its original length of 120 mm
(4.72 in.).
(b) In this portion of the problem we are asked to calculate the final length, after load release, when
the load is increased to 23,500 N (5280 lbf). Again, computing the stress
σ =
23, 500 N
⎛ 10 x 10−3 m ⎞
π⎜
⎟⎟
⎜
2
⎝
⎠
2
= 300 MPa (44, 200 psi)
143
The point on the stress-strain curve corresponding to this stress is in the plastic region. We are able
to estimate the amount of permanent strain by drawing a straight line parallel to the linear elastic
region; this line intersects the strain axis at a strain of about 0.012 which is the amount of plastic
strain. The final specimen length li may be determined from Equation (6.2) as
li = lo(1 + ε) = (120 mm)(1 + 0.012) = 121.44 mm (4.78 in.)
6.47 (a) We are asked to determine both the elastic and plastic strains when a tensile force of 110,000 N
(25,000 lbf) is applied to the steel specimen and then released. First it becomes necessary to
determine the applied stress using Equation (6.1); thus
F
F
=
Ao b od o
σ =
where bo and do are cross-sectional width and depth (19 mm and 3.2 mm, respectively). Thus
σ =
(
110,000 N
)(
)
19 x 10 −3 m 3.2 x 10 −3 m
= 1.810 x 10 9 N / m2 = 1810 MPa (265,000 psi)
From Figure 6.24, this point is in the plastic region so there will be both elastic and plastic strains
present. The total strain at this point, εt, is about 0.020. We are able to estimate the amount of
permanent strain recovery εe from Hooke's law, Equation (6.5) as
εe =
σ
E
And, since E = 207 GPa for steel (Table 6.1)
εe =
1810 MPa
207 x 103 MPa
= 0.009
The value of the plastic strain, εp is just the difference between the total and elastic strains; that is
εp = εt - εe = 0.020 - 0.0087 = 0.011
(b) If the initial length is 610 mm (24.0 in.) then the final specimen length li may be determined from
Equation (6.2) using the plastic strain value as
144
li = lo(1 + εp) = (610 mm)(1 + 0.011) = 616.7 mm (24.26 in.)
6.48 (a) We are asked to compute the Brinell hardness for the given indentation. It is necessary to use
the equation in Table 6.4 for HB, where P = 1000 kg, d = 2.50 mm, and D = 10 mm. Thus, the
Brinell hardness is computed as
HB =
=
2P
⎡
πD ⎢D −
⎣
2
2⎤
D −d ⎥
⎦
(2)(1000 kg)
⎡
(π)(10 mm) ⎢10 mm −
⎣
2
2⎤
(10 mm) − (2.50 mm) ⎥
⎦
= 200.5
(b) This part of the problem calls for us to determine the indentation diameter d which will yield a
300 HB when P = 500 kg. Solving for d from this equation in Table 6.4 gives
d=
=
2
⎡
2P ⎤
D − ⎢D −
(HB)πD ⎥⎦
⎣
2
2
⎡
(2)(500 kg) ⎤
(10 mm)2 − ⎢10 mm −
= 1.45 mm
(300)(π)(10 mm) ⎥⎦
⎣
6.49 This problem calls for estimations of Brinell and Rockwell hardnesses.
(a) For the brass specimen, the stress-strain behavior for which is shown in Figure 6.12, the tensile
strength is 450 MPa (65,000 psi). From Figure 6.19, the hardness for brass corresponding to this
tensile strength is about 125 HB or 70 HRB.
(b) The steel alloy (Figure 6.24) has a tensile strength of about 1970 MPa (285,000 psi). This
corresponds to a hardness of about 560 HB or ~55 HRC from the line (extended) for steels in Figure
6.19.
6.50 This problem calls for us to specify expressions similar to Equations (6.20a) and (6.20b) for nodular
cast iron and brass. These equations, for a straight line, are of the form
TS = C + (E)(HB)
145
where TS is the tensile strength, HB is the Brinell hardness, and C and E are constants, which need
to be determined.
One way to solve for C and E is analytically--establishing two equations from TS and HB
data points on the plot, as
(TS)1 = C + (E)(BH)1
(TS)2 = C + (E)(BH)2
Solving for E from these two expressions yields
E =
(TS)1 − (TS) 2
(HB) − (HB)
2
1
For nodular cast iron, if we make the arbitrary choice of (HB)1 and (HB)2 as 200 and 300,
respectively, then, from Figure 6.19, (TS)1 and (TS)2 take on values of 87,000 psi (600 MPa) and
160,000 psi (1100 MPa), respectively. Substituting these values into the above expression and
solving for E gives
E =
87, 000 psi − 160, 000 psi
= 730 psi/HB (5.0 MPa/HB)
200 HB − 300 HB
Now, solving for C yields
C = (TS)1 - (E)(BH)1
= 87,000 psi - (730 psi/HB)(200 HB) = -59,000 psi (-400 MPa)
Thus, for nodular cast iron, these two equations take the form
TS(psi) = -59,000 + 730 x HB
TS(MPa) = -400 + 5.0 x HB
Now for brass, we take (HB)1 and (HB)2 as 100 and 200, respectively, then, from Figure
6.19, (TS)1 and (TS)2 take on values of 54,000 psi (370 MPa) and 95,000 psi (660 MPa),
respectively. Substituting these values into the above expression and solving for E gives
146
E =
54, 000 psi − 95,000 psi
= 410 psi/HB (2.9 MPa/HB)
100 HB − 200 HB
Now, solving for C yields
C = (TS)1 - (E)(BH)1
= 54,000 psi - (410 psi/HB)(100 HB) = 13,000 psi (80 MPa)
Thus, for brass these two equations take the form
TS(psi) = 13,000 + 410 x HB
TS(MPa) = 80 + 2.9 x HB
6.51 The five factors that lead to scatter in measured material properties are the following: 1) test
method; 2) variation in specimen fabrication procedure; 3) operator bias; 4) apparatus calibration;
and 5) material inhomogeneities and/or compositional differences.
6.52 The average of the given hardness values is calculated using Equation (6.21) as
18
∑HRGi
HRG =
=
i =1
18
47.3 + 52.1 + 45.6 . . . . + 49.7
= 48.4
18
And we compute the standard deviation using Equation (6.22) as follows:
18
∑ (HRGi − HRG)
s =
2
i=1
18 − 1
⎡ (47.3 − 48.4 )2 + (52.1 − 48.4 )2 + . . . . + (49.7 − 48.4)2 ⎤
⎥
=⎢
17
⎢⎣
⎥⎦
147
1/2
64.95
= 1.95
17
=
6.53 The criteria upon which factors of safety are based are 1) consequences of failure, 2) previous
experience, 3) accuracy of measurement of mechanical forces and/or material properties, and 4)
economics.
6.54 The working stresses for the two alloys the stress-strain behaviors of which are shown in Figures
6.12 and 6.24 are calculated by dividing the yield strength by a factor of safety, which we will take to
be 2. For the brass alloy (Figure 6.12), since σy = 250 MPa (36,000 psi), the working stress is 125
MPa (18,000 psi), whereas for the steel alloy (Figure 6.24), σy = 1570 MPa (228,000 psi), and,
therefore, σw = 785 MPa (114,000 psi).
Design Problems
6.D1 For this problem the working stress is computed using Equation (6.24) with N = 2, as
σw =
σy
2
=
860 MPa
= 430 MPa (62, 500 psi )
2
Since the force is given, the area may be determined from Equation (6.1), and subsequently the
original diameter do may be calculated as
Ao =
⎛ do ⎞
F
= π⎜
⎟
σ
⎝ 2 ⎠
w
2
And
do =
4F
πσ
w
=
(
(4)(13,300 N)
π 430 x 106 N/ m 2
)
= 6.3 x 10-3 m = 6.3 mm (0.25 in.)
6.D2 (a) This portion of the problem asks for us to compute the wall thickness of a thin-walled cylindrical
Ni tube at 300&deg;C through which hydrogen gas diffuses. The inside and outside pressures are,
respectively, 1.013 and 0.01013 MPa, and the diffusion flux is to be no greater than 1 x 10-7 mol/m2s. This is a steady-state diffusion problem, which necessitates that we employ Equation (5.3). The
148
concentrations at the inside and outside wall faces may be determined using Equation (6.39), and,
furthermore, the diffusion coefficient is computed using Equation (6.40). Solving for Δx
Δx = −
=
D ΔC
J
1
1 x 10 −7 mol/ m 2 / s
x
⎞
39,560 J/ mol
⎟ x
(4.76 x 10-7 )exp ⎛⎜⎝ − (8.31 J / mol
- K)(300 + 273 K) ⎠
⎞
⎛
12, 300 J / mol
(30.8) exp ⎜ −
⎟
⎝ (8.31 J / mol - K)(300 + 273 K) ⎠
( 1.013
MPa −
0.01013 MPa
)
= 0.0025 m = 2.5 mm
(b) Now we are asked to determine the circumferential stress; from Equation (6.41)
σ =
=
r Δp
4 Δx
(1.013 MPa − 0.01013 MPa)(0.1 m)
(4)(0.0025 m)
= 10 MPa
(c) Now we are to compare this value of stress to the yield strength of Ni at 300&deg;C, from which it is
possible to determine whether or not the 2.5 mm wall thickness is suitable. From the information
given in the problem, we may write an equation for the dependence of yield strength on temperature
as follows:
σ y = 100 MPa − 0.1 MPa (T − 20)
for temperature in degrees Celsius. Thus, at 300&deg;C
σ y = 100 MPa − 0.1 MPa (300 − 20) = 72 MPa
149
Inasmuch as the circumferential stress (10 MPa) is much less than the yield strength (72 MPa), this
thickness is entirely suitable.
(d) And, finally, this part of the problem asks that we specify how much this thickness may be
reduced and still retain a safe design. Let us use a working stress by dividing the yield stress by a
factor of safety, according to Equation (6.24). On the basis of our experience, let us use a value of
2.0 for N. Thus
σw =
σy
N
=
72 MPa
= 36 MPa
2
Using this value for σw and Equation (6.41), we now compute the tube thickness as
Δx =
=
r Δp
4 σw
(0.1 m)(1.013 MPa − 0.01013 MPa)
4(36 MPa)
= 0.0007 m = 0.7 mm
Substitution of this value into Fick's first law [Equation (5.3)] we calculate the diffusion flux as follows:
J = −D
(
= 4.76 x 10
-7
ΔC
Δx
560 J / mol
)exp ⎡⎢⎣− (8.31 J /39,
mol - K)(300 + 273
⎡
⎤
12,300 J / mol
(30.8)exp ⎢ −
⎥
(8.31
J
/
mol
K)(300
+
273
K)
⎣
⎦
0.0007 m
( 1.013
MPa −
⎤
⎥ x
K) ⎦
0.01013 MPa
)
= 3.63 x 10-7 mol/m2-s
Thus, the flux increases by approximately a factor of 3.5, from 1 x 10-7 to 3.63 x 10-7 mol/m2-s with
this reduction in wall thickness.
150
6.D3 This problem calls for the specification of a temperature and cylindrical tube wall thickness that will
give a diffusion flux of 5 x 10-8 mol/m2-s for the diffusion of hydrogen in nickel; the tube radius is
0.125 m and the inside and outside pressures are 2.026 and 0.0203 MPa, respectively. There are
probably several different approaches that may be used; and, of course, there is not one unique
solution. Let us employ the following procedure to solve this problem: 1) assume some wall
thickness, and, then, using Fick's first law for diffusion [which also employs Equations (5.3) and
(5.8)], compute the temperature at which the diffusion flux is that required; 2) compute the yield
strength of the nickel at this temperature using the dependence of yield strength on temperature as
stated in Problem 6.D2; 3) calculate the circumferential stress on the tube walls using Equation
(6.41); and 4) compare the yield strength and circumferential stress values--the yield strength
should probably be at least twice the stress in order to make certain that no permanent deformation
occurs. If this condition is not met then another iteration of the procedure should be conducted with
a more educated choice of wall thickness.
As a starting point, let us arbitrarily choose a wall thickness of 2 mm (2 x 10-3 m). The
steady-state diffusion equation, Equation (5.3), takes the form
J = −D
ΔC
Δx
= 5 x 10-8 mol/m2-s
(
= 4.76 x 10
-7
39,560 J / mol ⎤
⎥
)exp ⎡⎢⎣− (8.31
J / mol - K)(T) ⎦
⎡
12,300 J / mol ⎤
(30.8)exp ⎢ −
⎥ 2.026 MPa −
⎣ (8.31 J / mol - K)(T) ⎦
0.002 m
(
x
0.0203 MPa
)
Solving this expression for the temperature T gives T = 514 K = 241&deg;C.
The next step is to compute the stress on the wall using Equation (6.41); thus
σ =
=
r Δp
4 Δx
(0.125 m)(2.026 MPa − 0.0203 MPa)
(
(4) 2 x 10 −3 m
151
)
= 31.3 MPa
Now, the yield strength of Ni at this temperature may be computed as
σy = 100 MPa - 0.1 MPa (241&deg;C - 20&deg;C) = 77.9 MPa
Inasmuch as this yield strength is greater than twice the circumferential stress, wall thickness and
temperature values of 2 mm and 241&deg;C, respectively, are satisfactory design parameters.
6.D4 (a) This portion of the problem asks for us to determine which of the materials listed in the
database of Appendix B (or contained on the CD-ROM) have torsional strength performance indices
greater than 12.5 (in SI units) and, in addition, shear strengths greater that 300 MPa. To begin, it is
noted in Section 6.13 that the shear yield strength, τy = 0.6σy. On this basis, and given that
2/3
P=
τy
ρ
[Equation (6.33) in the textbook], it follows that
⎛0.6σ ⎞
y⎠
⎝
P=
ρ
2 /3
Thus, the minimum value of the performance index in terms of yield strength value is (12.5)/(0.6)2/3
2/3
τy
= 17.57. When a ratio query is performed on the CD-ROM for
using a minimum value of
ρ
17.57, ten metal alloys are found to satisfy this criterion; these are listed in the table below.
____________________________________________
Alloy
Condition
⎛ 0.6 σ ⎞
y⎠
⎝
ρ
2 /3
σy
____________________________________________
4340 Steel
Q/T, 315&deg;C
17.57
1620
440A Stainless
Q/T, 315&deg;C
17.90
1650
2024 Al
T3
17.75
345
7075 Al
T6
22.64
505
7075 Al
T651
22.64
505
AZ31B Mg
Rolled
20.59
220
AZ31B Mg
Extruded
19.32
200
Ti-5Al-2.5Sn
Annealed
18.59
760
152
Ti-6Al-4V
Annealed
19.94
830
Ti-6Al-4V
Aged
24.10
1103
_____________________________________________
Now, the second criterion calls for the material to have a shear strength greater than 300
MPa. Again, since σy = τy/0.6, the minimum yield strength required is σy = 300 MPa/0.6, or σy =
500 MPa. Values of σy from the database are also given in this table. It is noted that the 2024 Al
and both magnesium alloys are eliminated on the basis of this second criterion.
(b) This portion of the problem calls for us to conduct a cost analysis for these seven remaining
ρ
, relative cost c (as taken from
alloys. Below is given a tabulation of values for
(0.6 σ y )2 / 3
Appendix C), and the product of these two parameters. (It should be noted that no values of c are
given for four of these materials.) The three remaining materials are ranked on the basis of cost,
from least to most expensive.
___________________________________________________
Alloy
Condition
ρ
⎛ 0.6σ ⎞
y⎠
⎝
2/3
c
(c)
ρ
⎛0.6σ ⎞
y⎠
⎝
2/ 3
___________________________________________________
7075 Al
T6
0.0621
13.4
0.832
Ti-6Al-4V
Annealed
0.0705
132
9.31
Ti-5Al-2.5Sn
Annealed
0.0756
157
11.87
Ti-6Al-4V
Aged
0.0583
--
--
4340 Steel
Q/T, 315&deg;C
0.0800
--
--
440A Stain.
Q/T, 315&deg;C
0.0785
--
--
7075 Al
T651
0.0621
--
--
___________________________________________________
Thus, the 7075-T6 aluminum alloy is the overwhelming choice of the three materials for which cost
2 / 3⎤
data are given since it has the lowest value for the (c) ⎣⎡ρ /(0.6σ y )
⎦ product.
6.D5 This problem asks that we conduct a stiffness-to-mass performance analysis on a solid cylindrical
shaft that is subjected to a torsional stress. The stiffness performance index Ps is given as Equation
(6.35) in the textbook:
153
Ps =
G
ρ
in which G is the shear modulus and ρ is the density. Densities for the five materials are tabulated in
Table 6.6.
Shear moduli for the glass- and fiber-reinforced composites were stipulated in the
problem (8.6 and 9.2 GPa, respectively). For the three metal alloys, values of the shear modulus
may be computed using Equation (6.9) and the values of the modulus of elasticity and Poisson's
ratio given in Tables B.2 and B.3 in Appendix B. For example, for the 2024-T6 aluminum alloy
G =
E
2(1 + ν)
72.4 GPa
= 27.2 GPa
2 (1 + 0.33)
=
Values of G for the titanium alloy and 4340 steel are, respectively, 42.5 and 79.6 GPa.
Below are tabulated the density, shear modulus, and stiffness performance index for these
five materials.
___________________________________________________
Material
ρ
G
(Mg/m3)
(GPa)
G
ρ
[(GPa)1/2m3 /Mg]
___________________________________________________
Carbon fiber-reinforced
composite
1.5
9.2
2.02
Aluminum alloy (2024-T6)
2.8
27.2
1.86
Titanium alloy (Ti-6Al-4V)
4.4
42.5
1.48
2.0
8.6
1.47
7.8
79.6
1.14
Glass fiber-reinforced
composite
4340 Steel (oil-quenched
and tempered)
___________________________________________________
Thus, the carbon fiber-reinforced composite has the highest stiffness performance index,
the tempered steel the least.
154
ρ
, and
G
The table shown below contains the reciprocal of the performance index in the first column,
the relative cost ( c ), and the product of these two factors, which provides a comparison of the
relative costs of the materials to be used for this torsional shaft, when stiffness is an important
consideration.
___________________________________________________
ρ
G
Material
[Mg/(GPa)1/2m 3 ]
c
⎛ ρ ⎞
c⎜
⎟
⎝ G⎠
(\$/\$)
⎡
1/2 3 ⎤
(\$/\$) Mg/(GPa) m
⎣
⎦
{
}
___________________________________________________
4340 Steel (oil-quenched
and tempered)
0.877
5
4.39
Aluminum alloy (2024-T6)
0.538
15
8.06
Glass fiber-reinforced
composite
0.680
40
27.2
Carbon fiber-reinforced
composite
0.495
80
39.6
Titanium alloy (Ti-4Al-6V)
0.676
110
74.4
___________________________________________________
Thus, a shaft constructed of the tempered steel would be the least expensive, whereas the most
costly shaft would employ the titanium alloy.
6.D6 (a) This portion of the problem asks that we derive a performance index expression for strength
analogous to Equation (6.33) for a cylindrical cantilever beam that is stressed in the manner shown
in the accompanying figure. The stress on the unfixed end, σ, for an imposed force, F, is given by
the expression [Equation (6.42) in the textbook]
σ =
FLr
I
(6.D1)
where L and r are the rod length and radius, respectively, and I is the moment of inertia; for a
cylinder the expression for I is provided in Figure 12.29:
I=
πr 4
4
155
(6.D2)
Substitution for I into Equation (6.D1) leads to
σ=
4FL
(6.D3)
π r3
Now, the mass m of some given quantity of material is the product of its density (ρ) and volume.
Inasmuch as the volume of a cylinder is just πr2L, then
m = π r 2Lρ
(6.D4)
From this expression, the radius is just
r =
m
πLρ
(6.D5)
Inclusion of Equation (6.D5) into Equation (6.D3) yields
4Fπ 1/ 2L5 / 2ρ3 / 2
σ =
m3/ 2
(6.D6)
And solving for the mass gives
(
)
ρ
2 5 1/ 3
m = 16πF L
σ2/ 3
(6.D7)
To ensure that the beam will not fail, we replace stress in Equation (6.D7) with the yield strength (σy)
divided by a factor of safety (N) as
(
)
2 5 2 1/ 3
m = 16πF L N
ρ
σ2/ 3
y
(6.D8)
Thus, the best materials to be used for this cylindrical cantilever beam when strength is a
ρ
consideration are those having low 2 / 3 ratios. Furthermore, the strength performance index, P, is
σ
y
just the reciprocal of this ratio, or
156
σ2 / 3
y
P =
(6.D9)
ρ
The second portion of the problem asks for an expression for the stiffness performance
index. Let us begin by consideration of Equation (6.43) which relates δ, the elastic deflection at the
unfixed end, to the force (F), beam length (L), the modulus of elasticity (E), and moment of inertia (I)
as
δ =
FL3
3E I
(6.43)
Again, Equation (6.D2) gives an expression for I for a cylinder, which when substituted into Equation
(6.43) yields
δ =
4FL3
(6.D10)
3πEr 4
And, substitution of the expression for r [Equation (6.D5)] into Equation (6.D10), leads to
4FL3
δ =
⎛ m ⎞4
3πE ⎜
⎟
⎝ πLρ ⎠
=
4FL5πρ2
(6.D11)
3Em2
Now solving this expression for the mass m yields
⎛ 4FL5π ⎞
m = ⎜⎜
⎟⎟
⎝ 3δ ⎠
1/2
ρ
E
(6.D12)
Or, for this cantilever situation, the mass of material experiencing a given deflection produced by a
ρ
specific force is proportional to the
ratio for that material. And, finally, the stiffness performance
E
index, P, is just the reciprocal of this ratio, or
157
P =
E
ρ
(6.D13)
(b) Here we are asked to select those metal alloys in the database that have stiffness performance
indices greater than 3.0 (in SI units). (Note: for this performance index of 3.0, density has been
taken in terms of g/cm3 rather than in the SI units of kg/m3.) Seventeen metal alloys satisfy this
criterion; they and their
E / ρ values are listed below, and ranked from highest to lowest value.
__________________________________
Alloy
E
ρ
Condition
__________________________________
AZ31B Mg
Rolled
3.790
AZ31B Mg
Extruded
3.790
AZ91D Mg
As cast
3.706
356.0 Al
As cast, high production
3.163
356.0 Al
As cast, custom
3.163
356.0 Al
T6
3.163
6061 Al
O
3.077
6061 Al
T6
3.077
6061 Al
T651
3.077
2024 Al
O
3.072
2024 Al
T3
3.072
2024 Al
T351
3.072
1100 Al
O
3.065
1100 Al
H14
3.065
7075 Al
O
3.009
7075 Al
T6
3.009
7075 Al
T651
3.009
__________________________________
(c) We are now asked to do a cost analysis on the above alloys. Below are tabulated the
ρ
ratio,
E
the relative material cost ( c ), and the product of these two parameters; also those alloys for which
cost data are provided are ranked, from least to most expensive.
___________________________________________________
158
Alloy
ρ
E
Condition
⎛ ρ ⎞
c⎜
⎟
⎝ E⎠
c
___________________________________________________
AZ91D Mg
As cast
0.2640
5.4
1.43
6061 Al
T6
0.3250
7.6
2.47
356.0 Al
As cast, high production
0.3162
7.9
2.50
6061 Al
T651
0.3250
8.7
2.83
AZ31B Mg
Extruded
0.2640
12.6
3.33
1100 Al
O
0.3263
12.3
4.01
AZ31B Mg
Rolled
0.2640
15.7
4.14
7075 Al
T6
0.3323
13.4
4.45
2024 Al
T3
0.3255
14.1
4.59
356.0 Al
As cast, custom
0.3162
15.7
4.96
356.0 Al
T6
0.3162
16.6
5.25
2024 Al
T351
0.3255
16.2
5.27
1100 Al
H14
0.3263
--
--
2024 Al
O
0.3255
--
--
6061 Al
O
0.3250
--
--
7075 Al
O
0.3323
--
--
7075 Al
T651
0.3323
--
--
___________________________________________________
It is up to the student to select the best metal alloy to be used for this cantilever beam on a stiffnessper-mass basis, including the element of cost, and other relevant considerations.
(d) We are now asked to select those metal alloys in the database that have strength performance
indices greater than 18.0 (in SI units). (Note: for this performance index of 18.0, density has been
taken in terms of g/cm3 rather than in the SI units of kg/m3.) Seven alloys satisfy this criterion; they
3
σ 2/
y
and their
ratios [Equation (6.D9)] are listed below; here they are ranked from highest to
ρ
lowest ratio value.
__________________________________
σ2/ 3
Alloy
y
Condition
ρ
__________________________________
159
Ti-6Al-4V
Soln. treated/aged
24.10
7075 Al
T6
22.65
7075 Al
T651
22.65
AZ31B Mg
Rolled
20.59
Ti-6Al-4V
Annealed
19.94
AZ31B Mg
Extruded
19.32
Ti-5Al-2.5Sn
Annealed
18.59
__________________________________
(e) We are now asked to do a cost analysis on the above alloys. Below are tabulated the
ρ
/3
σ2
y
values, the relative material cost ( c ), and the product of these two parameters; also those alloys for
which cost data are provided are ranked, from least to most expensive.
___________________________________________________
Alloy
Condition
ρ
-2
10
σ2y / 3
c
⎛
⎞
ρ ⎟
⎜
c
⎜ σ2/ 3 ⎟
⎝ y ⎠
___________________________________________________
7075 Al
T6
4.42
13.4
0.592
AZ31B Mg
Extruded
5.18
12.6
0.653
AZ31B Mg
Rolled
4.86
15.7
0.763
Ti-6Al-4V
Soln. treated/aged
4.15
132
5.48
Ti-6Al-4V
Annealed
5.02
132
6.63
Ti-5Al-2.5Sn
Annealed
5.38
157
8.45
7075 Al
T651
4.42
--
--
___________________________________________________
It is up to the student to select the best metal alloy to be used for this cantilever beam on a stiffnessper-mass basis, including the element of cost and any other relevant considerations.
(f) The student should use his or her own discretion in selecting the material to be used for this
application when stiffness- and strength-per-mass, as well as cost are to be considered.
Furthermore, the student should be able to justify the decision.
160
6.D7 (a) This portion of the problem asks that we derive strength and stiffness performance index
expressions analogous to Equations (6.33) and (6.35) for a bar specimen having a square crosssection that is pulled in uniaxial tension along it longitudinal axis.
For stiffness, we begin by consideration of the elongation, Δl, in Equation (6.2) where the
initial length lo is replaced by L. Thus, Equation (6.2) may now be written as
Δl = Lε
(6.D14)
in which ε is the engineering strain. Furthermore, assuming that the deformation is entirely elastic,
Hooke's law, Equation (6.5), is obeyed by this material (i.e., σ = Eε), where σ is the engineering
stress. Thus
Δl = Lε =
Lσ
E
(6.D15)
And, since σ is defined by Equation (6.1) as
σ =
F
Ao
(6.1)
Ao being the original cross-sectional area; in this case Ao = c2. Thus, incorporation of these
relationships into Equation (6.D15) leads to an expression for Δl as
Δl =
LF
Ec2
(6.D16)
The mass of material, m, is just the product of the density, ρ, and the volume of the beam, which
volume is just Lc2; that is
m = ρ Lc2
(6.D17)
Or
2
c =
m
ρL
Substitution for c2 into Equation (6.D16) yields
161
(6.D18)
Δl =
L2Fρ
Em
(6.D19)
And solving for the mass
⎛ L2F ⎞ ρ
⎟⎟
m = ⎜⎜
⎝ Δl ⎠ E
(6.D20)
Thus, the best materials to be used for a light bar that is pulled in tension when stiffness is a
consideration are those having low ρ/E ratios. The stiffness performance index, Ps, is the reciprocal
of this ratio, or
Ps =
E
ρ
(6.D21)
The stress σ imposed on this beam by F may be
Now we will consider rod strength.
determined using Equation (6.1); that is
σ =
F
F
=
Ao c2
(6.D22)
In the stiffness treatment [(Equation (6.D18)] it was shown that c2 = m/ρL, and thus
σ =
FLρ
m
(6.D23)
Now, solving for the mass, m, leads to
m = (FL)
ρ
σ
(6.D24)
And replacement of stress with yield strength, σy, divided by a factor of safety, N
m = (FLN)
ρ
σ
(6.D25)
y
Hence, the best materials to be used for a light bar that is pulled in tension when strength is a
consideration are those having low ρ/σy ratios; and the strength performance index, P, is just the
reciprocal of this ratio, or
162
σ
P =
y
(6.D26)
ρ
(b) Here we are asked to select those metal alloys in the database that have stiffness performance
indices [i.e., E/ρ ratios, Equation (6.D21)] greater than 26.3 (in SI units). (Note: for this performance
index of 26.3, density has been taken in terms of g/cm3 rather than in the SI units of kg/m3.) Twenty
seven metal alloys satisfy this criterion. All of the twenty-one plain carbon and low alloy steels
contained in the database fall into this group, and, in addition several other alloys. These E/ρ ratios
are listed below, and are ranked from highest to lowest value. (All of the twenty one steel alloys
have the same E/ρ ratio, and therefore are entered as a single item in the table.) These materials
are ranked from highest to lowest ratio.
__________________________________
Alloy(s)
E
ρ
Condition
__________________________________
Molybdenum
Sheet/rod
31.31
356.0 Al
As cast, high production
26.91
356.0 Al
As cast, custom
26.91
356.0 Al
T6
26.91
17-7PH stainless
Plate, CR
26.67
17-7PH stainless
Pptn. hardened
26.67
Plain carbon/low
alloy steels
Various
26.37
__________________________________
(c) We are now asked to do a cost analysis on the above alloys. Below are tabulated the ρ/E ratio,
the relative material cost ( c ), and the product of these two parameters; only those alloys in the
previous table for which cost data are given are included in the table; these are ranked, from least to
most expensive.
___________________________________________________
Alloy
Condition
10
-2 ρ
E
c
-2
10
⎛ ρ⎞
c⎜ ⎟
⎝ E⎠
___________________________________________________
1020 steel
Plate, HR
3.79
0.8
3.03
A36 steel
Plate, HR
3.79
1.0
3.79
163
1040 steel
Plate, HR
3.79
1.1
4.17
A36 steel
Angle bar, HR
3.79
1.6
6.06
1020 steel
Plate, CR
3.79
1.6
6.06
1040 steel
Plate, CR
3.79
1.9
7.20
4140 steel
Bar, normalized
3.79
2.6
9.85
4340 steel
Bar, annealed
3.79
3.5
13.3
4140H steel
Round, normalized
3.79
4.2
15.9
4340 steel
Bar, normalized
3.79
4.7
17.8
356.0 Al
Cast, high prod.
3.72
7.9
29.4
17-7PH SS
Plate, CR
3.75
12
45.0
356.0 Al
Cast, custom
3.72
15.7
58.4
356.0 Al
T6
3.72
16.6
61.8
Molybdenum
Sheet/rod
3.19
143
456
___________________________________________________
It is up to the student to select the best metal alloy to be used for this bar pulled in tension on a
stiffness-per-mass basis, including the element of cost and other relevant considerations.
(d) We are now asked to select those metal alloys in the database that have strength performance
indices greater than 100 (in SI units). (Note: for this performance index of 100, density has been
taken in terms of g/cm3 rather than in the SI units of kg/m3.) Eighteen alloys satisfy this criterion;
they and their σy/ρ ratios [per Equation (6.D26)] are listed below; here the ranking is from highest to
lowest ratio value.
164
__________________________________
σ
Alloy
Condition
y
ρ
__________________________________
Ti-6Al-4V
Soln. treated/aged
249
440A stainless
Q/T, 315&deg;C
212
4340 steel
Q/T, 315&deg;C
206
4140 steel
Q/T, 315&deg;C
200
Ti-6Al-4V
Annealed
187
7075 Al
T6
180
7075 Al
T651
180
17-7PH stainless
Pptn. hardened
171
Ti-5Al-2.5Sn
Annealed
170
17-7PH stainless
Plate, CR
158
C17200 Cu
Soln. treated/aged
132
2024 Al
T3
125
AZ31B Mg
Sheet, rolled
124
2024 Al
T351
117
AZ31B Mg
Sheet, extruded
113
4340 steel
Normalized @870&deg;C
110
6061 Al
T6
102
6061 Al
T651
102
__________________________________
(e) We are now asked to do a cost analysis on the above alloys. Below are tabulated the ρ/σy
values, the relative material cost ( c ), and the product of these two parameters; also those alloys for
which cost data are provided are ranked, from least to most expensive.
___________________________________________________
Alloy
Condition
ρ
σ
10-3
c
y
-2
10
⎛
⎞
ρ⎟
c⎜
⎜σ ⎟
⎝ y⎠
___________________________________________________
4340 steel
Normalized @ 870&deg;C
9.09
4.7
4.3
6061 Al
T6
9.80
7.6
7.4
7075 Al
T6
5.56
13.4
7.5
165
17-7PH SS
Plate, CR
6.33
12.0
7.6
6061 Al
T651
9.80
8.7
8.5
AZ31B Mg
Sheet, extruded
8.85
12.6
11.2
2024 Al
T3
8.00
14.1
11.3
AZ31B Mg
Sheet, rolled
8.06
15.7
12.7
2024 Al
T351
8.55
16.2
13.9
C17200 Cu
Soln. treated/aged
7.58
51.4
39.0
Ti-6Al-4V
Soln. treated/aged
4.02
132
53.1
Ti-6Al-4V
Annealed
5.35
132
70.6
Ti-5Al-2.5Sn
Annealed
5.88
157
92.3
440A SS
Q/T, 315&deg;C
4.72
--
--
4340 steel
Q/T, 315&deg;C
4.85
--
--
4140 steel
Q/T, 315&deg;C
5.00
--
--
7075 Al
T651
5.56
--
--
17-7PH SS
Pptn. hardened
5.85
--
--
___________________________________________________
It is up to the student to select the best metal alloy to be used for this bar pulled in tension on a
strength-per-mass basis, including the element of cost and other relevant considerations.
(f) The student should use his or her own discretion in the selection the material to be used for this
application when stiffness- and strength-per-mass, as well as cost are to be considered.
Furthermore, the student should be able to justify the decision.
6.D8 (a) The first portion of this problem asks that we derive a performance index expression for the
strength for a plate that is supported at its ends and subjected to a force that is uniformly distributed
over the upper face. Equation (6.44) in the textbook is an expression for the deflection δ of the
underside of the plate at L/2 in terms of the force F, the modulus of elasticity E, as well as the plate
dimensions as shown in the accompanying figure. This equation is as follows:
δ=
5FL3
32Ewt 3
(6.D27)
Now, the mass m of the plate is the product of its density (ρ) and volume. Inasmuch as the volume
of the plate is Lwt, then
166
(6.D28)
m = Lw tρ
From this expression, the thickness t is just
t =
m
Lw ρ
(6.D29)
Inclusion of Equation (6.D29) into Equation (6.D27) yields
δ=
5FL6 w 2ρ3
(6.D30)
32Em3
And solving for the mass gives
⎛ 5FL6 w 2 ⎞
m = ⎜⎜
⎟⎟
⎝ 32δ ⎠
1/3
ρ
Now, the stiffness performance index P1 is just the reciprocal of the
P1 =
(6.D31)
E 1/ 3
E1/ 3
ρ
ρ
E1/ 3
term of this expression, or
(6.D32)
For determination of the strength performance index, we substitute the expression for t
[Equation (6.D29)] into Equation (6.45) in the textbook, which yields
σ=
3FL3 wρ 2
4m 2
(6.D33)
Now, as in the previous problems, in order to ensure that the plate will not fail, we replace stress in
the previous expression with the yield strength (σy) divided by a factor of safety (N) as
σ
y
N
=
3FL3wρ 2
4m 2
Now solving Equation (6.D34) for the mass
167
(6.D34)
⎛ 3 NFL3w ⎞
m = ⎜⎜
⎟⎟
4
⎝
⎠
1/2
ρ
(6.D35)
σ1/ 2
y
And, finally, the stiffness performance index P2 is the reciprocal of the
ρ
σ1/ 2
y
ratio as
1/ 2
P2 =
σy
(6.D36)
ρ
(b) Here we are asked to select those metal alloys in the database that have stiffness performance
E1/ 3
ratios, Equation (6.D32)] greater than 1.50 (in SI units). (Note: for this
indices [i.e.,
ρ
performance index of 1.50, density has been taken in terms of g/cm3 rather than in the SI units of
1/ 3
E
ratios are listed below.
kg/m3.) Fourteen metal alloys satisfy this criterion. They and their
ρ
Furthermore, these materials are ranked from highest to lowest ratio.
__________________________________
Alloy
E1/ 3
ρ
Condition
__________________________________
AZ31B Mg
Rolled
2.010
AZ31B Mg
Extruded
2.010
AZ91B Mg
As cast
1.965
356.0 Al
Cast, high production
1.549
356.0 Al
As cast, custom
1.549
356.0 Al
T6
1.549
6061 Al
O
1.519
6061 Al
T6
1.519
6061 Al
T651
1.519
1100 Al
O
1.513
1100 Al
H14
1.513
2024 Al
O
1.505
2024 Al
T3
1.505
2024 Al
T351
1.505
__________________________________
168
(c) We are now asked to do a cost analysis on the above alloys. Below are tabulated the
ρ
E1/ 3
ratio, the relative material cost ( c ), and the product of these two parameters; these alloys are
ranked from least to most expensive.
___________________________________________________
Alloy
Condition
ρ
E1/ 3
c
⎛ ρ ⎞
c ⎜ 1/ 3 ⎟
⎝E ⎠
___________________________________________________
AZ91B Mg
As cast
0.509
5.4
2.75
6061 Al
T6
0.658
7.6
5.00
356.0 Al
Cast, high production
0.645
7.9
5.10
6061 Al
T651
0.658
8.7
5.72
AZ31B Mg
Extruded
0.498
12.6
6.27
AZ31B Mg
Rolled
0.498
15.7
7.82
1100 Al
O
0.661
12.3
8.13
2024 Al
T3
0.665
14.1
9.38
356.0 Al
Cast, custom
0.645
15.7
10.13
356.0 Al
T6
0.645
16.6
10.71
2024 Al
T351
0.665
16.2
10.77
1100 Al
H14
0.661
--
--
2024 Al
O
0.665
--
--
6061 Al
O
0.658
--
--
___________________________________________________
It is up to the student to select the best metal alloy to be used for this plate on a stiffness-per-mass
basis, including the element of cost, as well as other relevant considerations.
(d) We are now asked to select those metal alloys in the database that have strength performance
indices greater than 6.0 (in SI units). (Note: for this performance index of 6.0, density has been
taken in terms of g/cm3 rather than in the SI units of kg/m3.) Twelve alloys satisfy this criterion; they
1/ 2
σy
and their
ratios [per Equation (6.D36)] are listed below; here the ranking is from highest to
ρ
lowest ratio value.
169
__________________________________
σ1/ 2
Alloy
y
Condition
ρ
__________________________________
AZ31B Mg
Sheet, rolled
8.380
AZ31B Mg
Sheet, extruded
8.380
7075 Al
T6
8.026
7075 Al
T651
8.026
Ti-6Al-4V
Soln. treated/aged
7.497
2024 Al
T3
6.706
2024 Al
T351
6.508
Ti-6Al-4V
Annealed
6.503
Ti-5Al-2.5Sn
Annealed
6.154
6061 Al
T6
6.153
6061 Al
T651
6.153
AZ91D Mg
As cast
6.104
__________________________________
(e) We are now asked to do a cost analysis on the above alloys. Below are tabulated the
ρ
2
σ1/
y
values, the relative material cost (c ) , and the product of these two parameters; also those alloys for
which cost data are provided are ranked, from least to most expensive.
___________________________________________________
Alloy
Condition
ρ
2
σ1/
y
c
⎛
⎞
ρ ⎟
⎜
c
⎜ σ1 / 2 ⎟
⎝ y ⎠
___________________________________________________
AZ91D Mg
As cast
0.1639
5.4
0.885
6061 Al
T6
0.1625
7.6
1.24
6061 Al
T651
0.1625
8.7
1.41
AZ31B Mg
Sheet, extruded
0.1193
12.6
1.50
7075 Al
T6
0.1246
13.4
1.67
AZ31B Mg
Sheet, rolled
0.1193
15.7
1.87
2024 Al
T3
0.1491
14.1
2.10
2024 Al
T351
0.1537
16.2
2.49
170
Ti-6Al-4V
Soln. treated/aged
0.1334
132
17.61
Ti-6Al-4V
Annealed
0.1538
132
20.30
Ti-5Al-2.5Sn
Annealed
0.1625
157
25.51
7075 Al
T651
0.1246
--
--
___________________________________________________
It is up to the student to select the best metal alloy to be used for this plate on a strength-per-mass
basis, including the element of cost, as well as other relevant considerations.
(f) The student should use his or her own discretion in the selection the material to be used for this
application when stiffness- and strength-per-mass, as well as cost are to be considered.
Furthermore, the student should be able to justify the decision.
171
CHAPTER 7
DISLOCATIONS AND STRENGTHENING MECHANISMS
PROBLEM SOLUTIONS
7.1 The dislocation density is just the total dislocation length per unit volume of material (in this case per
3
5
-2
cubic millimeters). Thus, the total length in 1000 mm of material having a density of 10 mm is
just
(105 mm-2 )(1000
3
mm
)= 108 mm = 105 m = 62
mi
9
-2
Similarly, for a dislocation density of 10 mm , the total length is
(109 mm-2 )(1000 mm3 )= 1012 mm = 10 9 m = 6.2 x 10 5 mi
7.2 When the two edge dislocations become aligned, a planar region of vacancies will exist between the
dislocations as:
7.3 It is possible for two screw dislocations of opposite sign to annihilate one another if their dislocation
lines are parallel. This is demonstrated in the figure below.
172
7.4 For the various dislocation types, the relationships between the direction of the applied shear stress
and the direction of dislocation line motion are as follows:
edge dislocation--parallel
screw dislocation--perpendicular
mixed dislocation--neither parallel nor perpendicular
7.5
(a)
A slip system is a crystallographic plane, and, within that plane, a direction along which
dislocation motion (or slip) occurs.
(b) All metals do not have the same slip system. The reason for this is that for most metals, the slip
system will consist of the most densely packed crystallographic plane, and within that plane the most
closely packed direction. This plane and direction will vary from crystal structure to crystal structure.
7.6 (a) For the FCC crystal structure, the planar density for the (110) plane is given in Equation (3.12) as
PD110 (FCC) =
1
4 R2
2
0.177
=
R2
Furthermore, the planar densities of the (100) and (111) planes are calculated in Homework
Problem 3.47, which are as follows:
1
PD100 (FCC) =
PD111(FCC) =
(b)
4R 2
1
2R 2 3
=
0.25
=
R2
0.29
R2
For the BCC crystal structure, the planar densities of the (100) and (110) planes were
determined in Homework Problem 3.48, which are as follows:
PD100 (BCC) =
PD110 (BCC) =
3
16 R2
3
8R 2
2
=
0.19
=
0.27
R2
R2
Below is a BCC unit cell, within which is shown a (111) plane.
173
(a)
The centers of the three corner atoms, denoted by A, B, and C lie on this plane. Furthermore, the
(111) plane does not pass through the center of atom D, which is located at the unit cell center. The
atomic packing of this plane is presented in the following figure; the corresponding atom positions
from the Figure (a) are also noted.
(b)
Inasmuch as this plane does not pass through the center of atom D, it is not included in the atom
count. One sixth of each of the three atoms labeled A, B, and C is associated with this plane, which
gives an equivalence of one-half atom.
In Figure (b) the triangle with A, B, and C at its corners is an equilateral triangle. And, from
Figure (b), the area of this triangle is xy/2. The triangle edge length, x, is equal to the length of a
face diagonal, as indicated in Figure (a). And its length is related to the unit cell edge length, a, as
x 2 = a 2 + a 2 = 2a 2
174
or
x =a
For BCC, a =
2
4R
, and, therefore,
3
x=
4R
2
3
Also, with respect to the length y we may write
y
3
x
2
2
⎛ x⎞
+⎜ ⎟
⎝ 2⎠
2
=x
2
. And, substitution for the above expression for x yields
y =
x
3
2
⎛ 4R 2 ⎞ ⎛ 3 ⎞
4R 2
=⎜
⎟⎜
⎟ =
2
3 ⎠⎝ 2 ⎠
⎝
Thus, the area of this triangle is equal to
AREA =
1
8R2
⎛ 1 ⎞ ⎛ 4R 2 ⎞ ⎛ 4 R 2 ⎞
xy = ⎜ ⎟⎜
⎟⎜
⎟ =
2
⎝ 2⎠ ⎝
3 ⎠⎝ 2 ⎠
3
And, finally, the planar density for this (111) plane is
PD111(BCC) =
0.5 atom
8R 2
=
3
16R2
=
0.11
R2
3
7.7 Below is shown the atomic packing for a BCC {110} type plane. The arrows indicate two different
&lt;111&gt; type directions.
175
7.8 Below is shown the atomic packing for an HCP {0001} type plane. The arrows indicate three
different &lt; 11 20 &gt; type directions.
7.9
Resolved shear stress is the shear component of an applied tensile (or compressive) stress
resolved along a slip plane that is other than perpendicular or parallel to the stress axis. The critical
resolved shear stress is the value of resolved shear stress at which yielding begins; it is a property
of the material.
7.10 We are asked to compute the Schmid factor for an FCC crystal oriented with its  direction
parallel to the loading axis. With this scheme, slip may occur on the (111) plane and in the [1 1 0]
direction as noted in the figure below.
The angle between the  and [1 1 0] directions, λ, is 45&deg;. For the (111) plane, the angle
⎛a 2⎞
between its normal (which is the  direction) and the  direction, φ, is tan-1 ⎜
⎟ = 54.74&deg;,
⎝ a ⎠
therefore
176
cos λ cos φ = cos(45&deg;)cos(54.74&deg;) = 0.408
7.11 This problem calls for us to determine whether or not a metal single crystal having a specific
orientation and of given critical resolved shear stress will yield. We are given that φ = 60&deg;, λ = 35&deg;,
and that the values of the critical resolved shear stress and applied tensile stress are 6.2 MPa (900
psi) and 12 MPa (1750 psi), respectively. From Equation (7.1)
τ R = σ cos φ cos λ = (12 MPa)(cos 60&deg;)(cos 35&deg;) = 4.91 MPa
(717 psi)
Since the resolved shear stress (4.91 MPa) is less that the critical resolved shear stress (6.2 MPa),
the single crystal will not yield.
However, from Equation (7.3), the stress at which yielding occurs is
σy =
cos φ cos λ
=
6.2 MPa
(cos 60&deg;)(cos 35&deg;)
= 15.1MPa (2200 psi)
7.12 We are asked to compute the critical resolved shear stress for Zn. As stipulated in the problem, φ =
65&deg;, while possible values for λ are 30&deg;, 48&deg;, and 78&deg;.
(a) Slip will occur along that direction for which (cos φ cos λ) is a maximum, or, in this case, for the
largest cos λ. The cosines for the possible λ values are given below.
cos(30&deg;) = 0.87
cos(48&deg;) = 0.67
cos(78&deg;) = 0.21
Thus, the slip direction is at an angle of 30&deg; with the tensile axis.
(b) From Equation (7.3), the critical resolved shear stress is just
τ crss = σ y (cos φ cos λ)max
= (2.5 MPa)[cos(65&deg;)cos(30&deg;)] = 0.90 MPa (130 psi)
7.13 This problem asks that we compute the critical resolved shear stress for silver. In order to do this,
we must employ Equation (7.3), but first it is necessary to solve for the angles λ and φ from the
sketch below.
177
If the unit cell edge length is a, then
λ = tan
-1 ⎛ a ⎞
⎜ ⎟ = 45&deg;
⎝ a⎠
For the angle φ, we must examine the triangle OAB. The length of line OA is just a, whereas, the
length of AB is a 2 . Thus,
φ = tan
-1 ⎛ a 2 ⎞
⎜
⎟ = 54.7&deg;
⎝ a ⎠
And, finally
τ crss = σ y (cos φ cos λ)
= (1.1 MPa) [cos(54.7&deg;)cos(45&deg;)] = 0.45 MPa (65.4 psi)
7.14 This problem asks that, for a metal that has the FCC crystal structure, we compute the applied
stress(s) that are required to cause slip to occur on a (111) plane in each of the [1 1 0 ] , [10 1 ] , and
[0 1 1] directions. In order to solve this problem it is necessary to employ Equation (7.3), which
means that we will need to solve for the for angles λ and φ for the three slip systems.
In the sketch below is shown the unit cell and (111)- [1 1 0 ] slip configuration.
178
The angle between the  and [1 1 0] directions, λ, is 45&deg;. For the (111) plane, the angle between
⎛a 2⎞
its normal (which is the  direction) and the  direction, φ, is tan-1 ⎜
⎟ = 54.7&deg;, therefore,
⎝ a ⎠
solving for the yield strength from Equation (7.3)
σy =
=
(cos φ cosλ)
0.5 MPa
0.5 MPa
=
= 1.22 MPa
cos (54.7&deg;) cos(45&deg;) (0.578)(0.707)
The (111)- [10 1 ] slip configuration is represented in the following sketch.
179
For this situation values for λ and φ are the same as for the previous situation—i.e., λ = 45&deg; and φ =
54.7&deg;. This means that the yield strength for this slip system is the same as for (111)- [1 1 0 ] ; that is
σy = 1.22 MPa.
The unit cell and final (111)- [0 1 1] slip system are presented in the following illustration.
In this case, φ has the same value as previously (i.e., 54.7&deg;); however the value for λ is 90&deg;. Thus,
the yield strength for this configuration is
σy =
=
(cos φ cosλ)
0.5 MPa
0.5 MPa
=
=∞
cos (54.7&deg;) cos(90&deg;) (0.578)(0)
which means that slip will not occur on this (111)- [0 1 1] slip system.
7.15 This problem asks, for a BCC metal, that we compute the applied stress(s) that are required to
cause slip to occur in the [1 1 1] direction on each of the (110), (011), and (10 1 ) planes. In order to
solve this problem it is necessary to employ Equation (7.3), which means that we need to solve for
the for angles λ and φ for the three slip systems.
In the sketch below is shown the unit cell and the (110)- [1 1 1] slip configuration.
180
The angle φ between the [1 1 1] slip direction and the normal to the (110) plane (i.e., the 
direction) is 45&deg;. Now, in order to determine the angle between the [1 1 1] direction and the 
direction (i.e., the direction of stress application), λ, we consult the illustration of this same unit cell
as shown below.
For the triangle ABC, the angle λ is equal to tan
edge length a. From triangle ABD, A B = a
−1 ⎛ A B ⎞
⎜
⎟ . The length B C is equal to the unit cell
⎝ BC⎠
⎛a 2⎞
2 , and, therefore, λ = ⎜
⎟ = 54.7&deg;. And, solving
⎝ a ⎠
for the resolved shear stress from Equation (7.1)
τ R = σ cos φ cos λ
= (4.0 MPa)[cos(45&deg;)cos(54.7&deg;)] = (4.0 MPa)(0.707)(0.578) = 1.63 MPa
The (011)- [1 1 1] slip configuration is represented in the following sketch.
181
In this case, λ has the same value as previously (i.e., 54.7&deg;); however the value for φ is 90&deg;. Thus,
the resolved shear stress for this configuration is
τ R = σ cos φ cos λ
= (4.0 MPa)[cos(90&deg;)cos(54.7&deg;)] = (4.0 MPa)(0)(0.578) = 0 MPa
And, finally the (10 1 ) - [1 1 1] slip configuration is shown below.
Here, the value of φ is 45&deg;, which again leads to
τ R = σ cos φ cos λ
= (4.0 MPa)[cos(45&deg;)cos(54.7&deg;)] = (4.0 MPa)(0.707)(0.578) = 1.63 MPa
182
(b) The most favored slip system(s) is (are) the one(s) that has (have) the largest τ R value. Both
(110)- [1 1 1] and (10 1 ) - [1 1 1] slip systems are most favored since they have the same τ R (1.63
MPa), which is larger than the τ R value for (011)- [1 1 1] (viz., 0 MPa).
7.16 In order to determine the maximum possible yield strength for a single crystal of Cu pulled in
tension, we simply employ Equation (7.4) as
σ y = 2τcrss = (2)(0.48 MPa) = 0.96 MPa (140 psi)
7.17W Four major differences between deformation by twinning and deformation by slip are as follows:
1) with slip deformation there is no crystallographic reorientation, whereas with twinning there is a
reorientation; 2) for slip, the atomic displacements occur in atomic spacing multiples, whereas for
twinning, these displacements may be other than by atomic spacing multiples; 3) slip occurs in
metals having many slip systems, whereas twinning occurs in metals having relatively few slip
systems;
and 4) normally slip results in relatively large deformations, whereas only small
deformations result for twinning.
7.18 Small-angle grain boundaries are not as effective in interfering with the slip process as are highangle grain boundaries because there is not as much crystallographic misalignment in the grain
boundary region for small-angle, and therefore not as much change in slip direction.
7.19 Hexagonal close packed metals are typically more brittle than FCC and BCC metals because there
are fewer slip systems in HCP.
7.20 These three strengthening mechanisms are described in Sections 7.8, 7.9, and 7.10.
7.21 (a) Perhaps the easiest way to solve for σo and k in Equation (7.5) is to pick two values each of
y
-1/2
σy and d
from Figure 7.13, and then set up and solve two simultaneous equations. For example
d-1/2 (mm)-1/2
σy (MPa)
4
75
12
175
The two equations are thus
75 = σ o + 4ky
183
175 = σ o + 12k y
These yield the values of
[
k y = 12.5 MPa (mm)1/2 1810 psi(mm)1/ 2
]
σo = 25 MPa (3630 psi)
-1/2
-3
-1/2
= 31.6 mm
, and, using Equation (7.5),
(b) When d = 1.0 x 10 mm, d
σ y = σo + k y d
[
= (25 MPa) + 12.5 MPa (mm)
1/ 2
-1/2
](31.6 mm )= 420 MPa
-1/2
(61,000 psi)
7.22 We are asked to determine the grain diameter for an iron which will give a yield strength of 205 MPa
(30,000 psi). The best way to solve this problem is to first establish two simultaneous expressions of
Equation (7.5), solve for σo and k , and finally determine the value of d when σy = 205 MPa. The
y
data pertaining to this problem may be tabulated as follows:
σy
d (mm)
135 MPa
260 MPa
d-1/2 (mm)-1/2
-2
5 x 10
-3
8 x 10
4.47
11.18
The two equations thus become
135 MPa = σ o + (4.47) k y
260 MPa = σo + (11.18) k y
Which yield the values, σo = 51.7 MPa and k = 18.63 MPa(mm)
y
[
1/2
. At a yield strength of 205 MPa
205 MPa = 51.7 MPa + 18.63 MPa(mm)
-1/2
-2
-1/2
= 8.23 (mm)
, which gives d = 1.48 x 10 mm.
or d
184
1/2
]d
-1/2
7.23 This problem asks that we determine the grain size of the brass which is the subject of Figure 7.17.
From Figure 7.17(a), the yield strength of brass at 0%CW is approximately 175 MPa (26,000 psi).
-1/2
-1/2
This yield strength from Figure 7.13 corresponds to a d
value of approximately 12.0 (mm)
.
-3
Thus, d = 6.9 x 10 mm.
7.24 Below is shown an edge dislocation and the location where an interstitial impurity atom would be
situated. Compressive lattice strains are introduced by the impurity atom. There will be a net
reduction in lattice strain energy when these lattice strains partially cancel tensile strains associated
with the edge dislocation; such tensile strains exist just below the bottom of the extra half-plane of
atoms (Figure 7.4).
7.25
The hardness measured from an indentation that is positioned very close to a preexisting
indentation will be high. The material in this vicinity was cold-worked when the first indentation was
7.26 (a) We are asked to show, for a tensile test, that
⎛ ε ⎞
%CW = ⎜
⎟ x 100
⎝ ε + 1⎠
From Equation (7.6)
⎡A − A ⎤
⎡
A ⎤
d
%CW = ⎢ o
⎥ x 100 = ⎢1 − d ⎥ x 100
A ⎥⎦
⎢⎣ A o ⎥⎦
⎢⎣
o
Which is also equal to
185
⎡
l ⎤
⎢1 − o ⎥ x 100
l ⎦⎥
⎢⎣
d
since A /A = lo/ld, the conservation of volume stipulation in the problem. Now, from the definition
d o
of engineering strain [Equation (6.2)]
l − lo
ε= d
=
lo
ld
lo
−1
Or,
lo
ld
=
1
ε+1
Substitution in the %CW expression above gives
⎡
l ⎤
⎡
⎡ ε ⎤
1 ⎤
%CW = ⎢1 − o ⎥ x 100 = ⎢1 −
x 100 = ⎢
⎥
⎥ x 100
ld ⎥⎦
ε + 1⎦
⎣
⎣ ε + 1⎦
⎢⎣
(b) From Figure 6.12, a stress of 415 MPa (60,000 psi) corresponds to a strain of 0.16. Using the
above expression
⎡ ε ⎤
⎡
⎤
0.16
%CW = ⎢
⎥ x 100 = ⎢
⎥ x 100 = 13.8%CW
⎣ ε + 1⎦
⎣ 0.16 + 1.00 ⎦
7.27 In order for these two cylindrical specimens to have the same deformed hardness, they must be
deformed to the same percent cold work. For the first specimen
2
%CW =
2
π ro − πrd
x 100 =
x 100
A
πr 2
o
o
=
π (15 mm)2 − π(12 mm)2
π (15 mm)2
x 100 = 36%CW
For the second specimen, the deformed radius is computed using the above equation and solving
for rd as
186
rd = ro 1 −
= (11 mm) 1 −
%CW
100
36%CW
= 8.80 mm
100
7.28 We are given the original and deformed cross-sectional dimensions for two specimens of the same
metal, and are then asked to determine which is the hardest after deformation.
The hardest
specimen will be the one that has experienced the greatest degree of cold work. Therefore, all we
need do is to compute the %CW for each specimen using Equation (7.6). For the circular one
%CW = ⎢ o
⎥ x 100
Ao
⎢⎣
⎥⎦
2
⎡ ⎛ 15.2 mm ⎞ 2
⎛ 11.4 mm ⎞ ⎤
⎢π⎜
⎟ − π⎜
⎟ ⎥
⎝
⎠
⎝
⎠ ⎥
2
2
x 100 = 43.8%CW
=⎢
2
⎢
⎥
15.2 mm ⎞
⎛
⎢
⎥
⎟
π⎜
⎝
⎠
2
⎣
⎦
For the rectangular one
⎡ (125 mm)(175 mm) − (75 mm)(200 mm) ⎤
%CW = ⎢
⎥ x 100 = 31.4%CW
(125 mm)(175 mm)
⎣
⎦
Therefore, the deformed circular specimen will be harder.
7.29 This problem calls for us to calculate the precold-worked radius of a cylindrical specimen of copper
that has a cold-worked ductility of 25%EL. From Figure 7.17(c), copper that has a ductility of 25%EL
will have experienced a deformation of about 11%CW. For a cylindrical specimen, Equation (7.6)
becomes
⎡ πr 2 − πr 2 ⎤
o
d⎥
x 100
%CW = ⎢
⎢⎣
⎥⎦
π ro2
Since r = 10 mm (0.40 in.), solving for r yields
d
o
187
ro =
rd
=
%CW
1−
100
10 mm
11.0
1−
100
= 10.6 mm (0.424 in.)
7.30 (a) We want to compute the ductility of a brass that has a yield strength of 275 MPa (40,000 psi).
In order to solve this problem, it is necessary to consult Figures 7.17(a) and (c). From Figure
7.17(a), a yield strength of 275 MPa for brass corresponds to 10%CW. A brass that has been coldworked 10% will have a ductility of about 44%EL [Figure 7.17(c)].
(b) This portion of the problem asks for the Brinell hardness of a 1040 steel having a yield strength
of 690 MPa (100,000 psi). From Figure 7.17(a), a yield strength of 690 MPa for a 1040 steel
corresponds to about 11%CW. A 1040 steel that has been cold worked 11% will have a tensile
strength of about 790 MPa [Figure 7.17(b)]. Finally, using Equation (6.20a)
HB =
TS (MPa) 790 MPa
=
= 230
3.45
3.45
7.31 We are asked in this problem to compute the critical resolved shear stress at a dislocation density
6
-2
of 10 mm . It is first necessary to compute the value of the constant A from the one set of data as
A =
0.69 MPa − 0.069 MPa
−3
=
= 6.21 x 10 MPa − mm (0.90 psi − mm)
4
−2
ρ
10 mm
D
6
-2
Now, the critical resolved shear stress may be determined at a dislocation density of 10 mm as
τ crss = τ o + A ρD
(
= (0.069 MPa) + 6.21 x 10
-3
) 106 mm−2 = 6.28 MPa (910 psi)
MPa - mm
7.32 For recovery, there is some relief of internal strain energy by dislocation motion; however, there are
virtually no changes in either the grain structure or mechanical characteristics.
During
recrystallization, on the other hand, a new set of strain-free grains forms, and the material becomes
softer and more ductile.
7.33 We are asked to estimate the fraction of recrystallization from the photomicrograph in Figure 7.19c.
Below is shown a square grid onto which is superimposed the recrystallized regions from the
188
micrograph. Approximately 400 squares lie within the recrystallized areas, and since there are 672
total squares, the specimen is about 60% recrystallized.
7.34
During cold-working, the grain structure of the metal has been distorted to accommodate the
deformation.
Recrystallization produces grains that are equiaxed and smaller than the parent
grains.
7.35 Metals such as lead and tin do not strain harden at room temperature because their recrystallization
temperatures lie below room temperature (Table 7.2).
7.36 (a) The driving force for recrystallization is the difference in internal energy between the strained
and unstrained material.
(b) The driving force for grain growth is the reduction in grain boundary energy as the total grain
boundary area decreases.
7.37 In this problem, we are asked for the length of time required for the average grain size of a brass
material to increase a specified amount using Figure 7.23.
(a) At 500&deg;C, the time necessary for the average grain diameter to increase from 0.01 to 0.1 mm is
approximately 3500 min.
(b) At 600&deg;C the time required for this same grain size increase is approximately 150 min.
7.38 (a) Using the data given and Equation (7.7) and taking n = 2, we may set up two simultaneous
equations with d and K as unknowns; thus
o
189
(3.9 x 10 -2 mm) − d2o = (30 min)K
2
(6.6 x 10-2 mm) − d2o = (90 min)K
2
Solution of these expressions yields a value for d , the original grain diameter, of
o
do = 0.01 mm,
Also
K = 4.73 x 10-5 mm2/min
(b) At 150 min, the diameter is computed as
d=
=
d2
o + Kt
(
)
(0.01 mm) 2 + 4.73 x 10−5 mm 2 / min (150 min) = 0.085 mm
7.39 Yes, it is possible to reduce the average grain diameter of an undeformed alloy specimen from
0.050 mm to 0.020 mm. In order to do this, plastically deform the material at room temperature (i.e.,
cold work it), and then anneal it at an elevated temperature in order to allow recrystallization and
some grain growth to occur until the average grain diameter is 0.020 mm.
7.40 (a) The temperature dependence of grain growth is incorporated into the constant K in Equation
(7.7).
(b) The explicit expression for this temperature dependence is of the form
⎛ Q⎞
⎟
K = K o exp ⎜ −
⎝ RT ⎠
in which Ko is a temperature-independent constant, the parameter Q is an activation energy, and R
and T are the gas constant and absolute temperature, respectively.
7.41 This problem calls for us to calculate the yield strength of a brass specimen after it has been heated
to an elevated temperature at which grain growth was allowed to occur; the yield strength was given
at a grain size of 0.01 mm. It is first necessary to calculate the constant ky in Equation (7.5) as
190
ky =
=
σy − σo
d -1/2
150 MPa − 25 MPa
−1/ 2
(0.01 mm)
= 12.5 MPa - mm1/ 2
Next, we must determine the average grain size after the heat treatment. From Figure 7.23 at 500&deg;C
after 1000 s (16.7 min) the average grain size of a brass material is about 0.016 mm. Therefore,
calculating σy at this new grain size using Equation (7.5) we get
-1/2
σ y = σo + k y d
(
1/2
= 25 MPa + 12.5 MPa - mm
)(0.016
-1/2
mm)
= 124 MPa (18,000 psi)
Design Problems
7.D1 This problem calls for us to determine whether or not it is possible to cold work steel so as to give a
minimum Brinell hardness of 240 and a ductility of at least 15%EL. According to Figure 6.19, a
Brinell hardness of 240 corresponds to a tensile strength of 800 MPa (116,000 psi). Furthermore,
from Figure 7.17(b), in order to achieve a tensile strength of 800 MPa, deformation of at least
13%CW is necessary. Finally, if we cold work the steel to 13%CW, then the ductility is 15%EL from
Figure 7.17(c). Therefore, it is possible to meet both of these criteria by plastically deforming the
steel.
7.D2 We are asked to determine whether or not it is possible to cold work brass so as to give a minimum
Brinell hardness of 150 and at the same time a ductility of at least 20%EL. According to Figure 6.19,
a Brinell hardness of 150 corresponds to a tensile strength of 500 MPa (72,000 psi.) Furthermore,
from Figure 7.17(b), in order to achieve a tensile strength of 500 MPa, deformation of at least
36%CW is necessary. Finally, if we are to achieve a ductility of at least 20%EL, then a maximum
deformation of 23%CW is possible from Figure 7.17(c). Therefore, it is not possible to meet both of
these criteria by plastically deforming brass.
7.D3 (a) For this portion of the problem we are to determine the ductility of cold-worked steel that has a
Brinell hardness of 240. From Figure 6.19, a Brinell hardness of 240 corresponds to a tensile
191
strength of 820 MPa (120,000 psi), which, from Figure 7.17(b), requires a deformation of 17%CW.
Furthermore, 17%CW yields a ductility of about 13%EL for steel, Figure 7.17(c).
(b) We are now asked to determine the radius after deformation if the uncold-worked radius is 10
mm (0.40 in.). From Equation (7.6) and for a cylindrical specimen
⎡ πr 2 − πr 2 ⎤
o
d⎥
⎢
x 100
%CW =
⎢⎣
⎥⎦
πro2
Now, solving for rd from this expression, we get
rd = ro 1 −
= (10 mm) 1 −
%CW
100
17
= 9.11 mm (0.364 in.)
100
7.D4 This problem asks us to determine which of copper, brass, and a 1040 steel may be cold-worked
so as to achieve a minimum yield strength of 345 MPa (50,000 psi) while maintaining a minimum
ductility of 20%EL. For each of these alloys, the minimum cold work necessary to achieve the yield
strength may be determined from Figure 7.17(a), while the maximum possible cold work for the
ductility is found in Figure 7.17(c). These data are tabulated below.
Yield Strength
Ductility
(&gt; 345 MPa)
(&gt; 20%EL)
Steel
Any %CW
&lt; 5%CW
Brass
&gt; 20%CW
&lt; 23%CW
Copper
&gt; 54%CW
&lt; 15%CW
Thus, both the 1040 steel and brass are possible candidates since for these alloys there is an
overlap of percents coldwork to give the required minimum yield strength and ductility values.
7.D5 This problem calls for us to explain the procedure by which a cylindrical rod of steel may be
deformed so as to produce a given final diameter, as well as a specific tensile strength and ductility.
First let us calculate the percent cold work and attendant tensile strength and ductility if the drawing
is carried out without interruption. From Equation (7.6)
192
2
%CW =
=
⎛ 15.2 mm ⎞
π⎜
⎟
⎝
⎠
2
⎛ do ⎞
⎛ dd ⎞
π⎜
⎟ − π⎜
⎟
⎝ 2 ⎠
⎝ 2 ⎠
⎛ do ⎞
π⎜
⎟
⎝ 2 ⎠
2
x 100
2
⎛ 10 mm ⎞
− π⎜
⎟
⎝
2 ⎠
⎛ 15.2 mm ⎞
π⎜
⎟
⎝
⎠
2
2
2
2
x 100 = 56%CW
At 56%CW, the steel will have a tensile strength on the order of 920 MPa (133,000 psi) [Figure
7.17(b)], which is adequate; however, the ductility will be less than 10%EL [Figure 7.17(c)], which is
insufficient.
Instead of performing the drawing in a single operation, let us initially draw some fraction of
the total deformation, then anneal to recrystallize, and, finally, cold-work the material a second time
in order to achieve the final diameter, tensile strength, and ductility.
Reference to Figure 7.17(b) indicates that 20%CW is necessary to yield a tensile strength of
840 MPa (122,000 psi). Similarly, a maximum of 21%CW is possible for 12%EL [Figure 7.17(c)].
The average of these extremes is 20.5%CW. If the final diameter after the first drawing is d o' , then
2
20.5%CW =
⎛ ' ⎞
d
10 mm ⎞ 2
π ⎜ o ⎟ − π ⎛⎜
⎟
⎜ 2 ⎟
⎝
2 ⎠
⎝
⎠
⎛ ' ⎞2
d
π⎜ o ⎟
⎜ 2 ⎟
⎝
⎠
x 100
And, solving for d o' , yields d o' = 11.2 mm (0.45 in.).
7.D6 Let us first calculate the percent cold work and attendant yield strength and ductility if the drawing is
carried out without interruption. From Equation (7.6)
2
%CW =
⎛ do ⎞
⎛ dd ⎞
π⎜
⎟ − π⎜
⎟
⎝ 2 ⎠
⎝ 2 ⎠
⎛ do ⎞
π⎜
⎟
⎝ 2 ⎠
193
2
2
x 100
=
⎛ 10.2 mm ⎞
⎟
π⎜
⎝
⎠
2
2
2
⎛ 7.6 mm ⎞
⎟
− π⎜
⎝
⎠
2
⎛ 10.2 mm ⎞
⎟
π⎜
2
⎝
⎠
2
x 100 = 44.5%CW
At 44.5%CW, the brass will have a yield strength on the order of 420 MPa (61,000 psi), Figure
7.17(a), which is adequate; however, the ductility will be about 5%EL, Figure 7.17(c), which is
insufficient.
Instead of performing the drawing in a single operation, let us initially draw some fraction of
the total deformation, then anneal to recrystallize, and, finally, cold work the material a second time
in order to achieve the final diameter, yield strength, and ductility.
Reference to Figure 7.17(a) indicates that 26%CW is necessary to give a yield strength of
380 MPa. Similarly, a maximum of 27.5%CW is possible for 15%EL [Figure 7.17(c)]. The average
of these two values is 26.8%CW, which we will use in the calculations. If the final diameter after the
first drawing is d o' , then
26.8%CW =
⎛d' ⎞
π⎜ o⎟
⎜ 2 ⎟
⎝ ⎠
2
⎛ 7.6 mm ⎞
− π⎜
⎟
⎝
2 ⎠
⎛ d' ⎞
π⎜ o⎟
⎜ 2 ⎟
⎝
⎠
2
2
x 100
And, solving for d o' yields d o' = 9.4 mm (0.37 in.).
7.D7 This problem calls for us to cold work some brass stock that has been previously cold worked in
order to achieve minimum tensile strength and ductility values of 450 MPa (65,000 psi) and 13%EL,
respectively, while the final diameter must be 12.7 mm (0.50 in.). Furthermore, the material may not
be deformed beyond 65%CW. Let us start by deciding what percent coldwork is necessary for the
minimum tensile strength and ductility values, assuming that a recrystallization heat treatment is
possible. From Figure 7.17(b), at least 27%CW is required for a tensile strength of 450 MPa.
Furthermore, according to Figure 7.17(c), 13%EL corresponds a maximum of 30%CW. Let us take
the average of these two values (i.e., 28.5%CW), and determine what previous specimen diameter
is required to yield a final diameter of 12.7 mm. For cylindrical specimens, Equation (7.6) takes the
form
194
2
%CW =
⎛ do ⎞
⎛ dd ⎞
π⎜
⎟ − π⎜
⎟
⎝ 2 ⎠
⎝ 2 ⎠
⎛ do ⎞
π⎜
⎟
⎝ 2 ⎠
2
x 100
2
Solving for the original diameter do yields
do =
dd
1−
%CW
12.7 mm
=
1 − 0.285
= 15.0 mm
(0.591 in.)
100
Now, let us determine its undeformed diameter realizing that a diameter of 19.0 mm
corresponds to 35%CW. Again solving for do using the above equation and assuming dd = 19.0
mm yields
do =
dd
1−
%CW
=
19.0 mm
1 − 0.35
= 23.6 mm
(0.930 in.)
100
At this point let us see if it is possible to deform the material from 23.6 mm to 15.0 mm without
exceeding the 65%CW limit. Again employing Equation (7.6)
%CW =
⎛ 23.6 mm ⎞
⎟
π⎜
⎝
⎠
2
2
⎛ 15.0 mm ⎞
⎟
− π⎜
⎝
⎠
2
⎛ 23.6 mm ⎞
⎟
π⎜
2
⎝
⎠
2
2
x 100 = 59.6%CW
In summary, the procedure which can be used to produce the desired material would be as
follows: cold work the as-received stock to 15.0 mm (0.591 in.), heat treat it to achieve complete
recrystallization, and then cold work the material again to 12.7 mm (0.50 in.), which will give the
desired tensile strength and ductility.
195
CHAPTER 8
FAILURE
PROBLEM SOLUTIONS
8.1 Several situations in which the possibility of failure is part of the design of a component or product
are as follows: (1) the pull tab on the top of aluminum beverage cans; (2) aluminum utility/light
poles that reside along freeways--a minimum of damage occurs to a vehicle when it collides with the
pole; and (3) in some machinery components, shear pin are used to connect a gear or pulley to a
shaft--the pin is designed shear off before damage is done to either the shaft or gear in an overload
situation.
8.2W The theoretical cohesive strength of a material is just E/10, where E is the modulus of elasticity.
For the ceramic materials listed in Table 12.5, all we need do is divide E by 10, and therefore
Si3N4--30.4 GPa (4.4 x 106 psi)
ZrO2--20.5 GPa (3.0 x 106 psi)
SiC--34.5 GPa (5.0 x 106 psi)
Al2O3--39.3 GPa (5.7 x 106psi)
Glass ceramic--12.0 GPa (1.7 x 106 psi)
Mullite--14.5 GPa (2.1 x 106 psi)
MgAl2O4--26 GPa (3.8 x 106 psi)
MgO--22.5 GPa (3.3 x 106 psi)
Fused silica--7.3 GPa (1.1 x 106 psi)
Soda-lime glass--6.9 GPa (1.0 x 106 psi )
8.3 This problem asks that we compute the magnitude of the maximum stress that exists at the tip of an
internal crack. Equation (8.1) is employed to solve this problem, as
⎛ a⎞
σm = 2 σo ⎜⎜ ⎟⎟
⎝ ρt ⎠
196
1/ 2
⎡ 2.5 x 10 −2 mm ⎤
⎢
⎥
2
⎥
= (2)(170 MPa) ⎢
⎢ 2.5 x 10 −4 mm ⎥
⎢⎣
⎥⎦
1/2
= 2404 MPa
(354,000 psi)
8.4 In order to estimate the theoretical fracture strength of this material it is necessary to calculate σm
using Equation (8.1) given that σo = 1035 MPa, a = 0.5 mm, and ρt = 5 x 10-3 mm. Thus,
σm = 2σ o
= (2)(1035 MPa)
0.5 mm
5 x 10 −3 mm
a
ρt
= 2.07 x 104 MPa = 207 GPa
(3 x 106 psi)
8.5 In order to determine whether or not this ceramic material will fail we must compute its theoretical
fracture (or cohesive) strength; if the maximum strength at the tip of the most severe flaw is greater
than this value then fracture will occur--if less than, then there will be no fracture. The theoretical
fracture strength is just E/10 or 25 GPa (3.63 x 106 psi), inasmuch as E = 250 GPa (36.3 x 106 psi).
The magnitude of the stress at the most severe flaw may be determined using Equation
(8.1) as
σm = 2σ o
= (2)(750 MPa)
a
ρt
(0.20 mm) / 2
= 15 GPa
0.001 mm
(2.2 x 106 psi)
Therefore, fracture will not occur since this value is less than E/10.
8.6 We may determine the critical stress required for the propagation of an internal crack in aluminum
oxide using Equation (8.3); taking the value of 393 GPa (Table 12.5) as the modulus of elasticity, we
get
σc =
2Eγ s
197
πa
(
9
2
(2) 393 x 10 N/ m
=
)(0.90 N/ m) = 33.6 x 106 N/m 2 = 33.6 MPa
⎛ 4 x 10 −4 m ⎞
(π) ⎜⎜
⎟⎟
2
⎝
⎠
8.7 The maximum allowable surface crack length for MgO may be determined using Equation (8.3);
taking the value of 225 GPa as the modulus of elasticity (Table 12.5), and solving for a, leads to
a=
2Eγ s
π σ2
c
(
)(1.0 N/ m)
6
2 2
(π) (13.5 x 10 N / m )
9
(2) 225 x 10 N/ m
=
2
= 7.9 x 10-4 m = 0.79 mm (0.031 in.)
8.8W This problem calls for us to calculate the normal σx and σy stresses in front on a surface crack of
length 2.0 mm at various positions when a tensile stress of 100 MPa is applied. Substitution for K =
σ
πa into Equations (8.9aW) and (8.9bW) leads to
σ x = σfx (θ)
a
2r
σ y = σfy (θ)
a
2r
where fx(θ) and fy(θ) are defined in the accompanying footnote 2. For θ = 0&deg;, fx(θ) = 1.0 and fy(θ) =
1.0, whereas for θ = 45&deg;, fx(θ) = 0.60 and fy(θ) = 1.25.
(a) For r = 0.1 mm and θ = 0&deg;,
a
2.0 mm
σ x = σy = σ(1.0)
= (100 MPa)
= 316 MPa (45, 800 psi)
2r
(2)(0.1 mm)
(b) For r = 0.1 mm and θ = 45&deg;,
σ x = σ(0.6)
σ y = σ(1.25)
a
2.0 mm
= (100 MPa)(0.6)
= 190 MPa (27, 500 psi)
2r
(2)(0.1 mm)
a
2.0 mm
= (100 MPa)(1.25)
= 395 MPa (57, 300 psi)
2r
(2)(0.1 mm)
198
(c) For r = 0.5 mm and θ = 0&deg;,
a
2.0 mm
σ x = σy = σ(1.0)
= (100 MPa)
= 141 MPa (20, 400 psi)
2r
(2)(0.5 mm)
(d) For r = 0.5 mm and θ = 45&deg;,
σ x = σ(0.6)
a
2.0 mm
= (100 MPa)(0.6)
= 84.8 MPa (12, 300 psi)
2r
(2)(0.5 mm)
σ y = σ(1.25)
a
2.0 mm
= (100 MPa)(1.25)
= 177 MPa (25, 600 psi)
2r
(2)(0.5 mm)
8.9W (a) In this portion of the problem we are asked to determine the radial position at which σx = 100
MPa (14,500 psi) for θ = 30&deg;, a = 2.0 mm, and σ = 150 MPa (21,750 psi). Substitution for K into
a
σ x = σfx (θ)
2r
Now, solving for r from this expression yields
a ⎡ σfx (θ ) ⎤
r= ⎢
⎥
2 ⎢⎣ σ ⎥⎦
2
x
For θ = 30&deg;, fx(θ) = 0.79, and therefore
2
r=
2 mm ⎡(150 MPa)(0.79) ⎤
⎥⎦ = 1.40 mm (0.055 in.)
100 MPa
2 ⎢⎣
(b) Now we are asked to compute σy at this position. This is done by using Equation (8.9bW); for θ
= 30&deg;, fy(θ) = 1.14, and therefore
σ y = σ fy (θ)
199
a
2r
= (150 MPa)(1.14)
2.0 mm
= 145 MPa (21,000 psi)
(2)(1.40 mm)
8.10W (a) In this portion of the problem it is necessary to compute the stress at point P when the applied
stress is 140 MPa (20,000 psi). In order to determine the stress concentration it is necessary to
consult Figure 8.2cW.
From the geometry of the specimen, w/h = (40 mm)/(20 mm) = 2.0;
furthermore, the r/h ratio is (4 mm)/(20 mm) = 0.20. Using the w/h = 2.0 curve in Figure 8.2cW, the
σ
Kt value at r/h = 0.20 is 1.8. And since K t = m , then
σ
o
σm = Ktσo = (1.8)(140 MPa) = 252 MPa (36,000 psi)
(b) Now it is necessary to determine how much r must be increased to reduce σm by 25%; this
reduction corresponds to a stress of (0.75)(252 MPa) = 189 MPa (27,000 psi). The value of Kt is
σ
189 MPa
= 1.35. Using the w/h = 2.0 curve in Figure 8.2cW, the value of
therefore, K t = m =
σ
140 MPa
o
r/h for Kt = 1.35 is about 0.60. Therefore
r = (0.60)h = (0.60)(20 mm) = 12.0 mm
Or, the radius r must be increased from 4.0 mm to 12.0 mm in order to reduce the stress
concentration by 25%.
8.11W (a) This portion of the problem calls for us to compute the stress at the edge of a circular throughthe-thickness hole in a steel sheet when a tensile stress is applied in a length-wise direction. We
19 mm
first must utilize Figure 8.2aW-- d/w =
= 0.15. From the figure and using this value, Kt =
127 mm
σ
2.5. Since K t = m and σo = 34.5 MPa (5000 psi) then
σ
o
σm = K t σ o = (2.5)(34.5 MPa) = 86.3 MPa (12,500 psi)
(b) Now it becomes necessary to compute the stress at the hole edge when the external stress is
applied in a width-wise direction; this simply means that w = 254 mm. The d/w then is 19 mm/254
mm = 0.075. From Figure 8.2aW, Kt is about 2.7. Therefore, for this situation
σm = K t σ o = (2.7)(34.5 MPa) = 93.2 MPa (13,500 psi)
200
8.12W The stress intensity factor is a parameter used in expressions such as Equations (8.9W); its
value is variable and dependent on applied stress and crack length according to the expression
provided in Problem 8.8W. On the other hand, plane strain and plane stress fracture toughnesses
represent unique and critical values of K at which crack propagation occurs. However, plane strain
fracture toughness is this critical value for specimens thicker than some minimum threshold
thickness, while plane stress is for specimens thinner than this threshold.
8.13W This problem calls for us to determine the value of B, the minimum component thickness for which
the condition of plane strain is valid using Equation (8.14W), for the metal alloys listed in Table 8.1.
For the 7075-T651 aluminum alloy
⎛K ⎞
Ic ⎟
B = 2.5 ⎜
⎜σ ⎟
⎝ y⎠
2
⎛ 24 MPa m ⎞ 2
⎟ = 0.0059 m = 5.9 mm (0.23 in.)
= (2.5) ⎜
⎝ 495 MPa ⎠
For the 2024-T3 aluminum alloy
⎛K ⎞
Ic ⎟
B = 2.5 ⎜
⎜σ ⎟
⎝ y⎠
2
⎛ 44 MPa m ⎞ 2
⎟ = 0.0406 m = 40.6 mm (1.60 in.)
= (2.5) ⎜
⎝ 345 MPa ⎠
For the Ti-6Al-4V titanium alloy
⎛ 55 MPa m ⎞
B = (2.5) ⎜
⎟
⎝ 910 MPa ⎠
2
= 0.0091 m = 9.1 mm (0.36 in.)
For the 4340 alloy steel tempered at 260&deg;C
⎛ 50 MPa m ⎞
B = (2.5) ⎜
⎟
⎝ 1640 MPa ⎠
2
= 0.0023 m = 2.3 mm (0.09 in.)
For the 4340 alloy steel tempered at 425&deg;C
⎛ 87.4 MPa m ⎞
B = (2.5) ⎜
⎟
⎝ 1420 MPa ⎠
2
= 0.0095 m = 9.5 mm (0.38 in.)
201
8.14 This problem asks us to determine whether or not the 4340 steel alloy specimen will fracture when
exposed to a stress of 1030 MPa, given the values of KIc, Y, and the largest value of a in the
material. This requires that we solve for σc from Equation (8.7). Thus
σc =
K Ic
Y πa
=
54.8 MPa m
(
)
(1) (π) 0.5 x 10 −3 m
= 1380 MPa (199,500 psi)
Therefore, fracture will not occur because this specimen will tolerate a stress of 1380 MPa (199,500
psi) before fracture, which is greater than the applied stress of 1030 MPa (150,000 psi).
8.15 We are asked to determine if an aircraft component will fracture for a given fracture toughness (40
MPa m ), stress level (260 MPa), and maximum internal crack length (6.0 mm), given that fracture
occurs for the same component using the same alloy for another stress level and internal crack
length. It first becomes necessary to solve for the parameter Y for the conditions under which
fracture occurred using Equation (8.5). Therefore,
Y=
K Ic
σ πa
=
40 MPa m
⎛ 4 x 10−3 m ⎞
⎟⎟
(300 MPa) (π) ⎜⎜
2
⎝
⎠
= 1.68
Now we will solve for the product Yσ π a for the other set of conditions, so as to ascertain whether
or not this value is greater than the KIc for the alloy. Thus,
⎛ 6 x 10 −3 m⎞
⎟⎟
Yσ π a = (1.68)(260 MPa) (π) ⎜⎜
2
⎝
⎠
= 42.4 MPa m
(39 ksi in.)
Therefore, fracture will occur since this value (42.4 MPa m) is greater than the KIc of the material,
40 MPa m .
8.16 This problem asks us to determine the stress level at which an aircraft component will fracture for a
given fracture toughness (26 MPa m ) and maximum internal crack length (6.0 mm), given that
fracture occurs for the same component using the same alloy at one stress level and another internal
202
crack length. It first becomes necessary to solve for the parameter Y for the conditions under which
fracture occurred using Equation (8.5). Therefore,
K Ic
Y=
σ πa
=
26 MPa m
⎛ 8.6 x 10 −3 m⎞
⎟⎟
(112 MPa) (π) ⎜⎜
2
⎠
⎝
= 2.0
Now we will solve for σc using Equation (8.6) as
σc =
K Ic
Y πa
=
26 MPa m
⎛ 6 x 10−3 m ⎞
⎟⎟
(2.0) (π) ⎜⎜
2
⎝
⎠
= 134 MPa (19, 300 psi)
8.17 For this problem, we are given values of KIc, σ, and Y for a large plate and are asked to determine
the minimum length of a surface crack that will lead to fracture. All we need do is to solve for ac
using Equation (8.7); therefore
1⎛K ⎞
a c = ⎜ Ic ⎟
π ⎝ Yσ ⎠
2
1 ⎡ 82.4 MPa m ⎤
⎥
= ⎢
π ⎣ (1)(345 MPa) ⎦
2
= 0.0182 m = 18.2 mm (0.72 in.)
8.18 This problem asks us to calculate the maximum internal crack length allowable for the Ti-6Al-4V
titanium alloy in Table 8.1 given that it is loaded to a stress level equal to one-half of its yield
strength. For this alloy, KIc = 55 MPa m (50 ksi in.) ; also, σ = σy/2 = (910 MPa)/2 = 455 MPa
(66,000 psi). Now solving for 2ac using Equation (8.7) yields
2 ⎛K ⎞
2a c = ⎜ Ic ⎟
π ⎝ Yσ ⎠
2
2
=
π
2
⎡ 55 MPa m ⎤
⎢
⎥ = 0.0041 m = 4.1 mm (0.16 in.)
⎣(1.5 )(455 MPa) ⎦
8.19 This problem asks that we determine whether or not a critical flaw in a wide plate is subject to
detection given the limit of the flaw detection apparatus (3.0 mm), the value of KIc (98.9 MPa m) ,
the design stress (σy/2 in which σy = 860 MPa), and Y = 1.0. We first need to compute the value of
ac using Equation (8.7); thus
2
⎡
⎤
2
1 ⎛ K Ic ⎞
1 ⎢ 98.9 MPa m ⎥
⎥ = 0.0168 m = 16.8 mm
ac = ⎜
⎟ = ⎢
π ⎝ Yσ ⎠
π⎢
⎛ 860 MPa ⎞ ⎥
(1.0 ) ⎜
⎟⎥
⎢⎣
⎠⎦
⎝
2
203
(0.66 in.)
Therefore, the critical flaw is subject to detection since this value of ac is greater than the 3.0 mm
resolution limit.
8.20W We are asked in this problem to determine whether or not it is possible to compute the critical
length of a surface flaw within the flat plate given its thickness (25.4 mm), yield strength (700 MPa),
plane strain fracture toughness [49.5 MPa
m (45 ksi
in.)] and the value of Y (1.65). The first
thing we must do is to ascertain whether or not conditions of plane strain exist for this plate by using
Equation (8.14W) as
⎛K ⎞
Ic ⎟
B = 2.5 ⎜
⎜σ ⎟
⎝ y⎠
2
⎛ 49.5 MPa m ⎞ 2
⎟ = 0.0125 m = 12.5 mm (0.50 in.)
= (2.5) ⎜
⎝ 700 MPa ⎠
The situation is one of plane strain since the thickness of the plate (25.4 mm) is greater than this
calculated B (12.5 mm).
Now, in order to determine the value of ac we utilize Equation (8.7):
ac =
1 ⎛ K Ic ⎞
⎜
⎟
π ⎝ Yσ ⎠
2
⎡
⎤
1 ⎢ 49.5 MPa m ⎥
⎥
= ⎢
π⎢
⎛ 700 MPa ⎞ ⎥
(1.65) ⎜
⎟
⎢⎣
⎝
⎠ ⎥⎦
2
2
= 0.0023 m = 2.3 mm (0.092 in.)
8.21 The student should do this problem on his/her own.
8.22 (a) The plot of impact energy versus temperature is shown below.
(b) The average of the maximum and minimum impact energies from the data is
204
Average =
105 J + 24 J
= 64.5 J
2
As indicated on the plot by the one set of dashed lines, the ductile-to-brittle transition temperature
according to this criterion is about -100&deg;C.
(c)
Also, as noted on the plot by the other set of dashed lines, the ductile-to-brittle transition
temperature for an impact energy of 50 J is about -110&deg;C.
8.23 The plot of impact energy versus temperature is shown below.
(b) The average of the maximum and minimum impact energies from the data is
Average =
76 J + 2 J
= 39 J
2
As indicated on the plot by the one set of dashed lines, the ductile-to-brittle transition temperature
according to this criterion is about 10&deg;C.
(c)
Also, as noted on the plot by the other set of dashed lines, the ductile-to-brittle transition
temperature for an impact energy of 20 J is about -2&deg;C.
8.24 With decreasing temperature, FCC metals do not experience a ductile-to-brittle transition because a
relatively large number of slip systems remain operable at very low temperatures. On the other
hand, BCC and HCP metals normally experience this transition because the number of operable slip
systems decreases with decreasing temperature.
205
8.25
(a) Given the values of σm (70 MPa) and σa (210 MPa) we are asked to compute σmax and
σmin. From Equation (8.14)
σm =
σmax + σmin
2
= 70 MPa
Or,
σmax + σmin = 140 MPa
Furthermore, utilization of Equation (8.16) yields
σa =
σmax − σmin
2
= 210 MPa
Or,
σmax - σmin = 420 MPa
Simultaneously solving these two expressions leads to
σmax = 280 MPa (40,000 psi)
σmin = − 140 MPa (−20, 000 psi)
(b) Using Equation (8.17) the stress ratio R is determined as follows:
R=
σ min
σ
max
=
−140 MPa
= − 0.50
280 MPa
(c) The magnitude of the stress range σr is determined using Equation (8.15) as
σ r = σmax − σmin = 280 MPa − (−140 MPa) = 420 MPa (60,000 psi)
8.26 This problem asks that we determine the minimum allowable bar diameter to ensure that fatigue
failure will not occur for a 1045 steel that is subjected to cyclic loading for a load amplitude of 66,700
N (15,000 lbf). From Figure 8.44, the fatigue limit stress amplitude for this alloy is 310 MPa (45,000
psi). Stress is defined in Equation (6.1) as σ =
F
. For a cylindrical bar
Ao
⎛ do ⎞ 2
Ao = π⎜ ⎟
⎝ 2⎠
206
Now we may solve for do from these expressions, taking stress as the fatigue limit divided by the
factor of safety. Thus
do = 2
= (2)
F
⎛ σ⎞
π⎜ ⎟
⎝ N⎠
66,700 N
= 23.4 x 10−3 m = 23.4 mm (0.92 in.)
⎛ 310 x 106 N/ m 2 ⎞
(π) ⎜⎜
⎟⎟
2
⎝
⎠
8.27 We are asked to determine the fatigue life for a cylindrical 2014-T6 aluminum rod given its diameter
(6.4 mm) and the maximum tensile and compressive loads (+5340 N and -5340 N, respectively).
The first thing that is necessary is to calculate values of σmax and σmin using Equation (6.1). Thus
F
σmax = max =
Ao
=
5340 N
−3
⎛ 6.4 x 10
(π) ⎜
⎜
2
⎝
m⎞
⎟⎟
⎠
2
−5340 N
⎛ 6.4 x 10−3 m ⎞
(π) ⎜
⎟⎟
⎜
2
⎝
⎠
2
⎛ do ⎞
π⎜
⎟
⎝ 2 ⎠
2
= 166 x 106 N/m2 = 166 MPa (24,400 psi)
σmin =
=
Fmax
Fmin
⎛d ⎞
π⎜ o ⎟
⎝ 2⎠
2
= − 166 x 106 N/m2 = − 166 MPa (−24, 400 psi)
Now it becomes necessary to compute the stress amplitude using Equation (8.16) as
σa =
σmax − σmin 166 MPa − (−166 MPa)
=
= 166 MPa (24,400 psi)
2
2
From Figure 8.44, for the 2014-T6 aluminum, the number of cycles to failure at this stress amplitude
is about 1 x 107 cycles.
207
8.28 This problem asks that we compute the maximum and minimum loads to which a 15.2 mm (0.60 in.)
diameter 2014-T6 aluminum alloy specimen may be subjected in order to yield a fatigue life of 1.0 x
108 cycles; Figure 8.44 is to be used assuming that data were taken for a mean stress of 35 MPa
(5,000 psi). Upon consultation of Figure 8.44, a fatigue life of 1.0 x 108 cycles corresponds to a
stress amplitude of 140 MPa (20,000 psi). Or, from Equation (8.16)
σmax − σmin = 2σ a = (2)(140 MPa) = 280 MPa (40,000 psi)
Since σm = 35 MPa, then from Equation (8.14)
σmax + σmin = 2σm = (2)(35 MPa) = 70 MPa (10,000 psi)
Simultaneous solution of these two expressions for σmax and σmin yields
F
σmax = +175 MPa (+25,000 psi) and σmin = -105 MPa (-15,000 psi). Now, inasmuch as σ =
A
o
⎛ do ⎞
[Equation (6.1)], and A o = π ⎜ ⎟
⎝ 2 ⎠
Fmax =
Fmin =
σmax π d 2o
4
σmin π d 2o
4
2
then
175 x 106 N/ m 2 )(π) (15.2 x 10 −3 m)
(
=
= 31, 750 N
2
4
−105 x 106 N / m2 )(π) (15.2 x 10−3 m)
(
=
(7070 lb f )
2
4
= − 19,000 N (−4240 lb f )
8.29 (a) The fatigue data for this alloy are plotted below.
(b) As indicated by one set of dashed lines on the plot, the fatigue strength at 4 x 106 cycles [log (4
x 106) = 6.6] is about 100 MPa.
208
(c) As noted by the other set of dashed lines, the fatigue life for 120 MPa is about 6 x 105 cycles
8.30 We are asked to compute the maximum torsional stress amplitude possible at each of several
fatigue lifetimes for the brass alloy the fatigue behavior of which is given in Problem 8.29. For each
lifetime, first compute the number of cycles, and then read the corresponding fatigue strength from
the above plot.
(a) Fatigue lifetime = (1 yr)(365 days/year)(24 h/day)(60 min/h)(1800 cycles/min) = 9.5 x 108 cycles.
(b) Fatigue lifetime = (30 days)(24 h/day)(60 min/h)(1800 cycles/min) = 7.8 x 107 cycles. The stress
(c) Fatigue lifetime = (24 h)(60 min/h)(1800 cycles/min) = 2.6 x 106 cycles. The stress amplitude
(d) Fatigue lifetime = (60 min/h)(1800 cycles/min) = 108,000 cycles.
The stress amplitude
8.31 (a) The fatigue data for this alloy are plotted below.
(b) The fatigue limit is the stress level at which the curve becomes horizontal, which is 290 MPa
(42,200 psi).
209
(c) From the plot, the fatigue lifetimes at a stress amplitude of 415 MPa (60,000 psi) is about 50,000
cycles (log N = 4.7). At 275 MPa (40,000 psi) the fatigue lifetime is essentially an infinite number of
cycles since this stress amplitude is below the fatigue limit.
(d) Also from the plot, the fatigue strengths at 2 x 104 cycles (log N = 4.30) and 6 x 105 cycles (log
N = 5.78) are 440 MPa (64,000 psi) and 325 MPa (47,500 psi), respectively.
8.32 This problem asks that we determine the maximum lifetimes of continuous driving that are possible
at an average rotational velocity of 600 rpm for the alloy the fatigue data of which is provided in
Problem 8.31 and at a variety of stress levels.
(a) For a stress level of 450 MPa (65,000 psi), the fatigue lifetime is approximately 18,000 cycles.
This translates into (1.8 x 104 cycles)(1 min/600 cycles) = 30 min.
(b) For a stress level of 380 MPa (55,000 psi), the fatigue lifetime is approximately 1.5 x 105 cycles.
This translates into (1.5 x 105 cycles)(1 min/600 cycles) = 250 min = 4.2 h.
(c) For a stress level of 310 MPa (45,000 psi), the fatigue lifetime is approximately 1 x 106 cycles.
This translates into (1 x 106 cycles)(1 min/600 cycles) = 1667 min = 27.8 h.
(d) For a stress level of 275 MPa (40,000 psi), the fatigue lifetime is essentially infinite since we are
below the fatigue limit.
8.33 For this problem we are given, for three identical fatigue specimens of the same material, σmax and
σmin data and are asked to rank the lifetimes from the longest to the shortest. In order to do this it
is necessary to compute both the mean stress and stress amplitude for each specimen. Since from
Equation (8.14)
σm =
σm (A) =
2
450 MPa + (−150 MPa)
= 150 MPa
2
300 MPa + (−300 MPa)
= 0 MPa
2
σm ( B) =
σm (C ) =
σmax + σmin
500 MPa + (−200 MPa)
= 150 MPa
2
Furthermore, using Equation (8.16)
σa =
σmax − σmin
2
210
σ a (A) =
450 MPa − (−150 MPa)
= 300 MPa
2
σ a (B ) =
300 MPa − (−300 MPa)
= 300 MPa
2
σ a (C) =
500 MPa − (−200 MPa)
= 350 MPa
2
On the basis of these results, the fatigue lifetime for specimen B will be greater than specimen A
which in turn will be greater than specimen C. This conclusion is based upon the following S-N plot
on which curves are plotted for two σm values.
8.34
Five factors that lead to scatter in fatigue life data are 1) specimen fabrication and surface
preparation, 2) metallurgical variables, 3) specimen alignment in the test apparatus, 4) variation in
mean stress, and 5) variation in test cycle frequency.
8.35 For a stress ratio (R) of +1, then, from Equation (8.17),
σmax = σmin
This is to say that the stress remains constant (or does not fluctuate) with time. Thus, the fatigue
plot would appear as
211
8.36 This question asks us to demonstrate that increasing R produces a decrease in σa. From Equation
(8.17)
σmin = Rσ max
Furthermore, Equation (8.16) is
σa =
σmax − σmin
2
Incorporation of the former expression into the latter gives
σa =
σmax − R σmax σ max
=
(1 − R)
2
2
Therefore, as the magnitude of R increases (or becomes more positive) the magnitude of σa
decreases.
8.37 To crystallize means to become crystalline. Thus, the statement &quot;The metal fractured because it
crystallized&quot; is erroneous inasmuch as the metal was crystalline prior to being stressed (virtually all
metals are crystalline).
8.38 (a) With regard to size, beachmarks are normally of macroscopic dimensions and may be observed
with the naked eye; fatigue striations are of microscopic size and it is necessary to observe them
using electron microscopy.
(b) With regard to origin, beachmarks result from interruptions in the stress cycles; each fatigue
striation corresponds to the advance of a fatigue crack during a single load cycle.
212
8.39 Four measures that may be taken to increase the fatigue resistance of a metal alloy are:
1) Polish the surface to remove stress amplification sites.
2)
Reduce the number of internal defects (pores, etc.) by means of altering processing and
fabrication techniques.
3) Modify the design to eliminate notches and sudden contour changes.
4)
Harden the outer surface of the structure by case hardening (carburizing, nitriding) or shot
peening.
8.40 Creep becomes important at 0.4T , T being the absolute melting temperature of the metal.
m m
For Ni, 0.4T = (0.4)(1455 + 273) = 691 K or 418&deg;C (785&deg;F)
m
For Cu, 0.4T = (0.4)(1085 + 273) = 543 K or 270&deg;C (518&deg;F)
m
For Fe, 0.4T = (0.4)(1538 + 273) = 725 K or 450&deg;C (845&deg;F)
m
For W, 0.4T = (0.4)(3410 + 273) = 1473 K or 1200&deg;C (2190&deg;F)
m
For Pb, 0.4T = (0.4)(327 + 273) = 240 K or -33&deg;C (-27&deg;F)
m
For Al, 0.4T = (0.4)(660 + 273) = 373 K or 100&deg;C (212&deg;F)
m
8.41 Schematic creep curves at both constant stress and constant load are shown below.
With increasing time, the constant load curve becomes progressively higher than the constant stress
curve.
Since these tests are tensile ones, the cross-sectional area diminishes as deformation
progresses. Thus, in order to maintain a constant stress, the applied load must correspondingly be
8.42 These creep data are plotted below.
213
The steady-state creep rate (Δε/Δt) is the slope of the linear region as
Δε
0.230 − 0.09
=
= 7.0 x 10-3 min-1
Δt
30 min − 10 min
8.43
This problem asks that we determine the total elongation of a low carbon-nickel alloy that is
exposed to a tensile stress of 70 MPa (10,000 psi) at 427&deg;C for 10,000 h; the instantaneous and
primary creep elongations are 1.3 mm (0.05 in.).
From the 427&deg;C line in Figure 8.29, the steady state creep rate, ε&Yacute;s , is about 0.035 %/1000 h
(or 3.5 x 10-5 %/h) at 70 MPa. The steady state creep strain, εs, therefore, is just the product of ε&Yacute;s
and time as
εs = &Yacute;
ε s x (time)
(
= 3.5 x 10
-5
)
-3
%/h (10,000 h) = 0.35 % = 3.5 x10
Strain and elongation are related as in Equation (6.2); solving for the steady state elongation, Δls,
(
-3
Δls = lo ε s = (1015 mm) 3.5 x 10
)= 3.6 mm
(0.14 in.)
Finally, the total elongation is just the sum of this Δls and the total of both instantaneous and primary
creep elongations [i.e., 1.3 mm (0.05 in.)]. Therefore, the total elongation is 4.9 mm (0.19 in.).
214
8.44 We are asked to determine the tensile load necessary to elongate a 635 mm long low carbon-nickel
alloy specimen 6.4 mm after 5,000 h at 538&deg;C. It is first necessary to calculate the steady state
creep rate so that we may utilize Figure 8.29 in order to determine the tensile stress. The steady
state elongation, Δls, is just the difference between the total elongation and the sum of the
instantaneous and primary creep elongations; that is,
Δls = 6.4 mm − 1.8 mm = 4.6 mm (0.18 in.)
Now the steady state creep rate, ε&Yacute;s is just
ε&Yacute;s =
Δε Δl s / lo (4.6 mm) /(635 mm)
=
=
Δt
Δt
5,000 h
= 1.45 x 10-6 (h)-1 = 0.145 %/1000 h
Employing the 538&deg;C line in Figure 8.29, a steady state creep rate of 0.145 %/1000 h corresponds to
a stress σ of about 40 MPa (5,800 psi). From this we may compute the tensile load using Equation
(6.1) as
⎛ do ⎞
F = σAo = σπ ⎜ ⎟
⎝ 2⎠
(
6
2
= 40 x 10 N/m
⎛ 19.0 x 10−3 m⎞
(π) ⎜⎜
⎟⎟
2
⎝
⎠
)
2
2
= 11,300 N (2560 lb f )
8.45 This problem asks us to calculate the rupture lifetime of a component fabricated from a low carbonnickel alloy exposed to a tensile stress of 31 MPa at 649&deg;C. All that we need do is read from the
649&deg;C line in Figure 8.28 the rupture lifetime at 31 MPa; this value is about 10,000 h.
8.46 We are asked in this problem to determine the maximum load that may be applied to a cylindrical
low carbon-nickel alloy component that must survive 10,000 h at 538&deg;C. From Figure 8.28, the
stress corresponding to 104 h is 70 MPa (10,000 psi). Since stress is defined in Equation (6.1) as σ
= F/Ao, and for a cylindrical specimen, A o = πro2 , then
⎛ do ⎞
F = σAo = σπ ⎜ ⎟
⎝ 2⎠
215
2
(
6
= 70 x 10
⎛ 19.1 x 10−3 m ⎞
N/m (π) ⎜⎜
⎟⎟
2
⎝
⎠
2
)
2
= 20,000 N (4420 lbf )
8.47 The slope of the line from a log ε&Yacute;s versus log σ plot yields the value of n in Equation (8.19); that is
n=
Δ log ε&Yacute;s
Δ log σ
We are asked to determine the values of n for the creep data at the three temperatures in Figure
8.29. This is accomplished by taking ratios of the differences between two log ε&Yacute;s and log σ values.
Thus for 427&deg;C
( −1)
( −2 )
− log 10
log 10
Δ log ε&Yacute;s
n=
=
= 5.3
Δ log σ
log (85 MPa) − log (55 MPa)
While for 538&deg;C
( −2 )
log (1.0 ) − log 10
Δ log ε&Yacute;s
n=
=
= 4.9
Δ log σ
log (59 MPa) − log (23 MPa)
And at 649&deg;C
( −2 )
log (1.0 ) − log 10
Δ log ε&Yacute;s
n=
=
= 7.8
Δ log σ
log (15 MPa) − log (8.3 MPa)
8.48 (a) We are asked to estimate the activation energy for creep for the low carbon-nickel alloy having
the steady-state creep behavior shown in Figure 8.29, using data taken at σ = 55 MPa (8000 psi)
and temperatures of 427&deg;C and 538&deg;C. Since σ is a constant, Equation (8.20) takes the form
⎛ Qc⎞
⎛ Qc⎞
n
'
ε&Yacute;s = K 2σ exp ⎜ −
⎟ = K 2 exp ⎜ −
⎟
⎝ RT ⎠
⎝ RT ⎠
where K 2' is now a constant. (Note: the exponent n has about the same value at these two
temperatures per Problem 8.47.) Taking natural logarithms of the above expression
216
Q
ln &Yacute;
ε s = ln K2' − c
RT
For the case in which we have creep data at two temperatures (denoted as T1 and T2) and their
corresponding steady-state creep rates ( ε&Yacute;s and ε&Yacute;s ), it is possible to set up two simultaneous
1
2
equations of the form as above, with two unknowns, namely K 2' and Qc. Solving for Qc yields
⎛
R ⎜ln ε&Yacute;s −
⎝
1
Qc = −
⎡1
⎢
−
⎢⎣ T1
⎞
ln &Yacute;
εs ⎟
⎠
2
⎤
1
⎥
T2 ⎥⎦
Let us choose T1 as 427&deg;C (700 K) and T2 as 538&deg;C (811 K); then from Figure 8.29, at σ = 55 MPa,
ε&Yacute;s
1
= 0.01 %/1000 h = 1 x 10-7 (h)-1 and ε&Yacute;s
= 0.8 %/1000 h = 0.8 x 10-5 (h)-1. Substitution of
2
these values into the above equation leads to
( )
(
)
(8.31 J/ mol - K) ⎡ ln 10−7 − ln 0.8 x 10 −5 ⎤
⎣
⎦
Qc = −
⎡ 1
1 ⎤
⎢⎣ 700 K − 811 K ⎥⎦
= 186,200 J/mol
(b) We are now asked to calculate ε&Yacute;s at 649&deg;C (922 K). It is first necessary to determine the value
of K 2' , which is accomplished using the first expression above, the value of Qc, and one value each
of ε&Yacute;s and T (say ε&Yacute;s and T1). Thus,
1
⎛ Q ⎞
K 2' = ε&Yacute;s exp ⎜⎜ c ⎟⎟
1
⎝ RT1⎠
[
−7
= 10
(h)
⎤
200 J/ mol
6
-1
⎥ = 8.0 x 10 (h)
]exp ⎡⎢⎣ (8.31186,J / mol
- K)(700 K) ⎦
−1
Now it is possible to calculate ε&Yacute;s at 922 K as follows:
⎛ Q ⎞
ε&Yacute;s = K 2' exp ⎜ − c ⎟
⎝ RT ⎠
217
[
= 8.0 x 10
−6
−1
(h)
⎤
J / mol
⎥
]exp ⎡⎢⎣(8.31186,200
J / mol - K)(922 K) ⎦
= 2.23 x 10-4 (h)-1 = 22.3 %/1000 h
8.49 This problem gives ε&Yacute;s values at two different stress levels and 200&deg;C, and the activation energy for
creep, and asks that we determine the steady-state creep rate at 250&deg;C and 48 MPa (7000 psi).
Taking the natural logarithm of Equation (8.20) yields
Q
ln &Yacute;
ε s = ln K2 + n ln σ − c
RT
With the given data there are two unknowns in this equation--namely K2 and n. Using the data
provided in the problem we can set up two independent equations as follows:
[
]
[
]
ln 2.5 x 10 −3 (h)−1 = ln K 2 + n ln (55 MPa) −
140, 000 J / mol
(8.31 J/ mol - K)(473 K)
140,000 J / mol
ln 2.4 x 10−2 (h) −1 = ln K2 + n ln (69 MPa) −
(8.31 J/ mol - K)(473 K)
Now, solving simultaneously for K2 and n leads to n = 9.97 and K2 = 3.27 x 10-5 (h)-1. Thus it is
now possible to solve for ε&Yacute;s at 48 MPa and 523 K using Equation (8.20) as
⎛ Q ⎞
ε&Yacute;s = K 2σnexp ⎜ − c ⎟
⎝ RT ⎠
[
]
⎡
⎤
140, 000 J / mol
= 3.27 x 10−5 (h) −1 (48 MPa)9.97 exp ⎢−
⎥
⎣ (8.31 J / mol - K)(523 K) ⎦
1.94 x 10-2 (h)-1
8.50 This problem gives ε&Yacute;s values at two different temperatures and 140 MPa (20,000 psi), and the
stress exponent n = 8.5, and asks that we determine the steady-state creep rate at a stress of 83
MPa (12,000 psi) and 1300 K.
Taking the natural logarithm of Equation (8.20) yields
218
Q
ln &Yacute;
ε s = ln K2 + n ln σ − c
RT
With the given data there are two unknowns in this equation--namely K2 and Qc. Using the data
provided in the problem we can set up two independent equations as follows:
[
]
[
]
ln 6.6 x 10 −4 (h)−1 = ln K 2 + (8.5) ln (140 MPa) −
ln 8.8 x 10 −2 (h)−1 = ln K 2 + (8.5) ln (140 MPa) −
Qc
(8.31 J / mol - K)(1090 K)
Qc
(8.31 J / mol - K)(1200 K)
Now, solving simultaneously for K2 and Qc leads to K2 = 57.5 (h)-1 and Qc = 483,500 J/mol. Thus,
it is now possible to solve for ε&Yacute;s at 83 MPa and 1300 K using Equation (8.20) as
⎛ Q ⎞
ε&Yacute;s = K 2σnexp ⎜ − c ⎟
⎝ RT ⎠
[
−1
= 57.5 (h)
⎤
500 J / mol
⎥
](83 MPa) 8.5 exp ⎡⎢⎣− (8.31483,
J/ mol - K)(1300 K) ⎦
4.31 x 10-2 (h)-1
8.51 Three metallurgical/processing techniques that are employed to enhance the creep resistance of
metal alloys are 1) solid solution alloying, 2) dispersion strengthening by using an insoluble second
phase, and 3) increasing the grain size or producing a grain structure with a preferred orientation.
Design Problems
8.D1W This problem asks us to calculate the minimum KIc necessary to ensure that failure will not occur
for a flat plate given the following: an expression from which Y(a/W) may be determined, the internal
crack length, 2a (25 mm), the plate width, W (100 mm), and the value of σ (415 MPa). First we
compute the value of Y(a/W) using Equation (8.12W), as follows:
⎡W
π a⎤
Y(a/W) = ⎢
tan
⎥
πa
W⎦
⎣
219
1/2
1/2
⎡ 100 mm
(π)(12.5 mm) ⎤
= ⎢
tan
= 1.027
⎥
100 mm ⎦
⎣(π)(12.5 mm)
Now, using Equation (8.13W) [or Equation (8.5)] it is possible to determine KIc; thus
KIc = Y(a/W)σ πa
(
)
= (1.027)(415 MPa) (π) 12.5 x 10−3 m = 84.5 MPa m (77.2 ksi in.)
8.D2W For this problem we are asked to determine the critical crack length for a flat plate containing a
centrally positioned, through-thickness crack as shown in Figure 8.6W;
for this plate,
KIc = 50 MPa m , W = 60 mm, and the design stress σ = 375 MPa. The plane-strain fracture
toughness is defined by Equation (8.13W) [or Equation (8.5)]; furthermore, for this case, Y is a
function of crack length a and plate width W according to Equation (8.12W). Combining these
KIc = Y(a/W)σ πa
⎡W
πa ⎤
= ⎢
tan
⎥
W⎦
⎣π a
1/2
σ πa
⎡
⎛ π a⎞ ⎤
⎟
= σ ⎢W tan ⎜
⎝ W ⎠ ⎥⎦
⎣
1/2
Now solving this expression for a which is just the critical crack length ac yields
⎡ 2 ⎤
⎛ W⎞
-1 K Ic
a c = ⎜ ⎟ tan ⎢ 2 ⎥
⎝ π⎠
⎢⎣ σ W ⎦⎥
(
)
2
⎡
⎛ 60 x 10−3 m ⎞
50 MPa m
-1 ⎢
⎟⎟ tan ⎢
= ⎜⎜
2
−3
π
⎝
⎠
⎢⎣(375 MPa) 60 x 10 m
(
= 5.5 x 10-3 m = 5.5 mm (0.22 in.)
220
⎤
⎥
⎥
⎦⎥
)
8.D3W This problem asks that we determine, for a steel plate having a through-thickness edge crack, the
minimum allowable plate width to ensure that fracture will not occur if the minimum crack length that
is subject to detection is 3 mm (0.12 in.). We are also given that KIc = 65 MPa m and that the
plate may be loaded to half its yield strength, where σy = 1000 MPa. First of all the applied stress is
just
σ =
σy
2
=
1000 MPa
= 500 MPa (72,500 psi)
2
Now, using Equation (8.13W) [equivalently Equation (8.5)] we solve for the value of Y assuming that
a = 3.0 mm, as
Y=
K Ic
σ πa
65 MPa m
=
(
−3
(500 MPa) (π) 3 x 10
)
= 1.34
m
In Figure 8.7aW is plotted Y versus a/W for the crack-plate geometry of this problem; from this plot,
for Y = 1.34, a/W = 0.20. Since the minimum crack length for detection is 3 mm, the minimum width
allowable is just
W=
a
3 mm
=
= 15 mm
0.20
0.20
(0.60 in.)
8.D4W This problem asks that we consider a steel plate having a through-thickness edge crack, and to
W = 40 mm, B = 6.0 mm,
determine if fracture will occur given the following:
KIc = 60 MPa m (54.6 ksi in. ) , σ = 1400 MPa, σ = 200 MPa, and a = 16 mm. The first thing to
y
do is determine whether conditions of plane strain exist. From Equation (8.14W),
⎛K ⎞
Ic ⎟
2.5 ⎜
⎜σ ⎟
⎝ y⎠
⎛ 60 MPa m ⎞
= 2.5 ⎜
⎟
⎝ 1400 MPa ⎠
2
2
= 0.0046 m = 4.6 mm
221
(0.19 in.)
Inasmuch as the plate thickness is 6 mm (which is greater than 4.6 mm), the situation is a plane
strain one. Next, we must determine the a/W ratio, which is just 16 mm/40 mm = 0.40. From this
ratio and using Figure 8.7aW, Y = 2.12. At this point it becomes necessary to determine the value of
the Yσ π a product; if it is greater than KIc then fracture will occur. Thus
(
)
Yσ πa = (2.12)(200 MPa) (π) 16 x 10 −3 m
= 95.0 MPa m
(86.5
ksi in.
Therefore, fracture will occur since this value (95.0 MPa
(60 MPa
)
m) is greater than the K
Ic for the steel
m) .
8.D5W We are to determine the maximum load that may be applied without failure to a thin bar of
rectangular cross-section that is loaded in three-point bending per Figure 8.7cW. It first becomes
necessary to determine the value of Y for the given geometry, which is possible using this figure;
however, this determination necessitates the computation of a/W and S/W ratios as
a
0.5 mm
=
= 0.20
W 2.5 mm
S
10 mm
=
=4
W 2.5 mm
From Figure 8.7cW, Y = 0.96 from the S/W = 4 curve and for a/W = 0.20. Now solving for the
applied load F using the equation also provided in this figure
2
F=
(
4KIc W B
3SY π a
)(
) (1.5 x 10−3 m)
(π) (0.5 x 10 −3 m)
4 0.60 MPa m 2.5 x 10 −3 m
=
(
)
3 10 x 10−3 m (0.96)
2
= 1.97 x 10-5 MN = 19.7 N (4.69 lbf)
222
8.D6 (a) This portion of the problem calls for us to rank four polymers relative to critical crack length in
the wall of a spherical pressure vessel. In the development of Design Example 8.1, it was noted that
critical crack length is proportional to the square of the KIc-σy ratio. Values of KIc and σy as taken
from Tables B.4 and B.5 are tabulated below. (Note: when a range of σy or KIc values is given, the
average value is used.)
KIc (MPa m)
σy (MPa)
Nylon 6,6
2.75
51.7
Polycarbonate
2.2
62.1
Polyethylene terephthlate
5.0
59.3
Polymethyl methacrylate
1.2
63.5
Material
On the basis of these values, the five polymers are ranked per the squares of the KIc-σy ratios as
follows:
⎛K ⎞
⎜ Ic ⎟
⎜σ ⎟
⎝ y⎠
Material
2
PET
7.11
Nylon 6,6
2.83
PC
1.26
PMMA
0.36
(mm)
These values are smaller than those for the metal alloys given in Table 8.2, which range from 0.93 to
43.1 mm.
2
(b) Relative to the leak-before-break criterion, the KIc - σ y ratio is used. The five polymers are
ranked according to values of this ratio as follows:
2
KIc
Material
σ
(MPa -m)
y
PET
0.422
Nylon 6,6
0.146
PC
0.078
PMMA
0.023
223
These values are all smaller than those for the metal alloys given in Table 8.3, which values range
from 1.2 to 11.2 MPa-m.
8.D7W We are asked in this problem to estimate the maximum tensile stress that will yield a fatigue life
of 3.2 x 105 cycles, given values of ao, ac, m, A, and Y. Since Y is independent of crack length we
may utilize Equation (8.29W) which, upon integration, takes the form
Nf =
ac
1
∫ a−m / 2 da
Aπm / 2 (Δσ)m Y m
ao
And for m = 4
Nf =
= −
1
Aπ 2(Δσ) 4 Y 4
ac
∫ a −2 da
ao
⎡
⎤
⎢ 1 − 1⎥
Aπ 2(Δσ)4 Y 4 ⎢⎣ a c
a o ⎦⎥
1
Now, solving for Δσ from this expression yields
1 ⎤
⎡ 1
⎢a − a ⎥
o
c⎥
Δσ = ⎢
⎢N Aπ 2 Y 4 ⎥
⎢ f
⎥
⎣
⎦
1/4
1/4
⎡
⎤
1
1
−
⎢
⎥
−4
−3
2.5 x 10 m 5 x 10 m
⎥
=⎢
⎢ 3.2 x 105 cycles 5 x 10−15 (π) 2(2) 4 ⎥
⎢
⎥
⎣
⎦
(
)(
= 350 MPa
224
)
This 350 MPa will be the maximum tensile stress since we can show that the minimum stress is a
compressive one--when σmin is negative, Δσ is taken to be σmax. If we take σmax = 350 MPa, and
since σm is stipulated in the problem to have a value of 25 MPa, then from Equation (8.14)
σmin = 2σ m − σ max = 2(25 MPa) − 350 MPa = − 300 MPa
Therefore σmin is negative and we are justified in taking σmax to be 350 MPa.
8.D8W This problem calls for us to estimate the fatigue life of a large flat plate given that σa = 150 MPa,
ao = 0.75 mm, KIc = 35 MPa m , m = 2.5, A = 2 x 10-12, and Y = 1.75. It first becomes necessary
to compute the critical crack length, ac. Employment of Equation (8.7), and assuming a stress level
of 150 MPa, since this is the maximum tensile stress, leads to
ac =
1 ⎛ KIc ⎞
⎜
⎟
π ⎝ σY ⎠
1 ⎛ 35 MPa m ⎞
⎟
= ⎜
π ⎝ (150 MPa)(1.75) ⎠
2
2
= 5.66 x 10-3 m
We now want to solve Equation (8.29W) using a lower integration limit, ao, of 7.5 x 10-4 m as stated
in the problem; also, the value Δσ is 150 MPa. Therefore, integration yields for Nf
Nf =
ac
1
Aπm / 2 (Δσ)m Y m
∫ a−m / 2 da
ao
And for m = 2.5
Nf =
ac
1
Aπ 2.5 / 2 (Δσ )2.5 Y 2.5
∫ a−2.5 / 2 da
ao
1 ⎞ −0.25
⎛
=
⎜−
⎟a
1.25
2.5
2.5
⎝
⎠
0.25
(Δσ) Y
Aπ
a
1
225
a
c
o
=
⎤
⎡
⎥
⎢
1
1
−
⎥
⎢
0.25
−4 0.25 ⎥
2 x 10−12 (π)1.25(150 )2.5(1.75)2.5 ⎢ 5.66 x 10 −3
7.5 x 10
⎦
⎣
(
−4
)
(
)
(
)
= 1.0 x 106 cycles
8.D9W We are asked in this problem to estimate the critical surface crack length that will yield a fatigue
life of 5 x 106 cycles, given that ao = 2.0 x 10-2 in., σmax = 25,000 psi, m = 3.5, A = 1.3 x 10-23,
and Y = 2.25. Since Y is independent of crack length we may utilize Equation (8.29W) which, upon
integration, takes the form
Nf =
ac
1
Aπm / 2 (Δσ)m Y m
∫ a−m / 2 da
ao
And for m = 3.5
Nf =
= −
ac
1
Aπ 3.5 / 2 (Δσ )3.5 Y 3.5
∫ a−3.5 / 2 da
ao
( )
( )
−0.75
−0.75 ⎤
⎛ 1 ⎞ ⎡
⎜
⎟ ⎢ ac
− ao
⎥⎦
Aπ1.75(Δσ) 3.5 Y 3.5 ⎝ −0.75 ⎠ ⎣
1
Solving for ac from this expression leads to
⎧
⎪
1
ac = ⎨
−0.75
⎪ a
+ N A (−0.75)(π)1.75 (Δσ)3.5 Y 3.5
f
⎩ o
[
( )
1 / 0.75
⎫
⎪
⎬
⎪
⎭
]
1/ 0.75
⎧
⎫
⎪⎪
⎪⎪
1
⎬
= ⎨
−0.75
6
−23
1.75
3.5
3.5 ⎤ ⎪
⎪ 2 x 10-2
⎡
+ 5 x 10 1.3 x 10
(−0.75)(π)
(25, 000) (2.25)
⎪⎩
⎣
⎦ ⎪⎭
(
)
(
)(
)
= 0.185 in.
226
8.D10W (a) For this part of the problem we are asked to calculate, for the plot of Figure 8.17W, values of
the A and m parameters in Equation (8.24W). Taking logarithms of both sides of this expression
leads to Equation (8.26bW), that is
⎛ da ⎞
⎟ = m log ΔK + log A
log ⎜
⎝ dN⎠
Then all we need do is take two values of log (da/dN) from the line shown in Figure 8.17W, and their
corresponding log (ΔK) values, and then develop two expressions of the above equation and solve
simultaneously for A and m. First of all, for SI units, let us take log (da/dN)1 = -2 and log (da/dN)2 =
-4; thus, their corresponding log (ΔK) values are log (ΔK)1 = 2.041 and log (ΔK)2 = 1.442. Thus,
the resulting two equations are as follows:
− 2 = 2.041 (m) + log A
− 4 = 1.442 (m) + log A
Simultaneous solution of these expressions leads to m = 3.34 and A = 1.52 x 10-9.
Now for Customary U.S. units, let us take log (da/dN)1 = -4 and log (da/dN)2 = -5, which
lead to log (ΔK)1 = 1.9140 and log (ΔK)2 = 1.5530. And the two equations are
− 4 = 1.9140 (m) + log A
− 5 = 1.5530 (m) + log A
And, the resulting solutions are m =2.77 and A = 5 x 10-10.
(b) And, for this problem part, for this Ni-Mo-V alloy, we are to compute the maximum initial surface
crack length to yield a minimum fatigue lifetime of 3 x 105 cycles, assuming a critical surface crack
length of 1.5 mm, a maximum tensile stress of 30 MPa, and Y has a value of 1.25 that is
independent of crack length.
Using values of m and A (for SI units), Equation (8.29W) takes the form
Nf =
ac
1
Aπm / 2 (Δσ)m Y m
227
∫ a−m / 2 da
ao
Nf =
= −
ac
1
Aπ 3.34 / 2 (Δσ)3.34 Y 3.34
1 ⎞ ⎡
⎛
1
∫ a−3.34 / 2 da
ao
( )
⎜
⎟ ⎢a
Aπ1.67(Δσ) 3.34 Y 3.34 ⎝ −0.67 ⎠ ⎣ c
−0.67
( )
− ao
−0.67 ⎤
⎥⎦
Solving for ao from this expression leads to
⎧
⎪
1
ao = ⎨
−0.67
⎪a
− N A (−0.67)(π)1.67 (Δσ)3.34 Y 3.34
f
⎩ c
( )
[
⎫
⎪
⎬
⎪
⎭
1/ 0.67
]
⎧
⎫
⎪⎪
⎪⎪
1
⎬
= ⎨
−0.67
⎪ 1.5 x 10-3
⎡ 3.0 x 10 5 1.52 x 10-9 (−0.67)(π)1.67 (30)3.34 (1.25)3.34 ⎤ ⎪
−
⎪⎩
⎣
⎦ ⎪⎭
(
)
(
)(
1/ 0.67
)
= 1.1 x 10-4 m = 0.11 mm
8.11W This problem asks that we estimate the fatigue life of a flat plate that has a centrally positioned
through-thickness crack, given that W = 25 mm, 2ao = 0.10 mm, 2ac = 6.0 mm, m = 4.0, and A = 6 x
10-12. Furthermore, inasmuch as reverse stress cycling is to be used Δσ = 120 MPa. For this plate
and crack geometry, the parameter Y in Equation (8.5) is defined by Equation (8.12W), and,
therefore, is dependent on crack length. Hence, the equation for Nf [Equation (8.29W)] now
becomes
ac
⌠
da
⎮
Nf =
⎮
m
/
2
m
m/2
Aπ
(Δσ) ⎮ m / 2 ⎛ W
πa⎞
⌡ a
tan
⎜
⎟
W⎠
⎝ πa
a
1
o
ac
=
1
⌠
⎮ cot
AWm / 2 (Δσ)m ⌡
ao
For m = 4, this equation takes the form
228
m/2 ⎛ πa⎞
⎜
⎟ da
⎝ W⎠
ac
Nf =
⌠
2 ⎛ π a⎞
⎟ da
⎮ cot ⎜
2
4
⎝W⎠
AW (Δσ) ⌡
ao
1
Here, values for ao and ac are 0.05 mm and 3.0 mm, respectively. Integration of the preceding
a
c
⎡ ⎛ W⎞
⎤
⎛ πa⎞
Nf =
−
⎜
⎟
cot
⎜
⎟
−
a
⎢
⎥
⎝ W⎠
⎦
AW2 (Δσ)4 ⎣ ⎝ π ⎠
a
o
1
⎡ ⎛ 25 x 10−3 ⎞
⎛ 3π ⎞
−3
⎢− ⎜
⎟⎟ cot ⎜ ⎟ − 3 x 10
⎜
2
⎠
⎝
π
25
−12
−3
4 ⎢⎣ ⎝
⎠
6 x 10
25 x 10
(120)
=
+
(
)(
1
(
)
⎤
)⎥⎥⎦
⎡⎛ 25 x 10 −3 ⎞
⎛ 0.05π ⎞
⎢⎜
⎟ + 0.05 x 10−3
⎟⎟ cot ⎜
⎜
2
⎠
⎝
π
25
−12
−3
4 ⎢⎣⎝
⎠
25 x 10
(120 )
6 x 10
(
)(
1
(
)
⎤
⎥
⎥⎦
)
= 1.6 x 106 cycles
8.D12W For this problem we are given an expression for Y(a/W) for an edge crack of finite width (Figure
8.7aW), and are asked to estimate the fatigue life for a tension-compression reversed cycle situation
given the following:
W = 60 mm (0.06 m)
ao = 5 mm (5 x 10-3 m)
ac = 12 mm (1.2 x 10-2 m)
m = 3.5
A = 1.5 x 10-12
Since it is a reversed stress cycle and given that σmin = -135 MPa, it is the case that σmax = +135
MPa;
this also means that Δσ in Equation (8.29W) is also 135 MPa.
Upon substitution the
expression for Y(a/W) [Equation (8.21)] into Equation (8.29W), the fatigue life is equal to the
following expression:
229
ac
Nf =
⌠
⎮
⎮
a -1.75 da
1
⎮
1.5 x 10−12 (π)1.75 (135)3.5 ⎮ ⎡
⎤ 3.5
⎮ ⎢1.1 ⎛⎜ 1 − 0.2a ⎞⎟ ⎥
⎮⎢
W ⎠⎥
⎝
⌡
3/2 ⎥
⎢ ⎛
a⎞
ao
⎢ ⎜1 − ⎟
⎥
⎣ ⎝
⎦
W⎠
(
)
Nf may now be determined using the E-Z Solve equation solver.
After opening E-Z Solve, the following text is entered into the workspace of the window that
appears:
a=t
T' = 1/K * a^(-1.75) / (1.1 * (1 - 0.2 * a / W) / (1 - a / W)^(3/2))^3.5
K = 1.5e-12 * pi^1.75 * 135^3.5
W = 0.06
It is next necessary to click on the calculator icon (&quot;Solve new run&quot;) located on the tool bar near the
top of the window. At this time another window appears within which the integration limits are
specified. In the &quot;IC&quot; window, under the &quot;Independent Variable&quot; column, in the &quot;Start&quot; box is entered
&quot;5e-3&quot;, which is the lower limit of the integral (i.e., ao). Furthermore, in the &quot;End&quot; box is entered the
upper integration limit (ac), which is &quot;1.2e-2&quot;, and in the &quot;# Points&quot; box is entered the value &quot;1&quot;.
Under the &quot;Initial Conditions&quot; column, in the &quot;t&quot; box is again entered the lower integration limit--&quot;5e3&quot;; in the &quot;T&quot; box is left the default value of &quot;0&quot;. It is now necessary to click on the &quot;Solve New Run&quot;
box at the bottom of this window, at which time the equation solver is engaged. Finally, at the
bottom of the first window now appears the data that has been entered as well as the solution. The
value for the fatigue life (Nf) is given as the nonzero value that appears in the T column--i.e., 4.17 x
104 cycles.
8.D13 This problem asks that we derive an expression for the fatigue life of the spherical tank shown in
Figure 8.10 that is alternately pressurized and depressurized between atmospheric pressure and a
positive pressure p. For Y being independent of crack length a, Equation (8.29W) takes the form
Nf =
ac
1
Aπ m / 2 (Δσ)m Y m
230
∫ a −m / 2 da
ao
But Δσ is just equal to the expression for σ in Equation (8.8). Making this substitution into the above
ac
1
Nf =
∫a
da
ac
m m
=
−m / 2
m
m / 2 ⎛ pr ⎞
m
Aπ
⎜ ⎟ Y ao
⎝ 2t ⎠
2 t
∫ a−m / 2 da
Aπm / 2(p r)m Y m
ao
This expression must next be integrated which yields
Nf =
2 (m + 1) tm
A (2 − m)π m / 2 (pr)m Ym
[ac(1 - m / 2 ) − ao(1 - m / 2) ]
which is the desired result.
8.D14W (a) This portion of the problem asks that we compute the maximum tensile load that may be
applied to a spring constructed of a
1
hard 304 stainless steel such that the total deflection is less
4
than 5 mm; there are 10 coils in the spring, whereas, its center-to-center diameter is 15 mm, and the
wire diameter is 2.0 mm. The total spring deflection δs may be determined by combining Equations
(8.32W) and (8.33W); solving for the load F from the combined equation leads to
4
δs d G
F =
8N D3
c
However, it is also necessary to determine the value of the shear modulus G. This is possible using
Equation (6.9) and values of the modulus of elasticity (193 GPa) and Poisson's ratio (0.30) as taken
from Tables B.2 and B.3 in Appendix B. Thus
G =
=
E
2(1 + ν)
193 GPa
= 74.2 GPa
2(1 + 0.30)
231
Substitution of this value and values of the other parameters into the above equation for F leads to
(5 x 10−3 m)(2 x 10 −3 m) (74.2 x 109 N / m2 )
3
(8)(10 coils) (
15 x 10−3 m)
4
F =
= 22.0 N (5.1 lb f )
(b) We are now asked to compute the maximum tensile load that may be applied without any
permanent deformation of the spring wire. This requires that we combine Equations (8.30W) and
(8.31W), and then solve for F. However, it is first necessary to calculate the shear yield strength and
substitute it for τ in Equation (8.30W). The problem statement stipulates that τy = 0.6 σy. From
Table B.4 in Appendix B, we note that the tensile yield strength for this alloy in the 1/4 hardened
state is 515 MPa; thus τy = 309 MPa. Now, solving for F as outlined above
F =
(
πτy d 3
⎛ D⎞
(1.6)(8)(D) ⎜ ⎟
⎝ d⎠
6
π 309 x 10 N/ m
=
(
(1.6)(8) 15 x 10
−3
2
−0.140
)(2 x 10 −3 m)
⎛ 15 x 10 −3 m ⎞
m ⎜⎜
⎟⎟
−3
⎝ 2 x 10 m ⎠
)
3
−0.140
= 53.6 N (12.5 lb f )
8.D15W (a) In this portion of the problem we are asked to select candidate materials for a spring that
consists of eight coils and which is not to plastically deform nor experience a deflection of more that
10 mm when a tensile force of 30 N is applied. The coil-to-coil diameter and wire diameter are 12
mm and 1.75 mm, respectively. In addition, we are to assume that τy = 0.6σy and G = 0.4E. Let us
first determine the minimum modulus of elasticity that is required such that the total deflection δs is
less than 10 mm. This requires that we begin by computation of the deflection per coil δc using
Equation (8.33W) as
232
δc =
δs
N
=
10 mm
= 1.25 mm/coil
8 coils
Now, upon rearrangement of Equation (8.32W) and solving for E, realizing that G = 0.4E, we have
E =
8 FD3
(0.4)δ c d 4
(
(8)(30 N) 12 x 10
=
(
)(
−3
)
m
3
)
(0.4) 1.25 x 10 −3 m 1.75 x 10 −3 m
4
= 88.4 x 109 N/m2 = 88.4 GPa
Next, we will calculate the minimum required tensile yield strength by employing Equations (8.36W)
and (8.31W). Solving for σy, and since τy = 0.6σy the following may be written
σy =
=
−0.140 ⎤
δ c (0.4E)d ⎡
⎛ D⎞
1.60
⎥
⎜
⎟
⎢
⎝ d⎠
(0.6)πD 2 ⎢⎣
⎦⎥
(1.25 x 10−3 m)(0.4) (88.4 x 10 9 N/ m 2 )(1.75 x 10 −3 m )⎡⎢1.60 ⎛ 12 mm ⎞ −0.140 ⎤⎥
⎟
⎜
2
⎢
⎥
⎝ 1.75 mm ⎠
−3
⎣
⎦
(0.6)( π ) (12 x 10 m)
= 348 x 106 N/m2 = 348 MPa
After perusing the database on the CD-ROM or Appendix B in the textbook, it is observed
that 30 materials satisfy the two criteria that were determined above (viz. E = 88.4 GPa and σy = 348
MPa). These materials are listed below, along with their values of E, σy, %EL, and relative cost ( c ).
233
___________________________________________________
Material
Condition
E (GPa)
σ y (MPa)
%EL
c(\$ / \$)
___________________________________________________
1020 steel
Plate, CR
207
350
15
1.6
1040 steel
Plate, CR
207
490
12
1.9
1040 steel
Annealed
207
355
30.2
--
1040 steel
Normalized
207
375
28
--
4140 steel
Annealed
207
417
25.7
--
4140 steel
Bar, normalized
207
655
17.7
2.6
4140 steel
Q/T @ 315&deg;C
207
1570
11.5
--
4340 steel
Bar, annealed
207
472
22
3.5
4340 steel
Bar, normalized
207
862
12.2
4.7
4340 steel
Q/T @ 315&deg;C
207
1620
12
--
304 SS
CW, 1/4 hard
193
515
10
4.0
440A SS
Plate, annealed
200
415
20
6.7
440A SS
Q/T @ 315&deg;C
200
1650
5
--
17-7PH SS
Plate, CR
204
1210
1
12.0
17-7PH SS
Ptn. hardened
204
1310
3.5
Ductile Iron
(80-55-06)
As cast, high prod.
168
379
6
2.4
Ductile Iron
(80-55-06)
As cast, low prod.
168
379
6
5.9
Ductile Iron
(120-90-02) Q/T, high prod.
164
621
2
2.4
Ductile Iron
(120-90-02) Q/T, low prod.
164
621
2
5.9
C17200 Cu
Soln. treated/aged
128
4-10
51.4
C26000 Cu
CW, H04
110
435
8
6.0
C71500 Cu
CW, H80
150
545
3
12.9
Ti-5Al-2.5Sn
Annealed
110
760
16
157
Ti-6Al-4V
Annealed
114
830
14
132
Ti-6Al-4V
Soln. treated/aged
114
1103
10
132
Molybdenum
Sheet/rod
320
500
25
143
Tungsten
Sheet
400
760
2
111
Tungsten
Rod
400
760
2
166
Inconel 625
Annealed
207
517
42.5
234
905-1205
--
35.0
Haynes 25
--
236
445
62
135
___________________________________________________
The student should make his or her own decision as to which material would be most desirable for
this application. Consideration should be given to the magnitude of both the elastic modulus and
yield strength, in that they should be somewhat greater than the required minima, yet not excessively
greater than the minima. Furthermore, the alloy will have to be drawn into a wire, and, thus, the
ductility in percent elongation is also a parameter to be considered. And, of course cost is important,
as well as the corrosion resistance of the material; corrosion resistant issues for these various alloys
are discussed in Chapter 17. And, as called for in the problem statement, the student should justify
his or her decision.
8.D16W This problem involves a spring having 10 coils, a coil-to-coil diameter of 0.4 in., which is to
deflect no more than 0.80 in. when a tensile load of 12.9 lbf is applied. We are asked to calculate
the minimum diameter to which a cold-drawn steel wire may be drawn such that plastic deformation
of the spring wire will not occur. The spring will plastically deform when the right-hand side of
Equation (8.36W) equals the shear yield strength of the cold-drawn wire. Furthermore, the shear
yield strength is a function of wire diameter according to Equation (8.22).
When we set this
expression equal to the right-hand side of Equation (8.36W), the only unknown is the wire diameter,
d, since, from Equation (8.33W)
δc =
δs
N
=
0.80 in.
10 coils
= 0.080 in./coil
Therefore,
τy =
63,000
d0.2
−0.140 ⎤
δ Gd
δ Gd ⎡
⎛ D⎞
= c 2 Kw = c 2 ⎢1.60 ⎜ ⎟
⎥
⎝ d⎠
πD
πD ⎢⎣
⎦⎥
Now, this expression reduces to
63,000
d0.2
(
6
)
−0.140 ⎤
(0.08 in. / coil) 11.5 x 10 psi (d) ⎡
⎛ 0.40 in.⎞
⎢
⎥
⎜
⎟
=
1.60
⎝
d ⎠
π(0.40 in.)2
⎢⎣
⎥⎦
235
Or
63,000
d0.2
6
1.14
= 3.33 x 10 (d)
And
1.89 x 10-2 = (d)1.34
Finally, solving for d leads to
d = 0.052 in.
8.D17W
This problem involves a spring that is to be constructed from a 4340 steel wire 2 mm in
diameter;
the design also calls for 12 coils, a coil-to-coil diameter of 12 mm, and the spring
deflection is to be no more than 3.5 mm when a tensile load of 27 N is applied. We are asked to
specify the heat treatment for this 4340 alloy such that plastic deformation of the spring wire will not
occur. The spring will plastically deform when the right-hand side of Equation (8.36W) equals the
shear yield strength of wire. However, we must first determine the value of δc using Equation
(8.33W). Thus,
δc =
δs
N
=
3.5 mm
12 coils
= 0.292 mm/coil
Now, solving for τy
τy =
−0.140 ⎤
δ Gd ⎡
⎛ D⎞
⎢1.60 ⎜ ⎟
Kw = c
⎥
⎝ d⎠
πD2
πD2 ⎢⎣
⎦⎥
δ c Gd
−3
9
2
−3
−0.140 ⎤
0.292 x 10 m )(80 x 10 N/ m )(2 x 10 m)⎡
(
⎛ 12 mm ⎞
⎥
⎢1.60 ⎜
=
⎟
2
⎥
⎢
⎝ 2 mm ⎠
−3
⎦
⎣
(π ) (12 x 10 m)
= 129 x 106 N/m2 = 129 MPa
236
It is now possible to solve for the tensile yield strength σy as
σy =
τ
y
0.6
=
129 MPa
= 214 MPa
0.6
Thus, it is necessary to heat treat this 4340 steel in order to have a tensile yield strength of 214 MPa.
One way this could be accomplished is by first austenitizing the steel, quenching it in oil, and then
tempering it. In Figure 10.25 is shown the yield strength as a function of tempering temperature for
a 4340 alloy that has been oil quenched. From this plot, in order to achieve a yield strength of 214
MPa, tempering (for 1 h) at approximately 380&deg;C is required.
8.18W This problem asks that we compute the maximum allowable stress level to give a rupture lifetime
of 20 days for an S-590 iron component at 923 K. It is first necessary to compute the value of the
Larson-Miller parameter as follows:
(
)
T 20 + log t r = (923 K){20 + log [(20 days)(24 h/day)]}
= 20.9 x 103
From the curve in Figure 8.25W, this value of the Larson-Miller parameter corresponds to a stress
level of about 280 MPa (40,000 psi).
8.D19W We are asked in this problem to calculate the temperature at which the rupture lifetime is 200 h
when an S-590 iron component is subjected to a stress of 55 MPa (8000 psi). From the curve
shown in Figure 8.25W, at 55 MPa, the value of the Larson-Miller parameter is 26.7 x 103 (K-h).
Thus,
(
3
26.7 x 10 (K - h) = T 20 + log tr
)
= T [20 + log(200 h)]
Or, solving for T yields T = 1197 K (924&deg;C).
8.20W This problem asks that we determine, for an 18-8 Mo stainless steel, the time to rupture for a
component that is subjected to a stress of 100 MPa (14,500 psi) at 600&deg;C (873 K). From Figure
237
8.45, the value of the Larson-Miller parameter at 100 MPa is about 22.4 x 103, for T in K and tr in h.
Therefore,
(
3
22.4 x 10 = T 20 + log tr
(
= 873 20 + log tr
)
)
And, solving for tr
25.77 = 20 + log tr
which leads to tr = 4.6 x 105 h = 52 yr.
8.D21W We are asked in this problem to calculate the stress levels at which the rupture lifetime will be 1
year and 15 years when an 18-8 Mo stainless steel component is subjected to a temperature of
650&deg;C (923 K). It first becomes necessary to calculate the value of the Larson-Miller parameter for
each time. The values of tr corresponding to 1 and 15 years are 8.76 x 103 h and 1.31 x 105 h,
respectively. Hence, for a lifetime of 1 year
(
)
(
)
)
(
)
T 20 + log t r = 923 ⎣⎡20 + log 8.76 x 103 ⎤⎦ = 22.10 x 103
And for tr = 15 years
(
T 20 + log tr = 923 ⎣⎡20 + log 1.31 x 105 ⎤⎦ = 23.18 x 103
Using the curve shown in Figure 8.45, the stress values corresponding to the one- and fifteen-year
lifetimes are approximately 110 MPa (16,000 psi) and 80 MPa (11,600 psi), respectively.
8.D22W Each student or group of students is to submit their own report on a failure analysis investigation
that was conducted.
238
CHAPTER 9
PHASE DIAGRAMS
PROBLEM SOLUTIONS
9.1 Three variables that determine the microstructure of an alloy are 1) the alloying elements present, 2)
the concentrations of these alloying elements, and 3) the heat treatment of the alloy.
9.2 In order for a system to exist in a state of equilibrium the free energy must be a minimum for some
specified combination of temperature, pressure, and composition.
9.3 Diffusion occurs during the development of microstructure in the absence of a concentration gradient
because the driving force is different than for steady state diffusion as described in Section 5.3; for
the development of microstructure, the driving force is a decrease in free energy.
9.4 For the condition of phase equilibrium the free energy is a minimum, the system is completely stable
meaning that over time the phase characteristics are constant. For metastability, the system is not
at equilibrium, and there are very slight (and often imperceptible) changes of the phase
characteristics with time.
9.5
This problem asks that we cite the phase or phases present for several alloys at specified
temperatures.
(a) For an alloy composed of 15 wt% Sn-85 wt% Pb and at 100&deg;C, from Figure 9.7, α and β phases
are present, and
Cα = 5 wt% Sn-95 wt% Pb
Cβ = 98 wt% Sn-2 wt% Pb
(b) For an alloy composed of 25 wt% Pb-75 wt% Mg and at 425&deg;C, from Figure 9.18, only the α
phase is present; its composition is 25 wt% Pb-75 wt% Mg.
(c) For an alloy composed of 85 wt% Ag-15 wt% Cu and at 800&deg;C, from Figure 9.6, β and liquid
phases are present, and
Cβ = 92 wt% Ag-8 wt% Cu
CL = 77 wt% Ag-23 wt% Cu
239
(d) For an alloy composed of 55 wt% Zn-45 wt% Cu and at 600&deg;C, from Figure 9.17, β and γ phases
are present, and
Cβ = 51 wt% Zn-49 wt% Cu
Cγ = 58 wt% Zn-42 wt% Cu
(e) For an alloy composed of 1.25 kg Sn and 14 kg Pb and at 200&deg;C, we must first determine the Sn
and Pb concentrations, as
1.25 kg
&times; 100 = 8.2 wt%
1.25 kg + 14 kg
CSn =
CPb =
14 kg
&times; 100 = 91.8 wt%
1.25 kg + 14 kg
From Figure 9.7, only the α phase is present; its composition is 8.2 wt% Sn-91.8 wt% Pb.
(f) For an alloy composed of 7.6 lbm Cu and 114.4 lbm Zn and at 600&deg;C, we must first determine the
Cu and Zn concentrations, as
CCu =
C Zn =
7.6 lbm
7.6 lb + 144.4 lb
m
&times; 100 = 5.0 wt%
m
144.4 lbm
7.6 lb + 144.4 lb
m
&times; 100 = 95.0 wt%
m
From Figure 9.17, only the L phase is present; its composition is 95.0 wt% Zn-5.0 wt% Cu
(g) For an alloy composed of 21.7 mol Mg and 35.4 mol Pb and at 350&deg;C, it is first necessary to
determine the Mg and Pb concentrations, which we will do in weight percent as follows:
'
mPb
= nm A Pb = (35.4 mol)(207.2 g/mol) = 7335 g
Pb
'
mMg
= nm
Mg
A Mg = (21.7 mol)(24.3 g/mol) = 527 g
240
CPb =
7335 g
&times; 100 = 93 wt%
7335 g + 527 g
CMg = 100 wt% − 93 wt% = 7 wt%
From Figure 9.18, L and Mg2Pb phases are present, and
CL = 94 wt % Pb − 6 wt% Mg
CMg Pb = 81 wt% Pb − 19 wt% Mg
2
(h) For an alloy composed of 4.2 mol Cu and 1.1 mol Ag and at 900&deg;C, it is first necessary to
determine the Cu and Ag concentrations, which we will do in weight percent as follows:
'
mCu
= nm A Cu = (4.2 mol)(63.55 g/mol) = 266.9 g
Cu
'
mAg
= nm A Ag = (1.1 mol)(107.87 g/mol) = 118.7 g
Ag
CCu =
266.9 g
&times; 100 = 69.2 wt%
266.9 g + 118.7 g
C Ag =
118.7 g
&times; 100 = 30.8 wt%
266.9 g + 118.7 g
From Figure 9.6, α and liquid phases are present; and
Cα = 8 wt% Ag-92 w% Cu
CL = 45 wt% Ag-55 wt% Cu
9.6
This problem asks us to determine the phases present and their concentrations at several
temperatures, as an alloy of composition 52 wt% Zn- 48 wt% Cu is cooled. From Figure 9.17:
At 1000&deg;C, a liquid phase is present; W = 1.0
L
At 800&deg;C, the β phase is present, and Wβ = 1.0
At 500&deg;C, β and γ phases are present, and
241
Wγ =
C o − Cβ
C γ − Cβ
=
52 − 49
= 0.33
58 − 49
Wβ = 1.00 – 0.33 = 0.67
At 300&deg;C, the β' and γ phases are present, and
Cγ − C o
Wβ' =
C − C
γ
=
β'
59 − 52
= 0.78
59 − 50
Wγ = 1.00 – 0.78 = 0.22
9.7 This problem asks that we determine the phase mass fractions for the alloys and temperatures in
Problem 9.5.
(a)
(b)
Wα =
Cβ − C o
98 − 15
=
= 0.89
98 − 5
Cβ − C
α
Wβ =
Co − Cα 15 − 5
=
= 0.11
98 − 5
C − C
β
α
Wα = 1.0
(c)
Wβ =
WL =
(d)
Wβ =
Co − CL
C − C
β
=
L
85 − 77
= 0.53
92 − 77
Cβ − C o 92 − 85
=
= 0.47
92 − 77
Cβ − CL
Cγ − Co
C − C
γ
=
β
242
58 − 55
= 0.43
58 − 51
Wγ =
(e)
Wα = 1.0
(f)
WL = 1.0
(g)
Co − Cβ
55 − 51
= 0.57
58 − 51
=
C γ − Cβ
CL − Co
94 − 93
WMg Pb =
=
= 0.08
94 − 81
CL − CMg Pb
2
2
WL =
Co − CMg Pb
2
C
(h)
Wα =
WL =
L
− C
=
Mg2Pb
CL − Co
CL − Cα
Co − Cα
CL − C α
93 − 81
= 0.92
94 − 81
=
45 − 30.8
= 0.38
45 − 8
=
30.8 − 8
= 0.62
45 − 8
9.8 (a) In this problem we are asked to derive Equation (9.6a), which is used to convert from phase
weight fraction to phase volume fraction. Volume fraction of phase α, Vα, is defined by Equation
(9.5) as
Vα =
vα
v α + vβ
(9.S1)
where vα and vα are the volumes of the respective phases in the alloy. Furthermore, the density of
each phase is equal to the ratio of its mass and volume, or upon rearrangement
vα =
mα
ρ
243
α
(9.S2a)
vβ =
mβ
(9.S2b)
ρ
β
Substitution of these expressions into Equation (9.S1) leads to
m
α
Vα =
ρα
mα
ρ
+
α
mβ
(9.S3)
ρ
β
in which m's and ρ's denote masses and densities, respectively. Now, the mass fractions of the α
and β phases (i.e., Wα and Wβ) are defined in terms of the phase masses as
Wα =
Wβ =
mα
mα + mβ
mβ
+ m
m
α
(9.S4a)
(9.S4b)
β
Which, upon rearrangement yield
mα = Wα ⎛ mα + mβ ⎞
⎝
⎠
(9.S5a)
mβ = Wβ ⎛m α + mβ ⎞
⎝
⎠
(9.S5b)
Incorporation of these relationships into Equation (9.S3) leads to the desired expression
W
α
Vα =
ρα
Wα
ρ
α
+
Wβ
(9.S6)
ρ
β
(b) For this portion of the problem we are asked to derive Equation (9.7a), which is used to convert from
phase volume fraction to phase mass fraction. Mass fraction of the α phase, Wα, is defined as
244
Wα =
mα
mα + mβ
(9.S7)
From Equations (9.S2a) and (9.S2b)
mα = v αρ α
(9.S8a)
mβ = v βρβ
(9.S8b)
Substitution of these expressions into Equation (9.S7) yields
Wα =
vα ρ α
v αρα + v βρβ
(9.S9)
From Equation (9.S1) and its equivalent for Vβ the following may be written
v α = Vα ⎛ vα + vβ ⎞
⎝
⎠
(9.S10a)
v β = Vβ ⎛ vα + vβ ⎞
⎝
⎠
(9.S10b)
Substitution of Equations (9.S10a) and (9.S10b) into Equation (9.S9) yields the desired expression
Wα =
Vαρ α
Vαρ α + Vβρβ
(9.S11)
9.9 This problem asks that we determine the phase volume fractions for the alloys and temperatures in
Problems 9.5a, b, and d.
This is accomplished by using the technique illustrated in Example
Problem 9.3, and the results of Problems 9.5 and 9.7.
(a) This is a Sn-Pb alloy at 100&deg;C, wherein
Cα = 5 wt% Sn-95 wt% Pb
Cβ = 98 wt% Sn-2 wt% Pb
Wα = 0.89
Wβ = 0.11
245
ρSn = 7.29 g/cm3
ρPb = 11.27 g/cm3
Using these data it is first necessary to compute the densities of the α and β phases using Equation
(4.10a). Thus
ρα =
CSn(α )
100
+
ρ
Sn
CPb(α )
ρ
Pb
100
=
5
+
7.29 g / cm3
ρβ =
= 10.97 g/cm3
95
11.27 g / cm3
100
C Sn(β)
ρ
+
Sn
CPb(β)
ρ
Pb
100
=
98
7.29 g / cm3
+
2
= 7.34 g/cm3
11.27 g / cm3
Now we may determine the Vα and Vβ values using Equation 9.6. Thus,
Wα
ρ
α
Vα =
Wβ
Wα
+
ρ
ρβ
α
0.89
=
10.97 g/ cm3
= 0.84
0.89
0.11
+
10.97 g / cm3
7.34 g / cm3
246
W
β
ρβ
Vβ =
Wβ
Wα
+
ρ
ρ
β
α
0.11
=
7.34 g / cm3
= 0.16
0.11
0.89
+
7.34 g / cm3
10.97 g / cm3
(b) This is a Pb-Mg alloy at 425&deg;C, wherein only the α phase is present. Therefore, Vα = 1.0.
(d) This is a Zn-Cu alloy at 600&deg;C, wherein
Cβ = 51 wt% Zn-49 wt% Cu
Cγ = 58 wt% Zn-42 wt% Cu
Wβ = 0.43
Wγ = 0.57
ρZn = 6.67 g/cm3
ρCu = 8.68 g/cm3
Using this data it is first necessary to compute the densities of the β and γ phases. Thus
ρβ =
100
C Zn(β)
ρ
=
+
Zn
CCu(β)
ρ
Cu
100
51
6.67 g / cm3
ργ =
+
= 7.52 g/cm 3
49
8.68 g / cm3
100
CZn( γ)
ρ
Zn
247
+
C Cu(γ )
ρ
Cu
100
=
58
6.67 g / cm3
= 7.39 g/cm 3
42
+
8.68 g / cm3
Now we may determine the Vβ and Vγ values using Equation (9.6). Thus,
W
β
Vβ =
ρβ
Wβ
+
ρ
β
Wγ
ρ
γ
0.43
=
7.52 g / cm3
= 0.43
0.57
0.43
+
7.39 g / cm3
7.52 g/ cm3
W
γ
Vγ =
ργ
Wβ
ρ
β
+
Wγ
ρ
γ
0.57
=
7.39 g / cm3
= 0.57
0.57
0.43
+
7.39 g / cm3
7.52 g/ cm3
9.10 (a) Spreading salt on ice will lower the melting temperature, since the liquidus line decreases from
0&deg;C to the eutectic temperature at about -21&deg;C. Thus, ice at a temperature below 0&deg;C (and above
-21&deg;C) can be made to form a liquid phase by the addition of salt.
(b) We are asked to compute the concentration of salt necessary to have a 50% ice-50% brine
solution at -10&deg;C (14&deg;F). At -10&deg;C,
C
C
ice
= 0 wt% NaCl-100 wt% H O
2
brine
= 13 wt% NaCl-87 wt% H O
2
Thus,
248
Wice = 0.5 =
Cbrine − Co
Cbrine − Cice
=
13 − Co
13 − 0
Solving for C (the concentration of salt) yields a value of 6.5 wt% NaCl-93.5 wt% H O.
o
2
9.11 (a) This part of the problem calls for us to cite the temperature to which a 90 wt% Pb-10 wt% Sn
alloy must be heated in order to have 50% liquid. Probably the easiest way to solve this problem is
by trial and error--that is, moving vertically at the given composition, through the α + L region until
the tie-line lengths on both sides of the given composition are the same (Figure 9.7). This occurs at
approximately 300&deg;C (570&deg;F).
(b) We can also produce a 50% liquid solution at 250&deg;C, by adding Sn to the alloy. At 250&deg;C and
within the α + L phase region
Cα = 13 wt% Sn-87 wt% Pb
CL = 39 wt% Sn-61 wt% Pb
Let C be the new alloy composition to give Wα = WL = 0.5. Then,
o
Wα = 0.5 =
And solving for C
o
CL − Co
CL − C α
=
gives 26 wt% Sn. Now, let m
39 − C o
39 − 13
Sn
be the mass of Sn added to the alloy to
achieve this new composition. The amount of Sn in the original alloy is
(0.10)(1.5 kg) = 0.15 kg
Then, using a modified form of Equation (4.3)
⎡0.15 kg + m ⎤
Sn
⎥ &times; 100 = 26
⎢
1.5
kg
+
m
⎢⎣
Sn ⎥⎦
And, solving for m
Sn
yields m
Sn
= 0.324 kg.
9.12 (a) We are asked to determine how much sugar will dissolve in 1000 g of water at 80&deg;C. From the
solubility limit curve in Figure 9.1, at 80&deg;C the maximum concentration of sugar in the syrup is about
74 wt%. It is now possible to calculate the mass of sugar using Equation (4.3) as
249
msugar
C sugar (wt%) =
74 wt% =
m
sugar
+ m
&times; 100
water
msugar
msugar + 1000 g
&times; 100
Solving for msugar yields msugar = 2846 g
(b) Again using this same plot, at 20&deg;C the solubility limit (or the concentration of the saturated
solution) is about 64 wt% sugar.
(c) The mass of sugar in this saturated solution at 20&deg;C (msugar') may also be calculated using
Equation (4.3) as follows:
64 wt% =
msugar '
m
sugar
' + 1000 g
&times; 100
which yields a value for msugar' of 1778 g. Subtracting the latter from the former of these sugar
concentrations yields the amount of sugar that precipitated out of the solution upon cooling
msugar&quot;; that is
msugar&quot; = msugar - msugar' = 2846 g - 1778 g = 1068 g
9.13 This problem asks us to consider a specimen of ice I which is at -10&deg;C and 1 atm pressure.
(a)
In order to determine the pressure at which melting occurs at this temperature, we move
vertically at this temperature until we cross the Ice I-Liquid phase boundary of Figure 9.33. This
occurs at approximately 570 atm; thus the pressure of the specimen must be raised from 1 to 570
atm.
(b) In order to determine the pressure at which sublimation occurs at this temperature, we move
vertically downward from 1 atm until we cross the Ice I-Vapor phase boundary of Figure 9.33. This
intersection occurs at approximately 0.0023 atm.
9.14 The melting and boiling temperatures for ice I at a pressure of 0.01 atm may be determined by
moving horizontally across the pressure-temperature diagram of Figure 9.33 at this pressure. The
temperature corresponding to the intersection of the Ice I-Liquid phase boundary is the melting
temperature, which is approximately 1&deg;C. On the other hand, the boiling temperature is at the
intersection of the horizontal line with the Liquid-Vapor phase boundary--approximately 28&deg;C.
250
9.15 (a) This portion of the problem asks that we calculate, for a Pb-Mg alloy, the mass of lead in 7.5 kg
of the solid α phase at 300&deg;C just below the solubility limit. From Figure 9.18, the composition of an
alloy at this temperature is about 17 wt% Pb. Therefore, the mass of Pb in the alloy is just (0.17)(7.5
kg) = 1.3 kg.
(b) At 400&deg;C, the solubility limit of the α phase increases to approximately 32 wt% Pb. In order to
determine the additional amount of Pb that may be added (mPb'), we utilize a modified form of
Equation (4.3) as
CPb = 32 wt% =
1.3 kg + mPb'
7.5 kg + mPb'
&times; 100
Solving for mPb' yields mPb' = 1.62 kg.
9.16
(a)
Coring is the phenomenon whereby concentration gradients exist across grains in
polycrystalline alloys, with higher concentrations of the component having the lower melting
temperature at the grain boundaries. It occurs, during solidification, as a consequence of cooling
rates that are too rapid to allow for the maintenance of the equilibrium composition of the solid
phase.
(b) One undesirable consequence of a cored structure is that, upon heating, the grain boundary
regions will melt first and at a temperature below the equilibrium phase boundary from the phase
diagram; this melting results in a loss in mechanical integrity of the alloy.
9.17 This problem asks if a noncold-worked Cu-Ni solid solution alloy is possible having a minimum
tensile strength of 380 MPa (55,000 psi) and also a ductility of at least 45%EL. From Figure 9.5a, a
tensile strength greater than 380 MPa is possible for compositions between about 34 and 87 wt% Ni.
On the other hand, according to Figure 9.5b, ductilities greater than 45%EL exist for compositions
less than about 7 wt% and greater than about 71 wt% Ni. Therefore, the stipulated criteria are met
for all compositions between 71 and 87 wt% Ni.
9.18
It is not possible to have a Cu-Ni alloy, which at equilibrium, consists of a liquid phase of
composition 20 wt% Ni-80 wt% Cu and an α phase of composition 37 wt% Ni-63 wt% Cu. From
Figure 9.2a, a single tie line does not exist within the α + L region that intersects the phase
boundaries at the given compositions. At 20 wt% Ni, the L-(α + L) phase boundary is at about
1200&deg;C, whereas at 37 wt% Ni the (L + α)-α phase boundary is at about 1230&deg;C.
251
9.19 It is possible to have a Cu-Ag alloy, which at equilibrium consists of an α phase of composition 5
wt% Ag-95 wt% Cu and a β phase of composition 95 wt% Ag-5 wt% Cu. From Figure 9.6 a
horizontal tie can be constructed across the α + β region at 690&deg;C which intersects the α−(α + β)
phase boundary at 5 wt% Ag, and also the (α + β)-β phase boundary at 95 wt% Ag.
9.20 Upon heating a lead-tin alloy of composition 30 wt% Sn-70 wt% Pb from 150&deg;C and utilizing Figure
9.7:
(a) the first liquid forms at the temperature at which a vertical line at this composition intersects the
eutectic isotherm--i.e., at 183&deg;C;
(b) the composition of this liquid phase corresponds to the intersection with the (α + L)-L phase
boundary, of a tie line constructed across the α + L phase region just above this eutectic isotherm-i.e., CL = 61.9 wt% Sn;
(c) complete melting of the alloy occurs at the intersection of this same vertical line at 30 wt% Sn
with the (α + L)-L phase boundary--i.e., at about 260&deg;C;
(d)
the composition of the last solid remaining prior to complete melting corresponds to the
intersection with α-(α + L) phase boundary, of the tie line constructed across the α + L phase region
at 260&deg;C--i.e., Cα is about 13 wt% Sn.
9.21 Upon cooling a 50 wt% Ni-50 wt% Cu alloy from 1400&deg;C and utilizing Figure 9.2a:
(a)
The first solid phase forms at the temperature at which a vertical line at this composition
intersects the L-(α + L) phase boundary--i.e., at about 1320&deg;C;
(b) The composition of this solid phase corresponds to the intersection with the L-(α + L) phase
boundary, of a tie line constructed across the α + L phase region at 1320&deg;C--i.e., Cα = 62 wt% Ni-38
wt% Cu;
(c) Complete solidification of the alloy occurs at the intersection of this same vertical line at 50 wt%
Ni with the (α + L)-α phase boundary--i.e., at about 1270&deg;C;
(d) The composition of the last liquid phase remaining prior to complete solidification corresponds to
the intersection with the L-(α + L) boundary, of the tie line constructed across the α + L phase region
at 1270&deg;C--i.e., CL is about 37 wt% Ni-63 wt% Cu.
9.22 (a) In order to determine the temperature of a 65 wt% Ni-35 wt% Cu alloy for which α and liquid
phases are present with the α phase of composition 70 wt% Ni, we need to construct a tie line
across the α + L phase region of Figure 9.2a that intersects the solidus line at 70 wt% Ni; this is
(b) The composition of the liquid phase at this temperature is determined from the intersection of
this same tie line with liquidus line, which corresponds to about 59 wt% Ni.
252
(c) The mass fractions of the two phases are determined using the lever rule, Equations (9.1) and
(9.2) with Co = 65 wt% Ni, CL = 59 wt% Ni, and Cα = 70 wt% Ni, as
Wα =
WL =
C o − CL
Cα − CL
Cα − Co
C
α
− C
=
65 − 59
= 0.55
70 − 59
=
70 − 65
= 0.45
70 − 59
L
9.23 The copper-gold phase diagram is constructed below.
9.24 (a) We are given that the mass fractions of α and liquid phases are both 0.5 for a 40 wt% Pb-60
wt% Mg alloy and asked to estimate the temperature of the alloy. Using the appropriate phase
diagram, Figure 9.18, by trial and error with a ruler, a tie line within the α + L phase region that is
divided in half for an alloy of this composition exists at about 540&deg;C.
(b) We are now asked to determine the compositions of the two phases. This is accomplished by
noting the intersections of this tie line with both the solidus and liquidus lines.
intersections, Cα = 26 wt% Pb, and CL = 54 wt% Pb.
From these
9.25 The problem is to solve for compositions at the phase boundaries for both α and β phases (i.e., Cα
and Cβ). We may set up two independent lever rule expressions, one for each composition, in terms
of Cα and Cβ as follows:
253
Wα1 = 0.57 =
Wα 2 = 0.14 =
C β − Co1
C β − Cα
=
C β − 60
Cβ − Cα
C β − Co 2
Cβ − 30
=
Cβ − Cα
Cβ − Cα
In these expressions, compositions are given in weight percent A. Solving for Cα and Cβ from these
equations, yield
Cα = 90 (or 90 wt% A-10 wt% B)
Cβ = 20.2 (or 20.2 wt% A-79.8 wt% B)
9.26 For this problem
Co = 55 (or 55 wt% B-45 wt% A)
Cβ = 90 (or 90 wt% B-10 wt% A)
Wα = Wβ = 0.5
If we set up the lever rule expression for Wα
Wα = 0.5 =
Cβ − Co
Cβ − C α
=
90 − 55
90 − C α
And solving for Cα
Cα = 20 (or 20 wt% B-80 wt% A)
9.27 Yes, it is possible to have a Cu-Ag alloy of composition 20 wt% Ag-80 wt% Cu which consists of
mass fractions Wα = 0.80 and WL = 0.20. Using the appropriate phase diagram, Figure 9.6, by trial
and error with a ruler, the tie-line segments within the α + L phase region are proportioned such that
Wα = 0.8 =
254
CL − Co
CL − Cα
for Co = 20 wt% Ag. This occurs at about 800&deg;C.
9.28 It is not possible to have a 50 wt% Pb-50 wt% Mg alloy which has masses of 5.13 kg and 0.57 kg
for the α and Mg2Pb phases, respectively. In order to demonstrate this, it is first necessary to
determine the mass fraction of each phase as follows:
Wα =
mα
mα + mMg Pb
2
=
5.13 kg
= 0.90
5.13 kg + 0.57 kg
WMg Pb = 1.00 − 0.90 = 0.10
2
Now, if we apply the lever rule expression for Wα
Wα =
C Mg Pb − C o
2
C
Mg 2Pb
− C
α
Since the Mg2Pb phase exists only at 81 wt% Pb, and Co = 50 wt% Pb
Wα = 0.90 =
81 − 50
81 − C α
Solving for Cα from this expression yields Cα = 46.6 wt% Pb. From Figure 9.18, the maximum
concentration of Pb in the α phase in the α + Mg2Pb phase field is about 42 wt% Pb. Therefore, this
alloy is not possible.
9.29 (a) From Figure 9.6, the maximum solubility of Cu in Ag at 700&deg;C corresponds to the position of the
β-(α + β) phase boundary at this temperature, or to about 6 wt% Cu.
(b) From this same figure, the maximum solubility of Ag in Cu corresponds to the position of the α(α + β) phase boundary at this temperature, or about 5 wt% Ag.
9.30 We are asked to determine the approximate temperature from which a Pb-Mg alloy was quenched,
given the mass fractions of α and Mg Pb phases. We can write a lever-rule expression for the mass
2
fraction of the α phase as
255
CMg Pb − Co
2
Wα = 0.65 =
C
Mg 2Pb
− C
α
is 81 wt% Pb-19 wt% Mg, which
The value of C is stated as 45 wt% Pb-55 wt% Mg, and C
Mg2Pb
o
is independent of temperature (Figure 9.18); thus,
81 − 45
81 − C α
0.65 =
which yields
Cα = 25.6 wt% Pb
The temperature at which the α-(α + Mg2Pb) phase boundary (Figure 9.18) has a value of 25.6 wt%
9.31 This problem asks if it is possible to have a Mg-Pb alloy for which the mass fractions of primary α
and total α are 0.60 and 0.85, respectively, at 460&deg;C. In order to make this determination we need
to set up the appropriate lever rule expression for each of these quantities. From Figure 9.18 and at
460&deg;C, Cα = 41 wt% Pb, CMg Pb = 81 wt% Pb, and Ceutectic = 67 wt% Pb.
2
For primary α
Wα' =
Ceutectic − Co
Ceutectic − C α
=
67 − Co
67 − 41
= 0.60
Solving for Co gives Co = 51.4 wt% Pb.
Now the analogous expression for total α
Wα =
C Mg Pb − C o
2
C
Mg 2Pb
− C
α
=
81 − C o
= 0.85
81 − 41
And this value of Co is 47 wt% Pb. Therefore, since these two Co values are different, this alloy is
not possible.
9.32 This problem asks if it is possible to have a Pb-Sn alloy for which the masses of primary β and total
β are 2.21 and 2.53 kg, respectively in 2.8 kg total of the alloy at 180&deg;C. In order to make this
determination we first need to convert these masses to mass fractions. Thus,
256
Wβ' =
2.21 kg
= 0.789
2.8 kg
Wβ =
2.53 kg
= 0.904
2.8 kg
Next it is necessary to set up the appropriate lever rule expression for each of these quantities.
From Figure 9.7 and at 180&deg;C, Cα = 18.3 wt% Sn, Cβ = 97.8 wt% Sn, and Ceutectic = 61.9 wt% Sn.
For primary β
Wβ' =
C o − Ceutectic
C − C
β
=
eutectic
C o − 61.9
97.8 − 61.9
= 0.789
Solving for Co gives Co = 90.2 wt% Sn.
Now the analogous expression for total β
Wβ =
Co − Cα
C
β
− C
=
α
Co − 18.3
97.8 − 18.3
= 0.904
And this value of Co is also 90.2 wt% Sn. Therefore, since these two Co values are identical, this
alloy is possible.
9.33 (a) This portion of the problem asks that we determine the mass fractions of α and β phases for an
80 wt% Sn-20 wt% Pb alloy (at 180&deg;C). In order to do this it is necessary to employ the lever rule
using a tie line that extends entirely across the α + β phase field (Figure 9.7), as follows:
Wα =
Wβ =
C β − Co
Cβ − Cα
Co − Cα
C
β
− C
α
=
97.8 − 80
= 0.224
97.8 − 18.3
=
80 − 18.3
= 0.776
97.8 − 18.3
(b) Now it is necessary to determine the mass fractions of primary β and eutectic microconstituents
for this same alloy. This requires us to utilize the lever rule and a tie line that extends from the
257
maximum solubility of Pb in the β phase at 180&deg;C (i.e., 97.8 wt% Sn) to the eutectic composition
(61.9 wt% Sn). Thus
Wβ' =
We =
C o − Ceutectic
β
80.0 − 61.9
= 0.504
97.8 − 61.9
=
C − C
eutectic
Cβ − Co
Cβ − Ceutectic
=
97.8 − 80.0
= 0.496
97.8 − 61.9
(c) And, finally, we are asked to compute the mass fraction of eutectic β, Weβ. This quantity is
simply the difference between the mass fractions of total β and primary β as
Weβ = Wβ - Wβ' = 0.776 - 0.504 = 0.272
9.34 This problem asks that we determine the composition of a Cu-Ag alloy at 775&deg;C given that Wα' =
0.73 and Weutectic = 0.27. Since there is a primary α microconstituent present, we know that the
alloy composition, Co is between 8.0 and 71.9 wt% Ag (Figure 9.6). Furthermore, this figure also
indicates that Cα = 8.0 wt% Ag and Ceutectic = 71.9 wt% Ag. Applying the appropriate lever rule
expression for Wα'
Wα' =
Ceutectic − C o
71.9 − C o
=
= 0.73
Ceutectic − Cα
71.9 − 8.0
and solving for Co yields Co = 25.2 wt% Ag.
9.35 We are given a hypothetical eutectic phase diagram for which Ceutectic = 64 wt% B, Cα = 12 wt% B
at the eutectic temperature, and also that Wβ' = 0.367 and Wβ = 0.768; from this we are asked to
determine the composition of the alloy. Let us write lever rule expressions for Wβ' and Wβ
Wβ =
Wβ' =
C o − Cα
C
β
− C
=
α
Co − 12
C − 12
= 0.768
β
C o − C eutectic
Co − 64
=
= 0.367
C − 64
C −C
β
eutectic
258
β
Thus, we have two simultaneous equations with Co and Cβ as unknowns. Solving them for Co
gives Co = 75 wt% B.
9.36 Upon solidification, an alloy of eutectic composition forms a microstructure consisting of alternating
layers of the two solid phases because during the solidification atomic diffusion must occur, and with
this layered configuration the diffusion path length for the atoms is a minimum.
9.37 Schematic sketches of the microstructures that would be observed for an 64 wt% Zn-36 wt% Cu
alloy at temperatures of 900&deg;C, 820&deg;C, 750&deg;C, and 600&deg;C are shown below.
The phase
compositions are also indicated.
9.38 Schematic sketches of the microstructures that would be observed for a 76 wt% Pb-24 wt% Mg
alloy at temperatures of 575&deg;C, 500&deg;C, 450&deg;C, and 300&deg;C are shown below.
compositions are also indicated.
259
The phase
9.39 Schematic sketches of the microstructures that would be observed for a 52 wt% Zn-48 wt% Cu alloy
at temperatures of 950&deg;C, 860&deg;C, 800&deg;C, and 600&deg;C are shown below. The phase compositions are
also indicated.
260
9.40
The principal difference between congruent and incongruent phase transformations is that for
congruent no compositional changes occur with any of the phases that are involved in the
transformation. For incongruent there will be compositional alterations of the phases.
9.41 In this problem we are asked to specify temperature-composition points for all eutectics, eutectoids,
peritectics, and congruent phase transformations for the tin-gold system.
There are two eutectics on this phase diagram. One exists at 10 wt% Au-90 wt% Sn and
217&deg;C. The reaction upon cooling is
L → α + β
The other eutectic exists at 80 wt% Au-20 wt% Sn and 280&deg;C. This reaction upon cooling is
L → δ + ζ
There are three peritectics. One exists at 30 wt% Au-70 wt% Sn and 252&deg;C. Its reaction
upon cooling is as follows:
L + γ → β
The second peritectic exists at 45 wt% Au-55 wt% Sn and 309&deg;C. This reaction upon cooling is
L + δ → γ
The third peritectic exists at 92 wt% Au-8 wt% Sn and 490&deg;C. This reaction upon cooling is
L + η → ζ
There is one congruent melting point at 62.5 wt% Au-37.5 wt% Sn and 418&deg;C. Its reaction
upon cooling is
L → δ
No eutectoids are present.
261
9.42 In this problem we are asked to specify temperature-composition points for all eutectics, eutectoids,
peritectics, and congruent phase transformations for a portion of the aluminum-copper phase
diagram.
There is one eutectic on this phase diagram, which exists at 8.3 wt% Al-91.7 wt% Cu and
1036&deg;C. Its reaction upon cooling is
L → α + β
There are four eutectoids for this system. One exists at 11.8 wt% Al-88.2 wt% Cu and
565&deg;C. This reaction upon cooling is
β → α + γ2
Another eutectoid exists at 15.4 wt% Al-84.6 wt% Cu and 964&deg;C. For cooling the reaction is
χ → β + γ1
A third eutectoid exists at 15.5 wt% Al-84.5 wt% Cu and 786&deg;C. For cooling the reaction is
γ1 → β + γ 2
The other eutectoid exists at 23.5 wt% Al-76.5 wt% Cu and 560&deg;C. For cooling the reaction is
ε 2 → δ + ζ1
There are four peritectics on this phase diagram. One exists at 15.3 wt% Al-84.7 wt% Cu
and 1037&deg;C. The reaction upon cooling is
β + L → χ
Another peritectic exists at 17 wt% Al-83 wt% Cu and 1021&deg;C. It's cooling reaction is
χ + L → γ1
Another peritectic exists at 20.5 wt% Al-79.5 wt% Cu and 961&deg;C. The reaction upon cooling is
262
γ 1 + L → ε1
Another peritectic exists at 28.4 wt% Al-71.6 wt% Cu and 626&deg;C. The reaction upon cooling is
ε 2 + L → η1
There is a single congruent melting point that exists at 12.5 wt% Al-87.5 wt% Cu and
1049&deg;C. The reaction upon cooling is
L → β
9.43W This problem asks for us to compute the maximum number of phases that may be present for a
ternary system assuming that pressure is held constant. For a ternary system (C = 3) at constant
pressure (N = 1), Gibbs phase rule, Equation (9.1W), becomes
P+F=C+N=3+1=4
Or,
P=4-F
Thus, when F = 0, P will have its maximum value of 4, which means that the maximum number of
phases present for this situation is 4.
9.44W We are asked to specify the value of F for Gibbs phase rule at points A, B, and C on the pressuretemperature diagram for H2O. Gibbs phase rule in general form is
P+F=C+N
For this system, the number of components, C, is 1, whereas N, the number of noncompositional
variables, is 2--viz. temperature and pressure. Thus, the phase rule now becomes
P+F=1+2=3
Or
F=3-P
where P is the number of phases present at equilibrium.
At point A, only a single (liquid) phase is present (i.e., P = 1), or
263
F=3-P=3-1=2
which means that both temperature and pressure are necessary to define the system.
At point B which is on the phase boundary between liquid and vapor phases, two phases are
in equilibrium (P = 2); hence
F=3-P=3-2=1
Or that we need to specify the value of either temperature or pressure, which determines the value
of the other (pressure or temperature).
And, finally, at point C, three phases are present—viz. ice I, vapor, and liquid—and the
number of degrees of freedom is zero since
F=3-P=3-3=0
Thus, point C is an invariant point (in this case a triple point), and we have no choice in the selection
of externally controllable variables in order to define the system.
9.45 Below is shown the phase diagram for these two A and B metals.
264
9.46 This problem gives us the compositions in weight percent for the two intermetallic compounds AB
and AB2, and then asks us to identify element B if element A is potassium. Probably the easiest
way to solve this problem is to first compute the ratio of the atomic weights of these two elements
using Equation (4.6a); then, since we know the atomic weight of potassium (39.10 g/mol), it is
possible to determine the atomic weight of element B, from which an identification may be made.
First of all, consider the AB intermetallic compound; inasmuch as it contains the same
numbers of A and B atoms, its composition in atomic percent is 50 at% A-50 at% B. Equation (4.6a)
may be written in the form:
'
CB
=
C A
B A
&times; 100
+ C A
C A
A B
B A
where AA and AB are the atomic weights for elements A and B, and CA and CB are their
compositions in weight percent. For this AB compound, and making the appropriate substitutions
into the above equation leads to
50 at% B =
(65.7 wt% B)(A A )
&times; 100
(34.3 wt % A)(A ) + (65.7 wt% B)(A )
B
A
Now, solving this expression yields,
AB = 1.916 AA
Since potassium is element A and it has an atomic weight of 39.10 g/mol, the atomic weight of
element B is just
AB = (1.916)(39.10 g/mol) = 74.92 g/mol
Upon consultation of the period table of the elements (Figure 2.6) we note that arsenic has an atomic
weight of 74.92 g/mol; therefore, element B is arsenic.
9.47 This problem asks that we compute the mass fractions of ferrite and cementite in pearlite. The
lever-rule expression for ferrite is
Wα =
CFe C − C o
3
C
Fe 3C
265
− C
α
and, since C
Fe3C
= 6.70 wt% C, C = 0.76 wt% C, and Cα = 0.022 wt% C
o
Wα =
6.70 − 0.76
= 0.89
6.70 − 0.022
Similarly, for cementite
Co − Cα
0.76 − 0.022
WFe C =
=
= 0.11
6.70 − 0.022
C
−
C
3
Fe C
α
3
9.48
A phase is a homogeneous portion of the system having uniform physical and chemical
characteristics, whereas a microconstituent is an identifiable element of the microstructure (that
may consist of more than one phase).
9.49 (a) A hypoeutectoid steel has a carbon concentration less than the eutectoid; on the other hand,
a hypereutectoid steel has a carbon content greater than the eutectoid.
(b) For a hypoeutectoid steel, the proeutectoid ferrite is a microconstituent that formed above the
eutectoid temperature. The eutectoid ferrite is one of the constituents of pearlite that formed at a
temperature below the eutectoid. The carbon concentration for both ferrites is 0.022 wt% C.
9.50
A proeutectoid phase normally forms along austenite grain boundaries because there is an
interfacial energy associated with these boundaries.
When a proeutectoid phase forms within
austenite, an interfacial energy also exists at the interface between the two phases. A lower net
interfacial energy increase results when the proeutectoid phase forms along the existing austenite
grain boundaries than when the proeutectoid phase forms within the interior of the grains.
9.51 This problem asks that we compute the carbon concentration of an iron-carbon alloy for which the
fraction of total ferrite is 0.94. Application of the lever rule [of the form of Equation (9.12)] yields
Wα = 0.94 =
CFe C − Co'
3
CFe C − C α
3
and solving for C 'o
266
=
6.70 − Co'
6.70 − 0.022
Co' = 0.42 wt% C
9.52 In this problem we are given values of Wα and WFe C (0.86 and 0.14, respectively) for an iron3
carbon alloy and then are asked to specify the proeutectoid phase. Employment of the lever rule for
Wα = 0.86 =
CFe C − Co
3
C
Fe 3C
− C
α
=
6.70 − Co
6.70 − 0.022
Now, solving for Co, the alloy composition, leads to Co = 0.96 wt% C. Therefore, the proeutectoid
phase is Fe3C since Co is greater than 0.76 wt% C.
9.53 This problem asks us to consider various aspects of 1.0 kg of austenite containing 1.15 wt% C that
is cooled to below the eutectoid.
(a) The proeutectoid phase will be Fe C since 1.15 wt% C is greater than the eutectoid (0.76 wt%
3
C).
(b) For this portion of the problem, we are asked to determine how much total ferrite and cementite
form. Application of the appropriate lever rule expression yields
Wα =
CFe C − C o
3
C
Fe 3C
=
− C
α
6.70 − 1.15
= 0.83
6.70 − 0.022
which, when multiplied by the total mass of the alloy (1.0 kg), gives 0.83 kg of total ferrite.
Similarly, for total cementite,
Co − Cα
1.15 − 0.022
WFe C =
=
= 0.17
6.70 − 0.022
CFe C − Cα
3
3
And the mass of total cementite that forms is (0.17)(1.0 kg) = 0.17 kg.
(c) Now we are asked to calculate how much pearlite and the proeutectoid phase (cementite) form.
Applying Equation (9.20), in which C1' = 1.15 wt% C
Wp =
6.70 − C '
1 = 6.70 − 1.15 = 0.93
6.70 − 0.76
6.70 − 0.76
267
which corresponds to a mass of 0.93 kg. Likewise, from Equation (9.21)
WFe C' =
3
C ' − 0.76
1
5.94
=
1.15 − 0.76
= 0.07
5.94
which is equivalent to 0.07 kg of the total 1 kg mass.
(d) Schematically, the microstructure would appear as:
9.54 We are called upon to consider various aspects of 2.5 kg of austenite containing 0.65 wt% C, that is
cooled to below the eutectoid.
(a) Ferrite is the proeutectoid phase since 0.65 wt% C is less than 0.76 wt% C.
(b) For this portion of the problem, we are asked to determine how much total ferrite and cementite
form. Application of the appropriate lever rule expression yields
Wα =
CFe C − C o
3
C
Fe 3C
− C
=
α
6.70 − 0.65
= 0.91
6.70 − 0.022
which corresponds to (0.91)(2.5 kg) = 2.26 kg of total ferrite.
Similarly, for total cementite,
Co − Cα
0.65 − 0.022
WFe C =
=
= 0.09
6.70 − 0.022
CFe C − Cα
3
3
Or (0.09)(2.5 kg) = 0.24 kg of total cementite form.
(c) Now consider the amounts of pearlite and proeutectoid ferrite. Using Equation (9.18)
Wp =
C o' − 0.022
0.74
=
0.65 − 0.022
= 0.85
0.74
268
This corresponds to (0.85)(2.5 kg) = 2.12 kg of pearlite.
Also, from Equation (9.19),
Wα ' =
0.76 − 0.65
= 0.15
0.74
Or, there are (0.15)(2.5 kg) = 0.38 kg of proeutectoid ferrite.
(d) Schematically, the microstructure would appear as:
9.55 The mass fractions of proeutectoid ferrite and pearlite that form in a 0.25 wt% C iron-carbon alloy
are considered in this problem. From Equation (9.18)
Wp =
Co' − 0.022
0.74
=
0.25 − 0.022
= 0.31
0.74
And, from Equation (9.19)
Wα' =
0.76 − C o'
0.76 − 0.25
=
= 0.69
0.74
0.74
9.56 This problem asks that we determine the carbon concentration in an iron-carbon alloy, given the
mass fractions of proeutectoid ferrite and pearlite (0.286 and 0.714, respectively). From Equation
(9.18)
Wp = 0.714 =
Co' − 0.022
269
0.74
which yields C 'o = 0.55 wt% C.
9.57 In this problem we are given values of Wα and WFe C for an iron-carbon alloy (0.91 and 0.09,
3
respectively), and then are asked to specify whether the alloy is hypoeutectoid or hypereutectoid.
Employment of the lever rule for total α leads to
Wα = 0.91 =
CFe C − Co
3
C
Fe3 C
− C
α
=
6.70 − C o
6.70 − 0.022
Now, solving for Co, the alloy composition, leads to Co = 0.62 wt% C. Therefore, the alloy is
hypoeutectoid since Co is less than 0.76 wt% C.
9.58 We are asked in this problem to determine the concentration of carbon in an alloy for which WFe C'
3
= 0.11 and Wp = 0.89. If we let Co equal the carbon concentration in the alloy, employment of the
appropriate lever rule expression, Equation (9.20), leads to
Wp =
6.7 − C o
= 0.89
6.7 − 0.76
Solving for Co yields Co = 1.41 wt% C.
9.59 In this problem we are asked to consider 2.0 kg of a 99.6 wt% Fe-0.4 wt% C alloy that is cooled to a
temperature below the eutectoid.
(a) Equation (9.19) must be used in computing the amount of proeutectoid ferrite that forms. Thus,
Wα' =
0.76 − C o'
0.76 − 0.40
=
= 0.49
0.74
0.74
Or, (0.49)(2.0 kg) = 0.99 kg of proeutectoid ferrite forms.
(b) In order to determine the amount of eutectoid ferrite, it first becomes necessary to compute the
amount of total ferrite using the lever rule applied entirely across the α + Fe3C phase field, as
Wα =
CFe C − C o'
3
CFe C − Cα
3
=
6.70 − 0.40
= 0.94
6.70 − 0.022
270
which corresponds to (0.94)(2.0 kg) = 1.89 kg. Now, the amount of eutectoid ferrite is just the
difference between total and proeutectoid ferrites, or
1.89 kg - 0.99 kg = 0.90 kg
(c) With regard to the amount of cementite that forms, again application of the lever rule across the
entirety of the α + Fe3C phase field, leads to
Co' − Cα
0.40 − 0.022
=
= 0.06
WFe C =
CFe C − Cα
6.70 − 0.022
3
3
which amounts to (0.06)(2 kg) = 0.11 kg cementite in the alloy.
9.60 This problem asks that we compute the maximum mass fraction of proeutectoid cementite possible
for a hypereutectoid iron-carbon alloy. This requires that we utilize Equation (9.21) with C1' = 2.14
wt% C, the maximum solubility of carbon in austenite. Thus,
WFe C' =
3
C ' − 0.76
1
5.94
=
2.14 − 0.76
= 0.232
5.94
9.61 This problem asks if it is possible to have an iron-carbon alloy for which WFe C = 0.057 and Wα' =
3
0.36. In order to make this determination, it is necessary to set up lever rule expressions for these
two mass fractions in terms of the alloy composition, then to solve for the alloy composition of each;
if both alloy composition values are equal, then such an alloy is possible. The expression for the
mass fraction of total cementite is
Co − Cα
C o − 0.022
WFe C =
=
= 0.057
CFe C − Cα
6.70 − 0.022
3
3
Solving for this Co yields Co = 0.40 wt% C. Now for Wα' we utilize Equation (9.19) as
Wα' =
0.76 − C o'
= 0.36
0.74
271
This expression leads to C 'o = 0.49 wt% C. And, since Co and C 'o are different this alloy is not
possible.
9.62 This problem asks if it is possible to have an iron-carbon alloy for which Wα = 0.860 and Wp =
0.969. In order to make this determination, it is necessary to set up lever rule expressions for these
two mass fractions in terms of the alloy composition, then to solve for the alloy composition of each;
if both alloy composition values are equal, then such an alloy is possible. The expression for the
mass fraction of total ferrite is
Wα =
CFe C − C o
3
C
Fe 3C
− C
=
α
6.70 − Co
6.70 − 0.022
= 0.860
Solving for this Co yields Co = 0.95 wt% C. Now for Wp we utilize Equation (9.20) as
Wp =
6.70 − C1'
5.94
= 0.969
This expression leads to C1' = 0.95 wt% C. Since Co = C1' , this alloy is possible.
9.63 This problem asks that we compute the mass fraction of eutectoid cementite in an iron-carbon alloy
that contains 1.00 wt% C. In order to solve this problem it is necessary to compute mass fractions of
total and proeutectoid cementites, and then to subtract the latter from the former. To calculate the
mass fraction of total cementite, it is necessary to use the lever rule and a tie line that extends
across the entire α + Fe3C phase field as
Co − Cα
1.00 − 0.022
WFe C =
=
= 0.146
6.70 − 0.022
CFe C − Cα
3
3
Now, for the mass fraction of proeutectoid cementite we use Equation (9.21)
WFe C' =
3
C1' − 0.76
5.94
=
1.00 − 0.76
= 0.040
5.94
And, finally, the mass fraction of eutectoid cementite WFe C'' is just
3
272
WFe C′′ = WFe C − WFe C ′ = 0.146 − 0.040 = 0.106
3
3
3
9.64 This problem asks whether or not it is possible to determine the composition of an iron-carbon alloy
for which the mass fraction of eutectoid cementite is 0.109; and if so, to calculate the composition.
Yes, it is possible to determine the alloy composition; and, in fact, there are two possible answers.
For the first, the eutectoid cementite exists in addition to proeutectoid cementite. For this case the
mass fraction of eutectoid cementite (WFe C'') is just the difference between total cementite and
3
proeutectoid cementite mass fractions; that is
WFe C'' = WFe C - WFe C'
3
3
3
Now, it is possible to write expressions for WFe C and WFe C' in terms of Co, the alloy composition.
3
3
Thus,
Co − C α
Co − 0.76
WFe C'' =
−
CFe C − C α
5.94
3
3
=
Co − 0.022
6.70 − 0.022
−
Co − 0.76
5.94
= 0.109
And, solving for Co yields Co = 0.84 wt% C.
For the second possibility, we have a hypoeutectoid alloy wherein all of the cementite is
eutectoid cementite. Thus, it is necessary to set up a lever rule expression wherein the mass
fraction of total cementite is 0.109. Therefore,
Co − Cα
C − 0.022
WFe C =
= o
= 0.109
CFe C − Cα
6.70 − 0.022
3
3
And, solving for Co yields Co = 0.75 wt% C.
9.65 This problem asks whether or not it is possible to determine the composition of an iron-carbon alloy
for which the mass fraction of eutectoid ferrite is 0.71; and if so, to calculate the composition. Yes, it
is possible to determine the alloy composition; and, in fact, there are two possible answers. For the
first, the eutectoid ferrite exists in addition to proeutectoid ferrite. For this case the mass fraction of
eutectoid ferrite (Wα'') is just the difference between total ferrite and proeutectoid ferrite mass
fractions; that is
Wα'' = Wα - Wα'
273
Now, it is possible to write expressions for Wα and Wα' in terms of Co, the alloy composition. Thus,
Wα '' =
=
CFe C − Co
3
− C
C
Fe 3C
α
−
0.76 − C o
0.74
6.70 − C o
0.76 − C o
−
= 0.71
6.70 − 0.022
0.74
And, solving for Co yields Co = 0.61 wt% C.
For the second possibility, we have a hypereutectoid alloy wherein all of the ferrite is
eutectoid ferrite. Thus, it is necessary to set up a lever rule expression wherein the mass fraction of
total ferrite is 0.71. Therefore,
Wα =
CFe C − C o
3
C
Fe 3C
− C
α
=
6.70 − Co
6.70 − 0.022
= 0.71
And, solving for Co yields Co = 1.96 wt% C.
9.66 Schematic microstructures for the iron-carbon alloy of composition 3 wt% C-97 wt% Fe and at
temperatures of 1250&deg;C, 1145&deg;C, and 700&deg;C are shown below; approximate phase compositions
are also indicated.
274
9.67 This problem asks that we determine the approximate Brinell hardness of a 99.8 wt% Fe-0.2 wt% C
alloy. First, we compute the mass fractions of pearlite and proeutectoid ferrite using Equations
(9.18) and (9.19), as
Wp =
C o' − 0.022
0.74
Wα' =
=
0.20 − 0.022
= 0.24
0.74
0.76 − C 'o
0.76 − 0.20
=
= 0.76
0.74
0.74
Now, we compute the Brinell hardness of the alloy as
HBalloy = HBα'Wα' + HBp Wp
= (80)(0.76) + (280)(0.24) = 128
9.68 We are asked in this problem to estimate the composition of the Pb-Sn alloy which microstructure is
shown in Figure 9.15. Primary α and eutectic microconstituents are present in the photomicrograph,
and it is given that their densities are 11.2 and 8.7 g/cm3, respectively. Below is shown a square
grid network onto which is superimposed outlines of the primary α phase areas.
The area fraction of this primary α phase may be determined by counting squares. There
are a total of 644 squares, and of these, approximately 104 lie within the primary α phase particles.
275
Thus, the area fraction of primary α is 104/644 = 0.16, which is also assumed to be the volume
fraction.
We now want to convert the volume fractions into mass fractions in order to employ the lever
rule to the Pb-Sn phase diagram. To do this, it is necessary to utilize Equations (9.7a) and (9.7b) as
follows:
Wα ' =
V ρ
α' α '
Vα ' ρ α'
+ V
ρ
eutectic eutectic
(
)
= 0.197
(0.16) (11.2 g / cm3 ) + (0.84) (8.7 g / cm3 )
3
(0.16) 11.2 g / cm
=
Weutectic =
Veutectic ρeutectic
Vα'ρα' + Veutectic ρeutectic
3
(
)
=
= 0.803
(0.16) (11.2 g / cm3 ) + (0.84) (8.7 g / cm3 )
(0.84) 8.7 g / cm
From Figure 9.7, we want to use the lever rule and a tie-line that extends from the eutectic
composition (61.9 wt% Sn) to the α-(α + β) phase boundary at 180&deg;C (about 18.3 wt% Sn).
Accordingly
Wα' = 0.197 =
61.9 − Co
61.9 − 18.3
wherein C is the alloy composition (in wt% Sn). Solving for C yields C = 53.3 wt% Sn. This C
o
o
o
o
is close to the 50 wt% Sn value cited in the legend of Figure 9.15.
9.69 This problem asks us to consider an alloy of composition 97.5 wt% Fe, 2.0 wt% Mo, and 0.5 wt% C.
(a) From Figure 9.31, the eutectoid temperature for 2.0 wt% Mo is approximately 850&deg;C.
(b) From Figure 9.32, the eutectoid composition is approximately 0.22 wt% C.
(c) Since the carbon concentration of the alloy (0.5 wt%) is greater than the eutectoid, cementite is
the proeutectoid phase.
9.70 We are asked to consider a steel alloy of composition 93.8 wt% Fe, 6.0 wt% Ni, and 0.2 wt% C.
(a) From Figure 9.31, the eutectoid temperature for 6 wt% Ni is approximately 650&deg;C (1200&deg;F).
276
(b) From Figure 9.32, the eutectoid composition is approximately 0.62 wt% C. Since the carbon
concentration in the alloy (0.2 wt%) is less than the eutectoid, the proeutectoid phase is ferrite.
(c) Assume that the α-(α + Fe3C) phase boundary is at a negligible carbon concentration.
Wα ' =
0.62 − C o'
0.62 − 0.20
=
= 0.68
0.62
0.62 − 0
Likewise, using a modified Equation (9.18)
Wp =
Co' − 0
0.62 − 0
=
277
0.20
= 0.32
0.62
CHAPTER 10
PHASE TRANSFORMATIONS IN METALS
PROBLEM SOLUTIONS
10.1 The two stages involved in the formation of particles of a new phase are nucleation and growth.
The nucleation process involves the formation of normally very small particles of the new phase(s)
which are stable and capable of continued growth. The growth stage is simply the increase in size of
the new phase particles.
10.2 This problem calls for us to compute the length of time required for a reaction to go to 99%
completion.
It first becomes necessary to solve for the parameter k in Equation (10.1).
Rearrangement of this equation leads to
k= −
ln (1 − y)
tn
=−
ln (1 − 0.5)
(100 s)1.7
= 2.76 x 10-4
Now, solving for the time to go to 99% completion
⎡ ln (1 − y) ⎤
t = ⎢−
⎥⎦
⎣
k
⎡ ln (1 − 0.99) ⎤
= ⎢−
⎥
⎢⎣ 2.76 x 10 −4 ⎥⎦
1/n
1/1.7
= 305 s
10.3 This problem asks that we compute the rate of some reaction given the values of n and k in
Equation (10.1). Since the reaction rate is defined by Equation (10.2), it is first necessary to
determine t0.5, or the time necessary for the reaction to reach y = 0.5. Solving for t0.5 from Equation
⎡ ln (1 − y) ⎤
t 0.5 = ⎢ −
⎥⎦
⎣
k
278
1/n
⎡ ln (1 − 0.5) ⎤
= ⎢−
⎥
⎢⎣ 5 x 10 −4 ⎥⎦
1/2
= 37.23 s
Now, the rate is just
rate =
1
1
=
= 2.69 x 10-2 (s)-1
t0.5 37.23 s
10.4 This problem gives us the value of y (0.30) at some time t (100 min), and also the value of n (5.0)
for the recrystallization of an alloy at some temperature, and then asks that we determine the rate of
recrystallization at this same temperature. It is first necessary to calculate the value of k in Equation
(10.1) as
k= −
=−
ln (1 − y)
tn
ln (1 − 0.3)
(100 min) 5
= 3.57 &times; 10-11
At this point we want to compute t0.5, the value of t for y = 0.5, also using Equation (10.1). Thus
1/n
⎡ ln (1 − 0.5) ⎤
t 0.5 = ⎢ −
⎥⎦
⎣
k
⎡ ln (1 − 0.5) ⎤
= ⎢−
⎥
⎢⎣ 3.57 x 10 −11 ⎥⎦
1/5
= 114.2 min
And, therefore, from Equation (10.2), the rate is just
rate =
1
t0.5
=
1
= 8.76 x 10-3 (min)-1
114.2 min
10.5 For this problem, we are given, for the austenite-to-pearlite transformation, two values of y and two
values of the corresponding times, and are asked to determine the time required for 95% of the
austenite to transform to pearlite.
The first thing necessary is to set up two expressions of the form of Equation (10.1), and
then to solve simultaneously for the values of n and k.
279
In order to expedite this process, we will
rearrange and do some algebraic manipulation of Equation (10.1). First of all, we rearrange as
follows:
( n)
1 − y = exp −kt
Now taking natural logarithms
ln (1 − y) = − ktn
Or
− ln (1 − y) = ktn
which may also be expressed as
⎛ 1 ⎞
n
ln ⎜
⎟ = kt
⎝1 − y⎠
Now taking natural logarithms again, leads to
⎡
ln ⎢ln
⎣
⎛ 1 ⎞⎤
⎜ 1 − y ⎟ ⎥ = ln k + n ln t
⎝
⎠⎦
which is the form of the equation that we will now use. The two equations are thus
⎧ ⎡
1 ⎤⎫
ln ⎨ ln ⎢
⎥⎬ = ln k + n ln(280 s)
⎩ ⎣ 1 − 0.2 ⎦⎭
⎧ ⎡
1 ⎤⎫
ln ⎨ ln ⎢
⎥⎬ = ln k + n ln(425 s)
⎩ ⎣ 1 − 0.6 ⎦⎭
Solving these two expressions simultaneously for n and k yields n = 3.385 and k = 1.162 x 10-9.
Now it becomes necessary to solve for the value of t at which y = 0.95.
Algebraic
manipulation of Equation (10.1) leads to an expression in which t is the dependent parameter as
280
⎡ ln (1 − y) ⎤
t = ⎢−
⎥⎦
⎣
k
⎡ ln (1 − 0.95) ⎤
= ⎢−
⎥
⎢⎣ 1.162 x 10−9 ⎥⎦
1/n
1/3.385
= 603 s
10.6 For this problem, we are given, for the recrystallization of aluminum, two values of y and two values
of the corresponding times, and are asked to determine the fraction recrystallized after a total time of
116.8 min.
The first thing necessary is to set up two expressions of the form of Equation (10.1), and
then to solve simultaneously for the values of n and k.
In order to expedite this process, we will
rearrange and do some algebraic manipulation of Equation (10.1). First of all, we rearrange as
follows:
( n)
1 − y = exp −kt
Now taking natural logarithms
ln (1 − y) = − ktn
Or
− ln (1 − y) = ktn
which may also be expressed as
⎛ 1 ⎞
n
ln ⎜
⎟ = kt
⎝1 − y⎠
Now taking natural logarithms again, leads to
⎡ ⎛ 1 ⎞⎤
ln ⎢ln ⎜
⎟ ⎥ = ln k + n ln t
⎣ ⎝1 − y⎠⎦
which is the form of the equation that we will now use. The two equations are thus
281
⎧ ⎡
⎤⎫
1
ln ⎨ ln ⎢
⎥ ⎬ = ln k + n ln (95.2 min)
⎩ ⎣ 1 − 0.30 ⎦ ⎭
⎧ ⎡
⎤⎫
1
ln ⎨ ln ⎢
⎥ ⎬ = ln k + n ln (126.6 min)
⎩ ⎣ 1 − 0.80 ⎦ ⎭
Solving these two expressions simultaneously for n and k yields n = 5.286 and k = 1.239 x 10-11.
Now it becomes necessary to solve for y when t = 116.8 min. Application of Equation (10.1)
( n)
y = 1 − exp −kt
(
)
5.286 ⎤
= 1 − exp ⎡⎣− 1.239 x 10-11 (116.8 min)
⎦ = 0.65
10.7 This problem asks us to consider the percent recrystallized versus logarithm of time curves for
copper shown in Figure 10.2.
(a) The rates at the different temperatures are determined using Equation (10.2), which rates are
tabulated below:
Temperature (&deg;C)
Rate (min)
-1
135
0.105
119
-2
4.4 x 10
113
-2
2.9 x 10
102
-2
1.25 x 10
88
-3
4.2 x 10
43
-5
3.8 x 10
(b) These data are plotted below.
282
The activation energy, Q, is related to the slope of the line drawn through the data points as
Q = − Slope (R)
4
where R is the gas constant. The slope of this line is -1.126 x 10 K, and thus
(
)
4
Q = − −1.126 x 10 K (8.31 J/mol - K)
= 93,600 J/mol
-3 -1
(c) At room temperature (20&deg;C), 1/T = 3.41 x 10 K . Extrapolation of the data in the plot to this
1/T value gives
ln (rate) ≅ − 12.8
rate ≅ exp (−12.8) = 2.76 x 10-6 (min)-1
But since
rate =
1
t0.5
then
283
t 0.5 =
1
1
=
rate 2.76 x 10 −6 (min)−1
= 3.62 x 105 min = 250 days
10.8 In this problem we are asked to determine, from Figure 10.2, the values of the constants n and k
[Equation (10.1)] for the recrystallization of copper at 119&deg;C. One way to solve this problem is to
take two values of percent recrystallization [which is just 100y, Equation (10.1)] and their
corresponding time values, then set up two simultaneous equations, from which n and k may be
determined. In order to expedite this process, we will rearrange and do some algebraic manipulation
of Equation (10.1). First of all, we rearrange as follows:
( n)
1 − y = exp −kt
Now taking natural logarithms
ln (1 − y) = − ktn
Or
− ln (1 − y) = ktn
which may also be expressed as
⎛ 1 ⎞
n
ln ⎜
⎟ = kt
1
−
y
⎝
⎠
Now taking natural logarithms again, leads to
⎡ ⎛ 1 ⎞⎤
ln ⎢ln ⎜
⎟ ⎥ = ln k + n ln t
⎣ ⎝1 − y⎠⎦
which is the form of the equation that we will now use. From the 119&deg;C curve of Figure 10.2, let us
arbitrarily choose two percent recrystallized values, 20% and 80% (i.e., y1 = 0.20 and y2 = 0.80).
284
Their corresponding time values are t1 = 16.1 min and t2 = 30.4 min (realizing that the time axis is
scaled logarithmically). Thus, our two simultaneous equations become
⎡
ln ⎢ln
⎣
⎛ 1 ⎞⎤
⎜ 1 − 0.2 ⎟ ⎥ = ln k + n ln (16.1)
⎝
⎠⎦
⎡
ln ⎢ln
⎣
⎛ 1 ⎞⎤
⎜ 1 − 0.8 ⎟ ⎥ = ln k + n ln (30.4 )
⎝
⎠⎦
from which we obtain the values n = 3.11 and k = 3.9 x 10-5.
10.9 Two limitations of the iron-iron carbide phase diagram are:
1) The nonequilibrium martensite phase does not appear on the diagram; and
2) The diagram provides no indication as to the time-temperature relationships for the formation of
pearlite, bainite, and spheroidite, all of which are composed of the equilibrium ferrite and cementite
phases.
10.10 (a) Superheating and supercooling correspond, respectively, to heating or cooling above or below
a phase transition temperature without the occurrence of the transformation.
(b) Superheating and supercooling occur because right at the phase transition temperature, the
driving force is not sufficient to cause the transformation to occur. The driving force is enhanced
during superheating or supercooling.
10.11 We are called upon to consider the isothermal transformation of an iron-carbon alloy of eutectoid
composition.
(a) From Figure 10.13, a horizontal line at 550&deg;C intersects the 50% and reaction completion curves
at about 2.5 and 6 seconds, respectively; these are the times asked for in the problem.
(b) The pearlite formed will be fine pearlite. From Figure 10.21(a), the hardness of an alloy of
composition 0.76 wt% C that consists of fine pearlite is about 265 HB (27 HRC).
10.12 The microstructures of pearlite, bainite, and spheroidite all consist of α-ferrite and cementite
phases. For pearlite, the two phases exist as layers that alternate with one another. Bainite consists
of very fine and parallel needles of ferrite that are separated by elongated particles of cementite. For
spheroidite, the matrix is ferrite, and the cementite phase is in the shape of spheroidal-shaped
particles.
285
Bainite is harder and stronger than pearlite, which, in turn, is harder and stronger than
spheroidite.
10.13 The driving force for the formation of spheroidite is the net reduction in ferrite-cementite phase
boundary area.
10.14 This problem asks us to determine the nature of the final microstructure of an iron-carbon alloy of
eutectoid composition, that has been subjected to various isothermal heat treatments. Figure 10.13
is used in these determinations.
(a) 50% coarse pearlite and 50% martensite
(b) 100% spheroidite
(c) 50% fine pearlite, 25% bainite , and 25% martensite
(d) 100% martensite
(e) 40% bainite and 60% martensite
(f) 100% bainite
(g) 100% fine pearlite
(h) 100% tempered martensite
10.15 Below is shown the isothermal transformation diagram for a eutectoid iron-carbon alloy, with timetemperature paths that will yield (a) 100% coarse pearlite; (b) 50% martensite and 50% austenite;
and (c) 50% coarse pearlite, 25% bainite, and 25% martensite.
286
10.16 We are asked to determine which microconstituents are present in a 1.13 wt% C iron-carbon alloy
that has been subjected to various isothermal heat treatments.
(a) Martensite
(b) Proeutectoid cementite and martensite
(c) Bainite
(d) Spheroidite
(e) Cementite, medium pearlite, bainite, and martensite
(f) Bainite and martensite
(g) Proeutectoid cementite, pearlite, and martensite
(h) Proeutectoid cementite and fine pearlite
287
10.17 This problem asks us to determine the approximate percentages of the microconstituents that form
for five of the heat treatments described in Problem 10.16.
(a) 100% martensite
(c) 100% bainite
(d) 100% spheroidite
(f) 60% bainite and 40% martensite
(h)
After holding for 7 s at 600&deg;C, the specimen has completely transformed to proeutectoid
cementite and fine pearlite; no further reaction will occur at 450&deg;C. Therefore, we can calculate the
mass fractions using the appropriate lever rule expressions, Equations (9.20) and (9.21), as follows:
WFe C' =
3
Wp =
C1' − 0.76
5.94
=
1.13 − 0.76
= 0.062 or 6.2%
5.94
6.70 − C1'
6.70 − 1.13
=
= 0.938 or 93.8%
5.94
5.94
10.18 Below is shown an isothermal transformation diagram for a 1.13 wt% C iron-carbon alloy, with
time-temperature paths that will produce (a) 6.2% proeutectoid cementite and 93.8% coarse pearlite;
(b) 50% fine pearlite and 50% bainite; (c) 100% martensite; and (d) 100% tempered martensite.
288
10.19 We are called upon to name the microstructural products that form for specimens of an iron-carbon
alloy of eutectoid composition that are continuously cooled to room temperature at a variety of rates.
Figure 10.18 is used in these determinations.
(a) At a rate of 200&deg;C/s, only martensite forms.
(b) At a rate of 100&deg;C/s, both martensite and pearlite form.
(c) At a rate of 20&deg;C/s, only fine pearlite forms.
10.20 Below is shown a continuous cooling transformation diagram for a 0.35 wt% C iron-carbon alloy,
with continuous cooling paths that will produce (a) fine pearlite and proeutectoid ferrite;
(b)
martensite; (c) martensite and proeutectoid ferrite; (d) coarse pearlite and proeutectoid ferrite;
and (e) martensite, fine pearlite, and proeutectoid ferrite.
10.21 Two major differences between martensitic and pearlitic transformations are 1) atomic diffusion is
necessary for the pearlitic transformation, whereas the martensitic transformation is diffusionless;
and 2) relative to transformation rate, the martensitic transformation is virtually instantaneous, while
the pearlitic transformation is time-dependent.
289
10.22 Two important differences between continuous cooling transformation diagrams for plain carbon
and alloy steels are: 1) for an alloy steel, a bainite nose will be present, which nose will be absent for
plain carbon alloys;
and 2) the pearlite-proeutectoid noses for plain carbon steel alloys are
positioned at shorter times than for the alloy steels.
10.23 There is no bainite transformation region on the continuous cooling transformation diagram for an
iron-carbon alloy of eutectoid composition (Figure 10.16) because by the time a cooling curve has
passed into the bainite region, the entirety of the alloy specimen will have transformed to pearlite.
10.24 This problem asks for the microstructural products that form when specimens of a 4340 steel are
continuously cooled to room temperature at several rates.
Figure 10.19 is used for these
determinations.
(a) At a cooling rate of 10&deg;C/s, only martensite forms.
(b) At a cooling rate of 1&deg;C/s, both martensite and bainite form.
(c) At a cooling rate of 0.1&deg;C/s, martensite, proeutectoid ferrite, and bainite form.
(d) At a cooling rate of 0.01&deg;C/s, martensite, proeutectoid ferrite, pearlite, and bainite form.
10.25
This problem asks that we briefly describe the simplest continuous cooling heat treatment
procedure that would be used in converting a 4340 steel from one microstructure to another.
Solutions to this problem require the use of Figure 10.19.
(a) In order to convert from (martensite + ferrite + bainite) to (martensite + ferrite + pearlite + bainite)
it is necessary to heat above about 720&deg;C, allow complete austenitization, then cool to room
temperature at a rate between 0.02 and 0.006&deg;C/s.
(b) To convert from (martensite + ferrite + bainite) to spheroidite the alloy must be heated to about
700&deg;C for several hours.
(c) In order to convert from (martensite + bainite + ferrite) to tempered martensite it is necessary to
heat to above about 720&deg;C, allow complete austenitization, then cool to room temperature at a rate
greater than 8.3&deg;C/s, and finally isothermally heat treat the alloy at a temperature between about 400
and 550&deg;C (Figure 10.25) for about one hour.
10.26 For moderately rapid cooling, the time allowed for carbon diffusion is not as great as for slower
cooling rates. Therefore, the diffusion distance is shorter, and thinner layers of ferrite and cementite
form (i.e., fine pearlite forms).
10.27 (a) Spheroiditic microstructures are more stable than pearlitic ones.
(b) Since pearlite transforms to spheroidite, the latter is more stable.
290
10.28 The hardness and strength of iron-carbon alloys that have microstructures consisting of α-ferrite
and cementite phases depend on the boundary area between the two phases. The greater this
area, the harder and stronger the alloy inasmuch as these boundaries impede the motion of
dislocations. Fine pearlite is harder and stronger than coarse pearlite because the alternating ferritecementite layers are thinner for fine, and therefore, there is more phase boundary area. The phase
boundary area between the sphere-like cementite particles and the ferrite matrix is less in
spheroidite than for the alternating layered microstructure found in coarse pearlite.
10.29 Two reasons why martensite is so hard and brittle are: 1) there are relatively few operable slip
systems for the body-centered tetragonal crystal structure, and 2) virtually all of the carbon is in solid
solution, which produces a solid-solution hardening effect.
10.30 This problem asks us to rank four iron-carbon alloys of specified composition and microstructure
according to tensile strength. This ranking is as follows:
0.6 wt% C, fine pearlite
0.6 wt% C, coarse pearlite
0.25 wt% C, coarse pearlite
0.25 wt% C, spheroidite
The 0.25 wt% C, coarse pearlite is stronger than the 0.25 wt% C, spheroidite since coarse pearlite is
stronger than spheroidite; the composition of the alloys is the same. The 0.6 wt% C, coarse pearlite
is stronger than the 0.25 wt% C, coarse pearlite, since increasing the carbon content increases the
strength.
Finally, the 0.6 wt% C, fine pearlite is stronger than the 0.6 wt% C, coarse pearlite
inasmuch as the strength of fine pearlite is greater than coarse pearlite because of the many more
ferrite-cementite phase boundaries in fine pearlite.
10.31 This question asks for an explanation as to why the hardness of tempered martensite diminishes
with tempering time (at constant temperature) and with increasing temperature (at constant
tempering time). The hardness of tempered martensite depends on the ferrite-cementite phase
boundary area; since these phase boundaries are barriers to dislocation motion, the greater the
area the harder the alloy. The microstructure of tempered martensite consists of small sphere-like
particles of cementite embedded within a ferrite matrix.
As the size of the cementite particles
increases, the phase boundary area diminishes, and the alloy becomes softer. Therefore, with
increasing tempering time, the cementite particles grow, the phase boundary area decreases, and
the hardness diminishes. As the tempering temperature is increased, the rate of cementite particle
291
growth also increases, and the alloy softens, again, because of the decrease in phase boundary
area.
10.32 In this problem we are asked to describe the simplest heat treatment that would be required to
convert a eutectoid steel from one microstructure to another. Figure 10.18 is used to solve the
several parts of this problem.
(a) For martensite to spheroidite, heat to a temperature in the vicinity of 700&deg;C (but below the
eutectoid temperature), for on the order of 24 h.
(b) For spheroiridte to martensite, austenitize at a temperature of about 760&deg;C, then quench to room
temperature at a rate greater than about 140&deg;C/s.
(c) For bainite to pearlite, first austenitize at a temperature of about 760&deg;C, then cool to room
temperature at a rate less than about 35&deg;C/s.
(d)
For pearlite to bainite, first austenitize at a temperature of about 760&deg;C, rapidly cool to a
temperature between about 220&deg;C and 540&deg;C, and hold at this temperature for the time necessary to
complete the bainite transformation (according to Figure 10.13).
(e) For spheroidite to pearlite, same as (c) above.
(f) For pearlite to spheroidite, heat at about 700&deg;C for approximately 20 h.
(g) For tempered martensite to martensite, first austenitize at a temperature of about 760&deg;C, and
rapidly quench to room temperature at a rate greater than about 140&deg;C/s.
(h) For bainite to spheroidite, simply heat at about 700&deg;C for approximately 20 h.
10.33 (a) Both tempered martensite and spheroidite have sphere-like cementite particles within a ferrite
matrix; however, these particles are much larger for spheroidite.
(b) Tempered martensite is harder and stronger inasmuch as there is much more ferrite-cementite
phase boundary area for the smaller particles; thus, there is greater reinforcement of the ferrite
phase, and more phase boundary barriers to dislocation motion.
10.34 This problem asks for Rockwell hardness values for specimens of an iron-carbon alloy of eutectoid
composition that have been subjected to some of the heat treatments described in Problem 10.14.
(b) The microstructural product of this heat treatment is 100% spheroidite. According to Figure
10.21(a) the hardness of a 0.76 wt% C alloy with spheroidite is about 87 HRB (180 HB).
(d) The microstructural product of this heat treatment is 100% martensite. According to Figure
10.23, the hardness of a 0.76 wt% C alloy consisting of martensite is about 64 HRC (690 HB).
(f) The microstructural product of this heat treatment is 100% bainite. From Figure 10.22, the
hardness of a 0.76 wt% C alloy consisting of bainite is about 385 HB. And, conversion from Brinell
to Rockwell hardness using Figure 6.18 leads to a hardness of 36 HRC.
292
(g) The microstructural product of this heat treatment is 100% fine pearlite. According to Figure
10.21(a), the hardness of a 0.76 wt% C alloy consisting of fine pearlite is about 27 HRC (270 HB).
(h) The microstructural product of this heat treatment is 100% tempered martensite. According to
Figure 10.26, the hardness of a water-quenched eutectoid alloy that was tempered at 315&deg;C for one
hour is about 56 HRC (560 HB).
10.35 This problem asks for estimates of Brinell hardness values for specimens of an iron-carbon alloy of
composition 1.13 wt% C that have been subjected to some of the heat treatments described in
Problem 10.16.
(a) The microstructural product of this heat treatment is 100% martensite. According to Figure
10.23, the hardness of a 1.13 wt% C alloy consisting of martensite is about 700 HB (by
extrapolation).
(d) The microstructural product of this heat treatment is 100% spheroidite. According to Figure
10.21(a), the hardness of a 1.13 wt% C alloy consisting of spheroidite
extrapolation).
(h) The microstructural product of this heat treatment is proeutectoid cementite and fine pearlite.
According to Figure 10.21(a), the hardness of a 1.13 wt% C alloy consisting of fine pearlite is about
310 HB (by extrapolation).
10.36 This problem asks for estimates of tensile strength values for specimens of an iron-carbon alloy of
eutectoid composition that have been subjected to some of the heat treatments described in
Problem 10.19.
(a) The microstructural product of this heat treatment is 100% martensite. According to Figure
10.23, the hardness of a 0.76 wt% C alloy is about 690 HB. For steel alloys, hardness and tensile
strength are related through Equation (6.20a), and therefore
TS (MPa) = 3.45 x HB = (3.45)(690 HB) = 2380 MPa (345,000 psi)
(c) The microstructural product of this heat treatment is 100% fine pearlite. According to Figure
10.21(a), the hardness of a 0.76 wt% C alloy consisting of fine pearlite is about 265 HB. Therefore,
the tensile strength is
TS (MPa) = 3.45 x HB = (3.45)(265 HB) = 915 MPa (132,500 psi)
10.37 For this problem we are asked to describe isothermal heat treatments required to yield specimens
having several Brinell hardnesses.
(a) From Figure 10.21(a), in order for a 0.76 wt% C alloy to have a Brinell hardness of 180, the
microstructure must be entirely spheroidite. Thus, utilizing the isothermal transformation diagram for
this alloy, Figure 10.13, we must rapidly cool to a temperature at which pearlite forms (i.e., to
293
between 540&deg; C and 660&deg;C), allow the specimen to isothermally and completely transform to
pearlite, cool to room temperature, and then reheat to about 700&deg;C for 18 to 24 h.
(b) This portion of the problem asks for a hardness of 220 HB. According to Figure 10.21(a), for an
alloy of this composition to have this hardness, the microstructure would have to be intermediate
between coarse and fine pearlite—that is, medium pearlite. Thus, an isothermal heat treatment is
necessary at a temperature in between those at which fine and coarse pearlites form—for example,
about 630&deg;C. At this temperature, an isothermal heat treatment for at least 25 s is required.
(c) In order to produce a Brinell hardness of 500, the microstructure could consist of either (1)
100% bainite (Figure 10.22), or (2) tempered martensite (Figure 10.26).
For case (1), according to Figure 10.22, bainite having a hardness of 500 HB results from an
isothermal treatment that is carried out at 320&deg;C. Therefore, after austenitizing, rapidly cool to
320&deg;C, and, from Figure 10.13, hold the specimen at this temperature for at least 1000 seconds in
order for the attainment of 100% bainite. This is followed by cooling to room temperature.
For case (2), after austenitizing, rapidly cool to room temperature in order to achieve 100%
martensite. Then temper this martensite for about 150 s at 425&deg;C (Figure 10.26).
10.38 The (a) and (b) portions of the problem ask that we make schematic plots on the same graph for
the tensile strength versus composition for copper-silver alloys at both room temperature and 600&deg;C;
such a graph is shown below.
(c) Upon consultation of the Cu-Ag phase diagram (Figure 9.6) we note that at room temperature
(20&deg;C), silver is virtually insoluble in copper (i.e., by extrapolation of the solvus curve, there is no α
phase region at the left extremity of the phase diagram); the same may be said the solubility of
294
copper in silver and for the β phase. Thus, only the α and β phases will exist for all compositions at
room temperature; in other words, there will be no solid solution strengthening effects at room
temperature. All other things being equal, the tensile strength will depend (approximately) on the
tensile strengths of each of the α and β phases as well as their phase fractions in a manner
described by the equation given in Problem 9.67 for the elastic modulus. That is, for this problem
(TS)alloy ≅ (TS)α Vα + (TS)β Vβ
in which TS and V denote tensile strength and volume fraction, respectively, and the subscripts
represent the alloy/phases.
Also, mass fractions of the α and β phases change linearly with
changing composition (according to the lever rule). Furthermore, inasmuch as the densities of both
Cu and Ag are similar, weight and volume fractions of the α and β phases will also be similar [see
Equation (9.6)]. In summary, the previous discussion explains the linear dependence of the room
temperature tensile strength on composition as represented in the above plot given that the TS of
pure copper is greater than for pure silver (as stipulated in the problem statement).
At 600&deg;C, the curve will be shifted to significantly lower tensile strengths inasmuch as tensile
strength diminishes with increasing temperature (Section 6.6, Figure 6.14). In addition, according to
Figure 9.6, about 4% of silver will dissolve in copper (i.e., in the α phase), and about 4% of copper
will dissolve in silver (i.e., in the β phase) at 600&deg;C. Therefore, solid solution strengthening will occur
over these compositions ranges, as noted in the graph shown above. Furthermore, between 4% Ag
and 96% Ag, the curve will be approximately linear for the same reasons noted in the previous
paragraph.
Design Problems
10.D1
This problem inquires as to the possibility of producing an iron-carbon alloy of eutectoid
composition that has a minimum hardness of 200 HB and a minimum ductility of 25%RA. If the alloy
is possible, then the continuous cooling heat treatment is to be stipulated.
According to Figures 10.21(a) and (b), the following is a tabulation of Brinell hardnesses and
percents reduction of area for fine and coarse pearlites and spheroidite for a 0.76 wt% C alloy.
Microstructure
HB
%RA
Fine pearlite
270
22
Coarse pearlite
205
29
295
Spheroidite
180
68
Therefore, coarse pearlite meets both of these criteria. The continuous cooling heat treatment which
will produce coarse pearlite for an alloy of eutectoid composition is indicated in Figure 10.18. The
cooling rate would need to be considerably less than 35&deg;C/s, probably on the order of 0.1&deg;C/s.
10.D2 This problem asks if it is possible to produce an iron-carbon alloy that has a minimum tensile
strength of 620 MPa (90,000 psi) and a minimum ductility of 50%RA. If such an alloy is possible, its
composition and microstructure are to be stipulated.
From Equation (6.20a), this tensile strength corresponds to a Brinell hardness of
HB =
TS(MPa) 620 MPa
=
= 180
3.45
3.45
According to Figures 10.21(a) and (b), the following is a tabulation of the composition ranges for fine
and coarse pearlites and spheroidite which meet the stipulated criteria.
Compositions for
Compositions for
Microstructure
HB ≥ 180
%RA ≥ 50%
Fine pearlite
&gt; 0.38 %C
&lt; 0.36 %C
Coarse pearlite
&gt; 0.47 %C
&lt; 0.42 %C
Spheroidite
&gt; 0.80 %C
0-1.0 %C
Therefore, only spheroidite has a composition range overlap for both of the hardness and ductility
restrictions; the spheroidite would necessarily have to have a carbon content greater than 0.80 wt%
C.
10.D3 This problem inquires as to the possibility of producing an iron-carbon alloy having a minimum
hardness of 200 HB and a minimum ductility of 35%RA. The composition and microstructure are to
be specified; possible microstructures include fine and coarse pearlites and spheroidite.
To solve this problem, we must consult Figures 10.21(a) and (b).
The following is a
tabulation of the composition ranges for fine and coarse pearlites and spheroidite which meet the
stipulated criteria.
Microstructure
Compositions for
Compositions for
HB ≥ 200
%RA ≥ 35%
296
Fine pearlite
&gt; 0.45 %C
&lt; 0.54 %C
Coarse pearlite
&gt; 0.67 %C
&lt; 0.64 %C
Spheroidite
not possible
&lt;1.0 %C
Thus, fine pearlite is the only possibility. Its composition would need to be between 0.45 and 0.54
wt% C. A spheroidite microstructure is not possible since a hardness of 200 HB is not attainable.
Furthermore, coarse pearlite is not possible because there is not a composition overlap for both
hardness and ductility restrictions.
10.D4 This problem asks us to consider the tempering of a water-quenched 1080 steel to achieve a
hardness of 50 HRC. It is necessary to use Figure 10.26.
(a) The time necessary at 425&deg;C is about 650 s.
(b) At 315&deg;C, the time required (by extrapolation) is approximately 4 x 106 s (about 50 days).
10.D5 We are to consider the tempering of an oil-quenched 4340 steel. From Figure 10.25, for a
minimum tensile strength of 1380 MPa (200,000 psi) a tempering temperature of less than 450&deg;C
(840&deg;F) is required. Also, for a minimum ductility of 43%RA, tempering must be carried out at a
temperature greater than 400&deg;C (760&deg;F). Therefore, tempering must occur at between 400 and
450&deg;C (750 and 840&deg;F) for 1 h.
10.D6 This problem asks if it is possible to produce an oil-quenched and tempered 4340 steel that has a
minimum yield strength of 1240 MPa (180,000 psi) and a minimum ductility of 50%RA, and, if
possible, to describe the tempering heat treatment.
In Figure 10.25 is shown the tempering
characteristics of this alloy. According to this figure, in order to achieve a minimum yield strength of
1240 MPa a tempering temperature of less that about 475&deg;C is required.
On the other hand,
tempering must be carried out at greater than about 520&deg;C for a minimum ductility of 50%RA. Since
there is no overlap of these temperature ranges, an oil-quenched and tempered 4340 alloy
possessing these characteristics is not possible.
297
CHAPTER 11
APPLICATIONS AND PROCESSING OF METAL ALLOYS
PROBLEM SOLUTIONS
11.1 This question asks that we list four classifications of steels, and, for each, to describe properties and
cite typical applications.
Low-Carbon Steels
Properties: nonresponsive to heat treatments; relatively soft and weak; machinable and
weldable.
Typical applications: automobile bodies, structural shapes, pipelines, buildings, bridges, and
tin cans.
Medium-Carbon Steels
Properties: heat treatable, relatively large combinations of mechanical characteristics.
Typical applications: railway wheels and tracks, gears, crankshafts, and machine parts.
High-Carbon Steels
Properties: hard, strong, and relatively brittle.
Typical applications: chisels, hammers, knives, and hacksaw blades.
High-Alloy Steels (Stainless and Tool)
Properties:
hard and wear resistant;
resistant to corrosion in a large variety of
environments.
Typical applications: cutting tools, drills, cutlery, food processing, and surgical tools.
11.2 (a) Ferrous alloys are used extensively because:
1) Iron ores exist in abundant quantities.
2) Economical extraction, refining, and fabrication techniques are available.
3) The alloys may be tailored to have a wide range of properties.
(b) Disadvantages of ferrous alloys are:
1) They are susceptible to corrosion.
2) They have relatively high densities.
3) They have relatively low electrical conductivities.
11.3 Ferritic and austenitic stainless steels are not heat treatable since &quot;heat treatable&quot; is taken to mean
that martensite may be made to form with relative ease upon quenching austenite from an elevated
temperature.
298
For ferritic stainless steels, austenite does not form upon heating, and, therefore, the
austenite-to-martensite transformation is not possible.
For austenitic stainless steels, the austenite phase field extends to such low temperatures
that the martensitic transformation does not occur.
11.4 The alloying elements in tool steels (e.g., Cr, V, W, and Mo) combine with the carbon to form very
hard and wear-resistant carbide compounds.
11.5 We are asked to compute the volume percent graphite in a 3.5 wt% C cast iron. It first becomes
necessary to compute mass fractions using the lever rule. From the iron-carbon phase diagram
(Figure 11.2), the tie-line in the α and graphite phase field extends from essentially 0 wt% C to 100
wt% C. Thus, for a 3.5 wt% C cast iron
Wα =
WGr =
CGr − Co
C o − Cα
C
Gr
100 − 3.5
= 0.965
100 − 0
=
C Gr − C α
−C
3.5 − 0
= 0.035
100 − 0
=
α
Conversion from weight fraction to volume fraction of graphite is possible using Equation (9.6a) as
WGr
VGr =
ρGr
W
Wα
+ Gr
ρα
ρGr
0.035
=
2.3 g / cm 3
0.965
0.035
+
3
7.9 g / cm
2.3 g / cm3
= 0.111 or 11.1 vol%
11.6 Gray iron is weak and brittle in tension because the tips of the graphite flakes act as points of stress
concentration.
11.7 This question asks us to compare various aspects of gray and malleable cast irons.
299
(a) With respect to composition and heat treatment:
Gray iron--2.5 to 4.0 wt% C and 1.0 to 3.0 wt% Si. For most gray irons there is no heat
treatment after solidification.
Malleable iron--2.5 to 4.0 wt% C and less than 1.0 wt% Si. White iron is heated in a
nonoxidizing atmosphere and at a temperature between 800 and 900&deg;C for an extended time period.
(b) With respect to microstructure:
Gray iron--Graphite flakes are embedded in a ferrite or pearlite matrix.
Malleable iron--Graphite clusters are embedded in a ferrite or pearlite matrix.
(c) With respect to mechanical characteristics:
Gray iron--Relatively weak and brittle in tension; good capacity for damping vibrations.
Malleable iron--Moderate strength and ductility.
11.8 Yes, it is possible to produce cast irons that consist of a martensite matrix in which graphite is
embedded in either flake, nodule, or rosette form. For graphite flakes, gray cast iron is formed (as
described in Section 11.2), which is then heated to a temperature at which the ferrite transforms to
austenite; the austenite is then rapidly quenched, which transforms to martensite. For graphite
nodules and rosettes, nodular and malleable cast irons are first formed (again as described in
Section 11.2), which are then austenitized and rapidly quenched.
11.9 This question asks us to compare white and nodular cast irons.
(a) With regard to composition and heat treatment:
White iron--2.5 to 4.0 wt% C and less than 1.0 wt% Si. No heat treatment; however,
cooling is rapid during solidification.
Nodular cast iron--2.5 to 4.0 wt% C, 1.0 to 3.0 wt% Si, and a small amount of Mg or Ce. A
heat treatment at about 700&deg;C may be necessary to produce a ferritic matrix.
(b) With regard to microstructure:
White iron--There are regions of cementite interspersed within pearlite.
Nodular cast iron--Nodules of graphite are embedded in a ferrite or pearlite matrix.
(c) With respect to mechanical characteristics:
White iron--Extremely hard and brittle.
Nodular cast iron--Moderate strength and ductility.
11.10 It is not possible to produce malleable iron in pieces having large cross-sectional dimensions.
White cast iron is the precursor of malleable iron, and a rapid cooling rate is necessary for the
formation of white iron, which may not be accomplished at interior regions of thick cross-sections.
300
11.11 The principal difference between wrought and cast alloys is as follows: wrought alloys are ductile
enough so as to be hot- or cold-worked during fabrication, whereas cast alloys are brittle to the
degree that shaping by deformation is not possible and they must be fabricated by casting.
11.12 Both brasses and bronzes are copper-based alloys. For brasses, the principal alloying element is
zinc, whereas the bronzes are alloyed with other elements such as tin, aluminum, silicon, or nickel.
11.13 Rivets of a 2017 aluminum alloy must be refrigerated before they are used because, after being
solution heat treated, they precipitation harden at room temperature. Once precipitation hardened,
they are too strong and brittle to be driven.
11.14 Strengthening of a 3003 aluminum alloy is accomplished by cold working. Welding a structure of a
cold-worked 3003 alloy will cause it to experience recrystallization, and a resultant loss of strength.
11.15 The chief difference between heat-treatable and nonheat-treatable alloys is that heat-treatable
alloys may be strengthened by a heat treatment wherein a precipitate phase is formed (precipitation
hardening) or a martensitic transformation occurs. Nonheat-treatable alloys are not amenable to
strengthening by such treatments.
11.16 This question asks us for the distinctive features, limitations, and applications of several alloy
groups.
Titanium Alloys
Distinctive features: relatively low densities, high melting temperatures, and high strengths
are possible.
Limitation: because of chemical reactivity with other materials at elevated temperatures,
these alloys are expensive to refine.
Applications: aircraft structures, space vehicles, and in chemical and petroleum industries.
Refractory Metals
Distinctive features: extremely high melting temperatures; large elastic moduli, hardnesses,
and strengths.
Limitation: some experience rapid oxidation at elevated temperatures.
Applications: extrusion dies, structural parts in space vehicles, incandescent light filaments,
x-ray tubes, and welding electrodes.
Superalloys
Distinctive features: able to withstand high temperatures and oxidizing atmospheres for long
time periods.
301
Applications: aircraft turbines, nuclear reactors, and petrochemical equipment.
Noble Metals
Distinctive features: highly resistant to oxidation, especially at elevated temperatures; soft
and ductile.
Limitation: expensive.
Applications: jewelry, dental restoration materials, coins, catalysts, and thermocouples.
11.17 The advantages of cold working are:
1) A high quality surface finish.
2) The mechanical properties may be varied.
3) Close dimensional tolerances.
The disadvantages of cold working are:
1) High deformation energy requirements.
2) Large deformations must be accomplished in steps, which may be expensive.
3) A loss of ductility.
The advantages of hot working are:
1) Large deformations are possible, which may be repeated.
2) Deformation energy requirements are relatively low.
The disadvantages of hot working are:
1) A poor surface finish.
2) A variety of mechanical properties is not possible.
11.18 (a) The advantages of extrusion over rolling are as follows:
1) Pieces having more complicated cross-sectional geometries may be formed.
2) Seamless tubing may be produced.
(b) The disadvantages of extrusion over rolling are as follows:
1) Nonuniform deformation over the cross-section.
2) A variation in properties may result over the cross-section of an extruded piece.
11.19 Four situations in which casting is the preferred fabrication technique are:
1) For large pieces and/or complicated shapes.
2) When mechanical strength is not an important consideration.
3) For alloys having low ductilities.
4) When it is the most economical fabrication technique.
11.20 This question asks us to compare sand, die, investment, and continuous casting techniques.
302
For sand casting, sand is the mold material, a two-piece mold is used, ordinarily the surface
finish is not an important consideration, the sand may be reused (but the mold may not), casting
rates are low, and large pieces are usually cast.
For die casting, a permanent mold is used, casting rates are high, the molten metal is
forced into the mold under pressure, a two-piece mold is used, and small pieces are normally cast.
For investment casting, a single-piece mold is used, which is not reusable; it results in high
dimensional accuracy, good reproduction of detail, and a fine surface finish; and casting rates are
low.
For continuous casting, at the conclusion of the extraction process, the molten metal is
cast into a continuous strand having either a rectangular or circular cross-section; these shapes are
desirable for subsequent secondary metal-forming operations.
The chemical composition and
mechanical properties are relatively uniform throughout the cross-section.
11.21 (a) Some of the advantages of powder metallurgy over casting are as follows:
1) It is used for alloys having high melting temperatures.
2) Better dimensional tolerances result.
3) Porosity may be introduced, the degree of which may be controlled (which is desirable in some
applications such as self-lubricating bearings).
(b) Some of the disadvantages of powder metallurgy over casting are as follows:
1) Production of the powder is expensive.
2) Heat treatment after compaction is necessary.
11.22 This question asks for the principal differences between welding, brazing, and soldering.
For welding, there is melting of the pieces to be joined in the vicinity of the bond; a filler
material may or may not be used.
For brazing, a filler material is used which has a melting temperature in excess of about
425&deg;C (800&deg;F); the filler material is melted, whereas the pieces to be joined are not melted.
For soldering, a filler material is used which has a melting temperature less than about
425&deg;C (800&deg;F); the filler material is melted, whereas the pieces to be joined are not.
11.23 This problem asks that we specify and compare the microstructures and mechanical properties in
the heat-affected weld zones for 1080 and 4340 alloys assuming that the average cooling rate is
10&deg;C/s. Figure 10.18 shows the continuous cooling transformation diagram for an iron-carbon alloy
of eutectoid composition (1080), and, in addition, cooling curves that delineate changes in
microstructure. For a cooling rate of 10&deg;C/s (which is less than 35&deg;C/s) the resulting microstructure
will be totally pearlite--probably a reasonably fine pearlite. On the other hand, in Figure 10.19 is
303
shown the CCT diagram for a 4340 steel. From this diagram it may be noted that a cooling rate of
10&deg;C/s produces a totally martensitic structure. Pearlite is softer and more ductile than martensite,
and, therefore, is most likely more desirable.
11.24 If a steel weld is cooled very rapidly, martensite may form, which is very brittle. In some situations,
cracks may form in the weld region as it cools.
11.25 Full annealing--Heat to between 15 and 40&deg;C above the A line (if the concentration of carbon is
3
less than the eutectoid) or above the A line (if the concentration of carbon is greater than the
1
eutectoid) until the alloy comes to equilibrium; then furnace cool to room temperature. The final
microstructure is coarse pearlite.
Normalizing--Heat to between 55 and 85&deg;C above the upper critical temperature until the specimen
has fully transformed to austenite, then cool in air. The final microstructure is fine pearlite.
Quenching--Heat to a temperature within the austenite phase region and allow the specimen to fully
austenitize, then quench to room temperature in oil or water. The final microstructure is martensite.
Tempering--Heat a quenched (martensitic) specimen, to a temperature between 450 and 650&deg;C, for
the time necessary to achieve the desired hardness.
The final microstructure is tempered
martensite.
11.26
Three sources of residual stresses in metal components are plastic deformation processes,
nonuniform cooling of a piece that was cooled from an elevated temperature, and a phase
transformation in which parent and product phases have different densities.
Two adverse consequences of these stresses are distortion (or warpage) and fracture.
11.27 This question asks that we cite the temperature range over which it is desirable to austenitize
several iron-carbon alloys during a normalizing heat treatment.
(a) For 0.20 wt% C, heat to between 890 and 920&deg;C (1635 and 1690&deg;F) since the A temperature is
3
835&deg;C (1535&deg;F).
(b) For 0.76 wt% C, heat to between 782 and 812&deg;C (1440 and 1494&deg;F) since the A temperature is
3
727&deg;C (1340&deg;F).
(c) For 0.95 wt% C, heat to between 840 and 870&deg;C (1545 and 1600&deg;F) since A
cm
is 785&deg;C
(1445&deg;F).
11.28
We are asked for the temperature range over which several iron-carbon alloys should be
austenitized during a full-anneal heat treatment.
304
(a) For 0.25 wt% C, heat to between 845 and 870&deg;C (1555 and 1600&deg;F) since the A temperature is
3
830&deg;C (1525&deg;F).
(b) For 0.45 wt% C, heat to between 790 and 815&deg;C (1450 and 1500&deg;F) since the A temperature is
3
775&deg;C (1425&deg;F).
(c) For 0.85 wt% C, heat to between 742 and 767&deg;C (1368 and 1413&deg;F) since the A temperature is
1
727&deg;C (1340&deg;F).
(d) For 1.10 wt% C, heat to between 742 and 767&deg;C (1368 and 1413&deg;F) since the A temperature is
1
727&deg;C (1340&deg;F).
11.29 The purpose of a spheroidizing heat treatment is to produce a very soft and ductile steel alloy
having a spheroiditic microstructure. It is normally used on medium- and high-carbon steels, which,
by virtue of carbon content, are relatively hard and strong.
11.30
Hardness is a measure of a material's resistance to localized surface deformation, whereas
hardenability is a measure of the depth to which a ferrous alloy may be hardened by the formation of
martensite. Hardenability is determined from hardness tests.
11.31 The presence of alloying elements (other than carbon) causes a much more gradual decrease in
hardness with position from the quenched end for a hardenability curve. The reason for this effect is
that alloying elements retard the formation of pearlitic and bainitic structures which are not as hard
as martensite.
11.32 A decrease of austenite grain size will decrease the hardenability. Pearlite normally nucleates at
grain boundaries, and the smaller the grain size, the greater the grain boundary area, and,
consequently, the easier it is for pearlite to form.
11.33 The three factors that influence the degree to which martensite is formed are as follows:
1) Alloying elements; adding alloying elements increases the extent to which martensite forms.
2) Specimen size and shape; the extent of martensite formation increases as the specimen
cross-section decreases and as the degree of shape irregularity increases.
3) Quenching medium; the more severe the quench, the more martensite is formed. Water
provides a more severe quench than does oil, which is followed by air. Agitating the medium also
enhances the severity of quench.
11.34 The two thermal properties of a liquid medium that influence its quenching effectiveness are
thermal conductivity and heat capacity.
305
11.35 (a) This part of the problem calls for us to construct a radial hardness profile for a 50 mm (2 in.)
diameter cylindrical specimen of an 8640 steel that has been quenched in moderately agitated oil. In
the manner of Example Problem 11.1, the equivalent distances and hardnesses tabulated below
were determined from Figures 11.13 and 11.16(b).
Position
Equivalent
Distance, mm (in.)
HRC
Hardness
Surface
7 (5/16)
54
3/4 R
11 (7/16)
50
14 (9/16)
45
Center
16 (10/16)
44
The resulting profile is plotted here.
(b) The radial hardness profile for a 75 mm (3 in.) diameter specimen of a 5140 steel that has been
quenched in moderately agitated oil is desired. The equivalent distances and hardnesses for the
various radial positions, as determined using Figures 11.13 and 11.16(b), are tabulated below.
Position
Equivalent
Distance, mm (in.)
HRC
Hardness
Surface
13 (1/2)
41
3/4 R
19 (3/4)
35
22 (14/16)
33
Center
25 (1)
31
306
The resulting profile is plotted here.
(c) The radial hardness profile for a 90 mm (3-1/2 in.) diameter specimen of an 8630 steel that has
been quenched in moderately agitated water is desired. The equivalent distances and hardnesses
for the various radial positions, as determined using Figures 11.14 and 11.16(a) are tabulated below.
Position
Equivalent
Distance, in. (mm)
HRC
Hardness
Surface
3 (1/8)
50
3/4 R
10 (3/8)
38
17 (11/16)
30
Center
20 (13/16)
28
The resulting profile is plotted here.
307
(d) The radial hardness profile for a 100 mm (4 in.) diameter specimen of a 8660 steel that has been
quenched in moderately agitated water is desired. The equivalent distances and hardnesses for the
various radial positions, as determined using Figures 11.14 and 11.16(a), are tabulated below.
Position
Equivalent
Distance, in. (mm)
HRC
Hardness
Surface
3 (1/8)
63
3/4 R
11 (7/16)
61
20 (13/16)
57
Center
27 (1-1/16)
53
The resulting profile is plotted here.
11.36 We are asked to compare the effectiveness of quenching in moderately agitated water and oil by
graphing, on a single plot, the hardness profiles for 75 mm (3 in.) diameter cylindrical specimens of
an 8640 steel that had been quenched in both media.
For moderately agitated water, the equivalent distances and hardnesses for the several
radial positions [Figures 11.16(a) and 11.13] are tabulated below.
Position
Equivalent
Distance, mm
HRC
Hardness
Surface
3
56
3/4 R
9
53
13.5
47
Center
16.5
43
308
While for moderately agitated oil, the equivalent distances and hardnesses for the several radial
positions [Figures 11.16(b) and 11.13] are tabulated below.
Position
Equivalent
Distance, mm
HRC
Hardness
Surface
13
48
3/4 R
19
41
22
38
Center
25
37
These data are plotted here.
11.37 This problem asks us to compare various aspects of precipitation hardening, and the quenching
and tempering of steel.
(a) With regard to the total heat treatment procedure, the steps for the hardening of steel are as
follows:
1) Austenitize above the upper critical temperature.
2) Quench to a relatively low temperature.
3) Temper at a temperature below the eutectoid.
4) Cool to room temperature.
With regard to precipitation hardening, the steps are as follows:
1) Solution heat treat by heating into the solid solution phase region.
2) Quench to a relatively low temperature.
3) Precipitation harden by heating to a temperature that is within the solid two-phase region.
309
4) Cool to room temperature.
(b) For the hardening of steel, the microstructures that form at the various heat treating stages in
part (a) are:
1) Austenite
2) Martensite
3) Tempered martensite
4) Tempered martensite
For precipitation hardening, the microstructures that form at the various heat treating stages in
part (a) are:
1) Single phase
2) Single phase--supersaturated
3) Small plate-like particles of a new phase within a matrix of the original phase.
4) Same as 3)
(c) For the hardening of steel, the mechanical characteristics for the various steps in part (a) are
as follows:
1) Not important
2) The steel becomes hard and brittle upon quenching.
3) During tempering, the alloy softens slightly and becomes more ductile.
4) No significant changes upon cooling to or maintaining at room temperature.
For precipitation hardening, the mechanical characteristics for the various steps in part (a) are
as follows:
1) Not important
2) The alloy is relatively soft.
3) The alloy hardens with increasing time (initially), and becomes more brittle; it may soften with
overaging.
4) The alloy may continue to harden or overage at room temperature.
11.38 For precipitation hardening, natural aging is allowing the precipitation process to occur at the
ambient temperature; artificial aging is carried out at an elevated temperature.
Design Problems
11.D1 This problem calls for us to select, from a list, the best alloy for each of several applications and
then to justify each choice.
310
(a) Gray cast iron would be the best choice for a milling machine base because it effectively absorbs
vibrations and is inexpensive.
(b) Stainless steel would be the best choice for the walls of a steam boiler because it is corrosion
resistant to the steam and condensate.
(c) Titanium alloys are the best choice for high-speed aircraft because they are light weight, strong,
and easily fabricated. However, one drawback is their cost.
(d) A tool steel would be the best choice for a drill bit because it is very hard and wear resistant,
and, thus, will retain a sharp cutting edge.
(e)
For a cryogenic (low-temperature) container, an aluminum alloy would be the best choice;
aluminum alloys have the FCC crystal structure, and therefore, are ductile down to very low
temperatures.
(f) As a pyrotechnic in flares and fireworks, magnesium is the best choice because it ignites easily
(g)
Platinum is the best choice for high-temperature furnace elements to be used in oxidizing
atmospheres because it is very ductile, has a relatively high melting temperature, and is highly
resistant to oxidation.
11.D2 (a) Important characteristics required of metal alloys that are used for coins are as follows: they
must be hard, somewhat ductile, corrosion and oxidation resistant, and nontoxic.
(b) Some of the metals and alloys that are used and have been used for coins are gold, silver,
copper, nickel, copper-nickel alloys, and brass alloys.
11.D3 The first part of this question asks for a description of the shape memory phenomenon. A part
having some shape and that is fabricated from a metal alloy that displays this phenomenon is
plastically deformed.
temperature. Thus, the material has a shape memory, or &quot;remembers&quot; its previous shape.
Next we are asked to explain the mechanism for this phenomenon. A shape memory alloy
is polymorphic (Section 3.6)--that is, it can exist having two crystal structures. One is body-centered
cubic structure (termed an austenite phase) that exists at elevated temperatures; upon cooling, and
at some temperature above the ambient, it transforms to a martensitic structure. Furthermore, this
martensitic phase is highly twinned. Upon application of a stress to this low-temperature martensitic
phase, plastic deformation is accomplished by the migration of twin boundaries to some preferred
orientation. Once the stress is removed, the deformed shape will be retained at this temperature.
When this deformed martensite is subsequently heated to above the phase transformation
temperature, the alloy reverts back to the BCC phase, and assumes the original shape.
procedure may then be repeated.
311
The
One material that exhibits this behavior is a nickel-titanium alloy. Furthermore, the desired
&quot;memory&quot; shape may is established by forming the material above its phase transition temperature.
Several applications for alloys displaying this effect are eyeglass frames, shrink-to-fit pipe
couplers, tooth-straightening braces, collapsible antennas, greenhouse window openers, antiscald
control valves on showers, women's foundations, and fire sprinkler valves.
11.D4 (a) Compositionally, the metallic glass materials are rather complex; several compositions are as
follows: Fe80B20, Fe72Cr8P13C7, Fe67Co18B14Si, Pd77.5Cu6.0Si16.5, and Fe40Ni38Mo4B18.
(b) These materials are exceptionally strong and tough, extremely corrosion resistant, and are easily
magnetized.
(c) Principal drawbacks for these materials are 1) complicated and exotic fabrication techniques are
required; and 2) inasmuch as very rapid cooling rates are required, at least one dimension of the
material must be small--i.e., they are normally produced in ribbon form.
(d) Potential uses include transformer cores, magnetic amplifiers, heads for magnetic tape players,
reinforcements for pressure vessels and tires, shields for electromagnetic interference, security
tapes for library books.
(e)
Production techniques include centrifuge melt spinning, planar-flow casting, rapid pressure
application, arc melt spinning.
11.D5 This question provides us with a list of several metal alloys, and then asks us to pick those that
may be strengthened by heat treatment, by cold work, or both. Those alloys that may be heat
treated are either those noted as &quot;heat treatable&quot; (Tables 11.6 through 11.9), or as martensitic
stainless steels (Table 11.4).
Alloys that may be strengthened by cold working must not be
exceptionally brittle, and, furthermore, must have recrystallization temperatures above room
Heat Treatable
Cold Workable
Both
6150 Steel
6150 Steel
6150 Steel
C17200 Be-Cu
C17200 Be-Cu
C17200 Be-Cu
6061 Al
6061 Al
6061 Al
304 Stainless Steel
R50500 Ti
C51000 Phosphor Bronze
AZ31B Mg
312
11.D6 This problem asks us to select from four alloys (brass, steel, titanium, and aluminum), the one that
will support a 50,000 N (11,250 lbf) load without plastically deforming, and having the minimum
weight. From Equation (6.1), the cross-sectional area (A ) must necessarily carry the load (F)
o
without exceeding the yield strength (σy), as
Ao =
F
σ
y
Now, given the length l, the volume of material required (V) is just
lF
V = l Ao =
σ
y
Finally, the mass of the member (m) is
m = Vρ =
ρ lF
σ
y
in which ρ is the density. Using the values given for these alloys
m(brass) =
m(steel) =
m(aluminum) =
m(titanium) =
(8.5 g/ cm3 )(10 cm)(50,000 N) = 102 g
⎛ 1m ⎞2
6 N / m2
415
x
10
(
)⎜⎝ 102 cm ⎟⎠
(7.9 g / cm 3 )(10 cm)(50, 000 N) = 46 g
⎛ 1m ⎞ 2
6 N/ m 2
860
x
10
(
)⎜⎝ 10 2 cm ⎟⎠
(2.7 g / cm3 )(10 cm)(50,000 N) = 43.5 g
⎛ 1m ⎞2
6
2
(310 x 10 N/ m )⎜⎝ 102 cm ⎟⎠
(4.5 g / cm3 )(10 cm)(50, 000 N) = 40.9 g
⎛ 1 m ⎞2
6
2
(550 x 10 N/ m )⎜⎝ 102 cm ⎟⎠
313
Thus, titanium would have the minimum weight (or mass), followed by aluminum, steel, and brass.
11.D7 This question asks for us to decide whether or not it would be advisable to hot-work or cold-work
several metals and alloys.
Tin would almost always be hot-worked. Even deformation at room temperature would be
considered hot-working inasmuch as its recrystallization temperature is below room temperature
(Table 7.2).
Tungsten is hard and strong at room temperature, has a high recrystallization temperature,
and experiences oxidation at elevated temperatures.
Cold-working is difficult because of its
strength, and hot-working is not practical because of oxidation problems. Most tungsten articles are
fabricated by powder metallurgy, or by using cold-working followed by annealing cycles.
Most aluminum alloys may be cold-worked since they are ductile and have relatively low
yield strengths.
Magnesium alloys are normally hot-worked inasmuch as they are quite brittle at room
temperature. Also, magnesium alloys have relatively low recrystallization temperatures.
A 4140 steel could be cold-worked in an over-tempered state which leaves it soft and
relatively ductile, after which quenching and tempering heat treatments may be employed to
strengthen and harden it. This steel would probably have a relatively high recrystallization
temperature, and hot-working may cause oxidation.
11.D8 A one-inch diameter steel specimen is to be quenched in moderately agitated oil. We are to
decide which of five different steels will have surface and center hardnesses of at least 55 and 50
HRC, respectively.
In moderately agitated oil, the equivalent distances from the quenched end for a one-inch
diameter bar for surface and center positions are 3 mm (1/8 in.) and 8 mm (11/32 in.), respectively
[Figure 11.16(b)]. The hardnesses at these two positions for the alloys cited (as determined using
Figure 11.13) are given below.
Alloy
Surface
Hardness (HRC)
Center
Hardness (HRC)
1040
50
30
5140
55
47
4340
57
57
4140
56
54
8640
56
52.5
314
Thus, alloys 4340, 4140, and 8640 will satisfy the criteria for both surface and center hardnesses.
11.D9 (a) This problem calls for us to decide which of 8660, 8640, 8630, and 8620 alloys may be
fabricated into a cylindrical piece 57 mm (2-1/4 in.) in diameter which, when quenched in mildly
agitated water, will produce a minimum hardness of 45 HRC throughout the entire piece.
The center of the steel cylinder will cool the slowest and therefore will be the softest. In
moderately agitated water the equivalent distance from the quenched end for a 57 mm diameter bar
for the center position is about 11 mm (7/16 in.) [Figure 11.16(a)]. The hardnesses at this position
for the alloys cited (Figure 11.14) are given below.
Alloy
Center
Hardness (HRC)
8660
61
8640
49
8630
36
8620
25
Therefore, only 8660 and 8640 alloys will have a minimum of 45 HRC at the center, and therefore,
throughout the entire cylinder.
(b) This part of the problem asks us to do the same thing for moderately agitated oil. In moderately
agitated oil the equivalent distance from the quenched end for a 57 mm diameter bar at the center
position is about 17.5 mm (11.16 in.) [Figure 11.16(b)]. The hardnesses at this position for the alloys
cited (Figure 11.14) are given below.
Alloy
Center
Hardness (HRC)
8660
59
8640
42
8630
30
8620
21
Therefore, only the 8660 alloy will have a minimum of 45 HRC at the center, and therefore,
throughout the entire cylinder.
315
11.D10 A thirty-eight millimeter diameter cylindrical steel specimen is to be heat treated such that the
microstructure throughout will be at least 80% martensite. We are to decide which of several alloys
will satisfy this criterion if the quenching medium is moderately agitated (a) oil, and (b) water.
(a) Since the cooling rate is lowest at the center, we want a minimum of 80% martensite at the
center position. From Figure 11.16(b), the cooling rate is equal to an equivalent distance from the
quenched end of 12 mm (1/2 in.). According to Figure 11.13, the hardness corresponding to 80%
martensite for these alloys is 50 HRC. Thus, all we need do is to determine which of the alloys have
a 50 HRC hardness at an equivalent distance from the quenched end of 12 mm (1/2 in.). At an
equivalent distance of 12 mm (1/2 in.), the following hardnesses are determined from Figure 11.13
for the various alloys.
Alloy
Hardness (HRC)
4340
55
4140
52
8640
48
5140
42
1040
25
Thus, only alloys 4340 and 4140 will qualify.
(b) For moderately agitated water, the cooling rate at the center of a 38 mm diameter specimen is 8
mm (5/16 in.) equivalent distance from the quenched end [Figure 11.16(a)]. At this position, the
following hardnesses are determined from Figure 11.13 for the several alloys.
Alloy
Hardness (HRC)
4340
56
4140
55
8640
54
5140
49
1040
32
It is still necessary to have a hardness of 50 HRC or greater at the center; thus, alloys 4340,
4140, and 8640 qualify.
11.D11 A fifty-millimeter (two-inch) diameter cylindrical steel specimen is to be quenched in moderately
agitated water.
We are to decide which of eight different steels will have surface and center
hardnesses of at least 50 and 40 HRC, respectively.
316
In moderately agitated water, the equivalent distances from the quenched end for a 50 mm
diameter bar for surface and center positions are 2 mm (1/16 in.) and 10 mm (3/8 in.), respectively
[Figure 11.16(a)]. The hardnesses at these two positions for the alloys cited are given below.
Alloy
Surface
Hardness (HRC)
Center
Hardness (HRC)
1040
53
28
5140
57
46
4340
57
56
4140
57
54
8620
43
28
8630
52
38
8640
57
52
8660
64
62
Thus, alloys 5140, 4340, 4140, 8640, and 8660 will satisfy the criteria for both surface and center
hardnesses.
11.D12 We are asked to determine the maximum diameter possible for a cylindrical piece of 4140 steel
that is to be quenched in moderately agitated oil such that the microstructure will consist of at least
50% martensite throughout the entire piece. From Figure 11.13, the equivalent distance from the
quenched end of a 4140 steel to give 50% martensite (or a 42.5 HRC hardness) is 26 mm (1-1/16
in.). Thus, the quenching rate at the center of the specimen should correspond to this equivalent
distance. Using Figure 11.16(b), the center specimen curve takes on a value of 26 mm (1-1/16 in.)
equivalent distance at a diameter of about 75 mm (3 in.).
11.D13 In this problem we are asked to describe a heat treatment that may be used on a 45 mm
diameter steel shaft of a 1040 steel such that it will have a uniform tensile strength of at least 620
MPa across the entirety of its cross-section. First of all, if the steel is heat treated so as to produce
martensite or tempered martensite, there will undoubtedly be a variation of tensile strength over the
cross-section. Thus, let us determine if either martensite or tempered martensite is required to give
this desired tensile strength, and, if not, what microstructure is necessary.
From Equation (6.20a) a tensile strength of 620 MPa corresponds to a Brinell hardness of
about 180. Upon consultation of Figure 10.21(a), we note that for an alloy of composition of 0.40
wt% C, in order to achieve a hardness of 180 HB, a microstructure of fine pearlite is required. One
possible heat treatment that may be used to produce fine pearlite is a continuous cooling one. In
317
Figure 10.29 is shown a continuous cooling transformation diagram for a 0.35 wt% C alloy, which
would be very similar to that for a 1040 steel.
According to this diagram, we would want to
austenitize the alloy at approximately 900&deg;C, and then continuously cool to room temperature such
that the cooling curve would pass through the fine pearlite region of the diagram (per Figure 10.17).
This would correspond to a cooling rate of approximately
3&deg;C/s (Figure 10.18), which would
probably result from air-cooling the shaft from the 900&deg;C austenitizing temperature.
For this
relatively low cooling rate, the microstructure, and therefore the tensile strength, will be quite uniform
across the specimen cross section.
11.D14 We are to determine, for a cylindrical piece of 8660 steel, the minimum allowable diameter
possible in order yield a surface hardness of 58 HRC, when the quenching is carried out in
moderately agitated oil.
From Figure 11.14, the equivalent distance from the quenched end of an 8660 steel to give
a hardness of 58 HRC is about 18 mm (3/4 in.). Thus, the quenching rate at the surface of the
specimen should correspond to this equivalent distance.
Using Figure 11.16(b), the surface
specimen curve takes on a value of 18 mm equivalent distance at a diameter of about 95 mm (3.75
in.).
11.D15 This problem is concerned with the precipitation-hardening of copper-rich Cu-Be alloys. It is
necessary for us to use the Cu-Be phase diagram (Figure 11.26 ).
(a) The range of compositions over which these alloys may be precipitation hardened is between
approximately 0.2 wt% Be (the maximum solubility of Be in Cu at about 300&deg;C) and 2.7 wt% Be (the
maximum solubility of Be in Cu at 866&deg;C).
(b) The heat treatment procedure, of course, will depend on the composition chosen. First of all, the
solution heat treatment must be carried out at a temperature within the α phase region, after which,
the specimen is quenched to room temperature. Finally, the precipitation heat treatment is
conducted at a temperature within the α + γ2 phase region.
For example, for a 1.5 wt% Be-98.5 wt% Cu alloy, the solution heat treating temperature
must be between about 600&deg;C (1110&deg;F) and 900&deg;C (1650&deg;F), while the precipitation heat treatment
would be below 600&deg;C (1110&deg;F), and probably above 300&deg;C (570&deg;F). Below 300&deg;C, diffusion rates
are low, and heat treatment times would be relatively long.
11.D16 We are asked to specify a practical heat treatment for a 2014 aluminum alloy that will produce a
minimum yield strength of 345 MPa (50,000 psi), and a minimum ductility of 12%EL. From Figure
11.25(a), the following heat treating temperatures and time ranges are possible to the give the
required yield strength.
318
Temperature (&deg;C)
Time Range (h)
260
not possible
204
0.3-15
149
10-700
121
300-?
With regard to temperatures and times to give the desired ductility [Figure 11.25(b)]:
Temperature (&deg;C)
Time Range (h)
260
&lt;0.02, &gt;10
204
&lt;0.4, &gt;350
149
&lt;20
121
&lt;1000
From these tabulations, the following may be concluded:
It is not possible to heat treat this alloy at 260&deg;C so as to produce the desired set of
properties--there is no overlap of the two sets of time ranges.
At 204&deg;C, the heat treating time would need to be about 0.4 h, which is practical.
At 149&deg;C, the time range is between 10 and 20 h, which is a little on the long side.
Finally, at 121&deg;C, the time range is unpractically long (300 to 1000 h).
11.D17 This problem inquires as to the possibility of producing a precipitation-hardened 2014 aluminum
alloy having a minimum yield strength of 380 MPa (55,000 psi) and a ductility of at least 15%EL. In
order to solve this problem it is necessary to consult Figures 11.25(a) and 11.25(b). Below are
tabulated the times required at the various temperatures to achieve the stipulated yield strength.
Temperature (&deg;C)
Time Range (h)
260
not possible
204
0.5-7
149
10-250
121
500-2500
With regard to temperatures and times to give the desired ductility:
319
Temperature (&deg;C)
Time Range (h)
260
&lt;0.005
204
&lt;0.13
149
&lt;10
121
&lt;450
Therefore, an alloy having this combination of yield strength and ductility is marginally possible. A
heat treatment at 149&deg;C for 10 h would probably just achieve the stipulated ductility and yield
strength.
320
CHAPTER 12
STRUCTURES AND PROPERTIES OF CERAMICS
PROBLEM SOLUTIONS
12.1
The two characteristics of component ions that determine the crystal structure are:
1) the
magnitude of the electrical charge on each ion; and 2) the relative sizes of the cations and anions.
12.2
In this problem we are asked to show that the minimum cation-to-anion radius ratio for a
coordination number of four is 0.225. If lines are drawn from the centers of the anions, then a
tetrahedron is formed. The tetrahedron may be inscribed within a cube as shown below.
The spheres at the apexes of the tetrahedron are drawn at the corners of the cube, and designated
as positions A, B, C, and D. (These are reduced in size for the sake of clarity.) The cation resides
at the center of the cube, which is designated as point E. Let us now express the cation and anion
radii in terms of the cube edge length, designated as a. The spheres located at positions A and B
touch each other along the bottom face diagonal. Thus,
AB = 2rA
But
(AB)2 = a 2 + a 2 = 2a 2
321
or
AB = a 2 = 2rA
And
2rA
a =
2
There will also be an anion located at the corner, point F (not drawn), and the cube diagonal
AEF will be related to the ionic radii as
(
AEF = 2 rA + rC
)
(The line AEF has not been drawn to avoid confusion.) From the triangle ABF
(AB)2 + (FB)2 = (AEF)2
But,
FB = a =
2rA
2
and
AB = 2rA
from above. Thus,
( )
2 rA
2
⎛2r ⎞
+ ⎜ A⎟
⎝ 2⎠
2
[(
= 2 rA + rC
)]
2
Solving for the r /r ratio leads to
C A
rC
rA
=
6 − 2
= 0.225
2
12.3 This problem asks us to show, using the rock salt crystal structure, that the minimum cation-to-anion
radius ratio is 0.414 for a coordination number of six. Below is shown one of the faces of the rock
salt crystal structure in which anions and cations just touch along the edges, and also the face
diagonals.
322
From triangle FGH,
GF = 2rA and FH = GH = rA + rC
Since FGH is a right triangle
(GH)2 + (FH)2 = (FG)2
or
(rA +
2
2
2
rC ) + (rA + rC ) = (2rA )
rA + rC =
2 rA
2
Or, solving for r /r
C A
⎛ 2
⎞
= ⎜
− 1⎟ = 0.414
rA
⎝ 2
⎠
rC
12.4 This problem asks us to show that the minimum cation-to-anion radius ratio for a coordination
number of 8 is 0.732. From the cubic unit cell shown below
323
the unit cell edge length is 2rA, and from the base of the unit cell
( )2 + (2rA )2
x 2 = 2 rA
= 8rA2
Or
x = 2rA 2
Now from the triangle that involves x, y, and the unit cell edge
( )
x 2 + 2 rA
(2 rA 2)
2
2
(
= y 2 = 2 rA + 2rC
(
+ 4rA2 = 2rA + 2 rC
)
2
)
2
Which reduces to
2 rA
(3
)
− 1 = 2rC
Or
rC
rA
=
3 − 1 = 0.732
12.5 This problem calls for us to predict crystal structures for several ceramic materials on the basis of
(a) For CsI, from Table 12.3
324
r
Cs +
=
r−
I
0.170 nm
= 0.773
0.220 nm
+
Now, from Table 12.2, the coordination number for each cation (Cs ) is eight, and, using Table 12.4,
the predicted crystal structure is cesium chloride.
(b) For NiO, from Table 12.3
r
Ni 2+
r
O
=
2−
0.069 nm
= 0.493
0.140 nm
The coordination number is six (Table 12.2), and the predicted crystal structure is sodium chloride
(Table 12.4).
(c) For KI, from Table 12.3
r
K+
r−
=
I
0.138 nm
= 0.627
0.220 nm
The coordination number is six (Table 12.2), and the predicted crystal structure is sodium chloride
(Table 12.4).
(d) For NiS, from Table 12.3
r
Ni 2+
r
S
=
2−
0.069 nm
= 0.375
0.184 nm
The coordination number is four (Table 12.2), and the predicted crystal structure is zinc blende
(Table 12.4).
12.6 We are asked to cite the cations in Table 12.3 which would form fluorides having the cesium
chloride crystal structure. First of all, the possibilities would include only the monovalent cations
Cs+, K+, and Na+. Furthermore, the coordination number for each cation must be 8, which means
that 0.732 &lt; rC/rA &lt; 1.0 (Table 12.2). From Table 12.3 the rC/rA ratios for these three cations are
as follows:
r
Cs +
r
F
−
=
0.170 nm
= 1.28
0.133 nm
325
r
K+
r
F
0.138 nm
= 1.04
0.133 nm
=
−
r
Na +
r
F
0.102 nm
= 0.77
0.133 nm
=
−
Thus, only sodium will form the CsCl crystal structure with fluorine.
12.7 This problem asks that we compute the atomic packing factor for the rock salt crystal structure when
r /r = 0.414. From Equation (3.2)
C A
APF =
VS
VC
With regard to the sphere volume, V , there are four cation and four anion spheres per unit cell.
S
Thus,
⎛ 4 3⎞
⎛ 4 3⎞
VS = (4) ⎜ πrA ⎟ + (4)⎜ π rC ⎟
⎝3
⎠
⎝3
⎠
But, since r /r = 0.414
C A
VS =
[
]
16 3
3
3
π r 1 + (0.414 ) = (17.94) rA
3 A
Now, for r /r = 0.414 the corner anions in Table 12.2 just touch one another along the cubic unit
C A
cell edges such that
3
VC = a
[(
= 2 rA + rC
[(
= 2 rA + 0.414rA
)]
3
)] = (22.62)rA3
3
Thus
APF =
VS
V
C
3
=
(17.94) rA
(22.62) r3
A
326
= 0.79
12.8 We are asked to describe the crystal structure for K O, and then explain why it is called the
2
2antifluorite structure. First, let us find the coordination number of each O ion for K O. Taking the
2
r
K+
r
O
2−
=
0.138 nm
= 0.985
0.140 nm
From Table 12.2, the coordination number for oxygen is eight. According to Table 12.4, for a
coordination number of eight for both cations and anions, the crystal structure should be cesium
+
2+
chloride. However, there are twice as many K as O ions. Therefore, the centers of the K ions
2are positioned at the corners of cubic unit cells, while half of the cube centers are occupied by O
ions.
This structure is called the antifluorite crystal structure because anions and cations are
interchanged with one another from the fluorite structure (Figure 12.5).
12.9 This question is concerned with the zinc blende crystal structure in terms of close-packed planes of
anions.
(a) The stacking sequence of close-packed planes of anions for the zinc blende crystal structure will
be the same as FCC (and not HCP) because the anion packing is FCC (Table 12.4).
(b) The cations will fill tetrahedral positions since the coordination number for cations is four (Table
12.4).
(c) Only one-half of the tetrahedral positions will be occupied because there are two tetrahedral
sites per anion, and yet only one cation per anion.
12.10 This question is concerned with the corundum crystal structure in terms of close-packed planes of
anions.
3+
(a) For this crystal structure, two-thirds of the octahedral positions will be filled with Al ions since
23+
2there is one octahedral site per O ion, and the ratio of Al to O ions is two-to-three.
23+
(b) Two close-packed O planes and the octahedral positions that will be filled with Al ions are
sketched below.
327
12.11 (a) This portion of the problem asks that we specify which type of interstitial site the Be2+ ions will
occupy in BeO if the ionic radius of Be2+ is 0.035 nm and the O2- ions form an HCP arrangement.
Since, from Table 12.4, rO2- = 0.140 nm, then
r
Be2 +
r
O
=
2−
0.035 nm
= 0.250
0.140 nm
Inasmuch as rC/rA is between 0.225 and 0.414, the coordination number for Be2+ is 4 (Table 12.2);
therefore, tetrahedral interstitial positions are occupied.
(b) We are now asked what fraction of these available interstitial sites are occupied by Be2+ ions.
Since there are two tetrahedral sites per O2- ion, and the ratio of Be2+ to O2- is 1:1, one-half of
these sites are occupied with Be2+ ions.
12.12 (a) We are first of all asked to cite, for FeTiO3, which type of interstitial site the Fe2+ ions will
occupy. From Table 12.3, the cation-anion radius ratio is
r
Fe 2+
r
O
2−
=
0.077 nm
= 0.550
0.140 nm
Since this ratio is between 0.414 and 0.732, the Fe2+ ions will occupy octahedral sites (Table 12.2).
(b) Similarly, for the Ti4+ ions
328
r
Ti4 +
r
O
2−
=
0.061 nm
= 0.436
0.140 nm
Since this ratio is between 0.414 and 0.732, the Ti4+ ions will also occupy octahedral sites.
(c) Since both Fe2+ and Ti4+ ions occupy octahedral sites, no tetrahedral sites will be occupied.
(d) For every FeTiO3 formula unit, there are three O2- ions, and, therefore, three octahedral sites;
since there is one ion each of Fe2+ and Ti4+, two-thirds of these octahedral sites will be occupied.
12.13 First of all, open ‘Notepad” in Windows. Now enter into “Notepad” commands to generate the PbO
unit cell. One set of commands that may be used is as follows:
[DisplayProps]
Rotatez=-30
Rotatey=-15
[AtomProps]
Oxygen=LtRed,0.14
[BondProps]
SingleSolid=LtGray
[Atoms]
O1=0,0,0,Oxygen
O2=1,0,0,Oxygen
O3=1,1,0,Oxygen
O4=0,1,0,Oxygen
O5=0,0,1.265,Oxygen
O6=1,0,1.265,Oxygen
O7=1,1,1.265,Oxygen
O8=0,1,1.265,Oxygen
O9=0.5,0.5,0,Oxygen
O10=0.5,0.5,1.265,Oxygen
[Bonds]
B1=O1,O2,SingleSolid
B2=O2,O3,SingleSolid
B3=O3,O4,SingleSolid
B4=O1,O4,SingleSolid
B5=O5,O6,SingleSolid
B6=O6,O7,SingleSolid
B7=O7,O8,SingleSolid
B8=O5,O8,SingleSolid
B9=O1,O5,SingleSolid
B10=O2,O6,SingleSolid
329
B11=O3,O7,SingleSolid
B12=O4,O8,SingleSolid
Under the &quot;File&quot; menu of &quot;Note Pad,&quot; click &quot;Save As&quot;, and then assign the file for this figure a name
followed by a period and &quot;mdf&quot;; for example, “PbO.mdf”. And, finally save this file in the “mdf” file
inside of the “Interactive MSE” folder (which may be found in its installed location).
Now, in order to view the unit cell just generated, bring up “Interactive MSE”, and then
open any one of the three submodules under “Crystallinity and Unit Cells” or the “Ceramic
Structures” module. Next select “Open” under the “File” menu, and then open the “mdf” folder.
Finally, select the name you assigned to the item in the window that appears, and hit the “OK”
button. The image that you generated will now be displayed.
12.14 We are asked to calculate the theoretical density of NiO. This density may be computed using
Equation (12.1) as
ρ =
(
n' A Ni + A O
V N
)
C A
Since the crystal structure is rock salt, n' = 4 formula units per unit cell, and
⎛
⎞
3
VC = a = ⎜ 2r 2+ + 2r 2- ⎟
⎝ Ni
O ⎠
= 0.0730
3
= [2(0.069 nm) + 2 (0.140 nm)]
3
nm3
cm3
= 7.30 x 10-23
unit cell
unit cell
Thus,
ρ =
(4 formula units/unit cell)(58.69 g/mol + 16.00 g/mol)
-23
3
23
7.30 x 10
cm /unit cell 6.023 x 10 formula units/mol
(
)(
)
= 6.79 g/cm3
12.15 This problem calls for us to determine the unit cell edge length for MgO. The density of MgO is
3
3.58 g/cm and the crystal structure is rock salt.
(a) From Equation (12.1)
330
n' ⎛⎜ AMg + A O ⎟⎞
n' ⎛⎜ A Mg + A O⎟⎞
⎠
⎠
⎝
⎝
ρ =
=
3
V N
a N
C A
A
Or,
⎡n' ⎛ A
+ A ⎞⎤
O⎠ ⎥
⎢ ⎝ Mg
a = ⎢
⎥
ρN
A
⎢
⎥
⎣
⎦
1/ 3
1/ 3
⎡
⎤
⎢ (4 formula units/unit cell)(24.31 g/mol + 16.00 g/mol) ⎥
= ⎢
⎥
3.58 g/cm3 6.023 x 1023 formula units/mol
⎢⎣
⎥⎦
(
)(
)
= 4.21 x 10
-8
cm = 0.421 nm
2+
2(b) The edge length is to be determined from the Mg and O radii for this portion of the problem.
Now
a = 2r
+ 2r 2Mg2+
O
From Table 12.3
a = 2(0.072 nm) + 2(0.140 nm) = 0.424 nm
12.16
This problem asks that we compute the theoretical density of diamond given that the C—C
distance and bond angle are 0.154 nm and 109.5&deg;, respectively. The first thing we need do is to
determine the unit cell edge length from the given C—C distance. The drawing below shows the
cubic unit cell with those carbon atoms that bond to one another in one-quarter of the unit cell.
331
From this figure, φ is one-half of the bond angle or φ = 109.5&deg;/2 = 54.75&deg;, which means that
θ = 90&deg; − 54.75&deg; = 35.25&deg;
since the triangle shown is a right triangle. Also, y = 0.154 nm, the carbon-carbon bond distance.
Furthermore, x = a/4, and therefore,
x =
a
= y sin θ
4
Or
a = 4y sin θ = (4)(0.154 nm)(sin 35.25 &deg;) = 0.356 nm
= 3.56 x 10-8 cm
The unit cell volume, VC, is just a3, that is
(
)
VC = a3 = 3.56 x 10-8 cm
3
= 4.51 x 10−23 cm 3
We must now utilize a modified Equation (12.1) since there is only one atom type. There are 8
equivalent atoms per unit cell, and therefore
ρ =
=
n' AC
VC NA
(8 atoms/unit cell)(12.01 g/mol)
23
-23
4.51 x 10
cm3 /unit cell 6.023 x 10 atoms/mol
(
)(
)
= 3.54 g/cm3
The measured density is 3.51 g/cm3.
12.17 This problem asks that we compute the theoretical density of ZnS given that the Zn—S distance
and bond angle are 0.234 nm and 109.5&deg;, respectively. The first thing we need do is to determine
the unit cell volume from the given Zn—S distance. From the previous problem, the unit cell volume
VC is just a3, a being the unit cell edge length, and
332
3
3
VC = [4y sin θ] = [(4)(0.234 nm)(sin 35.25&deg;)]
= 0.1576 nm3 = 1.576 x 10-22 cm3
Now we must utilize Equation (12.1) with n' = 4 formula units, and AZn and AS being 65.39 and
32.06 g/mol, respectively. Thus
ρ=
(
n' AZn + A S
V N
)
C A
=
(4 formula units/unit cell)(65.39 g/mol + 32.06 g/mol)
-22
3
23
1.576 x 10
cm /unit cell 6.023 x 10 formula units/mol
(
)(
)
= 4.11 g/cm3
The measured value of the density is 4.10 g/cm3.
2+
212.18 We are asked to determine the number of Cd
and S ions per unit cell for cadmium sulfide
3
(CdS). For CdS, a = 0.582 nm and ρ = 4.82 g/cm . Using Equation (12.1)
n' =
ρVCN A
A Cd + A S
3
=
ρa NA
A Cd + A S
(4.82 g/cm3 )(5.82 x 10-8 cm) (6.023 x 1023 formula units/mol)
3
=
(112.40 g/mol + 32.06 g/mol)
= 3.96 or almost 4
2+
2Therefore, there are four Cd and four S per unit cell.
12.19 (a) We are asked to compute the theoretical density of CsCl. Modifying the result of Problem 3.4,
we get
333
2r
a =
Cs+
+ 2r
Cl −
2 (0.170 nm) + 2( 0.181 nm)
3
=
3
= 0.405 nm = 4.05 x 10-8 cm
From Equation (12.1)
ρ =
( Cs + ACl) = n' (ACs + ACl)
n' A
3
a N
V N
C A
A
For the CsCl crystal structure, n' = 1 formula unit/unit cell, and thus
ρ =
(1 formula unit/unit cell)(132.91 g/mol + 35.45 g/mol)
3
⎡
⎤
-8
23
formula units/mol
⎢ 4.05 x 10 cm /unit cell ⎥ 6.023 x 10
⎣
⎦
(
)
(
)
3
= 4.20 g/cm
(b) This value of the theoretical density is greater than the measured density. The reason for this
discrepancy is that the ionic radii in Table 12.3, used for this computation, were for a coordination
+
number of six, when, in fact, the coordination number of both Cs and Cl- is eight. The ionic radii
should be slightly greater, leading to a larger V value, and a lower theoretical density.
C
12.20 This problem asks that we compute the theoretical density of CaF . A unit cell of the fluorite
2
structure is shown in Figure 12.5. It may be seen that there are four CaF units per unit cell (i.e., n'
2
= 4 formula units/unit cell). Using a modified form of the result of Problem 3.4, we may assume, for
each of the eight small cubes in the unit cell, that
2r
a =
Ca 2+
+ 2r
F−
3
and, from Table 12.3
a =
2(0.100 nm) + 2(0.133 nm)
-8
= 0.269 nm = 2.69 x 10 cm
3
The volume of the unit cell is just
334
(
)
VC = (2a)3 = ⎡⎢(2 ) 2.69 x 10-3 cm ⎤⎥
⎣
⎦
3
= 1.56 x 10−22 cm3
Thus, from Equation (12.1)
ρ =
(
n' ACa + 2AF
V N
)
C A
=
(4 formula units/unit cell) [40.08 g/mol + (2)(19.00 g/mol)]
-22
3
23
1.56 x 10
cm /unit cell 6.023 x 10
formula units/mol
(
)(
)
= 3.33 g/cm3
3
The measured density is 3.18 g/cm .
12.21 We are asked to specify possible crystal structures for an AX type of ceramic material given its
density (2.10 g/cm3), that the unit cell has cubic symmetry with edge length of 0.57 nm, and the
atomic weights of the A and X elements (28.5 and 30.0 g/mol, respectively). Using Equation (12.1)
and solving for n' yields
n' =
ρVCN A
∑ AC + ∑ AA
(2.10 g/cm3 )⎡⎢⎣(5.70 x 10-8 cm) /unit cell ⎤⎥⎦ (6.023 x 1023 formula units/mol)
3
=
(30.0 + 28.5) g/mol
= 4.00 formula units/unit cell
Of the three possible crystal structures, only sodium chloride and zinc blende have four formula units
per unit cell, and therefore, are possibilities.
12.22 This problem asks us to compute the atomic packing factor for Fe3O4 given its density and unit
cell edge length. It is first necessary to determine the number of formula units in the unit cell in order
to calculate the sphere volume. Solving for n' from Equation (12.1) leads to
335
n' =
ρVCN A
∑ AC + ∑ AA
(5.24 g/cm3 )⎡⎢⎣(8.39 x 10-8 cm) /unit cell ⎤⎥⎦ (6.023 x 1023 formula units/mol)
3
=
(3)(55.85 g/mol) + (4)(16.00 g/mol)
= 8.0 formula units/unit cell
Thus, in each unit cell there are 8 Fe2+, 16 Fe3+, and 32 O2- ions. From Table 12.3, rFe2+ = 0.077
nm, rFe3+ = 0.069 nm, and rO2- = 0.140 nm. Thus, the total sphere volume, VS in Equation (3.2),
is just
(
)
(
)
3
3
⎛4 ⎞
⎛4 ⎞
−9
−9
VS = (8) ⎜ π⎟ 7.7 x 10 cm + (16) ⎜ π⎟ 6.9 x 10 cm
⎝3 ⎠
⎝3 ⎠
(
)
3
⎛4 ⎞
−8
+ (32) ⎜ π ⎟ 1.40 x 10
cm
⎝3 ⎠
= 4.05 x 10-22 cm3
Now, the unit cell volume (VC) is just
(
) = 5.90 x 10
VC = a 3 = 8.39 x 10-8 cm
3
−22
cm 3
Finally, the atomic packing factor (APF) from Equation (3.2) is just
APF =
VS
V
C
=
4.05 x 10-22 cm3
= 0.686
5.90 x 10-22 cm3
12.23 This problem asks for us to calculate the atomic packing factor for aluminum oxide given values for
the a and c lattice parameters, and the density. It first becomes necessary to determine the value of
n' in Equation (12.1). This necessitates that we calculate the value of VC, the unit cell volume. In
Problem 3.7 it was shown that the area of the hexagonal base (AREA) is related to a as
336
⎛ a⎞
AREA = 6 3 ⎜ ⎟
⎝ 2⎠
(
2
= 1.5 a
2
3
)
2
= (1.5) 4.759 x 10-8 cm (1.732) = 5.88 x 10−15 cm2
The unit cell volume now is just
(
-15
VC = (AREA)(c) = 5.88 x 10
2
cm
)(1.2989 x 10 -7 cm)
= 7.64 x 10-22 cm3
Now, solving for n' in Equation (12.1) yields
n' =
ρNA VC
∑ AC + ∑ AA
3.99 g/cm3 )(6.023 x 1023 formula units/mol)(7.64 x 10-22 cm3 /unit cell)
(
=
(2)(26.98 g/mol) + (3)(16.00 g/mol)
= 18.0 formula units/unit cell
Thus, there are 18 Al2O3 units per unit cell, or 36 Al3+ ions and 54 O2- ions. From Table 12.3, the
radii of these two ion types are 0.053 and 0.140 nm, respectively. Thus, the total sphere volume, VS
in Equation (3.2), is just
(
)
(
)
3
3
⎛4 ⎞
⎛4 ⎞
−9
−8
VS = (36)⎜ π ⎟ 5.3 x 10 cm + (54)⎜ π⎟ 1.4 x 10 cm
⎝3 ⎠
⎝3 ⎠
= 6.43 x 10-22 cm3
Finally, the APF is just
APF =
VS
V
C
=
6.43 x 10-22 cm3
= 0.842
7.64 x 10-22 cm3
337
12.24 We are asked in this problem to compute the atomic packing factor for the diamond cubic crystal
structure, given that the angle between adjacent bonds is 109.5&deg;. The first thing that we must do is
to determine the unit cell volume VC in terms of the atomic radius r. From Problem 12.16 the
following relationship was developed
a = 4y sin θ
in which y = 2r and θ = 35.25&deg;. Furthermore, since the unit cell is cubic, VC = a3; therefore
VC = (4y sin θ)
3
= [(4)(2r)(sin 35.25 &deg;)] = 98.43 r
3
3
Now, it is necessary to determine the sphere volume in the unit cell, VS, in terms of r. For this unit
cell (Figure 12.15) there are 4 interior atoms, 6 face atoms, and 8 corner atoms. The entirety of
each of the interior atoms, one-half of each face atom, and one-eighth of each corner atom belong to
the unit cell. Therefore, there are 8 equivalent atoms per unit cell; hence
⎛ 4 3⎞
3
VS = (8)⎜ πr ⎟ = 33.51 r
⎝3
⎠
Finally, the atomic packing factor is just
APF =
VS
V
C
=
33.51 r3
98.43 r 3
= 0.340
12.25 We are asked in this problem to compute the atomic packing factor for the CsCl crystal structure.
This requires that we take the ratio of the sphere volume within the unit cell and the total unit cell
volume. From Figure 12.3 there is the equivalent of one Cs and one Cl ion per unit cell; the ionic
radii of these two ions are 0.170 nm and 0.181 nm, respectively (Table 12.3). Thus, the sphere
volume, VS, is just
VS =
[
4
(π ) (0.170 nm)3 + (0.181 nm)3
3
]=
0.0454 nm
3
Using a modified form of the result of Problem 3.4, for CsCl we may express the unit cell edge
length, a, in terms of the atomic radii as
338
a =
2r
Cs+
+ 2r Cl
=
3
2(0.170 nm) + 2(0.181 nm)
3
= 0.405 nm
Since VC = a3
VC = (0.405 nm)3 = 0.0664 nm3
And, finally the atomic packing factor is just
APF =
VS
V
C
=
0.0454 nm3
= 0.684
3
0.0664 nm
12.26 This problem asks that we represent specific crystallographic planes for various ceramic crystal
structures.
(a) A portion of the (100) plane for the rock salt crystal structure would appear as
(b) A portion of the (110) plane for the cesium chloride crystal structure would appear as
(c) A portion of the (111) plane for the zinc blende crystal structure would appear as
339
(d) A portion of the (110) plane for the perovskite crystal structure would appear as
12.27
The silicate materials have relatively low densities because the atomic bonds are primarily
covalent in nature (Table 12.1), and, therefore, directional. This limits the packing efficiency of the
atoms, and therefore, the magnitude of the density.
12.28 This problem asks for us to determine the angle between covalent bonds in an SiO 44 − tetrahedron.
Below is shown one such tetrahedron situated within a cube.
340
Now if we extend the base diagonal from one corner to the other, it is the case that
(2y)2 = a 2 + a 2 = 2a 2
or
y =
a 2
2
Furthermore, x = a/2, and
a
x
1
2
tan θ =
=
=
y a 2
2
2
From which
⎛ 1⎞
θ = tan-1⎜
⎟ = 35.26&deg;
⎝ 2⎠
Now, solving for the angle φ
φ = 180&deg; - 90&deg; - 35.26&deg; = 54.74&deg;
Finally, the bond angle is just 2φ, or 2φ = (2)(54.74&deg;) = 109.48&deg;.
12.29 (a) The chemical formula for kaolinite clay may also be written as Al2O3-2SiO2-2H2O. Thus, if
we remove the chemical water, the formula becomes Al2O3-2SiO2. The formula weight for Al2O3 is
just (2)(26.98 g/mol) + (3)(16.00 g/mole) = 101.96 g/mol; and for SiO2 the formula weight is 28.09
g/mol + (2)(16.00 g/mol) = 60.09 g/mol. Thus, the composition of this product, in terms of the
concentration of Al2O3, CAl O , in weight percent is just
2 3
341
101.96 g / mol
C Al O =
&times; 100 = 45.9 wt%
101.96 g/ mol + (2)(60.09 g / mol)
2 3
(b) The liquidus and solidus temperatures for this material as determined from the SiO2-Al2O3
phase diagram, Figure 12.27, are 1800&deg;C and 1587&deg;C, respectively.
12.30 Frenkel defects for anions would not exist in appreciable concentrations because the anion is quite
large and is highly unlikely to exist as an interstitial.
12.31 Stoichiometric means having the exact ratio of anions to cations as specified by the chemical
formula for the compound.
12.32 (a) For a Cu2+O2- compound in which a small fraction of the Cu2+ ions exist as Cu+, for each
Cu+ formed there is one less positive charge introduced (or one more negative charge). In order to
maintain charge neutrality, we must either add an additional positive charge or remove a negative
charge. This may be accomplished be either creating Cu2+ interstitials or O2- vacancies.
(b) There will be two Cu+ ions required for each of these defects.
(c) The chemical formula for this nonstoichiometric material may be expressed as Cu1+xO or CuO1, where x is some
x
small fraction.
+
2+
+
12.33 (a) For Li substituting for Ca
in CaO, oxygen vacancies would be created. For each Li
2+
substituting for Ca , one positive charge is removed; in order to maintain charge neutrality, a
single negative charge may be removed. Negative charges are eliminated by creating oxygen
+
vacancies, and for every two Li ions added, a single oxygen vacancy is formed.
2(b) For Cl substituting for O in CaO, calcium vacancies would be created. For each Cl
2substituting for an O , one negative charge is removed; in order to maintain charge neutrality, two
Cl ions will lead to the formation of one calcium vacancy.
2+
3+
12.34 For every Mg ion that substitutes for Al in Al O , a single positive charge is removed. Thus,
2 3
in order to maintain charge neutrality, either a positive charge must be added or a negative charge
must be removed.
3+
3+
Positive charges are added by forming Al
interstitials, and one Al
interstitial would be
2+
formed for every three Mg ions added.
342
2Negative charges may be removed by forming O vacancies, and one oxygen vacancy
2+
would be formed for every two Mg ions added.
12.35 There is only one eutectic for the portion of the ZrO2-CaO system shown in Figure 12.26, which,
upon cooling, is
Liquid → cubic ZrO2 + CaZrO3
There are two eutectoids, which reactions are as follows:
tetragonal → monoclinic ZrO 2 + cubic ZrO2
cubic → monoclinic ZrO2 + CaZr4O9
12.36 (a) For this portion of the problem we are to determine the type of vacancy defect that is
produced on the Al2O3-rich side of the spinel phase field (Figure 12.25) and the percentage of these
vacancies at the maximum nonstoichiometry (82 mol% Al2O3). On the alumina-rich side of this
phase field, there is an excess of Al3+ ions, which means that some of the Al3+ ions substitute for
Mg2+ ions. In order to maintain charge neutrality, Mg2+ vacancies are formed, and for every Mg2+
vacancy formed, two Al3+ ions substitute for three Mg2+ ions.
Now, we will calculate the percentage of Mg2+ vacancies that exist at 82 mol% Al2O3. Let
us arbitrarily choose as our basis 50 MgO-Al2O3 units of the stoichiometric material which consists
of 50 Mg2+ ions and 100 Al3+ ions. Furthermore, let us designate the number of Mg2+ vacancies
as x, which means that 2x Al3+ ions have been added and 3x Mg2+ ions have been removed (two
of which are filled with Al3+ ions). Using our 50 MgO-Al2O3 unit basis, the number of moles of
Al2O3 in the nonstoichiometric material is (100 + 2x)/2; similarly the number of moles of MgO is (50
- 3x). Thus, using a modified form of Equation (4.5), we may write an expression for the mole
percent of Al2O3 as
100 + 2x
⎡
⎤
⎢
⎥
2
mol% Al2 O3 = ⎢
⎥ &times; 100
100 + 2x
⎢
+ (50 − 3x) ⎥
⎣
⎦
2
343
If we solve for x when the mol% of Al2O3 = 82, then x = 12.1. Thus, adding 2x or (2)(12.1) = 24.2
Al3+ ions to the original material consisting of 100 Al3+ and 50 Mg2+ ions will produce 12.1 Mg2+
vacancies. Therefore, the percentage of vacancies is just
% vacancies =
12.1
&times; 100 = 8.1%
100 + 50
(b) Now, we are asked to make the same determinations for the MgO-rich side of the spinel phase
field, for 40 mol% Al2O3. In this case, Mg2+ ions are substituting for Al3+ ions. Since the Mg2+ ion
has a lower charge than the Al3+ ion, in order to maintain charge neutrality, negative charges must
be eliminated, which may be accomplished by introducing O2- vacancies. For every 2 Mg2+ ions
that substitute for 2 Al3+ ions, one O2- vacancy is formed.
Now, we will calculate the percentage of O2- vacancies that exist at 40 mol% Al2O3. Let us
arbitrarily choose as our basis 50 MgO-Al2O3 units of the stoichiometric material which consist of 50
Mg2+ ions 100 Al3+ ions. Furthermore, let us designate the number of O2- vacancies as y, which
means that 2y Mg2+ ions have been added and 2y Al3+ ions have been removed. Using our 50
MgO-Al2O3 unit basis, the number of moles of Al2O3 in the nonstoichiometric material is (100 2y)/2; similarly the number of moles of MgO is (50 + 2y). Thus, the expression for the mole percent
of Al2O3 is just
100 − 2y
⎡
⎤
⎢
⎥
2
mol% Al2 O3 = ⎢
⎥ &times; 100
100 − 2y
⎢
+ (50 + 2y) ⎥
⎣
⎦
2
If we solve for y when the mole percent of Al2O3 = 40, then y = 7.14. Thus, 7.14 O2- vacancies are
produced in the original material that had 200 O2- ions. Therefore, the percentage of vacancies is
just
% vacancies =
7.14
&times; 100 = 3.57%
200
12.37 (a) There may be significant scatter in the fracture strength for some given ceramic material
because the fracture strength depends on the probability of the existence of a flaw that is capable of
initiating a crack; this probability varies from specimen to specimen of the same material.
(b)
The fracture strength increases with decreasing specimen size because as specimen size
decreases, the probably of the existence of a flaw of that is capable of initiating a crack diminishes.
344
12.38 We are asked for the critical crack tip radius for an Al O material. From Equation (8.1)
2 3
⎛ a⎞
σm = 2 σo ⎜⎜ ⎟⎟
⎝ ρt ⎠
1/ 2
Fracture will occur when σm reaches the fracture strength of the material, which is given as E/10;
thus
⎛a⎞
E
= 2σ o ⎜⎜ ⎟⎟
10
⎝ ρt ⎠
1/ 2
Or, solving for ρt
2
ρt =
400 a σo
E2
From Table 12.5, E = 393 GPa, and thus,
ρt =
(
)
(400) 2 x 10 −3 mm (275 MPa)2
(393 x 103 MPa)
2
= 3.9 x 10-7 mm = 0.39 nm
12.39 This problem asks that we compute the crack tip radius ratio before and after etching. Let
ρ t = original crack tip radius, and
ρ 't = etched crack tip radius
Also,
σ f' = σ f
a
a' =
2
σ o' = 4σo
345
Solving for
ρt'
ρt
from the following
⎛ a⎞
σ f = 2 σo ⎜⎜ ⎟⎟
⎝ ρt ⎠
1/2
⎛ ⎞
a'
= σ f' = 2σ o' ⎜ ⎟
⎜ '⎟
⎝ ρt ⎠
1/2
yields
2
2
⎛ ' ⎞
σo ⎟ ⎛ a'⎞ ⎛ 4σ o ⎞ ⎛ a / 2 ⎞
⎜
⎟ =8
⎜ ⎟ =⎜
⎟ ⎜
=
⎜ σ ⎟ ⎝ a⎠ ⎜ σ ⎟ ⎝ a ⎠
ρ
⎝ o⎠
t
⎝ o⎠
ρ 't
12.40 (a) For this portion of the problem we are asked to compute the flexural strength for a glass
specimen that is subjected to a three-point bending test. The flexural strength [Equation 12.3(a)] is
just
σ fs =
3Ff L
2bd2
for a rectangular cross-section. Using the values given in the problem,
σ fs =
(
−3
(3)(290 N) 45 x 10
(
(2) 10 x 10
−3
)(
)
m
−3
m 5 x 10
)
m
2
= 78.3 MPa (10, 660 psi)
(b) We are now asked to compute the maximum deflection. From Table 12.5, the elastic modulus
6
(E) for glass is 69 GPa (10 x 10 psi). Also, the moment of inertia for a rectangular cross section
(Figure 12.29) is just
I =
bd 3
12
Thus,
Δy =
FL3
FL3
=
⎛ bd3 ⎞
4Ebd3
⎟⎟
48E ⎜⎜
⎝ 12 ⎠
346
−3
m)
(
=
9
2
−3
−3 3
(4) (69 x 10 N / m )(10 x 10 m)(5 x 10 m)
3
(266 N) 45 x 10
= 7.0 x 10-5 m = 7.0 x 10-2 mm (2.5 x 10-3 in.)
12.41 We are asked to calculate the maximum radius of a circular specimen that is loaded using threepoint bending. Solving for R from Equation (12.3b)
⎡ FL ⎤
R =⎢ f ⎥
⎢⎣ σ fs π ⎥⎦
1/3
which, when substituting the parameters stipulated in the problem, yields
(
)⎤⎥
⎡ (425 N) 50 x 10−3 m
R =⎢
⎢
6
2
⎢⎣ 105 x 10 N/ m (π)
(
)
1/3
⎥
⎥⎦
= 4.0 x 10-3 m = 4.0 mm (0.16 in.)
12.42 For this problem, the load is given at which a circular specimen of aluminum oxide fractures when
subjected to a three-point bending test; we are then are asked to determine the load at which a
specimen of the same material having a square cross-section fractures. It is first necessary to
compute the flexural strength of the alumina using Equation (12.3b), and then, using this value, we
may calculate the value of Ff in Equation (12.3a). From Equation (12.3b)
σ fs =
(
(3000 N) 40 x 10 −3 m
=
(
(π) 5.0 x 10
−3
m
)
3
)= 306
FfL
πR3
6
2
x 10 N/m
= 306 MPa (42, 970 psi)
Now, solving for Ff from Equation (12.3a), realizing that b = d = 12 mm, yields
Ff =
2σ fsd
3L
347
3
(
)(15 x 10 −3m)
(3) (40 x 10−3 m)
6
(2) 306 x 10 N/ m
=
3
2
= 17, 200 N (3870 lb f )
12.43 (a) This portion of the problem asks that we determine whether or not a cylindrical specimen of
aluminum oxide having a flexural strength of 300 MPa (43,500 psi) and a radius of 5 mm will fracture
when subjected to a load of 7500 N in a three-point bending test; the support point separation is
given as 15 mm. Using Equation (12.3b) we will calculate the value of σ; if this value is greater than
σfs (300 MPa), then fracture is expected to occur. Employment of Equation (12.3b) yields
σ =
FL
πR 3
(
(7500 N) 15 x 10
=
(
(π) 5 x 10
−3
−3
)
m
)= 286.5 x 106 N/m2 = 286.5 MPa
m
3
(40, 300 psi)
Since this value is less than the given value of σfs (300 MPa), then fracture is not predicted.
(b) The certainty of this prediction is not 100% because there is always some variability in the
flexural strength for ceramic materials, and since this value of σ is relatively close to σfs then there is
some chance that fracture will occur.
12.44 Crystalline ceramics are harder yet more brittle than metals because they (ceramics) have fewer
slip systems, and, therefore, dislocation motion is highly restricted.
12.45 (a) This portion of the problem requests that we compute the modulus of elasticity for nonporous
spinel given that E = 240 GPa for a material having 5 vol% porosity. Thus, we solve Equation (12.5)
for Eo, using P = 0.05, which gives
Eo =
=
E
1 − 1.9P + 0.9P2
240 GPa
1 − (1.9)(0.05) + (0.9)(0.05)2
(38.6 x 106 psi)
= 265 GPa
(b) Now we are asked to determine the value of E at P = 15 vol%. Using Equation (12.5) we get
(
2
E = E o 1 − 1.9P + 0.9P
348
)
[
]
(
= (265 GPa) 1 - (1.9)(0.15 ) + (0.09 )(0.15 )2 = 195 GPa 28.4 x 106 psi
)
12.46 (a) This portion of the problem requests that we compute the modulus of elasticity for nonporous
TiC given that E = 310 GPa (45 x 106 psi) for a material having 5 vol% porosity. Thus, we solve
Equation (12.5) for Eo, using P = 0.05, which gives
Eo =
=
E
1 − 1.9P + 0.9P2
310 GPa
1 − (1.9)(0.05) + (0.9)(0.05)2
= 342 GPa
(49.6 x 106 psi)
(b) Now we are asked to compute the volume percent porosity at which the elastic modulus of TiC is
240 MPa (35 x 106 psi). Since from part (a), Eo = 342 GPa, and using Equation (12.5) we get
E
240 MPa
=
= 0.702 = 1 − 1.9P + 0.9P2
Eo 342 MPa
Or
0.9P
2
− 1.9P + 0.298 = 0
Now, solving for the value of P using the quadratic equation solution yields
P =
1.9 &plusmn;
(−1.9) 2 − (4)(0.9)(0.298)
(2)(0.9)
The positive and negative roots are
P+ = 1.94
P- = 0.171
Obviously, only the negative root is physically meaningful, and therefore the value of the porosity to
give the desired modulus of elasticity is 17.1 vol%.
12.47
(a)
This part of the problem asks us to determine the flexural strength of nonporous MgO
assuming that the value of n in Equation (12.6) is 3.75. Taking natural logarithms of both sides of
Equation (12.6) yields
349
ln σfs = lnσ o − nP
In Table 12.5 it is noted that for P = 0.05, σfs = 105 MPa. For the nonporous material P = 0 and,
ln σo = ln σfs. Solving for ln σo from the above equation and using these data gives
ln σo = lnσ fs + nP
= ln (105 MPa) + (3.75)(0.05) = 4.841
or σo = e4.841 = 127 MPa (18,100 psi)
(b) Now we are asked to compute the volume percent porosity to yield a σfs of 74 MPa (10,700 psi).
Taking the natural logarithm of Equation (12.6) and solving for P leads to
P =
=
ln σ o − ln σ fs
n
ln (127 MPa) − ln (74 MPa)
3.75
= 0.144 or 14.4 vol%
12.48 (a) Given the flexural strengths at two different volume fraction porosities, we are asked to
determine the flexural strength for a nonporous material. If the natural logarithm is taken of both
sides of Equation (12.6), then
ln σfs = ln σo − nP
Using the data provided in the problem, two simultaneous equations may be written as
ln (100 MPa) = ln σ o − (0.05)n
ln (50 MPa) = ln σ o − (0.20)n
Solving for n and σo leads to n = 4.62 and σo = 126 MPa. For the nonporous material, P = 0, and,
from Equation (12.6), σo = σfs. Thus, σfs for P = 0 is 126 MPa.
350
(b) Now, we are asked for σfs at P = 0.1 for this same material. Utilizing Equation (12.6) yields
σ fs = σ o exp (− nP)
= (126 MPa) exp [− (4.62)(0.1)]
= 79.4 MPa
Design Problems
12.D1 This problem asks that we determine the concentration (in weight percent) of GaP that must be
added to GaAs to yield a unit cell edge length of 0.5570 nm. The densities of GaAs and GaP were
given in the problem as 5.307 and 4.130 g/cm3, respectively. To begin, it is necessary to employ
Equation (12.1), and solve for the unit cell volume, VC, for the GaP-GaAs alloy as
n' Aave
VC =
ρave NA
where Aave and ρave are the atomic weight and density, respectively, of the GaAs-GaP alloy.
Inasmuch as both of these materials have the zinc blende crystal structure, which has cubic
symmetry, VC is just the cube of the unit cell length, a. That is
VC = a3 = (0.5570 nm)3
(
= 5.570 x 10
−8
) = 1.728
cm
3
x 10
−22
3
cm
It is now necessary to construct expressions for Aave and ρave in terms of the concentration of
gallium phosphide, CGaP using Equations (4.11a) and (4.10a). For Aave we have
A ave =
100
C
GaP +
A
GaP
351
(100 −
A
C
GaP
GaAs
)
100
=
C
GaP
100.69 g / mol
+
(100 −
)
C
GaP
144.64 g / mol
Whereas for ρave
ρ ave =
100
C
GaP +
ρ
GaP
(100 −
ρ
C
GaP
)
GaAs
100
=
C GaP
4.130 g / cm 3
+
(100 −
CGaP
)
5.307 g / cm3
Within the zinc blende unit cell there are four formula units, and thus, the value of n' in Equation
(12.1) is 4; hence, this expression may be written in terms of the concentration of GaP in weight
percent as follows:
VC = 1.728 x 10-22 cm3
=
n' Aave
ρaveN A
⎡
⎤
⎢
⎥
100
⎢
⎥
(4 fu/ unitcell) ⎢
⎥
100 − C
CGaP
⎢
GaP ⎥
⎢⎣ 100.69 g / mol + 144.64 g / mol ⎥⎦
=
⎡
⎤
⎢
⎥
⎢
⎥
100
⎢
⎥ 6.023 x 1023 fu / mole
100 − C GaP ⎥
⎢
C
GaP
+
⎢
⎥
5.307 g / cm 3 ⎦
⎣ 4.130 g / cm 3
(
)(
(
)
)
And solving this expression for CGaP leads to CGaP = 34 wt%.
12.D2
This problem asks for us to determine which of the ceramic materials in Table 12.5, when
of 445 N (100 lbf) is applied, and also will not experience a center-point deflection of more than
352
0.021 mm (8.5 x 10-4 in.). The first of these criteria is met by those materials that have flexural
strengths greater than the stress calculated using Equation (12.3b). According to this expression
σ fs =
=
(
FL
π R3
) = 131 x 106 N / m2 = 131 MPa (18,900 psi)
(445 N) 50.8 x 10−3 m
(
−3
(π) 3.8 x 10
)
3
m
Of the materials in Table 12.5 the following have flexural strengths greater than this value: Si3N4,
ZrO2, SiC, Al2O3, glass-ceramic, mullite, and spinel.
For the second criterion we must solve for the magnitude of the modulus of elasticity, E,
from the equation given in Problem 12.40 where the expression for the cross-sectional moment of
πR 4
inertia appears in Figure 12.29; that is, for a circular cross-section I =
. Solving for E from
4
these two expressions
E =
FL3
12π R4 Δy
(
(445 N) 50.8 x 10
=
(
(12)(π) 3.8 x 10
−3
−3
)
m
3
) (0.021 x 10−3 m)
m
4
= 353 x 109 N/m2 = 353 GPa (49.3 x 106 psi)
Of those materials that satisfy the first criterion, only Al2O3 has a modulus of elasticity greater than
this value (Table 12.5), and, therefore, is a possible candidate.
353
CHAPTER 13
APPLICATIONS AND PROCESSING OF CERAMICS
PROBLEM SOLUTIONS
13.1 The two desirable characteristics of glasses are optical transparency and ease of fabrication.
13.2 (a) Devitrification is the process whereby a glass material is caused to transform to a crystalline
solid, usually by a heat treatment.
(b) Two properties that may be improved by devitrification are 1) a lower coefficient of thermal
expansion, and 2) a higher thermal conductivity. Two properties that may be impaired are 1) a loss
of optical transparency, and 2) a lowering of mechanical strength when stresses are introduced from
volume changes that attend the transformation. In some cases, however, strength may actually be
improved.
13.3 Glass-ceramics may not be transparent because they are polycrystalline. Light will be scattered at
grain boundaries in polycrystalline materials if the index of refraction is anisotropic, and when those
grains adjacent to the boundary have different crystallographic orientations. This phenomenon is
discussed in Section 21.10.
13.4 For refractory ceramic materials, three characteristics that improve with increasing porosity are
decreased thermal expansion and contraction upon thermal cycling, improved thermal insulation,
and resistance to thermal shock. Two characteristics that are adversely affected are load-bearing
capacity and resistance to attack by corrosive materials.
13.5
(a)
From Figure 12.25, the maximum temperature without a liquid phase corresponds to the
temperature at the MgO(ss)-[MgO(ss) + Liquid] boundary at this composition, which is approximately
2240&deg;C (4060&deg;F).
(b) This maximum temperature lies at the phase boundary between MgAl O (ss)-(MgAl O +
2 4
2 4
Liquid) phase fields (just slightly to the right of the congruent melting point at which the two phase
boundaries become tangent); this temperature is approximately 2090&deg;C (3790&deg;F).
13.6 For each section of this problem two SiO2-Al2O3 compositions are given; we are to decide, on the
basis of the SiO2-Al2O3 phase diagram (Figure 12.27), which is the more desirable as a refractory
and then justify the choice.
354
(a) The 99.8 wt% SiO2-0.2 wt% Al2O3 will be more desirable because the liquidus temperature will
be greater for this composition; therefore, at any temperature within the cristobalite + liquid region
on the phase diagram, there will be a lower fraction of the liquid phase present than for the 99.0 wt%
SiO2-1.0 wt% Al2O3 composition, and, thus, the mechanical integrity will be greater.
(b)
The 74 wt% Al2O3-26 wt% SiO2 composition will be more desirable because, for this
composition, a liquid phase does not form until about 1750&deg;C [i.e., the temperature at which a
vertical line at 74 wt% Al2O3 crosses the boundary between the mullite and (mullite + liquid) phase
regions];
for the 70 wt% Al2O3-30 wt% SiO2 material, a liquid phase forms at a much lower
temperature--1587&deg;C.
(c) The 95 wt% Al2O3-5 wt% SiO2 composition will be more desirable because the liquidus
temperature will be greater for this composition. Therefore, at any temperature within the alumina +
liquid region on the phase diagram, there will be a lower fraction of the liquid phase present than for
the 90 wt% Al2O3-10 wt% SiO2 composition, and, thus, the mechanical integrity of the 95 wt%
Al2O3-5 wt% SiO2 material will be greater.
13.7 This problem calls for us to compute the mass fractions of liquid for two fireclay refractory materials
at 1600&deg;C. In order to solve this problem it is necessary that we use the SiO2-Al2O3 phase diagram
(Figure 12.27). The mass fraction of liquid, WL, as determined using the lever rule and tie line at
1600&deg;C, is just
WL =
Cmullite − Co
Cmullite − CL
where Cmullite = 72 wt% Al2O3 and CL = 8 wt% Al2O3, as determined using the tie-line; also, Co
is the composition (in weight percent Al2O3) of the refractory material.
(a) For the 25 wt% Al2O3- 75 wt% SiO2 composition, Co = 25 wt% Al2O3, and
WL =
72 − 25
= 0.73
72 − 8
(b) For the 45 wt% Al2O3- 55 wt% SiO2 composition, Co = 45 wt% Al2O3, and
WL =
72 − 45
= 0.42
72 − 8
355
13.8 (a) This portion of the problem asks that we specify, for the SiO2-Al2O3 system, the maximum
temperature possible without the formation of a liquid phase. According to Figure 12.27 this
maximum temperature is 1890&deg;C, which is possible for compositions between about 77 Al2O3 and
virtually 100 wt% Al2O3.
(b) For the MgO-Al2O3 system, Figure 12.25, the maximum temperature without the formation of a
liquid phase is approximately 2800&deg;C which is possible for pure MgO.
13.9 For clay-based aggregates, a liquid phase forms during firing, which infiltrates the pores between
the unmelted particles; upon cooling, this liquid becomes a glass, which serves as the bonding
phase.
With cements, the bonding process is a chemical, hydration reaction between the water that
has been added and the various cement constituents. The cement particles are bonded together by
reactions that occur at the particle surfaces.
13.10 It is important to grind cement into a fine powder in order to increase the surface area of the
particles of cement. The hydration reactions between water and the cement occur at the surface of
the cement particles. Therefore, increasing the available surface area allows for more extensive
bonding.
13.11 We are asked to compute the weight of soda ash and limestone that must be added to 100 lbm of
SiO to yield a glass composition of 75 wt% SiO , 15 wt% Na O, and 10 wt% CaO. Inasmuch as
2
2
2
the concentration of SiO2 in the glass is 75wt%, the final weight of the glass (mglass) is just
mglass =
100 lbm
0.75
= 133.3 lbm
Therefore, the weights of Na2O (mNa O) and CaO (mCaO) are as follows:
2
⎛ 15 wt% ⎞
⎟ (133.3 lbm ) = 20.0 lbm
mNa O = ⎜
⎝ 100 ⎠
2
and
⎛ 10 wt% ⎞
⎟(133.3 lbm ) = 13.3 lbm
mCaO = ⎜
⎝ 100 ⎠
In order to compute the weights of Na CO and CaCO we must employ molecular weights, as
2 3
3
356
⎛ molecular wt. Na CO ⎞
2
3
mNa CO = (20.0 lb m ) ⎜⎜
⎟⎟
molecular
wt.
Na
O
2
3
⎠
⎝
2
⎛ 105.99 g / mol ⎞
= (20.0 lb m ) ⎜
⎟ = 34.2 lbm
⎝ 61.98 g / mol ⎠
and
mCaCO
3
⎛ molecular wt. CaCO 3 ⎞
= (13.3 lb m ) ⎜
⎟
⎝ molecular wt. CaO ⎠
⎛ 100.09 g / mol ⎞
= (13.3 lb m ) ⎜
⎟ = 23.8 lbm
⎝ 56.08 g / mol ⎠
13.12 The glass transition temperature is, for a noncrystalline ceramic, that temperature at which there is
a change of slope for the specific volume versus temperature curve (Figure 13.5).
The melting temperature is, for a crystalline material, that temperature at which there is a
sudden and discontinuous decrease in the specific volume versus temperature curve.
13.13 In order to be drawn into fibers, a material must exist as a viscous fluid. Crystalline aluminum
oxide is a solid below its melting temperature and a nonviscous fluid above. On the other hand, a
glass will be a viscous fluid as a supercooled liquid.
13.14 The annealing point is that temperature at which the viscosity of the glass is 10
12
13
Pa-s (10 P).
From Figure 13.6, these temperatures for the several glasses are as follows:
Glass
Annealing Temperature
Soda-lime
500&deg;C (930&deg;F)
Borosilicate
570&deg;C (1060&deg;F)
96% Silica
930&deg;C (1705&deg;F)
Fused Silica
1170&deg;C (2140&deg;F)
13.15 The softening point of a glass is that temperature at which the viscosity is 4 x 106 Pa-s; from
Figure 13.6, these temperatures for the 96% silica, borosilicate, and soda-lime glasses are 1540&deg;C
(2800&deg;F), 830&deg;C (1525&deg;F), and 700&deg;C (1290&deg;F), respectively.
357
13.16 (a) Below is shown the logarithm viscosity versus reciprocal of temperature plot for the borosilicate
glass, using the data in Figure 13.6.
(b) The activation energy, Q
vis
, may be computed from this plot according to
⎡
⎤
⎢ Δ ln η ⎥
Q vis = R ⎢
⎥
⎢ Δ ⎛⎜ 1 ⎞⎟ ⎥
⎢⎣ ⎝ T ⎠ ⎦⎥
where R is the gas constant, and Δln η/Δ(1/T) is the slope of the line that has been constructed. The
value of this slope is 4.36 x 104 K. Therefore,
(
4
Qvis = (8.31 J/mol- K) 4.36 x 10 K
)
= 362,000 J/mol
13.17 This problem calls for us to determine the maximum temperature to which a cylindrical specimen of
soda-lime glass may be heated in order that its deformation be less than 1 mm over a week's time.
According to Equation (6.1)
358
σ =
F
=
A
o
1N
⎛ 5 x 10−3 m ⎞
⎟⎟
π⎜⎜
2
⎝
⎠
2
= 5.1 x 104 Pa
Also,
(
d Δl/ l o
dε
=
dt
dt
=
)
1 mm / 100 mm
-8 -1
= 1.653 x 10 s
(1 wk)(7 days/ week)(24 h / day)(3600 s / h)
Thus,
η =
5.1 x 104 Pa
σ
=
= 3.1 x 1012 Pa - s
dε / dt
1.653 x 10−8 s −1
From Figure 13.6, the temperature at which the viscosity of the soda-lime glass is 3.1 x 10
12
Pa-s is
13.18 (a) Residual thermal stresses are introduced into a glass piece when it is cooled because surface
and interior regions cool at different rates, and, therefore, contract different amounts; since the
material will experience very little, if any deformation, stresses are established.
(b) Yes, thermal stresses will be introduced because of thermal expansion upon heating for the
same reason as for thermal contraction upon cooling.
(c) The thinner the thickness of a glass ware the smaller the thermal stresses that are introduced
when it is either heated or cooled. The reason for this is that the difference in temperature across
the cross-section of the ware, and, therefore, the difference in the degree of expansion or contraction
will decrease with a decrease in thickness.
13.19 Borosilicate glasses and fused silica are resistant to thermal shock because they have relatively
low coefficients of thermal expansion; therefore, upon heating or cooling, the difference in the
degree of expansion or contraction across the cross-section of a ware that is constructed from these
materials will be relatively low.
13.20 Thermal tempering of glasses is described in Section 13.8.
359
+
13.21 Chemical tempering will be accomplished by substitution, for Na , another monovalent cation with
+
+
a slightly larger diameter. From Table 12.3, both K and Cs fill this criterion, having ionic radii of
+
+
0.138 and 0.170 nm, respectively. In fact, soda-lime glasses are tempered using a K -Na ion
exchange.
13.22 Two desirable characteristics of clay minerals relative to fabrication processes are 1) they become
hydroplastic (and therefore formable) when mixed with water; and 2) during firing, a clay melts over
a range of temperatures, which allows some fusion and bonding of a ware without complete melting
and a loss of mechanical integrity and shape.
13.23 Clays become hydroplastic when water is added because the water molecules fill in regions
between the layered molecular sheets; these water molecules essentially eliminate the secondary
molecular bonds between adjacent sheets, and also form a thin film around the clay particles. The
net result is that the clay particles are relatively free to move past one another, which is manifested
as the hydroplasticity phenomenon.
13.24 Upon drying, thick ceramic wares are more likely to crack upon drying than thin wares because of
a greater difference in shrinkage between surface and interior cross-sectional regions for the thick
ware. Water being eliminated during drying has a longer distance to travel from the interior to the
surface for the thicker ware.
13.25 The phenomenon of hydroplasticity results when water molecules form a thin film around the small
clay particles. During firing, these individual particles become fused together by the viscous liquid
that fills in the pore volume between the particles--the pore volume occupied by water in the
hydroplastic state. This viscous liquid forms a glass matrix on subsequent cooling.
13.26 (a) The three components of a whiteware ceramic are clay, quartz, and a flux.
(b) With regard to the role that each component plays:
Quartz acts as a filler material.
Clay facilitates the forming operation since, when mixed with water, the mass may be made
to become either hydroplastic or form a slip. Also, since clays melt over a range of temperatures,
the shape of the piece being fired will be maintained.
The flux facilitates the formation of a glass having a relatively low melting temperature.
360
13.27 (a) It is important to control the rate of drying inasmuch as if the rate of drying is too rapid, there
will be nonuniform shrinkage between surface and interior regions, such that warping and/or
cracking of the ceramic ware will result.
(b) Three factors that affect the rate of drying are temperature, humidity, and rate of air flow. The
rate of drying is enhanced by increasing both the temperature and rate of air flow, and by decreasing
the humidity of the air.
13.28 The reason that drying shrinkage is greater for products having smaller clay particles is that there
is more particle surface area, and, consequently, more water will surround a given volume of
particles. The drying shrinkage will thus be greater as this water is removed, and as the interparticle
separation decreases.
13.29 (a) Three factors that influence the degree to which vitrification occurs in clay-based ceramic
wares are: 1) the composition (especially the concentration of flux present); 2) the temperature of
firing; and 3) the time at the firing temperature.
(b) Density will increase with degree of vitrification since the total remaining pore volume decreases.
Firing distortion will increase with degree of vitrification since more liquid phase will be
present at the firing temperature.
Strength will also increase with degree of vitrification inasmuch as more of the liquid phase
forms, which fills in a greater fraction of pore volume. Upon cooling, the liquid forms a glass matrix
of relatively high strength.
Corrosion resistance normally increases also, especially at service temperatures below that
at which the glass phase begins to soften. The rate of corrosion is dependent on the amount of
surface area exposed to the corrosive medium; hence, decreasing the total surface area by filling in
some of the surface pores, diminishes the corrosion rate.
Thermal conductivity will increase with degree of vitrification. The glass phase has a higher
conductivity than the pores that it has filled.
13.30 The principal disadvantage of hot-isostatic pressing is that it is expensive. The pressure is applied
on a pre-formed green piece by a gas. Thus, the process is slow, and the equipment required to
supply the gas and withstand the elevated temperature and pressure is costly.
Design Problem
13.D1
(a)
Important characteristics that are required of a ceramic material to be used for kitchen
cookware are:
1) it must have a high resistance to thermal shock (Section 19.5) in order to
361
withstand relatively rapid changes in temperature;
2) it must have a relatively high thermal
conductivity; 3) it must be relatively strong and tough in order to endure normal kitchen use; and 4)
it must be nontoxic.
(b) Possible materials worth considering are a common soda-lime glass, a borosilicate (Pyrex)
glass, and a glass ceramic. These materials and some of their characteristics are discussed in this
chapter. Using Equation (19.9) a comparison of the resistance to thermal shock may be made. The
student will need to obtain cost information.
(c) It is left to the student to make this determination and justify the decision.
362
CHAPTER 14
POLYMER STRUCTURES
PROBLEM SOLUTIONS
14.1
Polymorphism is when two or more crystal structures are possible for a material of given
composition. Isomerism is when two or more polymer molecules or mer units have the same
composition, but different atomic arrangements.
14.2 The mer structures called for are sketched below.
(a) Polyvinyl fluoride
(b) Polychlorotrifluoroethylene
(c) Polyvinyl alcohol
363
14.3 Mer weights for several polymers are asked for in this problem.
(a) For polytetrafluoroethylene, each mer unit consists of two carbons and four fluorines (Table
14.3). If A and A represent the atomic weights of carbon and fluorine, respectively, then
C
F
m = 2(AC) + 4(AF)
= (2)(12.01 g/mol) + (4)(19.00 g/mol) = 100.02 g/mol
(b) For polymethyl methacrylate, from Table 14.3, each mer unit has five carbons, eight hydrogens,
and two oxygens. Thus,
m = 5(AC) + 8(AH) + 2(AO)
= (5)(12.01 g/mol) + (8)(1.008 g/mol) + (2)(16.00 g/mol) = 100.11 g/mol
(c) For nylon 6,6, from Table 14.3, each mer unit has twelve carbons, twenty-two hydrogens, two
nitrogens, and two oxygens. Thus,
m = 12(AC) + 22(AH) + 2(AN) + 2(AO)
= (12)(12.01 g/mol) + (22)(1.008 g/mol) + (2)(14.01 g/mol) + (2)(16.00 g/mol)
= 226.32 g/mol
(d) For polyethylene terephthalate, from Table 14.3, each mer unit has ten carbons, eight hydrogens,
and four oxygens. Thus,
m = 10(AC) + 8(AH) + 4(AO)
= (10)(12.01 g/mol) + (8)(1.008 g/mol) + (4)(16.00 g/mol) = 192.16 g/mol
14.4 We are asked to compute the number-average degree of polymerization for polypropylene, given
that the number-average molecular weight is 1,000,000 g/mol.
polypropylene is just
m = 3(AC) + 6(AH)
364
The mer molecular weight of
= (3)(12.01 g/mol) + (6)(1.008 g/mol) = 42.08 g/mol
If we let n represent the number-average degree of polymerization, then from Equation (14.4a)
n
nn =
Mn
m
=
106 g/mol
= 23, 700
42.08 g/mol
14.5 (a) The mer molecular weight of polystyrene is called for in this portion of the problem. For
polystyrene, from Table 14.3, each mer unit has eight carbons and eight hydrogens. Thus,
m = 8(AC) + 8(AH)
= (8)(12.01 g/mol) + (8)(1.008 g/mol) = 104.14 g/mol
(b) We are now asked to compute the weight-average molecular weight. Since the weight-average
degree of polymerization, n , is 25,000, using Equation (14.4b)
w
Mw = n w m = (25,000)(104.14 g/mol) = 2.60 x 10 6 g/mol
14.6 (a) From the tabulated data, we are asked to compute Mn , the number-average molecular weight.
This is carried out below.
Molecular wt
Range
Mean M
i
x
i
xM
i i
8,000-16,000
12,000
0.05
600
16,000-24,000
20,000
0.16
3200
24,000-32,000
28,000
0.24
6720
32,000-40,000
36,000
0.28
10,080
40,000-48,000
44,000
0.20
8800
48,000-56,000
52,000
0.07
3640
____________________________
Mn =
365
∑ xiMi = 33, 040 g/mol
(b) From the tabulated data, we are asked to compute M w , the weight- average molecular weight.
Molecular wt.
Range
Mean M
i
w
wM
i i
8,000-16,000
12,000
0.02
240
16,000-24,000
20,000
0.10
2000
24,000-32,000
28,000
0.20
5600
32,000-40,000
36,000
0.30
10,800
40,000-48,000
44,000
0.27
11,880
48,000-56,000
52,000
0.11
5720
___________________________
i
Mw =
(c) Now we are asked to compute n
n
∑ w iMi = 36, 240 g/mol
(the number-average degree of polymerization), using the
Equation (14.4a). For polypropylene,
m = 3(AC) + 6(AH)
= (3)(12.01 g/mol) + (6)(1.008 g/mol) = 42.08 g/mol
And
nn =
Mn
m
=
33,040 g/mol
= 785
42.08 g/mol
(d) And, finally, we are asked to compute n , the weight-average degree of polymerization, which,
w
using Equation (14.4b), is just
nw =
Mw
m
=
36,240 g/mol
= 861
42.08 g/mol
14.7 (a) From the tabulated data, we are asked to compute Mn , the number-average molecular weight.
This is carried out below.
366
Molecular wt.
Range
Mean M
i
x
i
xM
i i
8,000-20,000
14,000
0.05
700
20,000-32,000
26,000
0.15
3900
32,000-44,000
38,000
0.21
7980
44,000-56,000
50,000
0.28
14,000
56,000-68,000
62,000
0.18
11,160
68,000-80,000
74,000
0.10
7400
80,000-92,000
86,000
0.03
2580
_________________________
Mn =
∑ xiMi = 47,720 g/mol
(b) From the tabulated data, we are asked to compute M w , the weight- average molecular weight.
This determination is performed as follows:
Molecular wt.
Range
Mean M
i
w
wM
i i
8,000-20,000
14,000
0.02
280
20,000-32,000
26,000
0.08
2080
32,000-44,000
38,000
0.17
6460
44,000-56,000
50,000
0.29
14,500
56,000-68,000
62,000
0.23
14,260
68,000-80,000
74,000
0.16
11,840
80,000-92,000
86,000
0.05
4300
_________________________
i
Mw =
∑ wiMi = 53,720 g/mol
(c) We are now asked if the number-average degree of polymerization is 477, which of the polymers
in Table 14.3 is this material? It is necessary to compute m in Equation (14.4a) as
m =
Mn
n
n
=
47, 720 g/mol
= 100.04 g/mol
477
The mer molecular weights of the polymers listed in Table 14.3 are as follows:
Polyethylene--28.05 g/mol
367
Polyvinyl chloride--62.49 g/mol
Polytetrafluoroethylene--100.02 g/mol
Polypropylene--42.08 g/mol
Polystyrene--104.14 g/mol
Polymethyl methacrylate--100.11 g/mol
Phenol-formaldehyde--133.16 g/mol
Nylon 6,6--226.32 g/mol
PET--192.16 g/mol
Polycarbonate--254.27 g/mol
Therefore, polytetrafluoroethylene is the material since its mer molecular weight is closest to that
calculated above.
(d) The weight-average degree of polymerization may be calculated using Equation (14.4b), since
M w and m were computed in portions (b) and (c) of this problem. Thus
nw =
Mw
m
=
53,720 g/mol
= 537
100.04 g/mol
14.8 This problem asks if it is possible to have a polyvinyl chloride homopolymer with the given molecular
weight data and a number-average degree of polymerization of 1120. The appropriate data are
given below along with a computation of the number-average molecular weight.
Molecular wt.
Range
Mean M
i
x
i
xM
i i
8,000-20,000
14,000
0.05
700
20,000-32,000
26,000
0.15
3900
32,000-44,000
38,000
0.21
7980
44,000-56,000
50,000
0.28
14,000
56,000-68,000
62,000
0.18
11,160
68,000-80,000
74,000
0.10
7440
80,000-92,000
86,000
0.03
2580
_________________________
Mw =
∑ xiMi = 47, 720 g/mol
For PVC, from Table 14.3, each mer unit has two carbons, three hydrogens, and one chlorine.
Thus,
368
m = 2(AC) + 3(AH) + (ACl)
= (2)(12.01 g/mol) + (3)(1.008 g/mol) + (35.45 g/mol) = 62.49 g/mol
Now, we will compute nn from Equation (14.4a) as
M
nn =
n
m
=
47, 720 g/mol
= 764
62.49 g/mol
Thus, such a homopolymer is not possible since the calculated nn is 764 not 1120.
14.9 (a) For chlorinated polyethylene, we are asked to determine the weight percent of chlorine added
for 5% Cl substitution of all original hydrogen atoms. Consider 50 carbon atoms; there are 100
possible side-bonding sites. Ninety-five are occupied by hydrogen and five are occupied by Cl.
Thus, the mass of these 50 carbon atoms, m , is just
C
mC = 50(AC) = (50)(12.01 g/mol) = 600.5 g
Likewise, for hydrogen and chlorine,
mH = 95(AH) = (95)(1.008 g/mol) = 95.76 g
mCl = 5(ACl) = (5)(35.45 g/mol) = 177.25 g
Thus, the concentration of chlorine, C , is just
Cl
CCl =
177.25 g
x 100 = 20.3 wt%
600.5 g + 95.76 g + 177.25 g
(b) Chlorinated polyethylene differs from polyvinyl chloride, in that, for PVC, 1) 25% of the sidebonding sites are substituted with Cl, and 2) the substitution is probably much less random.
14.10
Relative to polymer chains, the difference between configuration and conformation is that
conformation is used in reference to the outline or shape of the chain molecule, whereas,
369
configuration refers to the arrangement of atom positions along the chain that are not alterable
except by the breaking and reforming of primary bonds.
14.11 This problem first of all asks for us to calculate, using Equation (14.11), the average total chain
length, L, for a linear polyethylene polymer having a number-average molecular weight of 300,000
g/mol.
It is necessary to calculate the number-average degree of polymerization, nn, using
Equation (14.4a). For polyethylene, from Table 14.3, each mer unit has two carbons and four
hydrogens. Thus,
m = 2(AC) + 4(AH)
= (2)(12.01 g/mol) + (4)(1.008 g/mol) = 28.05 g/mol
and
nn =
Mn
m
=
300,000 g/mol
= 10,695
28.05 g/mol
which is the number of mer units along an average chain. Since there are two carbon atoms per mer
unit, there are two C--C chain bonds per mer, which means that the total number of chain bonds in
the molecule, N, is just (2)(10,695) = 21,390 bonds. Furthermore, assume that for single carboncarbon bonds, d = 0.154 nm and θ = 109&deg; (Section 14.4); therefore, from Equation (14.11)
⎛ θ⎞
L = Nd sin ⎜ ⎟
⎝ 2⎠
⎡
= (21,390)(0.154 nm) ⎢sin
⎣
⎛ 109&deg; ⎞ ⎤
⎜
⎟ = 2682 nm
⎝ 2 ⎠ ⎥⎦
It is now possible to calculate the average chain end-to-end distance, r, using Equation
(14.12) as
r = d N = (0.154 nm) 21,390 = 22.5 nm
14.12 (a) This portion of the problem asks for us to calculate the number-average molecular weight for a
linear polytetrafluoroethylene for which L in Equation (14.11) is 2000 nm. It is first necessary to
compute the value of N using this equation, where, for the C--C chain bond, d = 0.154 nm, and θ =
109&deg;. Thus
370
N =
=
L
⎛ θ⎞
d sin ⎜ ⎟
⎝ 2⎠
2000 nm
= 15,900
⎛ 109&deg; ⎞
(0.154 nm) sin ⎜
⎟
⎝ 2 ⎠
Since there are two C--C bonds per PTFE mer unit, there is an average of N/2 or 15,900/2 = 7950
mer units per chain, which is also the number-average degree of polymerization, nn. In order to
compute the value of Mn using Equation (14.4a), we must first determine m for PTFE. Each PTFE
mer unit consists of two carbon and four fluorine atoms, thus
m = 2(AC) + 4(AF)
= (2)(12.01 g/mol) + (4)(19.00 g/mol) = 100.02 g/mol
Therefore
Mn = nnm = (7950)(100.02 g/mol) = 795,000 g/mol
(b) Next, we are to determine the number-average molecular weight for r = 15 nm. Solving for N
N =
r2
(15 nm)2
=
= 9490
d2
(0.154 nm)2
which is the total number of bonds per average molecule. Since there are two C--C bonds per mer
unit, then nn = N/2 = 9490/2 = 4745. Now, from Equation (14.4a)
Mn = nnm = (4745)(100.02 g/mol) = 474,600 g/mol
14.13 We are asked to sketch portions of a linear polypropylene molecule for different configurations.
(a) Syndiotactic polypropylene
(b) Atactic polypropylene
371
(c) Isotactic polypropylene
14.14 (a) The structure of cis polybutadiene is
The structure of trans butadiene is
(b) The structure of cis chloroprene is
The structure of trans chloroprene is
372
14.15 This question asks for comparisons of thermoplastic and thermosetting polymers.
(a) Thermoplastic polymers soften when heated and harden when cooled, whereas thermosetting
polymers, harden upon heating, while further heating will not lead to softening.
(b) Thermoplastic polymers have linear and branched structures, while for thermosetting polymers,
the structures will normally be network or crosslinked.
14.16 Thermosetting polyesters will be crosslinked, while thermoplastic ones will have linear structures
14.17 (a) It is not possible to grind up and reuse phenol-formaldehyde because it is a network thermoset
polymer and, therefore, is not amenable to remolding.
(b) Yes, it is possible to grind up and reuse polypropylene since it is a thermoplastic polymer, will
soften when reheated, and, thus, may be remolded.
14.18 This problem asks for sketches of the mer structures for several alternating copolymers.
(a) For poly(ethylene-propylene)
(c) For poly(isobutylene-isoprene)
373
14.19 For a poly(styrene-butadiene) alternating copolymer with a number-average molecular weight of
1,350,000 g/mol, we are asked to determine the average number of styrene and butadiene mer units
per molecule.
Since it is an alternating copolymer, the number of both types of mer units will be the same.
Therefore, consider them as a single mer unit, and determine the number-average degree of
polymerization. For the styrene mer, there are eight carbon atoms and eight hydrogen atoms, while
the butadiene mer consists of four carbon atoms and six hydrogen atoms. Therefore, the styrenebutadiene combined mer weight is just
m = 12(AC) + 14(AH)
= (12)(12.01 g/mol) + (14)(1.008 g/mol) = 158.23 g/mol
From Equation (14.4a), the number-average degree of polymerization is just
nn =
Mn
m
=
135,000 g/mol
= 8530
158.23 g/mol
Thus, there is an average of 8530 of both mer types per molecule.
14.20 This problem asks for us to calculate the number-average molecular weight of a random nitrile
rubber copolymer.
For the acrylonitrile mer there are three carbon, one nitrogen, and three
hydrogen atoms. Thus, its mer molecular weight is
mAc = 3(AC) + (AN) + 3(AH)
= (3)(12.01 g/mol) + 14.01 g/mol + (3)(1.008 g/mol) = 53.06 g/mol
The butadiene mer is composed of four carbon and six hydrogen atoms. Thus, its mer molecular
weight is
mBu = 4(AC) + 6(AH)
= (4)(12.01 g/mol) + (6)(1.008 g/mol) = 54.09 g/mol
From Equation (14.5), the average mer molecular weight is just
374
m = fAcm Ac + fBumBu
= (0.70)(53.06 g/mol) + (0.30)(54.09 g/mol) = 53.37 g/mol
Since n = 2000 (as stated in the problem), Mn may be computed using Equation (14.4a) as
n
Mn = m nn = (53.37 g/mol)(2000) = 106,740 g/mol
14.21 For an alternating copolymer that has a number-average molecular weight of 100,000 g/mol and a
number-average degree of polymerization of 2210, we are to determine one of the mer types if the
other is ethylene. It is first necessary to calculate m using Equation (14.4a) as
m =
Mn
n
n
=
100,000 g/mol
= 42.25 g/mol
2210
Since this is an alternating copolymer we know that chain fraction of each mer type is 0.5; that is fe
= fx = 0.5, fe and fx being, respectively, the chain fractions of the ethylene and unknown mers.
Also, the mer molecular weight for ethylene is
ms = 2(AC) + 4(AH)
= 2(12.01 g/mol) + 4(1.008 g/mol) = 28.05 g/mol
Now, using Equation (14.5), it is possible to calculate the mer weight of the unknown mer type, mx.
Thus
mx =
=
m − feme
fx
45.25 g/mol - (0.5)(28.05 g/mol)
= 62.45 g/mol
0.5
Finally, it is necessary to calculate the mer molecular weights for each of the possible other mer
types. These are calculated below:
375
mstyrene = 8(AC) + 8(AH) = 8(12.01 g/mol) + 8(1.008 g/mol) = 104.16 g/mol
mpropylene = 3(AC) + 6(AH) = 3(12.01 g/mol) + 6(1.008 g/mol) = 42.08 g/mol
mTFE = 2(AC) + 4(AF) = 2(12.01 g/mol) + 4(19.00 g/mol) = 100.02 g/mol
mVC = 2(AC) + 3(AH) + (ACl) = 2(12.01 g/mol) + 3(1.008 g/mol) + 35.45 g/mol = 62.49 g/mol
Therefore, vinyl chloride is the other mer type since its m value is almost the same as the calculated
mx.
14.22 (a) This portion of the problem asks us to determine the ratio of butadiene to acrylonitrile mers in a
copolymer having a weight-average molecular weight of 250,000 g/mol and a weight-average degree
of polymerization of 4640. It first becomes necessary to calculate the average mer molecular weight
of the copolymer, m , using Equation (14.4b) as
m =
Mw
n
=
w
250,000 g/mol
= 53.88 g/mol
4640
If we designate fb as the chain fraction of butadiene mers, since the copolymer consists of only two
mer types, the chain fraction of acrylontrile mers fa is just 1 - fb. Now, Equation (14.5) for this
copolymer may be written in the form
m = fbmb + fama = fbmb + (1 - fb )ma
in which mb and ma are the mer molecular weights for butadiene and acrylontrile, respectively.
These values are calculated as follows:
mb = 4(AC) + 6(AH) = 4(12.01 g/mol) + 6(1.008 g/mol) = 54.09 g/mol
ma = 3(AC) + 3(AH) + (AN) = 3(12.01 g/mol) + 3(1.008 g/mol) + (14.01 g/mol)
= 53.06 g/mol.
Solving for fb in the above expression yields
fb =
m − ma
mb − ma
=
53.88 g/mol − 53.06 g/mol
= 0.80
54.09 g/mol − 53.06 g/mol
Furthermore, fa = 1 - fb = 1 - 0.80 = 0.20; or the ratio is just
376
fb
fa
=
0.80
= 4.0
0.20
(b) Of the possible copolymers, the only one for which there is a restriction on the ratio of mer types
is alternating; the ratio must be 1:1. Therefore, on the basis of the result in part (a), the possibilities
for this copolymer are random, graft, and block.
14.23 For a copolymer consisting of 60 wt% ethylene and 40 wt% propylene, we are asked to determine
the fraction of both mer types.
In 100 g of this material, there are 60 g of ethylene and 40 g of propylene. The ethylene
(C H ) molecular weight is
2 4
m(ethylene) = 2(AC) + 4(AH)
= (2)(12.01 g/mol) + (4)(1.008 g/mol) = 28.05 g/mol
The propylene (C H ) molecular weight is
3 6
m(propylene) = 3(AC) + 6(AH)
= (3)(12.01 g/mol) + (6)(1.008 g/mol) = 42.08 g/mol
Therefore, in 100 g of this material, there are
60 g
= 2.14 mol of ethylene
28.05 g / mol
and
40 g
= 0.95 mol of propylene
42.08 g / mol
Thus, the fraction of the ethylene mer, f(ethylene), is just
f(ethylene) =
2.14 mol
= 0.69
2.14 mol + 0.95 mol
377
Likewise,
f(propylene) =
0.95 mol
= 0.31
2.14 mol + 0.95 mol
14.24 For a random poly(isobutylene-isoprene) copolymer in which M w = 200,000 g/mol and n = 3000,
w
we are asked to compute the fractions of isobutylene and isoprene mers.
From Table 14.5, the isobutylene mer has four carbon and eight hydrogen atoms. Thus,
mib = (4)(12.01 g/mol) + (8)(1.008 g/mol) = 56.10 g/mol
Also, from Table 14.5, the isoprene mer has five carbon and eight hydrogen atoms, and
mip = (5)(12.01 g/mol) + (8)(1.008 g/mol) = 68.11 g/mol
From Equation (14.5)
m = fibmib + fipmip
Now, let x = f , such that
ib
m = 56.10x + (68.11)(1 - x)
since f
ib
+f
ip
= 1. Also, from Equation (14.4b)
nw =
M
w
m
Or
3000 =
Solving for x leads to x = f
ib
200, 000 g / mol
[56.10x + 68.11 (1 − x)] g / mol
= f(isobutylene) = 0.12. Also,
f(isoprene) = 1 - x = 1 - 0.12 = 0.88
378
14.25 (a) For crystalline metals, the individual atoms are positioned in a periodic or ordered arrangement
over relatively large atomic distances. The long-range order in polymer crystals results from the
(b) For noncrystalline ceramic glasses, the atomic randomness exists outside the SiO 44 − unit. The
disorder in polymers results from chain misalignment.
14.26 The tendency of a polymer to crystallize decreases with increasing molecular weight because as
the chains become longer it is more difficult for all regions along adjacent chains to align so as to
produce the ordered atomic array.
14.27 For each of four pairs of polymers, we are asked to 1) state whether it is possible to decide which
is more likely to crystallize; 2) if so, which is more likely and why; and 3) it is not possible to decide
then why.
(a) No, it is not possible to decide for these two polymers. On the basis of tacticity, the isotactic PP
is more likely to crystallize than the atactic PVC. On the other hand, with regard to side-group
bulkiness, the PVC is more likely to crystallize.
(b) Yes, it is possible to decide for these two copolymers. The linear and syndiotactic polypropylene
is more likely to crystallize than crosslinked cis-isoprene since linear polymers are more likely to
(c) Yes, it is possible to decide for these two polymers. The linear and isotactic polystyrene is more
likely to crystallize than network phenol-formaldehyde; network polymers rarely crystallize, whereas
isotactic ones crystallize relatively easily.
(d) Yes, it is possible to decide for these two copolymers. The block poly(acrylonitrile-isoprene)
copolymer is more likely to crystallize than the graft poly(chloroprene-isobutylene) copolymer. Block
copolymers crystallize more easily than graft ones.
14.28 Given that polyethylene has an orthorhombic unit cell with two equivalent mer units, we are asked
to compute the density of totally crystalline polyethylene.
In order to solve this problem it is
necessary to employ Equation (3.5), in which n represents the number of mer units within the unit
cell (n = 2), and A is the mer molecular weight, which for polyethylene is just
A = 2(AC) + 4(AH)
= (2)(12.01 g/mol) + (4)(1.008 g/mol) = 28.05 g/mol
379
Also, VC is the unit cell volume, which is just the product of the three unit cell edge lengths as shown
in Figure 14.10. Thus,
ρ =
=
nA
VC NA
(2 mers/uc)(28.05 g/mol)
⎡ 7.41 x 10-8 cm 4.94 x 10-8 cm 2.55 x 10-8 cm /uc ⎤ 6.023 x 10 23 mers/mol
⎣
⎦
(
)(
)(
) (
)
= 0.998 g/cm3
14.29 For this problem we are given the density of nylon 6,6 (1.213 g/cm3), an expression for the volume
of its unit cell, and the lattice parameters, and are asked to determine the number of mer units per
unit cell. This computation necessitates the use of Equation (3.5), in which we solve for n. Before
this can be carried out we must first calculate VC, the unit cell volume, and A the mer molecular
weight. For VC
VC = abc 1 − cos 2 α − cos 2 β − cos 2 γ + 2 cos α cosβ cos γ
= (0.497)(0.547)(1.729) 1 − 0.441 − 0.054 − 0.213 + 2(0.664)(0.232)(0.462)
= 0.3098 nm3 = 3.098 x 10-22 cm3
The mer unit for nylon 6,6 is shown in Table 14.3, from which the value of A may be determined as
follows:
A = 12(AC) + 22(AH) + 2(AO) + 2(AN)
= 12(12.01 g/mol) + 22(1.008 g/mol) + 2(16.00 g/mol) + 2(14.01 g/mol)
= 226.32 g/mol
Finally, solving for n from Equation (3.5) leads to
n =
ρVC NA
A
380
=
(1.213 g/cm3 )(3.098 x 10-22 cm3 /unit cell)(6.023 x 1023 mers/mol)
226.32 g/mol
= 1 mer/unit cell
14.30 (a) We are asked to compute the densities of totally crystalline and totally amorphous
polyethylene [ρc and ρa from Equation (14.10)]. From Equation (14.10) let C = (% crystallinity)/100,
such that
(
)
ρ s (ρ c − ρ a )
ρ c ρs − ρ a
C =
Rearrangement of this expression leads to
(
)
ρ c Cρs − ρ s + ρ c ρa − Cρ sρ a = 0
in which ρc and ρa are the variables for which solutions are to be found. Since two values of ρs and
C are specified in the problem, two equations may be constructed as follows:
(
)
(
)
ρ c C1 ρ s1 − ρs1 + ρ c ρa − C1ρ s1 ρ a = 0
ρ c C2 ρ s2 − ρs2 + ρc ρa − C2 ρs2 ρa = 0
In which ρs1 = 0.965 g/cm3, ρs2 = 0.925 g/cm3, C = 0.768, and C = 0.464. Solving the above
1
2
ρa =
=
(
ρ s1 ρs2 C1 − C2
C ρ − C ρ
1 s1
)
2 s2
(0.965 g/cm3 )(0.925 g/cm3 )(0.768 − 0.464) = 0.870 g/cm3
(0.768) (0.965 g/cm3 ) − (0.464) (0.925 g/cm3 )
And
381
ρc =
=
(
)
ρ (C − 1) - ρ (C − 1)
s2 2
s1 1
ρs1 ρ s2 C2 − C1
(0.965 g/cm3 )(0.925 g/cm3 )(0.464 − 0.768)
(0.925 g/cm3 )(0.464 − 1.0) − (0.965 g/cm3 )(0.768 − 1.0)
= 0.998 g/cm3
(b) Now we are to determine the % crystallinity for ρs = 0.950 g/cm3. Again, using Equation
(14.10)
% crystallinity =
=
(
ρ s (ρc
) x 100
− ρa )
ρ c ρs − ρ a
(0.998 g/cm3 )(0.950 g/cm3 −
(0.950 g/cm3 )(0.998 g/cm3 −
) x 100
0.870 g/cm3 )
0.870 g/cm
3
= 65.7%
14.31
(a)
We are asked to compute the densities of totally crystalline and totally amorphous
% crystallinity
,
polypropylene [ρc and ρa from Equation (14.10)]. From Equation (14.10) let C =
100
such that
C =
(
ρ s (ρ c
)
− ρa )
ρ c ρs − ρ a
Rearrangement of this expression leads to
(
)
ρ c Cρs − ρ s + ρ c ρa − Cρ sρ a = 0
in which ρc and ρa are the variables for which solutions are to be found. Since two values of ρs and
C are specified in the problem, two equations may be constructed as follows:
(
)
ρ c C1 ρ s1 − ρs1 + ρc ρ a − C1 ρs1ρ a = 0
382
(
)
ρ c C2ρ s2 − ρ s2 + ρ cρ a − C2ρ s2ρa = 0
In which ρs1 = 0.904 g/cm3, ρs2 = 0.895 g/cm3, C = 0.628, and C = 0.544. Solving the above
1
2
(
ρs1 ρs2 C1 − C 2
C ρ − C ρ
ρa =
=
(0.904
1 s1
)
2 s2
)(0.895 g / cm3 )(0.628 − 0.544) = 0.841 g/cm3
g / cm 3 )− (0.544) (0.895 g / cm3 )
3
g / cm
(
(0.628) 0.904
And
=
(0.904
(0.895
(
1) −
)
ρ s1ρ s2 C2 − C1
ρc =
(
ρs2 C 2 −
)
)(0.544 − 0.628) = 0.946 g/cm3
g / cm 3 )(0.544 − 1.0) − (0.904 g / cm3 )(0.628 − 1.0)
3
g/ cm
)(0.895
(
ρ s1 C1 − 1
g / cm
3
(b) Now we are asked to determine the density of a specimen having 74.6% crystallinity. Solving for
ρs from Equation (14.10) and substitution for ρa and ρc which were computed in part (a) yields
ρs =
(
(
− ρc ρa
)(0.841 g / cm3 )
g / cm 3 − 0.841 g / cm3 )− 0.946
− 0.946 g / cm
=
(
(0.746) 0.946
)
C ρ c − ρa − ρ c
3
= 0.917 g/cm3
383
g / cm 3
CHAPTER 15
CHARACTERISTICS, APPLICATIONS, AND PROCESSING OF POLYMERS
PROBLEM SOLUTIONS
15.1 From Figure 15.3, the elastic modulus is the slope in the elastic linear region of the 20&deg;C
curve, which is
E =
Δ(stress) 30 MPa − 0 MPa
=
= 3.3 GPa (483,000 psi)
Δ(strain)
9 x 10−3 − 0
The value range cited in Table 15.1 is 2.24 to 3.24 GPa (325,000 to 470,000 psi). Thus, the
plotted value is a little on the high side.
The tensile strength corresponds to the stress at which the curve ends, which is 52
MPa (7500 psi). This value lies within the range cited in the table--48.3 to 72.4 MPa (7,000
to 10,500 psi).
15.2 The reason that it is not necessary to specify specimen gauge length when citing percent
elongation for semicrystalline polymers is because, for semicrystalline polymers that
experience necking, the neck normally propagates along the entire gauge length prior to
fracture; thus, there is no localized necking as with metals and the magnitude of the percent
elongation is independent of gauge length.
15.3 The explanation of viscoelasticity is given in Section 15.4.
15.4 This problem asks for a determination of the relaxation modulus of a viscoelastic material,
which behavior is according to Equation (15.10)--i.e.,
⎛ t⎞
σ(t) = σ(0) exp ⎜ − ⎟
⎝ τ⎠
We want to determine σ(10), but it is first necessary to compute τ from the data provided in
the problem. Thus,
384
τ =
−t
⎡ σ(t) ⎤
ln ⎢
⎥
⎣ σ(0) ⎦
=
− 30 s
= 15.4 s
⎡ 0.5 MPa ⎤
ln ⎢
⎣ 3.5 MPa ⎥⎦
Therefore,
⎛ 10 s ⎞
⎟ = 1.83 MPa
σ(10) = (3.5 MPa) exp ⎜ −
⎝ 15.4 s ⎠
Now, using Equation (15.1)
Er (10) =
σ(10) 1.83 MPa
=
= 3.66 MPa (522 psi)
εo
0.5
15.5 Below is plotted the logarithm of Er(10) versus temperature.
The glass-transition temperature is that temperature corresponding to the abrupt decrease
in log Er(10), which for this PMMA material is about 115&deg;C.
15.6 We are asked to make schematic strain-time plots for various polystyrene materials and at
several temperatures.
(a) Crystalline polystyrene at 70&deg;C behaves in a glassy manner (Figure 15.8, curve A);
therefore, the strain-time behavior would be as Figure 15.5(b).
(b) Amorphous polystyrene at 180&deg;C behaves as a viscous liquid (Figure 15.8, curve C);
therefore, the strain-time behavior will be as Figure 15.5(d).
385
(c) Crosslinked polystyrene at 180&deg;C behaves as a rubbery material (Figure 15.8, curve B);
therefore, the strain-time behavior will be as Figure 15.5(c).
(d)
Amorphous polystyrene at 100&deg;C behaves as a leathery material (Figure 15.7);
therefore, the strain-time behavior will be as Figure 15.5(c).
15.7 (a) Stress relaxation tests are conducted by rapidly straining the material elastically in
tension, holding the strain level constant, and then measuring the stress as a function of
time. For viscoelastic creep tests, a stress (usually tensile) is applied instantaneously and
maintained constant while strain is measured as a function of time.
(b) The experimental parameters of interest from the stress relaxation and viscoelastic
creep tests are the relaxation modulus and creep modulus, respectively. The relaxation
modulus is the ratio of stress measured after 10 s and strain [Equation (15.1)];
creep
modulus is the ratio of stress and the strain taken at a specific time [Equation (15.2)].
15.8
(a)
This portion of the problem calls for a plot of log Er(10) versus temperature
demonstrating how the behavior changes with increased molecular weight. Such a plot is
given below.
Increasing molecular weight increases both glass-transition and melting
temperatures.
(b) We are now called upon to make a plot of log Er(10) versus temperature demonstrating
how the behavior changes with increased crosslinking.
Such a plot is given below.
Increasing the degree of crosslinking will increase the modulus in both glassy and rubbery
regions.
386
15.9 For thermoplastic polymers, five factors that favor brittle fracture are as follows: a reduction
in temperature, an increase in strain rate, the presence of a sharp notch, increased
specimen thickness, and modifications of the polymer structure.
15.10 (a) The fatigue limits for PMMA and the steel alloy are 19 MPa (2800 psi) and 290 MPa
(42,200 psi), respectively.
6
(b) At 10 cycles, the fatigue strengths for nylon 6 and 2014-T6 aluminum are 22 MPa
(3200 psi) and 200 MPa (30,000 psi ), respectively.
15.11 (a) and (b) The mechanisms by which semicrystalline polymers elastically and plastically
deform are described in Section 15.7.
(c) The explanation of the mechanism by which elastomers elastically deform is provided in
Section 15.9.
15.12 (a) The tensile modulus is not directly influenced by a polymer's molecular weight.
(b)
Tensile modulus increases with increasing degree of crystallinity for semicrystalline
polymers.
This is due to enhanced secondary interchain bonding which results from a
greater degree of chain segment alignment as percent crystallinity increases.
This
enhanced interchain bonding inhibits relative interchain motion.
(c) Deformation by drawing also increases the tensile modulus. The reason for this is that
drawing produces a highly oriented molecular structure, and a relatively high degree of
interchain secondary bonding.
(d)
When an undeformed semicrystalline polymer is annealed below its melting
temperature, its tensile modulus increases.
387
(e) A drawn semicrystalline polymer that is annealed experiences a decrease in tensile
modulus as a result of a reduction in chain-induced crystallinity, and a reduction in interchain
bonding forces.
15.13 (a) The tensile or yield strength of a semicrystalline polymer increases with increasing
molecular weight.
This effect is explained by increased chain entanglements at higher
molecular weights.
(b)
Increasing the degree of crystallinity of a semicrystalline polymer leads to an
enhancement of the tensile strength. Again, this is due to enhanced interchain bonding and
forces; in response to applied stresses, interchain motions are thus inhibited.
(c) Deformation by drawing increases the tensile strength of a semicrystalline polymer. This
effect is due to the highly oriented chain structure that is produced by drawing, which gives
rise to higher interchain secondary bonding forces.
(d) Annealing an undeformed semicrystalline polymer produces an increase in its tensile
strength.
15.14 Normal butane has a higher melting temperature as a result of its molecular structure
(Section 14.2). There is more of an opportunity for van der Waals bonds to form between
two molecules in close proximity to one another than for isobutane because of the linear
nature of each normal butane molecule.
15.15 This problem gives us the tensile strengths and associated number-average molecular
weights for two polymethyl methacrylate materials and then asks that we estimate the tensile
strength for Mn = 30,000 g/mol. Equation (15.3) provides the dependence of the tensile
strength on Mn .
Thus, using the data provided in the problem, we may set up two
simultaneous equations from which it is possible to solve for the two constants TS∞ and A.
These equations are as follows:
A
107 MPa = TS∞ −
40, 000 g / mol
A
170 MPa = TS∞ −
60, 000 g / mol
Thus, the values of the two constants are: TS∞ = 296 MPa and A = 7.56 x 106 MPag/mol. Substituting these values into the equation for which Mn = 30,000 g/mol leads to
388
A
TS = TS∞ −
30,000 g / mol
6
= 296 MPa −
7.56 x 10 MPa - g / mol
30,000 g / mol
= 44 MPa
15.16 This problem gives us the tensile strengths and associated number-average molecular
weights for two polyethylene materials and then asks that we estimate the Mn that is
required for a tensile strength of 195 MPa. Equation (15.3) provides the dependence of the
tensile strength on Mn . Thus, using the data provided in the problem, we may set up two
simultaneous equations from which it is possible to solve for the two constants TS∞ and A.
These equations are as follows:
A
85 MPa = TS∞ −
12,700 g / mol
A
150 MPa = TS∞ −
28, 500 g/ mol
Thus, the values of the two constants are: TS∞ = 202 MPa and A = 1.489 x 106 MPag/mol. Solving for Mn in Equation (15.3) and substituting TS = 195 MPa as well as the
above values for TS∞ and A leads to
Mn =
=
A
TS∞ − TS
1.489 x 10 6 MPa - g / mol
= 213,000 g/mol
202 MPa − 195 MPa
15.17 For each of four pairs of polymers, we are to do the following: 1) determine whether or not
it is possible to decide which has the higher tensile modulus; 2) if it is possible, then note
which has the higher tensile modulus and then state the reasons for this choice; and 3) if it
is not possible to decide, then state why.
(a) No, it is not possible. Both syndiotactic and isotactic polystyrene have a tendency to
crystallize, and, therefore, we assume that they have approximately the same crystallinity.
389
Furthermore, since tensile modulus is virtually independent of molecular weight, we would
expect both materials to have approximately the same modulus.
(b) Yes, it is possible. The linear and isotactic polyvinyl chloride will display a greater
tensile modulus. Linear polymers are more likely to crystallize than branched ones. In
addition, polymers having isotactic structures normally have higher degrees of crystallinity
than those having atactic structures. Increasing a polymer's crystallinity leads to an increase
in its tensile modulus. In addition, tensile modulus is independent of molecular weight--the
atactic/branched material has the higher molecular weight.
(c) Yes, it is possible. The block styrene-butadiene copolymer with 10% of possible sites
crosslinked will have the higher modulus. Block copolymers normally have higher degrees
of crystallinity than random copolymers of the same material. A higher degree of crystallinity
favors a larger modulus. In addition, the block copolymer also has a higher degree of
(d)
No, it is not possible.
Branched polyethylene will tend to have a low degree of
crystallinity since branched polymers don't normally crystallize. The atactic polypropylene
probably also has a relatively low degree of crystallinity; atactic structures also don't tend to
crystallize, and polypropylene has a more complex mer structure than does polyethylene.
Tensile modulus increases with degree of crystallinity, and it is not possible to determine
which polymer is more crystalline.
Furthermore, tensile modulus is independent of
molecular weight.
15.18 For each of four pairs of polymers, we are to do the following: 1) determine whether or not
it is possible to decide which has the higher tensile strength; 2) if it is possible, then note
which has the higher tensile strength and then state the reasons for this choice; and 3) if it
is not possible to decide, then state why.
(a) Yes, it is possible. The syndiotactic polystyrene has the higher tensile strength. Both
syndiotactic and isotactic polymers tend to crystallize, and, therefore, we assume that both
materials have approximately the same crystallinity. However, tensile modulus increases
with increasing molecular weight, and the syndiotactic PS has the higher molecular weight
(600,000 g/mol versus 500,000 g/mol for the isotactic material).
(b) Yes, it is possible. The linear and isotactic material will have the higher tensile strength.
Both linearity and isotacticity favor a higher degree of crystallinity than do branching and
atacticity;
and tensile strength increases with increasing degree of crystallinity.
Furthermore, the molecular weight of the linear/isotactic material is higher (100,000 g/mol
versus 75,000 g/mol), and tensile strength increases with increasing molecular weight.
390
(c) No, it is not possible. Alternating copolymers tend to be more crystalline than graft
copolymers, and tensile strength increases with degree of crystallinity. However, the graft
material has a higher degree of crosslinking, and tensile strength increases with the
(d)
Yes, it is possible.
Relative
chain
motion
The network polyester will display a greater tensile strength.
is
much
more
restricted
than
for
the
lightly
branched
polytetrafluoroethylene since there are many more of the strong covalent bonds for the
network structure.
15.19 The strength of a polychlorotrifluoroethylene having the mer structure
will be greater than for a polytetrafluoroethylene having the same molecular weight and
degree of crystallinity. The replacement of one fluorine atom within the PTFE mer with a
chlorine atom leads to a higher interchain attraction, and, thus, a stronger polymer.
Furthermore, polyvinyl chloride is stronger than polyethylene (Table 15.1) for the same
reason.
15.20 (a) Shown below are the stress-strain curves for the two polyisoprene materials, both of
which have a molecular weight of 100,000 g/mol. These two materials are elastomers and
will have curves similar to curve C in Figure 15.1. However, the curve for the material
having the greater number of crosslinks (20%) will have a higher elastic modulus at all
strains.
391
(b) Shown below are the stress-strain curves for the two polypropylene materials. These
materials will most probably display the stress-strain behavior of a normal plastic, curve B in
Figure 15.1. However, the syndiotactic polypropylene has a higher molecular weight and will
also undoubtedly have a higher degree of crystallinity;
therefore, it will have a higher
strength.
(c) Shown below are the stress-strain curves for the two polyethylene materials.
The
branched polyethylene will display the behavior of a normal plastic, curve B in Figure 15.1.
On the other hand, the heavily crosslinked polyethylene will be stiffer, stronger, and more
brittle (curve A of Figure 15.1).
392
15.21 Two molecular characteristics essential for elastomers are: 1) they must be amorphous,
having chains that are extensively coiled and kinked in the unstressed state; and 2) there
15.22 This question asks us to choose from a list of materials those which would be expected to
be elastomers and those which would be thermosetting polymers.
(a) Linear and crystalline polyethylene would be neither an elastomer nor a thermoset since
it is a linear polymer.
(b) Phenol-formaldehyde having a network structure would be a thermosetting polymer
since it has a network structure. It would not be an elastomer since it does not have a
(c) Heavily crosslinked polyisoprene having a glass transition temperature of 50&deg;C would be
a thermosetting polymer because it is heavily crosslinked. It would not be an elastomer
since it is heavily crosslinked and room temperature is below its Tg.
(d) Lightly crosslinked polyisoprene having a glass transition temperature of -60&deg;C is both
an elastomer and a thermoset. It is an elastomer because it is lightly crosslinked and has a
Tg below room temperature. It is a thermoset because it is crosslinked.
(e)
Linear and partially amorphous polyvinyl chloride is neither an elastomer nor a
thermoset. In order to be either it must have some crosslinking.
15.23 The molecules in elastomers must be two-dimensional chains that are lightly crosslinked
and capable of being twisted and kinked in the unstressed state. Phenol-formaldehyde has
a rigid three-dimensional structure consisting of trifunctional mer units, which does not meet
these criteria for chain conformation and flexibility.
15.24 This problem asks that we compute the fraction of possible crosslink sites in 10 kg of
polybutadiene when 4.8 kg of S is added, assuming that, on the average, 4.5 sulfur atoms
participate in each crosslink bond. Given the butadiene mer unit in Table 14.5, we may
calculate its molecular weight as follows:
= (4)(12.01 g/mol) + 6(1.008 g/mol) = 54.09 g/mol
Which means that in 10 kg of butadiene there are
393
10, 000 g
= 184.9 mol.
54.09 g / mol
For the vulcanization of polybutadiene, there are two possible crosslink sites per
mer--one for each of the two carbon atoms that are doubly bonded. Furthermore, each of
these crosslinks forms a bridge between two mers. Therefore, we can say that there is the
equivalent of one crosslink per mer. Therefore, let us now calculate the number of moles of
sulfur (nsulfur) that react with the butadiene, by taking the mole ratio of sulfur to butadiene,
and then dividing this ratio by 4.5 atoms per crosslink; this yields the fraction of possible
nsulfur =
4800 g
= 149.7 mol
32.06 g / mol
And
149.7 mol
fraction sites crosslinked = 184.9 mol = 0.180
4.5
15.25
For an alternating chloroprene-acrylonitrile copolymer, we are asked to compute the
weight percent sulfur necessary for complete crosslinking, assuming that, on the average,
five sulfur atoms participate in each crosslink. The chloroprene and acrylonitrile mers are
shown in Table 14.5, from which it may be noted that there are two possible crosslink sites
on each chloroprene mer (one site at each of the two carbon atoms that are doubly bonded),
and no possible crosslink sites for acrylonitrile; also, since it is an alternating copolymer, the
ratio of chloroprene to acrylonitrile mers is 1:1.
Thus, for each pair of combined
chloroprene-acrylonitrile mers which crosslink, ten sulfur atoms are required, or, for
complete crosslinking, the sulfur-to-(chloroprene-acrylonitrile) ratio is 5:1.
Now, let us consider as our basis, one mole of the combined chloropreneacrylonitrile mer. In order for complete crosslinking, five moles of sulfur are required. Thus,
for us to convert this composition to weight percent, it is necessary to convert moles to
mass. The acrylonitrile mer consists of three carbon atoms, three hydrogen atoms, and one
nitrogen atom; the chloroprene mer is composed of four carbons, five hydrogens, and one
chlorine. This gives a molecular weight for the combined mer of
m(chloroprene-acrylonitrile) = 3(AC) + 3(AH) + AN + 4(AC) + 5(AH) + ACl
= 7(12.01 g/mol) + 8(1.008 g/mol) + 14.007 g/mol + 35.45 g/mol = 141.59 g/mol
394
Or, in one mole of this combined mer, there are 141.59 g.
Furthermore, for complete
crosslinking, 5.0 mol of sulfur is required, which amounts to (5.0 mol)(32.06 g/mol) = 160.3
g. Thus, the concentration of S in weight percent CS is just
CS =
160.3 g
x 100 = 53.1 wt%
160.3 g + 141.59 g
15.26 This problem asks for us to determine how many crosslinks form per isoprene mer when
57 wt% sulfur is added. If we arbitrarily consider 100 g of the vulcanized material, 57 g will
be sulfur and 43 g will be polyisoprene. Next, let us find how many moles of sulfur and
isoprene correspond to these masses. The atomic weight of sulfur is 32.06 g/mol, and thus,
# moles S =
57 g
= 1.78 mol
32.06 g/ mol
However, there are 6 sulfur atoms in each crosslink, which requires us to divide the number
of moles of sulfur by 6 in order to get the number of moles of sulfur per crosslink, which is
equal to 0.297 moles.
Now, in each isoprene mer unit there are five carbon atoms and eight hydrogen
atoms. Thus, the molecular weight of a mole of isoprene units is
(5)(12.01 g/mol) + (8)(1.008 g/mol) = 68.11 g/mol
Or, in 43 g of polyisoprene
# moles isoprene =
43 g
= 0.631 mol
68.11 g / mol
Therefore, the ratio of moles of S per crosslink to the number of moles of polyisoprene is
1.78 mol
: 1 = 2.82 : 1
0.631 mol
When all possible sites are crosslinked, the ratio of the number of moles of sulfur to the
number of moles of isoprene is 6:1, since there are two crosslink sites per mer unit and each
crosslink is shared between mers on adjacent chains, and there are 6 sulfur atoms per
Finally, to determine the fraction of sites that are crosslinked, we just divide the
395
fraction of mer sites crosslinked =
2.82 /1
= 0.47
6/1
15.27 We are asked what weight percent of sulfur must be added to polyisoprene in order to
ensure that 8% of possible sites are crosslinked, assuming that, on the average, three sulfur
atoms are associated with each crosslink. Table 14.5 shows the chemical repeat unit for
cis-isoprene. For each of these units there are two possible crosslink sites; one site is
associated with each of the two carbon atoms that are involved in the chain double bond.
Since 8% of the possible sites are crosslinked, for each 100 isoprene mers 8 of them are
two chains. Furthermore, on the average we assume that each crosslink is composed of 3
sulfur atoms; thus, there must be 3 x 8 or 24 sulfur atoms added for every 100 isoprene
mers. In terms of moles, it is necessary to add 24 moles of sulfur to 100 moles of isoprene.
The atomic weight of sulfur is 32.06 g/mol, while the molecular weight of isoprene is
5(AC) + 8(AH)
= (5)(12.01 g/mol) + (8)(1.008 g/mol) = 68.11 g/mol
The mass of sulfur added (m ) is
S
mS = (24 mol)(32.06 g/mol) = 769.4 g
While for isoprene
mip = (100 mol)(68.11 g/mol) = 6811 g
Or, the concentration of sulfur in weight percent is just
CS =
769.4 g
x 100 = 10.2 wt%
769.4 g + 6811 g
15.28 The reaction by which a chloroprene rubber may become vulcanized is as follows:
396
15.29 (a) Shown below are specific volume-versus-temperature curves for the two polyethylene
materials.
The linear polyethylene will be highly crystalline, and, therefore, will exhibit
behavior similar to curve C in Figure 15.17.
The branched polyethylene will be
semicrystalline, and, therefore its curve will appear as curve B in this same figure.
Furthermore, since the linear polyethylene has the greater molecular weight, it will also have
the higher melting temperature.
(b) Shown below are specific volume-versus-temperature curves for the polyvinyl chloride
and polypropylene materials.
Since both are 50% crystalline, they will exhibit behavior
similar to curve B in Figure 15.17.
However, since the polypropylene has the greater
molecular weight it will have the higher melting temperature. Furthermore, polypropylene
will also have the higher glass-transition temperature inasmuch as its CH3 side group is
bulkier than the Cl for PVC.
397
(c) Shown below are specific volume-versus-temperature curves for the polystyrene and
polypropylene materials. Since both are totally amorphous, they will exhibit the behavior
similar to curve A in Figure 15.17. However, since the polystyrene mer has a bulkier side
group than polypropylene (Table 14.3), its chain flexibility will be lower, and, thus, its glasstransition temperature will be higher.
15.30 (a) Yes, it is possible to determine which polymer has the higher melting temperature. The
linear polyethylene will most likely have a higher percent crystallinity, and, therefore, a
higher melting temperature than the branched polyethylene. The molecular weights of both
materials are the same and, thus, molecular weight is not a consideration.
(b) Yes, it is possible to determine which polymer has the higher melting temperature. Of
these two polytetrafluoroethylene polymers, the PTFE with the higher density (2.20 g/cm3)
398
will have the higher percent crystallinity, and, therefore, a higher melting temperature than
the lower density PTFE. The molecular weights of both materials are the same and, thus,
molecular weight is not a consideration.
(c) Yes, it is possible to determine which polymer has the higher melting temperature. The
linear polyethylene will have the greater melting temperature inasmuch as it will have a
higher degree of crystallinity; polymers having a syndiotactic structure do not crystallize as
easily as those polymers having identical single-atom side groups. With regard to molecular
weight, or rather, the number-average degree of polymerization, it is about the same for both
materials (8000), and therefore, is not a consideration.
(d) No, it is not possible to determine which of the two polymers has the higher melting
temperature. The syndiotactic polypropylene will have a higher degree of crystallinity than
the atactic material. On the basis of this effect alone, the syndiotactic PP should have the
greater Tm, since melting temperature increases with degree of crystallinity. However, the
molecular weight for the syndiotactic polypropylene (500,000 g/mol) is less than for the
atactic material (750,000 g/mol);
and this factor leads to a lowering of the melting
temperature
15.31 For an amorphous polymer, the elastic modulus may be enhanced by increasing the
number of crosslinks (while maintaining the molecular weight constant);
this will also
enhance the glass transition temperature. Thus, the modulus-glass transition temperature
behavior would appear as
15.32 In this problem we are asked to determine the values of the constants n and k [Equation
(10.1)] for the crystallization of polypropylene at 150&deg;C (Figure 15.16). One way to solve this
problem is to take two values of percent recrystallization [which is just 100y, Equation (10.1)]
and their corresponding time values, then set up two simultaneous equations, from which n
399
and k may be determined. In order to expedite this process, we will rearrange and do some
algebraic manipulation of Equation (10.1). First of all, we rearrange as follows:
( n)
1 − y = exp −kt
Now taking natural logarithms
ln (1 − y) = − ktn
Or
− ln (1 − y) = ktn
which may also be expressed as
⎛ 1 ⎞
n
ln ⎜
⎟ = kt
⎝1 − y⎠
Now taking natural logarithms again, leads to
⎡
ln ⎢ln
⎣
⎛ 1 ⎞⎤
⎜ 1 − y ⎟ ⎥ = ln k + n ln t
⎝
⎠⎦
which is the form of the equation that we will now use. From the 150&deg;C curve of Figure
15.16, let us arbitrarily choose two percent crystallized values of 20% and 80% (i.e., y1 =
0.20 and y2 = 0.80). Their corresponding time values are t1 = 220 min and t2 = 460 min
(realizing that the time axis is scaled logarithmically). Thus, our two simultaneous equations
become
⎡ ⎛ 1 ⎞⎤
ln ⎢ln ⎜
⎟ ⎥ = ln k + n ln (220 )
⎣ ⎝ 1 − 0.2 ⎠ ⎦
⎡ ⎛ 1 ⎞⎤
ln ⎢ln ⎜
⎟ ⎥ = ln k + n ln (460)
⎣ ⎝ 1 − 0.8 ⎠ ⎦
from which we obtain the values n = 2.68 and k = 1.2 x 10-7.
400
15.33 This question asks us to name which, of several polymers, would be suitable for the
fabrication of cups to contain hot coffee. At its glass transition temperature, an amorphous
polymer begins to soften. The maximum temperature of hot coffee is probably slightly below
100&deg;C (212&deg;F). Of the polymers listed, only polystyrene and polycarbonate have glass
transition temperatures of 100&deg;C or above (Table 15.2), and would be suitable for this
application.
15.34 In order for a polymer to be suited for use as an ice cube tray it must have a glasstransition temperature below 0&deg;C. Of those polymers listed in Table 15.2 only low-density
and high-density polyethylene, PTFE, and polypropylene satisfy this criterion.
15.35
This question asks for us to determine which of several elastomers are suitable for
From Table 15.4, only natural polyisoprene, poly(styrene-
butadiene), and polysiloxane have useful temperature ranges that extend to below -55&deg;C. At
temperatures below the lower useful temperature range limit, the other elastomers listed in
this table become brittle, and, therefore, are not suitable for automobile tires.
15.36 The backbone chain of most polymers consists of carbon atoms that are linked together.
For the silicone polymers, this backbone chain is composed of silicon and oxygen atoms that
alternate positions.
15.37 The liquid silicones will have low molecular weights and very little crosslinking, whereas
the molecular weights for the elastomers will be much higher; the elastomers will also have
15.38 Two important characteristics for polymers that are to be used in fiber applications are: 1)
a high molecular weight, and 2) a chain configuration/structure that allows for a high degree
of crystallinity.
15.39 Five important characteristics for polymers that are to be used in thin film applications are:
1) low density; 2) high flexibility; 3) high tensile and tear strengths; 4) resistance to
moisture/chemical attack; and 5) low gas permeability.
15.40 For addition polymerization, the reactant species have the same chemical composition as
the monomer species in the molecular chain. This is not the case for condensation
401
polymerization, wherein there is a chemical reaction between two or more monomer
species, producing the repeating mer unit. There is often a low molecular weight by-product
15.41 In this question we are asked to cite whether the molecular weight of a polymer that is
synthesized by addition polymerization is relatively high, medium, or low for four situations.
(a) For rapid initiation, slow propagation, and rapid termination the molecular weight will be
relatively low.
(b) For slow initiation, rapid propagation, and slow termination the molecular weight will be
relatively high.
(c) For rapid initiation, rapid propagation, and slow termination a medium molecular weight
will be achieved.
(d) For slow initiation, slow propagation, and rapid termination the molecular weight will be
low or medium.
15.42 (a) This problem asks that we determine how much ethylene glycol must be added to 20.0
kg of adipic acid to produce a linear chain structure of polyester according to Equation 15.9.
Since the chemical formulas are provided in this equation we may calculate the molecular
weights of each of these materials as follows:
A(adipic) = 6(A C ) + 10(AH ) + 4(A O )
= 6(12.01 g/mol) + 10(1.008 g/mol) + 4 (16.00 g/mol) = 146.14 g/mol
A(glycol) = 2(AC ) + 6(AH ) + 2(A O )
= 2(12.01 g/mol) + 6(1.008 g/mol) + 2(16.00 g/mol) = 62.07 g/mol
The 20.0 kg mass of adipic acid equals 20,000 g or
20, 000 g
= 136.86 mol. Since,
146.14 g / mol
according to Equation (15.9), each mole of adipic acid used requires one mole of ethylene
glycol, which is equivalent to (136.86 mol)(62.07 g/mol) = 8495 g = 8.495 kg.
(b) Now we are asked for the mass of the resulting polyester. Inasmuch as one mole of
water is given off for every mer unit produced, this corresponds to 136.86 moles or (136.86
mol)(18.02 g/mol) = 2466 g or 2.466 kg since the molecular weight of water is 18.02 g/mol.
402
The mass of polyester is just the sum of the masses of the two reactant materials [as
computed in part (a)] minus the mass of water released, or
mass(polyester) = 20.0 kg + 8.495 kg − 2.466 kg = 26.03 kg
15.43 The following represents the reaction between hexamethylene diamine and adipic acid to
produce nylon 6,6 with water as a by-product.
15.44 This problem asks for us to calculate the masses of hexamethylene diamine and adipic
acid necessary to yield 20 kg of completely linear nylon 6,6. Let us first calculate the
molecular weights of these molecules. (The chemical formula for hexamethylene diamine is
given in Problem 15.43)
A(adipic) = 6(A C ) + 10(AH ) + 4(A O )
= 6(12.01 g/mol) + 10(1.008 g/mol) + 4 (16.00 g/mol) = 146.14 g/mol
A(hexamethylene) = 6(AC ) + 16(AH ) + 2(AN )
= 6(12.01 g/mol) + 16(1.008 g/mol) + 2 (14.01 g/mol) = 116.21 g/mol
A(nylon) = 12(AC ) + 22(AH ) + 2(AN ) + 2(A O )
= 12 (12.01 g/mol) + 22 (1.008 g/mol) + 2(14.01 g/mol) + 2(16.00 g/mol)
403
= 226.32 g/mol
The mass of 20 kg of nylon 6,6 equals 20,000 g or
m(nylon) =
20,000 g
= 88.37 mol
226.32 g / mol
Since, according to the chemical equation in Problem 15.43, each mole of nylon 6,6 that is
produced requires one mole each of adipic acid and hexamethylene diamine, with two moles
of water as the by-product. The masses corresponding to 88.37 moles of adipic acid and
hexamethylene diamine are as follows:
m(adipic) = (88.37 mol)(146.14 g/mol) = 12,914 g = 12.914 kg
m(hexamethylene) = (88.37 mol)(116.21 g/mol) = 10,269 g = 10.269 kg
15.45 (a) If the vapor pressure of a plasticizer is not relatively low, the plasticizer may vaporize,
which will result in an embrittlement of the polymer.
(b) The crystallinity of a polymer to which has been added a plasticizer will be diminished,
inasmuch as the plasticizer molecules fit in between the polymer molecules, which will cause
more misalignment of the latter.
(c) It would be difficult for a crosslinked polymer to be plasticized since the plasticizer
molecules must fit between the chain molecules. This necessarily forces apart adjacent
molecules, which the crosslinked bonds between the chains will resist.
(d) The tensile strength of a polymer will be diminished when a plasticizer is added. As the
plasticizer molecules force the polymer chain molecules apart, the magnitude of the
secondary interchain bonds are lessened, which weakens the material since strength is a
function of the magnitude of these bonds.
15.46 The distinction between dye and pigment colorants is that a dye dissolves within and
becomes a part of the polymer structure, whereas a pigment does not dissolve, but remains
as a separate phase.
15.47 Four factors that determine which fabrication technique is used to form polymeric materials
are: 1) whether the polymer is thermoplastic or thermosetting; 2) if thermoplastic, the
404
softening temperature;
3) atmospheric stability;
and 4) the geometry and size of the
finished product.
15.48 This question requests that we compare polymer molding techniques. For compression
molding, both heat and pressure are applied after the polymer and necessary additives are
situated between the mold members. For transfer molding, the solid materials (normally
thermosetting in nature) are first melted in the transfer chamber prior to being forced into the
die. And, for injection molding (normally used for thermoplastic materials), the raw materials
are impelled by a ram through a heating chamber, and finally into the die cavity.
15.49 Vulcanization of a rubber component should be carried out prior to the forming operation
since, once it has been vulcanized, plastic deformation (and thus forming) is not possible
since chain crosslinks have been introduced.
15.50 Fiber materials that are melt spun must be thermoplastic because: 1) In order to be melt
spun, they must be capable of forming a viscous liquid when heated, which is not possible
for thermosets. 2) During drawing, mechanical elongation must be possible; inasmuch as
thermosetting materials are, in general, hard and relatively brittle, they are not easily
elongated.
15.51 Of the two polymers cited, the one that was formed by extrusion and then rolled would
have the higher strength.
Both blown and extruded materials would have roughly
comparable strengths; however the rolling operation would further serve to enhance the
strength of the extruded material.
Design Problems
15.D1 (a) Several advantages of using transparent polymeric materials for eyeglass lenses are:
they have relatively low densities, and, therefore, are light in weight; they are relatively easy
to grind to desired contours; they are less likely to shatter than are glass lenses; wraparound lenses for protection during sports activities are possible; and they filter out more
ultraviolet radiation than do glass lenses.
The principal disadvantage of these types of lenses is that some are relatively soft
and are easily scratched (although antiscratch coatings may be applied). Plastic lenses are
not as mechanically stable as glass, and, therefore, are not as precise optically.
405
(b) Some of the properties that are important for polymer lens materials are: they should be
relatively hard in order to resist scratching; they must be impact resistant; they should be
shatter resistant; they must have a relatively high index of refraction such that thin lenses
may be ground for very nearsighted people; and they should absorb significant proportions
of all types of ultraviolet radiation, which radiation can do damage to the eye tissues.
(c) Of those polymers discussed in this chapter and Chapter 14, ones that might appear to
be likely lens candidates are polystyrene, polymethyl methacrylate, and polycarbonate;
these three materials are not easily crystallized, and, therefore, are normally transparent.
Upon consultation of their fracture toughnesses (Table B.5 in Appendix B), polycarbonate is
the most superior of the three.
Commercially, the two plastic lens materials of choice are polycarbonate and allyl
diglycol carbonate (having the trade name CR-39). Polycarbonate is very impact resistant,
but not as hard as CR-39. Furthermore, PC comes in both normal and high refractive-index
15.D2
There are three primary requirements for polymeric materials that are utilized in the
packaging of food products and drinks; these are: 1) sufficient strength, to include tensile,
tear, and impact strengths; 2) provide barrier protection--that is, be resistant to permeation
by oxygen, water vapor, and carbon dioxide; and 3) be nonreactive with the food/drink
contents--such reactions can compromise the integrity of the packaging material, or they can
produce toxic by-products.
With regard to strength, polyethylene terephthalate (PET or PETE) and oriented
polypropylene (OPP) have high tensile strengths, linear low-density polyethylene (LLDPE)
and low-density polyethylene (LDPE) have high tear strengths, while those polymers having
the best impact strengths are PET and polyvinyl chloride (PVC).
Relative to barrier
characteristics, ethylene vinyl alcohol (EVOH) and polyvinylidene chloride (PVDC)
copolymers are relatively impermeable to oxygen and carbon dioxide, whereas high-density
polyethylene (HDPE), polyvinylidene chloride, polypropylene, and LDPE are impervious to
water vapor.
Most common polymers are relatively nonreactive with food products, and are
considered safe; exceptions are acrylonitrile and plasticizers used in PVC materials that
may be harmful.
The aesthetics of packaging polymers are also important in the marketing of food
and drink products. Some packages will be colored, many are adorned with printing, others
need to be transparent and clear, and many need to be resistant to scuffing.
406
On the basis of the preceding discussion, some examples of polymers that are used
for specific applications are as follows:
PET(E) for soda pop containers;
PVC for beer containers;
LDPE and HDPE films for packaging bread and bakery products.
407
CHAPTER 16
COMPOSITES
PROBLEM SOLUTIONS
16.1
The major difference in strengthening mechanism between large-particle and dispersionstrengthened particle-reinforced composites is that for large-particle the particle-matrix interactions
are not treated on the molecular level, whereas, for dispersion-strengthening these interactions are
treated on the molecular level.
16.2 The similarity between precipitation hardening and dispersion strengthening is the strengthening
mechanism--i.e., the precipitates/particles effectively hinder dislocation motion.
The two differences are: 1) the hardening/strengthening effect is not retained at elevated
temperatures for precipitation hardening--however, it is retained for dispersion strengthening; and 2)
the strength is developed by a heat treatment for precipitation hardening--such is not the case for
dispersion strengthening.
16.3 The elastic modulus versus volume percent of WC is shown below, on which is included both upper
and lower bound curves;
these curves were generated using Equations (16.1) and (16.2),
respectively, as well as the moduli of elasticity for cobalt and WC given in the problem statement.
408
16.4 This problem asks for the maximum and minimum thermal conductivity values for a TiC-Co cermet.
Using a modified form of Equation (16.1) the maximum thermal conductivity kmax is calculated as
kmax = kmVm + k pVp = kCo VCo + k TiCVTiC
= (69 W/m - K)(0.15) + (27 W/m -K)(0.85) = 33.3 W/m -K
And, from a modified form of Equation (16.2), the minimum thermal conductivity kmin is
kmin =
=
kCo k TiC
VCo k TiC + VTiCk Co
(69 W / m - K)(27 W / m -K)
(0.15)(27 W / m- K) + (0.85)(69 W / m -K)
= 29.7 W/m-K
16.5 Given the elastic moduli and specific gravities for copper and tungsten we are asked to estimate the
upper limit for specific stiffness when the volume fractions of tungsten and copper are 0.70 and 0.30,
respectively. There are two approaches that may be applied to solve this problem. The first is to
estimate both the upper limits of elastic modulus [Ec(u)] and specific gravity (ρc) for the composite,
using equations of the form of Equation (16.1), and then take their ratio. Using this approach
E c (u) = ECu VCu + EW VW
= (110 GPa)(0.30) + (407 GPa)(0.70)
= 318 GPa
And
ρ c = ρ CuVCu + ρ W VW
= (8.9)(0.30) + (19.3)(0.70) = 16.18
Therefore
409
Specific Stiffness =
Ec (u)
ρc
=
318 GPa
= 19.65 GPa
16.18
With the alternate approach, the specific stiffness is calculated, again employing a
modification of Equation (16.1), but using the specific stiffness-volume fraction product for both
metals, as follows:
Specific Stiffness =
=
E Cu
ρ
Cu
VCu +
E
ρ
W V
W
W
110 GPa
407 GPa
(0.30) +
(0.70) = 18.47 GPa
8.9
19.3
16.6 (a) The matrix phase is a continuous phase that surrounds the noncontinuous dispersed phase.
(b) In general, the matrix phase is relatively weak, has a low elastic modulus, but is quite ductile.
On the other hand, the fiber phase is normally quite strong, stiff, and brittle.
16.7 (a) Concrete consists of an aggregate of particles that are bonded together by a cement.
(b) Three limitations of concrete are: 1) it is a relatively weak and brittle material; 2) it experiences
relatively large thermal expansions (contractions) with changes in temperature; and 3) it may crack
when exposed to freeze-thaw cycles.
(c) Three reinforcement strengthening techniques are: 1) reinforcement with steel wires, rods, etc.;
2) reinforcement with fine fibers of a high modulus material;
and 3) introduction of residual
compressive stresses by prestressing or posttensioning.
16.8 (a) Three functions of the polymer-matrix phase are: 1) to bind the fibers together so that the
applied stress is distributed among the fibers; 2) to protect the surface of the fibers from being
damaged; and 3) to separate the fibers and inhibit crack propagation.
(b) The matrix phase must be ductile and is usually relatively soft, whereas the fiber phase must be
stiff and strong.
(c) There must be a strong interfacial bond between fiber and matrix in order to: 1) maximize the
stress transmittance between matrix and fiber phases;
probability of failure.
410
and 2) minimize fiber pull-out, and the
16.9 This problem asks that, for a glass fiber-epoxy matrix combination, to determine the fiber-matrix
bond strength if the critical fiber length-fiber diameter ratio is 40. Thus, we are to solve for τc in
l
Equation (16.3). Since we are given that σ f∗ = 3.45 GPa from Table 16.4, and that c = 40, then
d
⎛ d ⎞
1
3
τ c = σ ∗f ⎜⎜
= 43.1 MPa
⎟⎟ = 3.45 x 10 MPa
2l
(2)(40)
⎝ c⎠
(
)
16.10 (a) The plot of reinforcement efficiency versus fiber length is given below.
(b) This portion of the problem asks for the length required for a 0.90 efficiency of reinforcement.
Solving for l from the given expression
l =
2x
1− η
Or, when x = 1.25 mm (0.05 in.) and η = 0.90, then
l =
(2)(1.25 mm)
= 25 mm (1.0 in.)
1 − 0.90
411
16.11 This problem calls for us to compute the longitudinal tensile strength and elastic modulus of an
aramid fiber-reinforced polycarbonate composite.
(a) The longitudinal tensile strength is determined using Equation (16.17) as
(
)
∗
' 1 − V + σ∗ V
σ cl
= σm
f
f f
= (45 MPa)(0.70) + (3600 MPa)(0.30)
= 1100 MPa (160, 000 psi)
(b) The longitudinal elastic modulus is computed using Equation (16.10a) as
Ecl = Em Vm + Ef Vf
= (2.4 GPa)(0.70) + (131 GPa)(0.30)
= 41 GPa (5.95 x 106 psi)
16.12 This problem asks for us to determine if it is possible to produce a continuous and oriented aramid
fiber-epoxy matrix composite having longitudinal and transverse moduli of elasticity of 35 GPa and
5.17 GPa, respectively, given that the modulus of elasticity for the epoxy is 3.4 GPa. Also, from
Table 16.4 the value of E for aramid fibers is 131 GPa. The approach to solving this problem is to
calculate two values of Vf using the data and Equations (16.10b) and (16.16); if they are the same
then this composite is possible.
For the longitudinal modulus Ecl,
(
)
E cl = Em 1 - Vfl + E f Vfl
(
)
35 GPa = (3.4 GPa) 1 - Vfl + (131 GPa)Vfl
Solving this expression for Vfl yields Vfl = 0.248.
Now, repeating this procedure for the transverse modulus Ect
E ct =
E mE f
(1 − Vft )Ef + VftEm
412
(3.4 GPa)(131 GPa)
(1 − Vft )(131 GPa) + Vft(3.4 GPa)
5.17 GPa =
Solving this expression for Vft leads to Vft = 0.351. Thus, since Vfl and Vft are not equal, the
proposed composite is not possible.
16.13 (a) This portion of the problem calls for us to calculate the specific longitudinal strengths of glassfiber, carbon-fiber, and aramid-fiber reinforced epoxy composites, and then to compare these values
with the specific strengths of several metal alloys.
The longitudinal specific strength of the glass-reinforced epoxy material (V = 0.60) in Table
f
16.5 is just the ratio of the longitudinal tensile strength and specific gravity as
1020 MPa
= 486 MPa
2.1
For the carbon-fiber reinforced epoxy
1240 MPa
= 775 MPa
1.6
And, for the aramid-fiber reinforced epoxy
1380 MPa
= 986 MPa
1.4
Now, for the metal alloys we use data found in Tables B.1 and B.4 in Appendix B. For the
cold-rolled 7-7PH stainless steel
1380 MPa
= 180 MPa
7.65
For the normalized 1040 plain carbon steel, the ratio is
590 MPa
= 75 MPa
7.85
For the 7075-T6 aluminum alloy
413
572 MPa
= 204 MPa
2.80
For the C26000 brass (cold worked)
525 MPa
= 62 MPa
8.53
For the AZ31B (extruded) magnesium alloy
262 MPa
= 148 MPa
1.77
For the annealed Ti-5Al-2.5Sn titanium alloy
790 MPa
= 176 MPa
4.48
(b) The longitudinal specific modulus is just the longitudinal tensile modulus-specific gravity ratio.
For the glass-fiber reinforced epoxy, this ratio is
45 GPa
= 21.4 GPa
2.1
For the carbon-fiber reinforced epoxy
145 GPa
= 90.6 GPa
1.6
And, for the aramid-fiber reinforced epoxy
76 GPa
= 54.3 GPa
1.4
The specific moduli for the metal alloys (Tables B.1 and B.2) are as follows:
For the cold rolled 17-7PH stainless steel
204 GPa
= 26.7 GPa
7.65
For the normalized 1040 plain-carbon steel
414
207 GPa
= 26.4 GPa
7.85
For the 7075-T6 aluminum alloy
71 GPa
= 25.4 GPa
2.80
For the cold worked C26000 brass
110 GPa
= 12.9 GPa
8.53
For the extruded AZ31B magnesium alloy
45 GPa
= 25.4 GPa
1.77
For the Ti-5Al-2.5Sn titanium alloy
110 GPa
= 24.6 GPa
4.48
16.14 This problem asks for us to compute the elastic moduli of fiber and matrix phases for a continuous
and oriented fiber-reinforced composite.
We can write expressions for the longitudinal and
transverse elastic moduli using Equations (16.10b) and (16.16), as
(
)
E cl = Em 1 - Vf + E f Vf
19.7 GPa = Em (1 - 0.25) + E f (0.25)
And
Ect =
3.66 GPa =
E E
m f
(1 − Vf )Ef + VfEm
E E
m f
(1 − 0.25)E + 0.25E
f
415
m
Solving these two expressions simultaneously for Em and Ef leads to
Em = 2.79 GPa (4.04 x 10 5 psi)
E f = 70.4 GPa (10.2 x 106 psi)
16.15 (a) In order to show that the relationship in Equation (16.11) is valid, we begin with Equation
(16.4), F = F + F , which may be manipulated to read
c
m
f
Fc
F
= 1 +
m
F
f
F
m
or
F
f = c − 1
F
F
m
m
F
For elastic deformation [Equation (6.5)]
σ =
F
= εE
A
or
F = AεE
Now we may write expressions for F and F as
c
m
Fc = A c εE c
Fm = A mεEm
which, when substituted into the above expression gives
A c εE c
f =
− 1
F
A εE
m
m m
F
But, V = A /A , or
m
m c
416
E
F
c
f =
− 1
F
E V
m
m m
Also, from Equation (16.10a), E = E V + E V , which, when substituted into the previous
c
m m
f f
expression, yields
f =
F
m
=
E V
m m
+ EV
E V
F
m m
f f − 1
E V
m m
+ EV − E V
f f
m m =
E V
m m
EV
f f
E V
m m
(b) This portion of the problem asks that we establish an expression for F /F . We determine this
f c
ratio in a similar manner. Now F = F + F , or
c
f
m
1 =
F
F
f + m
F
F
c
c
which gives
A εE
F
F
A E
f = 1− m = 1− m m = 1− m m
F
F
A εE
A E
c
c
c c
c c
Since A /A = V , then
m c
m
V E
F
f = 1−
F
c
m m
E
V E
m m
= 1−
V E
m m
=
V E
m m
f f
f f
VmE m + Vf Ef
f f
+ VE
V E
VE
+ VE
+ VE − V E
m m
=
c
=
m m
f f
(
VE
)
f f
1 − Vf Em + Vf Ef
417
16.16 (a) Given some data for an aligned glass-fiber-reinforced nylon 6,6, we are asked to compute the
volume fraction of fibers that is required such that the fibers carry 94% of a load applied in the
longitudinal direction. From Equation (16.11)
F
EV
EV
f =
f f =
f f
Fm
E mVm
Em 1 − Vf
(
)
Now,
F
f = 0.94 = 15.67
0.06
F
m
Substituting in for E and E
f
m
F
(72.5 GPa)V
f = 15.67 =
f
Fm
(3.0 GPa) 1 − Vf
(
)
And, solving for V yields, V = 0.418.
f
f
(b) We are now asked for the tensile strength of this composite. From Equation (16.17), and using
' (30 MPa) given in the problem statement,
values for σ f∗ (3400 MPa) and σ m
(
)
∗
' 1− V
σ cl∗ = σm
f + σf Vf
= (30 MPa)(1 − 0.418) + (3400 MPa)(0.0.418)
= 1440 MPa (207,000 psi)
2
2
16.17 This problem stipulates that the cross-sectional area of a composite, A , is 320 mm (0.50 in. ),
c
and that the longitudinal load, F , is 44,500 N (10,000 lbf) for the composite described in Problem
c
16.11.
(a) First, we are asked to calculate the F /F ratio. According to Equation (16.11)
f m
EV
f =
f f = (131 GPa)(0.30) = 23.4
(2.4 GPa)(0.70)
F
E V
m
m m
F
418
Or, F = 23.4F
f
m
(b) Now, the actual loads carried by both phases are called for. Since
Ff + Fm = Fc = 44,500 N
23.4Fm + Fm = 44,500 N
Fm = 1824 N (410 lb f )
Ff = 44,500 N − 1824 N = 42,676 N (9590 lb f )
(c) To compute the stress on each of the phases, it is first necessary to know the cross-sectional
areas of both fiber and matrix. These are determined as
A f = Vf A c = (0.30)(320 mm2 ) = 96 mm 2 (0.15 in.2 )
A m = Vm A c = (0.70)(320 mm2 ) = 224 mm2 (0.35 in.2 )
Now, for the stresses,
σf =
σm =
Ff
A
=
42,676 N
96 mm 2
f
Fm
A
m
=
=
1824 N
224 mm 2
42,676 N
96 x 10 −6 m2
=
= 445 MPa (63, 930 psi)
1824 N
224 x 10-6 m2
= 8.14 MPa (1170 psi)
(d) The strain on the composite is the same as the strain on each of the matrix and fiber phases, as
εm =
εf =
σ
8.14 MPa
m =
= 3.39 x 10 -3
3 MPa
E
2.4
x
10
m
σ
445 MPa
f =
= 3.39 x 10-3
3 MPa
E
131
x
10
f
419
16.18 For a continuous and aligned fibrous composite, we are given its cross-sectional area (970 mm2),
the stresses sustained by the fiber and matrix phases (215 and 5.38 MPa), the force sustained by
the fiber phase (76,800 N), and the total longitudinal strain (1.56 x 10-3).
(a) For this portion of the problem we are asked to calculate the force sustained by the matrix
phase. It is first necessary to compute the volume fraction of the matrix phase, Vm. This may be
accomplished by first determining Vf and then Vm from Vm = 1 - Vf. The value of Vf may be
calculated realizing that
σf =
F
F
f =
f
A
VA
f
f c
Or
Vf =
Ff
σf A c
=
76,800 N
(
)(
215 x 10 6 N / m2 0.970 x 10 −3 m 2
)
= 0.369
Now
Vm = 1 − Vf = 1 − 0.369 = 0.631
Therefore, since
σm =
F
F
m =
m
A
V A
m
m c
then
(
6
2
Fm = Vm σm A c = (0.631) 5.38 x 10 N/m
)(0.970 x 10-3 m2 ) = 3290 N
(738 lb f )
(b) We are now asked to calculate the modulus of elasticity in the longitudinal direction. This is
σc
F +F
f . Thus
possible realizing that Ec =
and that σ c = m
ε
A
c
Ec =
=
(
F
m
+ F
εA
3290 N + 76, 800 N
)(
1.56 x 10−3 0.970 x 10−3 m 2
)
f
c
6
= 52.9 GPa (7.69 x 10 psi)
(c) Finally, it is necessary to determine the moduli of elasticity for the fiber and matrix phases. This
is possible as follows:
420
Em =
σm
=
ε
σm
ε
m
c
=
5.38 x 106 N / m2
1.56 x 10 −3
9
2
= 3.45 x 10 N/m
= 3.45 GPa (5.0 x 105 psi)
Ef =
σf
ε
=
f
σf
ε
c
=
215 x 106 N/ m 2
1.56 x 10−3
11
= 1.38 x 10
2
N/m
= 138 GPa (20 x 106 psi)
16.19 In this problem, for an aligned carbon fiber-epoxy matrix composite, we are given the volume
fraction of fibers (0.20), the average fiber diameter (6 x 10-3 mm), the average fiber length (8.0 mm),
the average fiber fracture strength (4.5 GPa), the fiber-matrix bond strength (75 MPa), the matrix
stress at composite failure (6.0 MPa), and the matrix tensile strength (60 MPa); and we are asked to
compute the longitudinal strength. It is first necessary to compute the value of the critical fiber length
using Equation (16.3). If the fiber length is much greater than lc, then we may determine the
longitudinal strength using Equation (16.17), otherwise, use of either Equation (16.18) or (16.19) is
necessary. Thus,
lc =
σ f∗ d
2τ
c
=
(4.5 x 103 MPa)(6 x 10 −3 mm)= 0.18 mm
2 (75 MPa)
Inasmuch as l &gt;&gt; lc (8.0 mm &gt;&gt; 0.18 mm), then use of Equation (16.17) is appropriate. Therefore,
(
)
∗
' 1 − V + σ∗ V
σ cl
= σm
f
f f
= (6 MPa)(1 - 0.20) + (4500 MPa)(0.20)
= 905 MPa (130,700 psi)
16.20 In this problem, for an aligned carbon fiber-epoxy matrix composite, we are given the desired
longitudinal tensile strength (500 MPa), the average fiber diameter (1.0 x 10-2 mm), the average
fiber length (0.5 mm), the fiber fracture strength (4000 MPa), the fiber-matrix bond strength (25
MPa), and the matrix stress at composite failure (7.0 MPa); and we are asked to compute the
421
volume fraction of fibers that is required. It is first necessary to compute the value of the critical fiber
length using Equation (16.3). If the fiber length is much greater than lc, then we may determine Vf
using Equation (16.17), otherwise, use of either Equation (16.18) or Equation (16.19) is necessary.
Thus,
lc =
σ f∗ d
2τ c
(
(4000 MPa) 1.0 x 10
=
−2
mm
2(25 MPa)
)= 0.80 mm
Inasmuch as l &lt; lc (0.50 mm &lt; 0.80 mm), then use of Equation (16.19) is required. Therefore,
∗
σ cd'
=
500 MPa =
lτ c
d
(
' 1− V
Vf + σm
f
)
(0.5 x 10 −3 m)(25 MPa) (V ) +
0.01 x 10 −3 m
f
(
(7 MPa) 1 − Vf
)
Solving this expression for Vf leads to Vf = 0.397.
16.21 In this problem, for an aligned glass fiber-epoxy matrix composite, we are asked to compute the
longitudinal tensile strength given the following: the average fiber diameter (0.015 mm), the average
fiber length (2.0 mm), the volume fraction of fibers (0.25), the fiber fracture strength (3500 MPa), the
fiber-matrix bond strength (100 MPa), and the matrix stress at composite failure (5.5 MPa). It is first
necessary to compute the value of the critical fiber length using Equation (16.3). If the fiber length is
∗
using Equation (16.17), otherwise, use of either
much greater than lc, then we may determine σ cl
Equation (16.18) or (16.19) is necessary. Thus,
lc =
σ f∗ d
2τ c
=
(3500 MPa)(0.015 mm)
= 0.263 mm (0.010 in.)
2(100 MPa)
Inasmuch as l &gt; lc (2.0 mm &gt; 0.263 mm), but l is not much greater than lc, then use of Equation
(16.18) is necessary. Therefore,
(
⎛
⎞
∗
' 1− V
σ cd
= σ f∗ Vf ⎜ 1 − c ⎟ + σm
f
2l⎠
⎝
l
422
)
⎡
0.263 mm ⎤
= (3500 MPa)(0.25)⎢1 −
⎥ + (5.5 MPa)(1 − 0.25)
(2)(2.0 mm) ⎦
⎣
= 822 MPa (117,800 psi)
16.22 (a) This portion of the problem calls for computation of values of the fiber efficiency parameter.
From Equation (16.20)
E cd = KEf Vf + E mVm
Solving this expression for K yields
K =
(
Ecd − Em 1 − Vf
E cd − EmVm
=
EV
EV
f f
)
f f
For glass fibers, E = 72.5 GPa (Table 16.4); using the data in Table 16.2, and taking an average
f
6
of the extreme Em values given, E = 2.29 GPa (0.333 x 10 psi). And, for V = 0.20
m
f
K =
5.93 GPa − (2.29 GPa)(1 − 0.2)
= 0.283
(72.5 GPa)(0.2)
K =
8.62 GPa − (2.29 GPa)(1 − 0.3)
= 0.323
(72.5 GPa)(0.3)
K =
11.6 GPa − (2.29 GPa)(1 − 0.4)
= 0.353
(72.5 GPa)(0.4)
For V = 0.3
f
And, for V = 0.4
f
(b) For 50 vol% fibers (V = 0.50), we must assume a value for K. Since K increases slightly with
f
V , let us assume that the increase in going from V = 0.4 to 0.5 is the same as from 0.3 to 0.4--that
f
f
is, by a value of 0.03. Therefore, let us assume a value for K of 0.383. Now, from Equation (16.20)
Ec = KE f Vf + EmVm
423
= (0.383)(72.5 GPa)(0.5) + (2.29 GPa)(0.5)
= 15.0 GPa (2.18 x 106 psi)
16.23 For discontinuous-oriented fiber-reinforced composites one desirable characteristic is that the
composite is relatively strong and stiff in one direction; a less desirable characteristic is that the
mechanical properties are anisotropic.
For discontinuous and random fiber-reinforced, one desirable characteristic is that the
properties are isotropic; a less desirable characteristic is there is no single high-strength direction.
16.24 (a) The four reasons why glass fibers are most commonly used for reinforcement are listed at the
beginning of Section 16.8 under &quot;Glass Fiber-Reinforced Polymer (GFRP) Composites.&quot;
(b) The surface perfection of glass fibers is important because surface flaws or cracks will act as
points of stress concentration, which will dramatically reduce the tensile strength of the material.
(c) Care must be taken not to rub or abrade the surface after the fibers are drawn. As a surface
protection, newly drawn fibers are coated with a protective surface film.
16.25 &quot;Graphite&quot; is crystalline carbon having the structure shown in Figure 12.17, whereas &quot;carbon&quot; will
consist of some noncrystalline material as well as areas of crystal misalignment.
16.26 (a) Reasons for the extensive use of fiberglass-reinforced composites are as follows: 1) glass
fibers are very inexpensive to produce; 2) these composites have relatively high specific strengths;
and 3) they are chemically inert in a wide variety of environments.
(b) Several limitations of these composites are: 1) care must be exercised in handling the fibers
inasmuch as they are susceptible to surface damage; 2) they lack the stiffness found in other
fibrous composites; and 3) they are limited as to maximum temperature use.
16.27 (a) A hybrid composite is one that is reinforced with two or more different fiber materials in a single
matrix.
(b) Two advantages of hybrid composites are: 1) better overall property combinations, and 2) failure
is not as catastrophic as with single-fiber composites.
16.28 (a) For a hybrid composite having all fibers aligned in the same direction
Ecl = Em Vm + Ef1Vf1 + E f2Vf2
424
in which the subscripts f1 and f2 refer to the two types of fibers.
(b) Now we are asked to compute the longitudinal elastic modulus for a glass- and aramid-fiber
hybrid composite. From Table 16.4, the elastic moduli of aramid and glass fibers are, respectively,
6
6
131 GPa (19 x 10 psi) and 72.5 GPa (10.5 x 10 psi). Thus, from the previous expression
Ecl = (2.5 GPa)(1.0 − 0.30 − 0.40) + (131 GPa)(0.30)
+ (72.5 GPa)(0.40)
= 69.1 GPa (10.0 x 106 psi)
16.29 This problem asks that we derive a generalized expression analogous to Equation (16.16) for the
transverse modulus of elasticity of an aligned hybrid composite consisting of two types of continuous
fibers. Let us use the subscripts f1 and f2 to denote the two fiber types, and m , c, and t as
subscripts for the matrix, composite, and transverse direction, respectively. For the isostress state,
the expressions analogous to Equations (16.12) and (16.13) are
σ c = σ m = σ f1 = σ f2
And
ε c = ε mVm + ε f1Vf1 + ε f2 Vf2
Since ε = σ/E, then
σ
σ
σ
σ
=
V +
V +
V
Em m
Ef1 f1
Ef2 f2
Ect
And
V
V
V
1
= m + f1 + f2
E
E
E
E
ct
m
f1
f2
V E E +V E E +V E E
1
f1 m f2
f2 m f1
= m f1 f2
E
E E E
ct
m f1 f2
And, finally
E ct =
E E E
m f1 f2
V E E
m f1 f2
+V E E
f1 m f2
425
+V E E
f2 m f1
16.30 Pultrusion, filament winding, and prepreg fabrication processes are described in Section 16.13.
For pultrusion, the advantages are: the process may be automated, production rates are
relatively high, a wide variety of shapes having constant cross-sections are possible, and very long
pieces may be produced. The chief disadvantage is that shapes are limited to those having a
constant cross-section.
For filament winding, the advantages are: the process may be automated, a variety of
winding patterns are possible, and a high degree of control over winding uniformity and orientation is
afforded. The chief disadvantage is that the variety of shapes is somewhat limited.
For prepreg production, the advantages are:
resin does not need to be added to the
prepreg, the lay-up arrangement relative to the orientation of individual plies is variable, and the layup process may be automated. The chief disadvantages of this technique are that final curing is
necessary after fabrication, and thermoset prepregs must be stored at subambient temperatures to
prevent complete curing.
16.31 Laminar composites are a series of sheets or panels, each of which has a preferred high-strength
direction. These sheets are stacked and then cemented together such that the orientation of the
high-strength direction varies from layer to layer.
These composites are constructed in order to have a relatively high strength in virtually all
directions within the plane of the laminate.
16.32
(a)
Sandwich panels consist of two outer face sheets of a high-strength material that are
separated by a layer of a less-dense and lower-strength core material.
(b) The prime reason for fabricating these composites is to produce structures having high in-plane
strengths, high shear rigidities, and low densities.
(c) The faces function so as to bear the majority of in-plane loading and also transverse bending
stresses. On the other hand, the core separates the faces and resists deformations perpendicular to
the faces.
Design Problems
16.D1 In order to solve this problem, we want to make longitudinal elastic modulus and tensile strength
computations assuming 50 vol% fibers for all three fiber materials, in order to see which meet the
6
stipulated criteria [i.e., a minimum elastic modulus of 50 GPa (7.3 x 10 psi), and a minimum tensile
426
strength of 1300 MPa (189,000 psi)]. Thus, it becomes necessary to use Equations (16.10b) and
∗ = 75 MPa.
(16.17) with V = 0.5 and V = 0.5, E = 3.1 GPa, and σ m
m
f
m
For glass, E = 72.5 GPa and σ f∗ = 3450 MPa. Therefore,
f
(
)
E cl = Em 1 − Vf + E f Vf
= (3.1 GPa)(1 − 0.5) + (72.5 GPa)(0.5) = 37.8 GPa (5.48 x 106 psi)
Since this is less than the specified minimum, glass is not an acceptable candidate.
For carbon (PAN standard-modulus), Ef = 230 GPa and σ f∗ = 4000 MPa (the average of the
extreme values in Table B.4), thus
E cl = (3.1 GPa)(0.5) + (230 GPa)(0.5) = 116.6 GPa
(16.9 x 10 6 psi)
which is greater than the specified minimum. In addition, from Equation (16.17)
(
)
∗
' 1 − V + σ∗ V
σ cl
= σm
f
f f
= (30 MPa)(0.5) + (4000 MPa)(0.5) = 2015 MPa (292, 200 psi)
which is also greater than the minimum. Thus, carbon (PAN standard-modulus) is a candidate.
For aramid, Ef = 131 GPa and σ f∗ = 3850 MPa (the average of the extreme values in Table
B.4), thus
E cl = (3.1 GPa)(0.5) + (131 GPa)(0.5) = 67.1 GPa (9.73 x 106 psi)
which value is greater than the minimum. Also, from Equation (16.17)
(
)
∗
' 1 − V + σ∗ V
σ cl
= σm
f
f f
= (50 MPa)(0.5) + (3850 MPa)(0.5) = 1950 MPa (283,600 psi)
427
which is also greater than the minimum strength value. Therefore, of the three fiber materials, both
the carbon (PAN standard-modulus) and the aramid meet both minimum criteria.
16.D2 This problem asks us to determine whether or not it is possible to produce a continuous and
oriented carbon fiber-reinforced epoxy having a modulus of elasticity of at least 83 GPa in the
direction of fiber alignment, and a maximum specific gravity of 1.40. We will first calculate the
minimum volume fraction of fibers to give the stipulated elastic modulus, and then the maximum
volume fraction of fibers required to yield the maximum permissible specific gravity; if there is an
overlap of these two fiber volume fractions then such a composite is possible.
With regard to the elastic modulus, from Equation (16.10b)
(
)
(
)
E cl = Em 1 − Vf + E f Vf
83 GPa = (2.4 GPa) 1 − Vf + (260 GPa)(Vf )
Solving for V yields V = 0.31. Therefore, V &gt; 0.31 to give the minimum desired elastic modulus.
f
f
f
Now, upon consideration of the specific gravity, ρ, we employ a modified form of Equation
(16.10b) as
(
)
(
)
ρ c = ρm 1 − Vf + ρf Vf
()
1.40 = 1.25 1 − Vf + 1.80 Vf
And, solving for V from this expression gives V = 0.27. Therefore, it is necessary for V &lt; 0.27 in
f
f
f
order to have a composite specific gravity less than 1.40.
Hence, such a composite is not possible since there is no overlap of the fiber volume
fractions (i.e., 0.31 &lt; V &lt; 0.27) as computed using the two stipulated criteria.
f
16.D3 This problem asks us to determine whether or not it is possible to produce a continuous and
oriented glass fiber-reinforced polyester having a tensile strength of at least 1250 MPa in the
longitudinal direction, and a maximum specific gravity of 1.80. We will first calculate the minimum
volume fraction of fibers to give the stipulated tensile strength, and then the maximum volume
fraction of fibers possible to yield the maximum permissible specific gravity; if there is an overlap of
these two fiber volume fractions then such a composite is possible.
With regard to tensile strength, from Equation (16.17)
428
(
)
(
) + (3500 MPa)(Vf)
∗
' 1 − V + σ∗ V
σ cl
= σm
f
f f
1250 MPa = (20 MPa) 1 − Vf
Solving for V yields V = 0.353. Therefore, V &gt; 0.353 to give the minimum desired tensile
f
f
f
strength.
Now, upon consideration of the specific gravity, ρ, we employ the following modified form of
Equation (16.10b) as
(
)
(
)
ρ c = ρm 1 − Vf + ρf Vf
1.80 = 1.35 1 − Vf + 2.50(Vf )
And, solving for V from this expression gives V = 0.391. Therefore, it is necessary for V &lt; 0.391
f
f
f
in order to have a composite specific gravity less than 1.80.
Hence, such a composite is possible if 0.353 &lt;Vf &lt; 0.391.
16.D4 In this problem, for an aligned and discontinuous glass fiber-epoxy matrix composite having a
longitudinal tensile strength of 1200 MPa, we are asked to compute the required fiber fracture
strength, given the following: the average fiber diameter (0.015 mm), the average fiber length (5.0
mm), the volume fraction of fibers (0.35), the fiber-matrix bond strength (80 MPa), and the matrix
stress at fiber failure (6.55 MPa).
To begin, since the value of σ f∗ is unknown, calculation of the value of lc in Equation (16.3)
is not possible, and, therefore, we are not able to decide which of Equations (16.18) and (16.19) to
use. Thus, it is necessary to substitute for lc in Equation (16.3) into Equation (16.18), solve for the
value of σ f∗ , then, using this value, solve for lc from Equation (16.3). If l &gt; lc, we use Equation
(16.18), otherwise Equation (16.19) must be used. Note: the σ f∗ parameters in Equations (16.18)
and (16.3) are the same. Realizing this, and substituting for lc in Equation (16.3) into Equation
⎤
⎡
σ∗d
f
⎥ + σ' 1 − V
⎢
σ cd = σ f Vf 1 −
m
f
4τ l⎥
⎢
c⎦
⎣
∗
(
∗
429
)
= σ f∗ Vf −
σ ∗f 2 Vf d
' − σ' V
+ σm
m f
4τ l
c
This expression is a quadratic equation in which σ f∗ is the unknown. Rearrangement into a more
⎡Vd⎤
σ f∗2 ⎢ f ⎥ − σ f∗ (Vf ) +
⎢⎣4τ c l ⎥⎦
(
)
⎡ ∗
⎤
'
⎢⎣σ cd − σm 1 − Vf ⎥⎦ = 0
Or
aσf∗ 2 + bσ ∗f + c = 0
In which
a =
Vd
f
4τ l
c
(
(0.35) 0.015 x 10
=
(
−3
) = 3.28 x 10-6 (MPa)-1 2.23 x 10−8 (psi)−1
[
]
)
m
(4)(80 MPa) 5 x 10−3 m
Furthermore,
b = − Vf = − 0.35
(
∗
' 1 − V
c = σcd
− σm
f
)
= 1200 MPa − (6.55 MPa)(1 − 0.35) = 1195.74 MPa
(174,383 psi)
Now solving the above quadratic equation for σ f∗ yields
σ f∗ =
− (− 0.35) &plusmn;
=
2
−b&plusmn;
[
b 2 − 4ac
2a
(− 0.35) − (4) 3.28 x 10
[
−6
(MPa)
]
(2) 3.28 x 10−6 (MPa)−1
430
](1195.74 MPa)
−1
0.3500 &plusmn; 0.3268
=
6.56 x 10 −6
⎡ 0.3500 &plusmn; 0.3270
⎤
MPa ⎢
psi⎥
⎢⎣ 4.46 x 10−8
⎥⎦
This yields the two possible roots as
σ f∗ (+) =
0.3500 + 0.3268
6.56 x 10 −6
σ f∗ (−) =
MPa = 103,200 MPa (15.2 x 106 psi)
0.3500 − 0.3268
6.56 x 10 −6
MPa = 3537 MPa (515,700 psi)
Upon consultation of the magnitudes of σ f∗ for various fibers and whiskers in Table 16.4, only
σ f∗ (-) is reasonable. Now, using this value, let us calculate the value of lc using Equation (16.3) in
order to ascertain if use of Equation (16.18) in the previous treatment was appropriate. Thus
lc =
σ f∗ d
2τ c
=
(3537 MPa)(0.015 mm)
= 0.33 mm (0.0131 in.)
(2)(80 MPa)
Since l &gt; lc (5.0 mm &gt; 0.33 mm), our choice of Equation (16.18) was indeed appropriate, and σ f∗ =
3537 MPa (515,700 psi).
16.D5 (a) This portion of the problem calls for the same volume fraction of fibers for the four fiber types
(i.e., Vf = 0.40); thus, the modulus of elasticity will vary according to Equation (16.24a) with cos θ =
cos (17.5&deg;) = 0.954. Hence
(
E cs = 0.954 E mVm + E f Vf
)
And, using data in Table 16.8, the value of Ecs may be determined for each fiber material; these are
tabulated in Table 16.D5a.
431
Table 16.D5a Composite Elastic Modulus for Each of Glass and Three Carbon Fiber Types for Vf = 0.40
______________________________________
Ecs
_____________________
Fiber Type
GPa
106 psi
_______________________________________
Glass
29.0
4.2
Carbon--standard modulus
89.1
12.9
Carbon--intermediate modulus
110
16.0
Carbon--high modulus
154
22.3
________________________________________
It now becomes necessary to determine, for each fiber type, the inside diameter di.
Rearrangement of Equation 16.23 leads to
1/4
⎡
4FL3 ⎤
4
⎥
d i = ⎢d o −
3πEΔy ⎥⎦
⎢⎣
The di values may be computed by substitution into this expression for E the Ecs data in Table
16.D5a and the following
F = 100 N
L = 0.75 m
Δy = 2.5 mm
do = 100 mm
These di data are tabulated in the second column of Table 16.D5b. No entry is included for glass.
The elastic modulus for glass fibers is so low that it is not possible to use them for a tube that meets
the stipulated criteria; mathematically, the term within brackets in the above equation for di is
negative, and no real root exists. Thus, only the three carbon types are candidate fiber materials.
432
Table 16.D5b Inside Tube Diameter, Total Volume, and Fiber, Matrix, and Total Costs for Three CarbonFiber Epoxy-Matrix Composites
___________________________________________________
Inside
Diameter
Fiber Type
(mm)
Total
Volume
(cm3)
Fiber
Cost
Matrix
Cost
Total
Cost
(\$)
(\$)
(\$)
___________________________________________________
Glass
-
-
-
-
-
Carbon--standard
modulus
66.6
3324
83.76
20.46
104.22
Carbon--intermediate
modulus
76.9
2407
121.31
14.82
136.13
Carbon--high modulus
85.5
1584
199.58
9.75
209.33
___________________________________________________
(b) Also included in Table 16.D5b is the total volume of material required for the tubular shaft for
each carbon fiber type; Equation (16.25) was utilized for these computations. Since Vf = 0.40, 40%
this volume is fiber and the other 60% is epoxy matrix. In the manner of Design Example 16.1, the
masses and costs of fiber and matrix materials were determined, as well as the total composite cost.
These data are also included in Table 16.D5b. Here it may be noted that the standard-carbon fiber
yields the least expensive composite, followed by the intermediate- and high-modulus materials.
16.D6 This problem is to be solved using the E-Z Solve software.
16.D7 Inasmuch as there are a number of different sports implements that employ composite materials,
no attempt will be made to provide a complete answer for this question. However, a list of this type
of sporting equipment would include skis and ski poles, fishing rods, vaulting poles, golf clubs,
hockey sticks, baseball and softball bats, surfboards and boats, oars and paddles, bicycle
components (frames, wheels, handlebars), canoes, and tennis and racquetball rackets.
16.D8 The primary reasons that the automotive industry has replaced metallic automobile components
with polymer and composite materials are: polymers/composites 1) have lower densities, and afford
higher fuel efficiencies;
2) may be produced at lower costs but with comparable mechanical
433
characteristics; 3) are in many environments more corrosion resistant; 4) reduce noise, and 5) are
thermally insulating and thus reduce the transference of heat.
These replacements are many and varied. Several are as follows:
Bumper fascia are molded from an elastomer-modified polypropylene.
Rocker arm covers are injection molded of a glass- and mineral-reinforced nylon 6,6
composite.
Torque converter reactors, water outlets, pulleys, and brake pistons, are made from phenolic
thermoset composites that are reinforced with glass fibers.
Air intake manifolds are made of a glass-reinforced nylon 6,6.
434
CHAPTER 17
PROBLEM SOLUTIONS
17.1 (a) Oxidation is the process by which an atom gives up an electron (or electrons) to become a
cation.
Reduction is the process by which an atom acquires an extra electron (or electrons) and
becomes an anion.
(b) Oxidation occurs at the anode; reduction at the cathode.
17.2 (a) This problem asks that we write possible oxidation and reduction half-reactions for magnesium
in various solutions.
(i) In HCl
Mg → Mg2+ + 2e- (oxidation)
2H + + 2e- → H2 (reduction)
(ii) In an HCl solution containing dissolved oxygen
Mg → Mg2+ + 2e- (oxidation)
4H + + O 2 + 4e - → 2H2O (reduction)
(iii) In an HCl solution containing dissolved oxygen and Fe
2+
Mg → Mg2+ + 2e- (oxidation)
4H + + O 2 + 4e - → 2H2O (reduction)
Fe2+ + 2e- → Fe (reduction)
435
ions
(b) The magnesium would probably oxidize most rapidly in the HCl solution containing dissolved
2+
oxygen and Fe
ions because there are two reduction reactions that will consume electrons from
the oxidation of magnesium.
17.3 Iron would not corrode in water of high purity because all of the reduction reactions, Equations
+
n+
(17.3) through (17.7), depend on the presence of some impurity substance such as H or M ions
or dissolved oxygen.
17.4 (a) The Faraday constant is just the product of the charge per electron and Avogadro's number;
that is
(
F = eN A = 1.602 x 10
-19
)(
23
C/electron 6.023 x 10
)
electrons/mol
= 96,488 C/mol
(b) At 25&deg;C (298 K),
RT
(8.31 J / mol - K)(298 K)
ln(x) =
(2.303) log(x)
nF
(n)(96,500 C / mol)
=
0.0592
log (x)
n
This gives units in volts since a volt is a J/C.
17.5 (a) We are asked to compute the voltage of a nonstandard Cd-Fe electrochemical cell. Since iron
is lower in the emf series (Table 17.1), we begin by assuming that iron is oxidized and cadmium is
reduced, as
2+
Fe + Cd
→ Fe
2+
+ Cd
and
o
o
ΔV = (VCd
− VFe
) −
0.0592
[Fe2+ ]
log
2
[Cd2 + ]
= [− 0.403 V − (− 0.440 V)] −
436
⎡ 0.40 ⎤
0.0592
log ⎢
⎥
2
⎢⎣ 2 x 10−3 ⎥⎦
= -0.031 V
(b) Since this ΔV is negative, the spontaneous cell direction is just the reverse of that above, or
Fe
17.6
2+
+ Cd → Fe + Cd
2+
2+
This problem calls for us to determine whether or not a voltage is generated in a Zn/Zn
2+
concentration cell, and, if so, its magnitude. Let us label the Zn cell having a 1.0 M Zn solution as
cell 1, and the other as cell 2. Furthermore, assume that oxidation occurs within cell 2, wherein
-2
2+
Zn 2 = 10 M. Hence,
+
2+
Zn 2 + Zn2
1 → Zn2 + Zn1
and
[ 2+ ]

Zn 2
0.0592
ΔV = −
log
2
Zn 2+
= −
⎡10−2 ⎤
0.0592
⎥ = + 0.0592 V
log ⎢
2
⎣⎢ 1.0 ⎥⎦
Therefore, a voltage of 0.0592 V is generated when oxidation occurs in the cell having the Zn
-2
concentration of 10 M.
2+
2+
17.7 We are asked to calculate the concentration of Pb
ions in a copper-lead electrochemical cell.
The electrochemical reaction that occurs within this cell is just
Pb + Cu
2+
→ Pb
2+
+ Cu
2+
while ΔV = 0.507 V and [Cu ] = 0.6 M. Thus, Equation (17.20) is written in the form
(o
o
)
ΔV = VCu − VPb −
2+
Solving this expression for [Pb ] gives
437
0.0592
[Pb2 + ]
log
2
[Cu2+ ]
2+
[Pb
2+
] = [Cu
(
o
o
⎡
− VPb
ΔV − VCu
⎢
] exp − ⎢(2.303 )
0.0296
⎢⎣
)⎤⎥
⎥
⎦⎥
o
o
The standard potentials from Table 17.1 are VCu
= +0.340 V and VPb
= -0.126 V. Therefore,
2+
[Pb
0.507 V − (0.340 V + 0.126 V) ⎤
⎡
] = (0.6 M) exp − ⎢(2.303 )
⎥⎦
0.0296
⎣
= 2.5 x 10
-2
M
17.8 This problem asks for us to calculate the temperature for a zinc-lead electrochemical cell when the
potential between the Zn and Pb electrodes is +0.568 V. On the basis of their relative positions in
the standard emf series (Table 17.1), assume that Zn is oxidized and Pb is reduced. Thus, the
electrochemical reaction that occurs within this cell is just
2+
Pb
+ Zn → Pb + Zn
2+
Thus, Equation (17.20) is written in the form
(o
o
ΔV = VPb − VZn
)−
RT [Zn 2+ ]
ln
nF [Pb 2+ ]
Solving this expression for T gives
⎡
o
o
⎢
nF ⎢ ΔV − VPb − VZn
T = −
R ⎢
[Zn2 + ]
⎢
ln
⎢⎣
[Pb 2+ ]
(
⎤
⎥
⎥
⎥
⎥
⎦⎥
)
o
o
= -0.126 V. Therefore,
The standard potentials from Table 17.1 are VZn
= -0.763 V and VPb
⎡
⎤
⎢
⎥
(2)(96,500 C / mol) ⎢ 0.568 V − (−0.126 V + 0.763 V) ⎥
T =−
⎢
⎥
8.31 J/ mol - K ⎢
⎛ 10−2 M ⎞
⎥
ln ⎜⎜
⎟⎟
⎢
⎥
−4
⎝ 10 M ⎠
⎣
⎦
438
= 348 K = 75&deg;C
17.9 We are asked to modify Equation (17.19) for the case when metals M and M are alloys. In this
1
2
case, the equation becomes
(
)
ΔV = V2o − V1o −
n+
RT [M1 ][M2 ]
ln
nF [Mn+ ][M ]
2
1
where [M ] and [M ] are the concentrations of metals M and M in their respective alloys.
1
2
1
2
17.10 This problem asks, for several pairs of alloys that are immersed in seawater, to predict whether or
not corrosion is possible, and if it is possible, to note which alloy will corrode. In order to make these
predictions it is necessary to use the galvanic series, Table 17.2. If both of the alloys in the pair
reside within the same set of brackets in this table, then galvanic corrosion is unlikely. However, if
the two alloys do not reside within the same set of brackets, then that alloy appearing lower in the
table will experience corrosion.
(a) For the aluminum-magnesium couple, corrosion is possible, and magnesium will corrode.
(b) For the zinc-low carbon steel couple, corrosion is possible, and zinc will corrode.
(c) For the brass-monel couple, corrosion is unlikely inasmuch as both alloys appear within the
same set of brackets.
(d) For the titanium-304 stainless steel pair, the stainless steel will corrode, inasmuch as it is below
titanium in both its active and passive states.
(e) For the cast iron-316 stainless steel couple, the cast iron will corrode since it is below stainless
steel in both active and passive states.
17.11 (a) The following metals and alloys may be used to galvanically protect 304 stainless steel in the
active state: cast iron, iron, steel, aluminum alloys, cadmium, commercially pure aluminum, zinc,
magnesium, and magnesium alloys.
(b) Zinc and magnesium may be used to protect a copper-aluminum galvanic couple.
17.12 This problem is just an exercise in unit conversions. The parameter K in Equation (17.23) must
convert the units of W, ρ, A, and t, into the unit scheme for the CPR.
For CPR in mpy (mil/yr)
439
K =
W(mg)(1 g / 1000 mg)
3
⎛ g ⎞ ⎛ 2.54 cm ⎞ ⎡
⎛ 1 in. ⎞
⎛ 1 day ⎞ ⎛ 1 yr ⎞
ρ⎜
⎟ ⎣A (in.2 )⎤⎦ ⎜
⎟ ⎜⎝
⎟ [t(h)] ⎜ 24 h ⎟ ⎜ 365 days ⎟
3
in.
1000
mil
⎠
⎝ cm ⎠
⎝
⎠
⎝
⎠⎝
⎠
= 534.6
For CPR in mm/yr
K =
W(mg)(1 g / 1000 mg)
3
⎛ g ⎞ ⎛ 1 cm ⎞ ⎡
2 ⎤ ⎛ 10 mm ⎞
ρ⎜
⎟
⎟⎜
⎟ ⎣A(cm )⎦ ⎜
3
⎝ cm ⎠
10
mm
⎝ cm ⎠ ⎝
⎠
2
⎛ 1 day ⎞ ⎛ 1 yr ⎞
⎟⎜
⎟
⎝ 24 h ⎠ ⎝ 365 days⎠
[t(h)]⎜
= 87.6
17.13 This problem calls for us to compute the time of submersion of a steel piece. In order to solve this
problem, we must first rearrange Equation (17.23), as
t =
KW
ρA (CPR)
Thus,
6
(
)
(7.9 g / cm3 )(10 in.2 )(200 mpy)
(534 ) 2.6 x 10 mg
t =
= 8.8 x 104 h = 10 yr
17.14 This problem asks for us to calculate the CPR in both mpy and mm/yr for a thick steel sheet of
area 100 in.2 which experiences a weight loss of 485 g after one year. Employment of Equation
CPR =
KW
ρA t
(
3
(87.6)(485 g) 10 mg / g
=
)
(7.9 g / cm 3 )(100 in.2 )(2.54 cm / in.)2 (24 h / day)(365 day / yr)(1 yr)
= 0.952 mm/yr
440
Also
(
3
(534)(485 g) 10 mg / g
CPR =
)
(7.9 g / cm3 )(100 in.2 )(24 h / day)(365 day / yr)(1 yr)
= 37.4 mpy
17.15 (a) We are to demonstrate that the CPR is related to the corrosion current density, i, in A/cm2
through the expression
CPR =
KAi
nρ
in which K is a constant, A is the atomic weight, n is the number of electrons ionized per metal atom,
and ρ is the density of the metal. Possibly the best way to make this demonstration is by using a unit
dimensional analysis. The corrosion rate, r, in Equation (17.24) has the units (SI)
r =
i
C / m2 - s
mol
=
=
(unitless)(C / mol)
nF
m2 - s
The units of CPR in Equation (17.23) are length/time, or in the SI scheme, m/s. In order to convert
the above expression to the units of m/s it is necessary to multiply r by the atomic weight A and
divide by the density ρ as
(mol / m2 - s)(g / mol)
rA
=
= m/s
ρ
g/ m3
Thus, the CPR is proportional to r, and substituting for r from Equation (17.24) into the above
CPR = K&quot;r =
K' A i
nFρ
in which K' and K &quot; are constants which will give the appropriate units for CPR. Also, since F is also
a constant, this expression takes the form
441
CPR =
KAi
nρ
in which K = K'/F.
(b) Now we will calculate the value of K in order to give the CPR in mpy for i in μA/cm2 (10-6
A/cm2). It should be noted that the units of A (amperes) are C/s. Substitution of the units normally
used into the former CPR expression above leads to
CPR = K'
= K'
Ai
nFρ
(g / mol)(C / s- cm 2 )
(unitless)(C/ mol)(g / cm3 )
= cm/s
Since we want the CPR in mpy and i is given in μA/cm2, and realizing that K = K'/F leads to
⎛
⎞ ⎛ 10 −6 C ⎞ ⎛ 1 in. ⎞ ⎛ 103 mil ⎞⎛ 3.1536 x 107
1
K = ⎜
⎟⎜
⎟⎜
⎟⎜
⎟⎜
yr
⎝ 96, 500 C/ mol⎠ ⎜⎝ μC ⎟⎠ ⎝ 2.54 cm ⎠ ⎜⎝ in. ⎟⎠⎜⎝
s⎞
⎟⎟
⎠
= 0.129
17.16 We are asked to compute the CPR in mpy for the corrosion of Fe for a corrosion current density of
8 x 10-5 A/cm2 (80 μA/cm2). From Problem 17.15, the value of K in Equation (17.35) is 0.129, and
therefore
CPR =
(
KAi
nρ
2
(0.129 )(55.85 g/ mol) 80 μA / cm
=
(
(2) 7.9 g / cm3
)
) = 36.5 mpy
17.17W (a) Activation polarization is the situation wherein a reaction rate is controlled by one step in a
series of steps that takes place at the slowest rate. For corrosion, activation polarization is possible
for both oxidation and reduction reactions. Concentration polarization occurs when a reaction rate is
limited by diffusion in a solution.
For corrosion, concentration polarization is possible only for
reduction reactions.
442
(b) Activation polarization is rate controlling when the reaction rate is low and/or the concentration of
active species in the liquid solution is high.
(c)
Concentration polarization is rate controlling when the reaction rate is high and/or the
concentration of active species in the liquid solution is low.
17.18W
(a)
The phenomenon of dynamic equilibrium is the state wherein oxidation and reduction
reactions are occurring at the same rate such that there is no net observable reaction.
(b) The exchange current density is just the current density which is related to both the rates of
oxidation and reduction (which are equal) according to Equation (17.24) for the dynamic equilibrium
state.
17.19W Concentration polarization is not normally rate controlling for oxidation reactions because there
will always be an unlimited supply of metal atoms at the corroding electrode interface.
17.20W (a) This portion of the problem asks that we compute the rate of oxidation for Ni given that both
the oxidation and reduction reactions are controlled by activation polarization, and also given the
polarization data for both nickel oxidation and hydrogen reduction. The first thing necessary is to
establish relationships of the form of Equation (17.1W) for the potentials of both oxidation and
reduction reactions. Next we will set these expressions equal to one another, and then solve for the
value of i which is really the corrosion current density, ic. Finally, the corrosion rate may be
calculated using Equation (17.24). The two potential expressions are as follows:
For hydrogen reduction
⎛
⎞
⎜ i ⎟
+
β
log
H
⎜i ⎟
(H + /H2 )
⎝ oH ⎠
VH = V
And for Ni oxidation
⎛
⎞
⎜ i ⎟
+
β
log
Ni
⎜i ⎟
(Ni/Ni2+ )
⎝ oNi ⎠
VNi = V
Setting VH = VNi and solving for log i (log ic) leads to
⎛
⎞
1
log ic = ⎜⎜
⎟⎟
⎝ βNi − βH ⎠
⎡
⎤
−V
⎢V +
2+ − βH logio + β Ni logio ⎥
(Ni/ Ni )
H
Ni ⎦
⎣ (H / H 2 )
443
{(
⎡
⎤⎡
1
−7
= ⎢
⎥ ⎢⎣0 − (− 0.25) − (−0.10) log 6 x 10
0.12
−
(−0.10)
⎣
⎦
)}+ (0.12) {log (10−8 )}⎤⎥⎦
= -6.055
Or
ic = 10-6.055 = 8.81 x 10 -7 A/cm 2
And from Equation (17.24)
r =
−7
=
ic
nF
2
8.81 x 10 C / s - cm
= 4.56 x 10 -12 mol/cm 2 - s
(2)(96, 500 C / mol)
(b) Now it becomes necessary to compute the value of the corrosion potential, Vc. This is possible
by using either of the above equations for VH or VNi and substituting for i the value determined
above for ic. Thus
⎛ i ⎞
⎜ c ⎟
+
β
log
H
⎜i ⎟
(H +/H 2 )
⎝ oH ⎠
Vc = V
⎛ 8.81 x 10−7 A / cm2 ⎞
⎟ = − 0.0167 V
= 0 + (−0.10 V) log ⎜⎜
−7
2 ⎟
⎝ 6 x 10 A / cm ⎠
17.21W (a) This portion of the problem asks that we compute the rate of oxidation for a divalent metal M
given that both the oxidation and reduction reactions are controlled by activation polarization, and
also given the polarization data for both M oxidation and hydrogen reduction.
The first thing
necessary is to establish relationships of the form of Equation (17.1W) for the potentials of both
oxidation and reduction reactions. Next we will set these expressions equal to one another, and
then solve for the value of i which is really the corrosion current density, ic. Finally, the corrosion
rate may be calculated using Equation (17.24). The two potential expressions are as follows:
For hydrogen reduction
444
⎛
⎞
⎜ i ⎟
+
β
log
H
⎜i ⎟
(H + /H2 )
⎝ oH ⎠
VH = V
And for M oxidation
⎛
⎞
⎜ i ⎟
+
β
log
M
⎜i ⎟
(M/M 2+ )
⎝ oM ⎠
VM = V
Setting VH = VM and solving for log i (log ic) leads to
⎛
⎞
1
log ic = ⎜⎜
⎟⎟
⎝ βM − βH ⎠
⎡
⎤
−V
⎢V +
2 + − β H logio + βM logio ⎥
(M /M )
H
M⎦
⎣ (H / H 2 )
{ ( )}+ (0.10){log (10 )}⎤⎥⎦
⎡
⎤⎡
1
−10
= ⎢
⎥ ⎢0 − (− 0.90) − ( −0.15) log 10
⎣ 0.10 − ( −0.15) ⎦ ⎣
−12
= -7.20
Or
ic = 10
-7.20
= 6.31 x 10
-8
A/cm
2
And from Equation (17.24)
r =
=
ic
nF
6.31 x 10−8 C / s - cm2
-13
2
= 3.27 x 10
mol/cm - s
(2)(96, 500 C / mol)
(b) Now it becomes necessary to compute the value of the corrosion potential, Vc. This is possible
by using either of the above equations for VH or VM and substituting for i the value determined
above for ic. Thus
⎛ i ⎞
Vc = V +
+ βH log ⎜ c ⎟
⎜i ⎟
(H /H 2 )
⎝ oH ⎠
445
⎛ 6.31 x 10−8 A / cm2 ⎞
= 0 + (−0.15 V) log ⎜⎜
⎟⎟ = −0.420 V
−10 A / cm 2
⎝ 10
⎠
17.22W This problem asks that we make a schematic plot of corrosion rate versus solution velocity. The
reduction reaction is controlled by combined activation-concentration polarization for which the
overvoltage versus logarithm current density is shown in Figure 17.21. The oxidation of the metal is
controlled by activation polarization, such that the electrode kinetic behavior for the combined
reactions would appear schematically as shown below.
Thus, the plot of corrosion rate versus solution velocity would be as
446
The corrosion rate initially increases with increasing solution velocity (for velocities v1, v2, and v3),
corresponding to intersections in the concentration polarization regions for the reduction reaction.
However, for the higher solution velocities (v4 and v5), the metal oxidation line intersects the
reduction reaction curve in the linear activation polarization region, and, thus, the reaction becomes
independent of solution velocity.
17.23 Passivity is the loss of chemical reactivity, under particular environmental conditions, of normally
active metals and alloys. Stainless steels and aluminum alloys often passivate.
17.24 The chromium in stainless steels causes a very thin and highly adherent surface coating to form
over the surface of the alloy, which protects it from further corrosion. For plain carbon steels, rust,
17.25 For each of the forms of corrosion, the conditions under which it occurs, and measures that may
be taken to prevent or control it are outlined in Section 17.7.
17.26
Two beneficial uses of galvanic corrosion are corrosion prevention by means of cathodic
protection, and the dry-cell battery.
17.27 Cold-worked metals are more susceptible to corrosion than noncold-worked metals because of the
increased dislocation density for the latter. A region in the vicinity of a dislocation that intersects the
surface is at a higher energy state, and, therefore, is more readily attacked by a corrosive solution.
17.28 For a small anode-to-cathode area ratio, the corrosion rate will be higher than for a large ratio.
The reason for this is that for some given current flow associated with the corrosion reaction, for a
small area ratio the current density at the anode will be greater than for a large ratio. The corrosion
rate is proportional to the current density according to Equation (17.24).
17.29 For a concentration cell, corrosion occurs at that region having the lower concentration. In order to
explain this phenomenon let us consider an electrochemical cell consisting of two divalent metal M
electrodes each of which is immersed in a solution containing a different concentration of its M2+
ion; let us designate the low and high concentrations of M2+ as [ M2L + ] and [ M2H+ ], respectively.
Now assuming that reduction and oxidation reactions occur in the high- and low-concentration
solutions, respectively, let us determine the cell potential in terms of the two [M2+]'s; if this potential
447
is positive then we have correctly chosen the solutions in which the reduction and oxidation reactions
occur.
Thus, the two half-reactions in the form of Equations (17.16) are
M2+
H + 2e → M
o
VM
M → M2+
L + 2e
o
− VM
Whereas the overall cell reaction is
2+
M2+
H + M → M + ML
From Equation (17.19), this yields a cell potential of
RT
o
o
ln
ΔV = VM − VM −
nF
=−
RT
ln
nF
⎛ [M2 + ]⎞
⎜ L ⎟
⎜ [M2 + ]⎟
⎝ H ⎠
⎛ [M2 + ]⎞
⎜ L ⎟
⎜ [M2 + ]⎟
⎝ H ⎠
Inasmuch as M2L + &lt; M2H+ then the natural logarithm of the [M
2+
] ratio is negative, which yields a
positive value for ΔV. This means that the electrochemical reaction is spontaneous as written, or
that oxidation occurs at the electrode having the lower M2+ concentration.
17.30 Equation (17.23) is not equally valid for uniform corrosion and pitting. The reason for this is that,
with pitting, the corrosion attack is very localized, and a pit may penetrate the entire thickness of a
piece (leading to failure) with very little material loss and a very small corrosion penetration rate.
With uniform corrosion, the corrosion penetration rate accurately represents the extent of corrosion
damage.
17.31
(a)
Inhibitors are substances that, when added to a corrosive environment in relatively low
concentrations, decrease the environment's corrosiveness.
(b) Possible mechanisms that account for the effectiveness of inhibitors are: 1) elimination of a
chemically active species in the solution; 2) attachment of inhibitor molecules to the corroding
448
surface so as to interfere with either the oxidation or reduction reaction; and 3) the formation of a
very thin and protective coating on the corroding surface.
17.32 Descriptions of the two techniques used for galvanic protection are as follows:
1) A sacrificial anode is electrically coupled to the metal piece to be protected, which anode is also
situated in the corrosion environment. The sacrificial anode is a metal or alloy that is chemically
more reactive in the particular environment. It (the anode) preferentially oxidizes, and, upon giving
up electrons to the other metal, protects it from electrochemical corrosion.
2) An impressed current from an external dc power source provides excess electrons to the
metallic structure to be protected.
17.33 Tin offers galvanic protection to the steel in tin cans even though it (tin) is electrochemically less
active than steel from the galvanic series. The reason for this is that the galvanic series represents
the reactivities of metals and alloys in seawater; however, for the food solutions that are contained
within the cans, tin is the more active metal.
17.34 For this problem we are given, for three metals, their densities, oxide chemical formulas, and oxide
densities, and are asked to compute the Pilling-Bedworth ratios, and then to specify whether or not
the oxide scales that form will be protective. The general form of the equation used to calculate this
ratio is Equation (17.30) [or Equation (17.29)]. For magnesium, oxidation occurs by the reaction
Mg +
1
O → MgO
2 2
and therefore, from Equation (17.29)
P - B ratio =
A MgO ρMg
A
ρ
Mg MgO
3
(
)= 0.81
(24.31 g / mol) (3.58 g / cm3 )
(40.31 g / mol) 1.74 g / cm
=
Thus, this would probably be a nonprotective oxide film since the P-B ratio is less than unity; to be
protective, this ratio should be between one and two.
The oxidation reaction for V is just
449
2V +
5
O → V2 O5
2 2
and the P-B ratio is [Equation (17.30)]
P - B ratio =
AV O ρ V
2 5
(2)A ρ
V V2 O5
3
(
) = 3.25
3
(2)(50.94 g / mol) (3.36 g / cm )
(181.88 g / mol) 6.11 g/ cm
=
Hence, the film would be nonprotective since the ratio does not lie between one and two.
Now for Zn, the reaction for its oxidation is analogous to that for Mg above. Therefore,
P - B ratio =
A ZnOρ Zn
A Zn ρZnO
3
(
) = 1.58
(65.39 g/ mol) (5.61 g / cm 3 )
(81.39 g / mol) 7.13 g / cm
=
Thus, the ZnO film would probably be protective since the ratio is between one and two.
17.35 Silver does not oxidize appreciably at room temperature and in air even though, according to Table
17.3, the oxide coating should be nonprotective because the oxidation of silver in air is not
thermodynamically favorable; therefore, the lack of a reaction is independent of whether or not a
protective scale forms.
17.36
For this problem we are given weight gain-time data for the oxidation of Ni at an elevated
temperature.
(a) We are first asked to determine whether the oxidation kinetics obey a parabolic, linear, or
logarithmic rate expression, which expressions are represented by Equations (17.31), (17.32), and
(17.33), respectively. One way to make this determination is by trial and error. Let us assume that
the parabolic relationship is valid; that is from Equation (17.31)
W 2 = K 1t + K 2
450
which means that we may establish three simultaneous equations using the three sets of given W
and t values, then using two combinations of two pairs of equations, solve for K1 and K2; if K1 and
K2 have the same values for both solutions, then the kinetics are parabolic. If the values are not
identical then the other kinetic relationships need to be explored. Thus, the three equations are
(0.527) 2 = 0.278 = 10K1 + K 2
(0.857) 2 = 0.734 = 30K1 + K 2
(1.526) 2 = 2.329 = 100K 1 + K 2
From the first two equations K1 = 0.0228 and K2 = 0.050; these same two values are obtained
using the last two equations. Hence, the oxidation rate law is parabolic.
(b) Since a parabolic relationship is valid, this portion of the problem calls for us to determine W after
a total time of 600 min. Again, using Equation (17.31) and the values of K1 and K2
W 2 = K 1t + K 2
= (0.0228)(600 min) + 0.05 = 13.37
Or W =
13.73 = 3.70 mg/cm2.
16.37 For this problem we are given weight gain-time data for the oxidation of some metal at an elevated
temperature.
(a) We are first asked to determine whether the oxidation kinetics obey a linear, parabolic, or
logarithmic rate expression, which expressions are described by Equations (17.32), (17.31), and
(17.33), respectively. One way to make this determination is by trial and error. Let us assume that
the rate expression is parabolic, that is from Equation (17.31)
W 2 = K 1t + K 2
which means that we may establish three simultaneous equations using the three sets of given W
and t values, then using two combinations of two pairs of equations, solve for K1 and K2; if K1 and
K2 have the same values for both solutions, then the rate law is parabolic. If the values are not the
same then the other kinetic relationships need to be explored. Thus, the three equations are
2
= 37.95 = 100K1 + K 2
2
= 73.79 = 250K 1 + K 2
(6.16)
(8.59)
451
(12.72)2 = 161.8 = 1000K 1 + K 2
From the first two equations K1 = 0.238 and K2 = 14.2; while from the second and third equations
K1 = 0.117 and K2 = 44.5. Thus, a parabolic rate expression is not obeyed by this reaction.
Let us now investigate linear kinetics in the same manner, using Equation (17.32), W = K3t.
The three equations are thus
6.16 = 100 K 3
8.59 = 250 K 3
12.72 = 1000 K 3
And the three K3 values may be computed (one for each equation) which are 6.16 x 10-2, 3.44 x
10-2, and 1.272 x 10-2. Since these K3 values are all different, a linear rate law is not a possibility,
and, by process of elimination, a logarithmic expression is obeyed.
(b) In order to determine the value of W after 5000 min, it is first necessary that we solve for the K4,
K5, and K6 constants of Equation (17.33). One way this may be accomplished is to use the E-Z
Solve equation solver, with Equation (17.33) expressed in exponential form, as
K 5 + K 6 = 10
W/K 4
The following is entered into the workspace of E-Z Solve
K5 *t1 + K6 = 10^(W1/K4)
K5 *t2 + K6 = 10^(W2/K4)
K5 *t3 + K6 = 10^(W3/K4)
t1 = 100;
W1 = 6.16
t2 = 250;
W2 = 8.59
t3 = 1000;
W3 = 12.72
452
After choosing the calculator icon in the menu bar, and clicking on the &quot;Solve&quot; button in the window
that appears (with &quot;1&quot; as the guess value for all three of K4, K5, and K6), the following values for the
three constants are displayed in the data grid near the bottom of the window:
K4 = 7.305
K5 = 0.0535
K6 = 1.622
Now solving Equation (17.33) for W at a time of 5000 min
(
W = K 4 log K 5t + K 6
)
= 7.305 log [(0.0535)(5000 min) + 1.622 ]
= 17.75 mg/cm2
17.38 For this problem we are given weight gain-time data for the oxidation of some metal at an elevated
temperature.
(a) We are first asked to determine whether the oxidation kinetics obey a linear, parabolic, or
logarithmic rate expression, which expressions are described by Equations (17.32), (17.31), and
(17.33), respectively. One way to make this determination is by trial and error. Let us assume that
the rate expression is linear, that is from Equation (17.32)
W = K3t
which means that we may establish three simultaneous equations using the three sets of given W
and t values, then solve for K3 for each; if K3 is the same for all three cases, then the rate law is
linear. If the values are not the same then the other kinetic relationships need to be explored. Thus,
the three equations are
1.54 = 10K3
23.24 = 150K3
95.37 = 620K3
In all three instances the value of K3 is about equal to 0.154, which means the oxidation rate obeys
a linear expression.
453
(b) Now we are to calculate W after a time of 1200 min; thus
W = K3t = (0.154)(1200 min) = 184.80 mg/cm2
17.39 During the swelling and dissolution of polymeric materials, the solute molecules diffuse to and
occupy positions among the polymer macromolecules, and thereby force the latter apart. Increasing
both the degrees of crosslinking and crystallinity will enhance a polymer's resistance to these types
of degradation since there will be a greater degree of intermolecular bonding between adjacent
chains; this restricts the number of solute molecules that can fit into these locations.
For linear polymers, the intermolecular bonds are
secondary ones (van der Waals and/or hydrogen), and relatively weak in comparison to the strong
covalent bonds associated with the crosslinks.
17.40 (a) Three differences between the corrosion of metals and the corrosion of ceramics are:
1) Ceramic materials are more corrosion resistant than metals in most environments.
2) Corrosion of ceramic materials is normally just a chemical dissolution process, whereas for
metals it is usually electrochemical.
3) Ceramics are more corrosion resistant at elevated temperatures.
(b) Three differences between the corrosion of metals and the degradation of polymers are:
1)
Degradation of polymers is ordinarily physiochemical, whereas for metals, corrosion is
electrochemical.
2) Degradation mechanisms for polymers are more complex than the corrosion mechanisms for
metals.
3) More types of degradation are possible for polymers--e.g., dissolution, swelling, and bond
rupture (by means of radiation, heat, and chemical reactions).
Design Problems
17.D1 Possible methods that may be used to reduce corrosion of the heat exchanger by the brine are as
follows:
1) Reduce the temperature of the brine; normally, the rate of a corrosion reaction increases with
increasing temperature.
2) Change the composition of the brine; the corrosion rate is often quite dependent on the
composition of the corrosion environment.
454
3) Remove as much dissolved oxygen as possible. Under some circumstances, the dissolved
oxygen may form bubbles, which can lead to erosion-corrosion damage.
4) Minimize the number of bends and/or changes in pipe contours in order to minimize erosioncorrosion.
6) Avoid connections between different metal alloys.
17.D2 This question asks that we suggest appropriate materials, and if necessary, recommend corrosion
prevention measures that should be taken for several specific applications. These are as follows:
(a) Laboratory bottles to contain relatively dilute solutions of nitric acid. Probably the best material
for this application would be polytetrafluoroethylene (PTFE). The reasons for this are: 1) it is
flexible and will not easily break if dropped; and 2) PTFE is resistant to this type of acid, as noted in
Table 17.4.
(b)
Barrels to contain benzene.
Polyethylene terephthalate (PET) would be suited for this
application, since it is resistant to degradation by benzene (Table 17.4), and is less expensive than
the other two materials listed in Table 17.4 (see Appendix C).
(c) Pipe to transport hot alkaline (basic) solutions. The best material for this application would
probably be a nickel alloy (Section 11.3). Polymeric materials listed in Table 17.4 would not be
suitable inasmuch as the solutions are hot.
(d) Underground tanks to store large quantities of high purity water. The outside of the tanks should
probably be some type of low-carbon steel that is cathodically protected (Sections 17.8 and 17.9).
The
inside
of
this
steel
shell
should
be
coated
with
an
inert
polymeric
material;
polytetrafluoroethylene or some other fluorocarbon would probably be the material of choice (Table
17.4).
(e) Architectural trim for high-rise buildings. The most likely candidate for this application would
probably be an aluminum alloy. Aluminum and its alloys are relatively corrosion resistant in normal
atmospheres (Section 17.8), retains their lustrous appearance, and are relatively inexpensive
(Appendix C).
17.D3 (a) Advantages of delivering drugs into the body using transdermal patches (as opposed to oral
administration) are: 1) Drugs that are taken orally must pass through the digestive system and,
consequently, may cause digestive discomfort.
2)
Orally delivered drugs will ultimately pass
through the liver which function is to filter out of the blood unnatural substances, including some
drugs; thus, drug concentrations in the blood are diluted. 3) It is much easier to maintain a constant
level of delivery over relatively long time periods using transdermal patches.
455
(b) In order for transdermal delivery, the skin must be permeable to the drug, or delivery agents
must be available that can carry the drug through the skin.
(c) Characteristics that are required for transdermal patch materials are the following: they must be
flexible; they must adhere to the skin; they must not cause skin irritation; they must be permeable
to the drug; and they must not interact with the drug over long storage periods.
17.D4
Each student or group of students is to submit their own report on a corrosion problem
investigation that was conducted.
456
CHAPTER 18
ELECTRICAL PROPERTIES
PROBLEM SOLUTIONS
18.1 This problem calls for us to compute the electrical conductivity and resistance of a silicon specimen.
(a) We use Equations (18.3) and (18.4) for the conductivity, as
σ=
1
Il
=
=
ρ VA
(
−3
(0.1 A) 38 x 10
=
Il
⎛ d⎞
Vπ ⎜ ⎟
⎝ 2⎠
)
m
−3
⎛ 5.1 x 10
(12.5 V)(π) ⎜
⎜
2
⎝
m⎞
⎟⎟
⎠
2
2
= 14.9 (Ω - m) -1
(b) The resistance, R, may be computed using Equations (18.2) and (18.4), as
R=
=
51 x 10
−3
l
σA
m
⎛ 5.1 x 10−3 m ⎞
14.9 (Ω − m)−1 (π) ⎜
⎟⎟
⎜
2
⎝
⎠
[
]
2
= 166.9 Ω
18.2 For this problem, given that an aluminum wire 10 m long must experience a voltage drop of less
than 1 V when a current of 5 A passes through it, we are to compute the minimum diameter of the
wire. Combining Equations (18.3) and (18.4) and solving for the cross-sectional area A leads to
A=
Il
Vσ
⎛ d⎞
From Table 18.1, for aluminum σ = 3.8 x 107 (Ω-m)-1. Furthermore, inasmuch as A = π ⎜ ⎟
⎝ 2⎠
cylindrical wire, then
457
2
for a
⎛ d⎞
π⎜ ⎟
⎝ 2⎠
2
=
Il
Vσ
or
4Il
πVσ
d=
=
(4)(5 A)(10 m)
[
]
(π)(1 V) 3.8 x 107 (Ω − m) −1
= 1.3 x 10-3 m = 1.3 mm
18.3 This problem asks that we compute, for a plain carbon steel wire 3 mm in diameter, the maximum
length such that the resistance will not exceed 20 Ω. From Table 18.1, for a plain carbon steel, σ =
0.6 x 107 (Ω-m)-1. If d is the diameter then, combining Equations (18.2) and (18.4) leads to
⎛ d⎞
l = RσA = Rσπ ⎜ ⎟
⎝ 2⎠
[
7
= (20 Ω) 0.6 x 10 (Ω − m)
⎛ 3 x 10−3 m ⎞
(π) ⎜⎜
⎟⎟
2
⎝
⎠
]
−1
2
2
= 848 m
18.4 Let us demonstrate that, by appropriate substitution and algebraic manipulation, Equation (18.5)
may be made to take the form of Equation (18.1). Now, Equation (18.5) is just
J = σE
But, by definition, J is just the current density, the current per unit cross-sectional area, or J = I/A.
Also, the electric field is defined by E = V/l. And, substituting these expressions into Equation (18.5)
I
V
=σ
l
A
But, from Equations (18.2) and (18.4)
458
σ=
l
RA
and
I ⎛ l ⎞
⎟
=⎜
A ⎝ RA⎠
⎛V⎞
⎜ ⎟
⎝ l⎠
Solving for V from this expression gives V = IR, which is just Equation (18.1).
18.5 (a) In order to compute the resistance of this copper wire it is necessary to employ Equations (18.2)
and (18.4). Solving for the resistance in terms of the conductivity,
R=
ρl
l
=
A
σA
7
-1
From Table 18.1, the conductivity of copper is 6.0 x 10 (Ω-m) , and
R=
l
=
σA
2 m
[6.0 x 10
7
(Ω − m)
−1
⎛ 3 x 10 −3 m ⎞
⎟⎟
(π)⎜⎜
2
⎝
⎠
]
2
= 4.7 x 10-3 Ω
(b) If V = 0.05 V then, from Equation (18.1)
I=
V
0.05 V
=
= 10.6 A
R 4.7 x 10 −3 Ω
(c) The current density is just
J=
I
=
A
I
⎛ d⎞
π⎜ ⎟
⎝ 2⎠
2
=
10.6 A
⎛ 3 x 10
π⎜
⎜
2
⎝
−3
m⎞
⎟⎟
⎠
2
= 1.5 x 10 6 A/m 2
(d) The electric field is just
E=
V 0.05 V
-2
=
= 2.5 x 10 V/m
l
2 m
459
18.6 When a current arises from a flow of electrons, the conduction is termed electronic; for ionic
conduction, the current results from the net motion of charged ions.
18.7
For an isolated atom, there exist discrete electron energy states (arranged into shells and
subshells); each state may be occupied by, at most, two electrons, which must have opposite spins.
On the other hand, an electron band structure is found for solid materials; within each band exist
closely spaced yet discrete electron states, each of which may be occupied by, at most, two
electrons, having opposite spins. The number of electron states in each band will equal the total
number of corresponding states contributed by all of the atoms in the solid.
18.8
This question asks that we explain the difference in electrical conductivity for metals,
semiconductors, and insulators in terms of their electron energy band structures.
For metallic materials, there are vacant electron energy states adjacent to the highest filled
state; thus, very little energy is required to excite large numbers of electrons into conducting states.
These electrons are those that participate in the conduction process, and, because there are so
many of them, metals are good electrical conductors.
There are no empty electron states adjacent to and above filled states for semiconductors
and insulators, but rather, an energy band gap across which electrons must be excited in order to
participate in the conduction process. Thermal excitation of electrons will occur, and the number of
electrons excited will be less than for metals, and will depend on the band gap energy.
semiconductors, the band gap is narrower than for insulators;
For
consequently, at a specific
temperature more electrons will be excited for semiconductors, giving rise to higher conductivities.
18.9 The electrical conductivity for a metallic glass will be less than for its crystalline counterpart. The
glass will have virtually no periodic atomic structure, and, as a result, electrons that are involved in
the conduction process will experience frequent and repeated scattering. (There is no electron
scattering in a perfect crystal lattice of atoms.)
18.10 The drift velocity of a free electron is the average electron velocity in the direction of the force
imposed by an electric field.
The mobility is the proportionality constant between the drift velocity and the electric field. It
is also a measure of the frequency of scattering events (and is inversely proportional to the
frequency of scattering).
460
18.11 (a) The drift velocity of electrons in Ge may be determined using Equation (18.7). Since the room
2
temperature mobility of electrons is 0.38 m /V-s (Table 18.2), and the electric field is 1000 V/m (as
stipulated in the problem),
v d = μ eE
(
2
)
= 0.38 m /V - s (1000 V/m) = 380 m/s
(b) The time, t, required to traverse a given length, l, of 25 mm is just
t =
l
25 x 10 −3 m
-5
=
= 6.6 x 10 s
380 m / s
v
d
18.12 The conductivity of this semiconductor is computed using Equation (18.16). However, it first
becomes necessary to determine the electron mobility from Equation (18.7) as
v
100 m / s
μe = d =
= 0.20 m 2/V - s
500 V / m
E
Thus,
σ = n e μe
(
18
= 3 x 10
-3
m
)(1.602 x 10-19 C)(0.20 m2 /V - s)
= 0.096 (Ω-m)-1
18.13
(a)
The number of free electrons per cubic meter for copper at room temperature may be
computed using Equation (18.8) as
n=
=
σ
e μe
6.0 x 107 (Ω − m)−1
(1.602 x 10−19 C)(0.0030 m 2 / V - s)
= 1.25 x 1029 m -3
461
(b) In order to calculate the number of free electrons per copper atom, we must first determine the
number of copper atoms per cubic meter, NCu. From Equation (4.2)
NCu =
NA ρ
A
Cu
23
3
6
3
3
6.023 x 10 atoms/ mol)(8.94 g / cm )(10 cm / m )
(
=
63.55 g / mol
= 8.47 x 10 28 m-3
The number of free electrons per copper atom is just
n 1.25 x 1029 m −3
=
= 1.48
N 8.47 x 10 28 m −3
18.14 (a) This portion of the problem asks that we calculate, for silver, the number of free electrons per
cubic meter (n) given that there are 1.3 free electrons per silver atom, that the electrical conductivity
'
is 6.8 x 107 (Ω-m)-1, and that the density ( ρAg
) is 10.5 g/cm3. (Note: in this discussion, the density
'
of silver is represented by ρAg
in order to avoid confusion with resistivity which is designated by ρ.)
Since n = 1.3N, and N is defined in Equation (4.2), then
⎡ '
⎢ ρAgNA
n = 1.3N = 1.3 ⎢
A
⎢ Ag
⎣
(
⎤
⎥
⎥
⎥⎦
)(
)⎤⎥
⎡ 10.5 g / cm 3 6.023 x 10 23 atoms/ mol
⎢
= 1.3 ⎢
107.87 g / mol
⎢⎣
⎥
⎦⎥
= 7.62 x 1022 cm-3 = 7.62 x 1028 m-3
(b) Now we are asked to compute the electron mobility, μe. Using Equation (18.8)
μe =
σ
ne
462
−1
7
=
6.8 x 10 (Ω − m)
(
)(
)
7.62 x 10 28 m−3 1.602 x 10 −19 C
= 5.57 x 10
-3
2
m /V - s
18.15 We want to solve for the parameter A in Equation (18.11) using the data in Figure 18.26. From
Equation (18.11)
A=
(
ρi
c i 1 − ci
)
However, the data plotted in Figure 18.26 is for the total resistivity, ρtotal, and includes both impurity
(ρi) and thermal (ρt) contributions [Equation (18.9)]. The value of ρt is taken as the resistivity at ci =
-8
0 in Figure 18.26, which has a value of 1.7 x 10 (Ω-m); this must be subtracted out. Below are
tabulated values of A determined at c = 0.10, 0.20, and 0.30, including other data that were used in
i
the computations.
ci
1 - ci
0.10
0.90
0.20
0.80
0.30
0.70
ρtotal (Ω-m)
ρi (Ω-m)
A (Ω-m)
-8
3.9 x 10
-8
5.3 x 10
-8
6.15 x 10
-8
2.2 x 10
-8
3.6 x 10
-8
4.45 x 10
2.44 x 10 7
2.25 x 10 7
2.12 x 10 7
There appears to be a slight decrease of A with increasing c .
i
18.16 (a) Perhaps the easiest way to determine the values of ρo and a in Equation (18.10) for pure
copper in Figure 18.8, is to set up two simultaneous equations and use resistivity values at two
different temperatures (labeled as 1 and 2). Thus,
ρ t1 = ρo + aT1
ρ t2 = ρ o + aT2
Solving these equations for a and ρo yield
ρ − ρt2
a = t1
T1 − T2
463
⎡ρ − ρ ⎤
t2
ρ o = ρ t1 − T1 ⎢ t1
⎥
T
−
T
⎣
⎦
1
2
⎡ρ − ρ ⎤
t2
= ρ t − T2 ⎢ t1
⎥
2
T
−
T
⎣ 1
2 ⎦
Let us take T = -150&deg;C, T = -50&deg;C, which gives ρt1 = 0.6 x 10-8 (Ω-m), and ρt2 = 1.25 x 10-8 (Ω1
2
m). Therefore
(
) (
)
⎡ 0.6 x 10-8 − 1.25 x 10-8 ⎤(Ω - m)
⎣
⎦
a =
−150&deg;C − (−50&deg;C )
= 6.5 x 10-11 (Ω - m)/&deg;C
and
(
-8
ρ o = 0.6 x 10
)
(
) (
)
⎡ 0.6 x 10-8 − 1.25 x 10-8 ⎤(Ω -m)
⎣
⎦
− (−150)
−150&deg;C − (-50&deg;C )
= 1.58 x 10-8 (Ω - m)
(b) For this part of the problem, we want to calculate A from Equation (18.11)—i.e.,
(
ρi = Ac i 1 − c i
)
In Figure 18.8, curves are plotted for three c values (0.0112, 0.0216, and 0.0332). Let us find A for
i
each of these c 's by taking a ρtotal from each curve at some temperature (say 0&deg;C) and then
i
-8
subtracting out ρi for pure copper at this same temperature (which is 1.7 x 10 Ω-m). Below are
tabulated values of A determined from these three c values, and other data that were used in the
i
computations.
ci
1 - ci
0.0112
0.989
0.0216
0.978
0.0332
0.967
ρtotal (Ω-m)
ρi (Ω-m)
A (Ω-m)
-8
3.0 x 10
-8
4.2 x 10
-8
5.5 x 10
-8
1.3 x 10
-8
2.5 x 10
-8
3.8 x 10
1.17 x 10 6
1.18 x 10 6
1.18 x 10 6
464
The average of these three A values is 1.18 x 10
-6
(Ω-m).
(c) We use the results of parts (a) and (b) to estimate the electrical resistivity of copper containing
1.75 at% Ni at 100&deg;C. The total resistivity is just
ρ total = ρ t + ρi
(
)
= ρ o + aT
{
[
(
+ Ac i 1 − ci
)
]
}
= 1.58 x 10-8 ( Ω - m) + 6.5 x 10-11 (Ω - m) / &deg;C (100&deg;C)
+
{[1.18 x 10
-6
]
(Ω - m) (0.0175)(1 − 0.0175)
}
= 4.26 x 10-8 (Ω - m)
18.17 We are asked to determine the electrical conductivity of a Cu-Ni alloy that has a tensile strength of
275 MPa. From Figure 7.14(a), the composition of an alloy having this tensile strength is about 8
wt% Ni. For this composition, the resistivity is about 13 x 10-8 Ω-m (Figure 18.9). And since the
conductivity is the reciprocal of the resistivity, Equation (18.4), we have
σ=
1
1
=
= 7.7 x 106 (Ω - m)-1
ρ 13 x 10 −8 Ω − m
18.18 This problem asks for us to compute the room-temperature conductivity of a two-phase Cu-Sn
alloy. It is first necessary for us to determine the volume fractions of the α and ε phases, after which
the resistivity (and subsequently, the conductivity) may be calculated using Equation (18.12).
Weight fractions of the two phases are first calculated using the phase diagram information provided
in the problem.
We might represent the phase diagram near room temperature as shown below.
465
Applying the lever rule to this situation
C
Wα =
ε
− Co
C − Cα
ε
37 − 11
= 0.703
37 − 0
=
C − Cα
11 − 0
Wε = o
=
= 0.297
37 − 0
C − Cα
ε
We must now convert these mass fractions into volume fractions using the phase densities given in
the problem. (Note: in the following expressions, density is represented by ρ' in order to avoid
confusion with resistivity which is designated by ρ.) Utilization of Equations (9.6a) and (9.6b) leads
to
Wα
Vα =
ρ'α
Wα
ρ'α
+
W
ε
ρ'
ε
0.703
=
8.94 g / cm3
0.297
0.703
+
3
8.25 g / cm3
8.94 g / cm
= 0.686
466
V =
ε
Wα
ρ'
W
ε
ρ'ε
+
α
W
ε
ρ'
ε
0.297
=
8.25 g / cm3
0.297
0.703
+
3
8.25 g / cm3
8.94 g / cm
= 0.314
Now, using Equation (18.12)
ρ = ρ α Vα + ρ V
ε ε
(
-8
= 1.88 x 10
)
(
-7
Ω - m (0.686) + 5.32 x 10
= 1.80 x 10
-7
)
Ω - m (0.314)
Ω -m
Finally, for the conductivity [Equation (18.4)]
σ=
1
1
=
= 5.56 x 106 (Ω - m)-1
ρ 1.80 x 10−7 Ω − m
18.19 The (a) and (b) portions of the problem ask that we make schematic plots on the same graph for
the electrical resistivity versus composition for lead-tin alloys at both room temperature and 150&deg;C;
such a graph is shown below.
467
(c) Upon consultation of the Pb-Sn phase diagram (Figure 9.7) we note, upon extrapolation of the
two solvus lines to room temperature (e.g., 20&deg;C), that the single phase α phase solid solution exists
between pure lead and a composition of about 2 wt% of Sn-98 wt% Pb. In addition, the composition
range over which the β phase is between approximately 99 wt% Sn-1 wt% Pb and pure tin. Within
both of these composition regions the resistivity increases in accordance with Equation (18.11);
also, in the above plot, the resistivity of pure Pb is represented (schematically) as being greater than
that for pure Sn, per the problem statement.
Furthermore, for compositions between these extremes, both α and β phases coexist, and
alloy resistivity will be a function of the resisitivities the individual phases and their volume fractions,
as described by Equation (18.12). Also, mass fractions of the α and β phases within the two-phase
region of Figure 9.7 change linearly with changing composition (according to the lever rule). There is
a reasonable disparity between the densities of Pb and Sn (11.35 g/cm3 versus 7.3 g/cm3). Thus,
according to Equation (9.6) phase volume fractions will not exactly equal mass fractions, which
means that the resistivity will not exactly vary linearly with composition. In the above plot, the curve
in this region has been depicted as being linear for the sake of convenience.
At 150&deg;C, the curve has the same general shape, and is shifted to significantly higher
resistivities inasmuch as resistivity increases with rising temperature [Equation (18.10) and Figure
18.8]. In addition, from Figure 9.7, at 150&deg;C the solubility of Sn in Pb increases to approximately 10
wt% Sn--i.e., the α phase field is wider and the increase of resistivity due to the solid solution effect
extends over a greater composition range, which is also noted in the figure.
The resistivity-
temperature behavior is similar on the tin-rich side, where, at 150&deg;C, the β phase field extends to
approximately 2 wt% Pb (98 wt% Sn). And, as with the room temperature case, for compositions
within the α + β two-phase region, the plot is approximately linear, extending between resistivity
values found at the maximum solubilities of the two phases.
18.20 We are asked to select which of several metals may be used for a 2 mm diameter wire to carry 10
A, and have a voltage drop of less than 0.03 V per foot (300 mm). Using Equations (18.3) and
(18.4), let us determine the minimum conductivity required, and then select from Table 18.1, those
metals that have conductivities greater than this value. The minimum conductivity is just
σ=
Il
=
VA
Il
⎛ d⎞
Vπ ⎜ ⎟
⎝ 2⎠
468
2
(
−3
(10 A) 300 x 10
=
)
m
⎛ 2 x 10 −3 m ⎞
(0.03 V) (π) ⎜
⎟⎟
⎜
2
⎝
⎠
2
= 3.2 x 107 (Ω - m) -1
Thus, from Table 18.1, only aluminum, gold, copper, and silver are candidates.
18.21 (a) For this part of the problem, we first read, from Figure 18.15, the number of free electrons (i.e.,
the intrinsic carrier concentration) at room temperature (298 K). These values are ni(Ge) = 5 x
1019 m-3 and ni(Si) = 3 x 1016 m-3.
and N , respectively) may
Now, the number of atoms per cubic meter for Ge and Si (N
Ge
Si
'
'
and ρSi
) and atomic weights
be determined using Equation (4.2) which involves the densities ( ρGe
(A
and A ). (Note: here we use ρ' to represent density in order to avoid confusion with
Ge
Si
resistivity, which is designated by ρ.) Therefore,
'
N Aρ Ge
NGe =
A Ge
23
3
6
3
3
6.023 x 10 atoms/ mol)(5.32 g / cm )(10 cm / m )
(
=
72.59 g / mol
= 4.4 x 10
28
3
atoms/m
Similarly
'
N AρSi
NSi =
A Si
23
3
6
3
3
6.023 x 10 atoms/ mol)(2.33 g / cm )(10 cm / m )
(
=
28.09 g / mol
28
= 5.00 x 10
3
atoms/m
Finally, the ratio of the number of free electrons per atom is calculated by dividing n by N. For Ge
nGe
N
Ge
=
5 x 1019 electrons / m 3
4.4 x 1028 atoms / m3
469
= 1.1 x 10
-9
electron/atom
And, for Si
nSi
N
Si
=
3 x 1016 electrons / m3
5.00 x 1028 atoms/ m 3
-13
= 6 x 10
electron/atom
(b) The difference is due to the magnitudes of the band gap energies (Table 18.2). The band gap
energy at room temperature for Si (1.11 eV) is larger than for Ge (0.67 eV), and, consequently, the
probability of excitation across the band gap for a valence electron is much smaller for Si.
18.22 This problem asks that we make plots of ln ni versus reciprocal temperature for both Si and Ge,
using the data presented in Figure 18.15, and then determine the band gap energy for each material
realizing that the slope of the resulting line is equal to – Eg/2k.
Below is shown such a plot for Si.
The slope of the line drawn is equal to –6400 which equals an Eg value of
470
Eg = − 2 k(slope)
= − 2(8.62 x 10−5 eV / K)((−6400) = 1.10 eV
The value cited in Table 18.2 is 1.11 eV.
Now for Ge, an analogous plot is shown below.
The slope of this line segment is – 4085, which leads to be band gap energy value of
−5
Eg = − 2 k (slope) = − 2(8.62 x 10
eV / K)((−4085 ) = 0.70 eV
This value is in good agreement with the 0.67 eV cited in Table 18.2.
18.23 The factor 2 in Equation (18.21a) takes into account the creation of two charge carriers (an
electron and a hole) for each valence-band-to-conduction-band intrinsic excitation; both charge
carriers may participate in the conduction process.
18.24 These semiconductor terms are defined in the Glossary. Examples are as follows: intrinsic--high
purity (undoped) Si, GaAs, CdS, etc.; extrinsic--P-doped Ge, B-doped Si, S-doped GaP, etc.;
compound--GaAs, InP, CdS, etc.; elemental--Ge and Si.
471
18.25 Yes, compound semiconductors can exhibit intrinsic behavior. They will be intrinsic even though
they are composed of two different elements as long as the electrical behavior is not influenced by
the presence of other elements.
18.26 This problem calls for us to decide for each of several pairs of semiconductors, which will have the
smaller band gap energy and then cite reasons for the choice.
(a) Germanium will have a smaller band gap energy than diamond since Ge is lower in row IVA of
the periodic table (Figure 2.6) than is C. In moving from top to bottom of the periodic table, Eg
decreases.
(b) Indium antimonide will have a smaller band gap energy than aluminum phosphide. Both of
these are III-V compounds, and the positions of both In and Sb are lower vertically in the periodic
table than Al and P.
(c) Gallium arsenide will have a smaller band gap energy than zinc selenide. All four of these
elements are in the same row of the periodic table, but Zn and Se are more widely separated
horizontally than Ga and As; as the distance of separation increases, so does the band gap.
(d) Cadmium telluride will have a smaller band gap energy than zinc selenide. Both are II-VI
compounds, and Cd and Te are both lower vertically in the periodic table than Zn and Se.
(e) Cadmium sulfide will have a smaller band gap energy than sodium chloride since Na and Cl
are much more widely separated horizontally in the periodic table than are Cd and S.
18.27 The explanations called for in this problem are found in Section 18.11.
18.28 (a) No hole is generated by an electron excitation involving a donor impurity atom because the
excitation comes from a level within the band gap, and thus, no missing electron is created from the
normally filled valence band.
(b) No free electron is generated by an electron excitation involving an acceptor impurity atom
because the electron is excited from the valence band into the impurity level within the band gap; no
free electron is introduced into the conduction band.
18.29 Nitrogen will act as a donor in Si. Since it (N) is from group VA of the periodic table (Figure 2.6),
an N atom has one more valence electron than an Si atom.
Boron will act as an acceptor in Ge. Since it (B) is from group IIIA of the periodic table, a B
atom has one less valence electron than a Ge atom.
Zinc will act as an acceptor in GaAs. Since Zn is from group IIB of the periodic table, it will
substitute for Ga; furthermore, a Zn atom has one less valence electron than a Ga atom.
472
Sulfur will act as a donor in InSb. Since S is from group VIA of the periodic table, it will
substitute for Sb; also, an S atom has one more valence electron than an Sb atom.
Indium will act as a donor in CdS. Since In is from group IIIA of the periodic table, it will
substitute for Cd; and, an In atom has one more valence electron than a Cd atom.
Arsenic will act as an acceptor in ZnTe. Since As is from group VA of the periodic table, it
will substitute for Te; furthermore, an As atom has one less valence electron than a Te atom.
18.30 (a) For an intrinsic semiconductor the Fermi energy is located in the vicinity of the center of the
band gap.
(b) For an n-type semiconductor the Fermi energy is located in the vicinity of the donor impurity
level.
(c)
Below is shown a schematic plot of Fermi energy versus temperature for an n-type
semiconductor.
At low temperatures, the material is extrinsic and the Fermi energy is located near the top of the
band gap, in the vicinity of the donor level. With increasing temperature, the material eventually
becomes intrinsic, and the Fermi energy resides near the center of the band gap.
18.31 (a) In this problem, for a Si specimen, we are given p and σ, while μh and μe are included in
Table 18.2. In order to solve for n we must use Equation (18.13), which, after rearrangement, leads
to
n=
σ − p e μh
eμ
e
473
3
−1
10 (Ω − m)
23 −3
−19
2
m )(1.602 x 10
C)(0.05 m / V - s)
(
(1.602 x 10−19 C)(0.14 m 2 / V - s )
− 1.0 x 10
=
= 8.9 x 10
21
(b) This material is p-type extrinsic since p (1.0 x 10
-3
m
23
-3
21 -3
m ) is greater than n (8.9 x 10 m ).
18.32 In this problem we are asked to compute the intrinsic carrier concentration for PbS at room
temperature. Since the conductivity and both electron and hole mobilities are provided in the
problem statement, all we need do is solve for n and p (i.e., ni) using Equation (18.15). Thus,
ni =
=
(
σ
e μe + μn
25 (Ω - m)
)
−1
(1.602 x 10−19 C)(0.06 + 0.02) m2 / V - s
= 1.95 x 10
21
-3
m
24 -3
18.33 (a) This germanium material to which has been added 10 m As atoms is n-type since As is a
donor in Ge. (Arsenic is from group VA of the periodic table--Ge is from group IVA.)
(b) Since this material is n-type extrinsic, Equation (18.16) is valid. Furthermore, each As atom will
donate a single electron, or the electron concentration is equal to the As concentration since all of
24 -3
the As atoms are ionized at room temperature; that is n = 10 m , and, as given in the problem
statement, μe = 0.1 m2/V-s. Thus
σ = n e μe
(
= 10
24
-3
m
)(1.602 x 10-19 C)(0.1 m2/V - s)
= 1.6 x 104 (Ω - m)-1
18.34 In order to solve for the electron and hole mobilities for InP, we must write conductivity expressions
for the two materials, of the form of Equation (18.13)--i.e.,
474
σ = n e μe + p e μh
For the intrinsic material
2.5 x 10
-6
)(1.602 x 10-19 C)μe
13 -3
-19
+ (3 x 10 m )(1.602 x 10
C)μh
(Ω -m)
-1
(
13
= 3.0 x 10
-3
m
which reduces to
0.52 = μe + μ h
Whereas, for the extrinsic InP
3.6 x 10
-5
)(1.602 x 10-19 C)μ e
12 -3
-19
+ (2.0 x 10 m )(1.602 x 10
C)μh
(Ω -m)
-1
(
14
= 4.5 x 10
-3
m
which may be simplified to
112.4 = 225μ e + μh
Thus, we have two independent expressions with two unknown mobilities. Solving for μe and μh, we
get μe = 0.50 m2/V-s and μh = 0.02 m2/V-s.
18.35 In order to estimate the electrical conductivity of intrinsic silicon at 80&deg;C, we must employ Equation
(18.15). However, before this is possible, it is necessary to determine values for ni, μe, and μh.
According to Figure 18.15, at 80&deg;C (353 K), ni = 1.5 x 1018 m-3, whereas from the &quot;&lt;1020 m-3&quot;
curves of Figures 18.18a and 18.18b, μe = 0.11 m2/V-s and μh = 0.035 m2/V-s (realizing that the
mobility axes of these two plot are scaled logarithmically). Thus, the conductivity at 80&deg;C is
(
σ = ni e μ e + μ h
(
18
σ = 1.5 x 10
m
−3
)
)(1.602 x 10−19 C)(0.11 m2 /V - s
= 0.035 (Ω - m)-1
475
2
+ 0.035 m / V − s
)
18.36 (a) This portion of the problem asks for us to assume that electron and hole mobilities for intrinsic
Ge are temperature-dependent, and proportional to T -3/2 for temperature in K. It first becomes
necessary to solve for C in Equation (18.22) using the room-temperature (298 K) conductivity [2.2
(Ω-m)-1] (Table 18.2). This is accomplished as follows:
ln C = ln σ +
= ln (2.2) +
Eg
3
ln T +
2
2 kT
3
0.67 eV
ln (298) +
2
(2) 8.62 x 10−5 eV / K (298 K)
(
)
= 22.38
Now, again using Equation (18.22) we are able to compute the conductivity at 423 K
ln σ = ln C −
= 22.38 −
Eg
3
ln T −
2
2kT
3
0.67 eV
ln (423 K) −
2
(2) 8.62 x 10−5 eV / K (423 K)
(
)
= 4.12
which leads to e4.12 = 61.4 (Ω-m)-1.
18.37
This problem asks that we determine the temperature at which the electrical conductivity of
intrinsic Ge is 40 (Ω-m)-1, using Equation 18.22 and the results of Problem 18.36. First of all, taking
logarithms of Equation 18.22
ln σ = ln C −
Eg
3
ln T −
2
2kT
And, from Problem 18.36 the value of ln C was determined to be 22.38. Using this and σ = 40 (Ωm)-1, the above equation takes the form
ln 40 = 22.38 −
3
0.67 eV
ln T −
2
(2) 8.62 x 10 −5 eV / K (T)
(
476
)
In order to solve for T from the above expression it is necessary to use an equation solver. Using EZ Solve and the following instructions
ln(40) = 22.38 –1.5*ln(T) – 0.67/(2*8.62*10^-5*T)
When the Calculator icon in the tool bar is selected (&quot;Solve new run&quot; text appears), and then the
&quot;Solve&quot; space is selected in the window that appears, the value of T = 400 appears in the data grid.
This value is the temperature in K which corresponds to 127&deg;C.
18.38 This problem asks that we estimate the temperature at which GaAs has an electrical conductivity
of 3.7 x 10-3 (Ω-m)-1 assuming that the conductivity has a temperature dependence as shown in
Equation (18.22). From the room temperature (298 K) conductivity [10-6 (Ω-m)-1] and band gap
energy (1.42 eV) of Table 18.2 we determine the value of C [Equation (18.22)] as
ln C = ln σ +
[
]
= ln 10 −6 (Ω − m)−1 +
Eg
3
ln T +
2
2kT
3
1.42 eV
ln (298 K) +
2
(2) 8.62 x 10 −5 eV / K (298 K)
(
)
= 22.37
Now we substitute this value into Equation (18.22) in order to determine the value of T for which σ =
3.7 x 10-3 (Ω-m)-1:
ln σ = ln C −
[
]
ln 3.7 x 10-3 (Ω - m) -1 = 22.37 −
Eg
3
ln T −
2
2 kT
3
1.42 eV
ln T −
2
(2) 8.62 x 10 −5 eV / K (T)
(
)
This equation may be solved for T using the E-Z Solve equation solver. The following text is entered
into the workspace
ln(3.7*10^-3) = 22.37 - 1.5*ln(T) - 1.42/(2*8.62*10^-5*T)
477
And when the Calculator icon in the tool bar is selected (&quot;Solve new run&quot; text appears) button in the
toolbar is clicked, and then the &quot;Solve&quot; space is selected in the window that appears, the value of T =
437 appears in the data grid. This value is the temperature in K which corresponds to 164&deg;C.
18.39 This question asks that we compare and then explain the difference in temperature dependence of
the electrical conductivity for metals and intrinsic semiconductors.
For a pure metal, this
temperature dependence is just
σ=
1
ρ o + aT
[This expression comes from Equations (18.4) and (18.10).]
That is, the electrical conductivity
decreases with increasing temperature.
By way of contrast, for an intrinsic semiconductor the temperature dependence is
represented by an equation of the form of Equation (18.22). This expression contains two terms that
involve temperature—a preexponential one (in this case T-3/2) and the other in the exponential.
T
With rising temperature the preexponential term decreases, while the exp (-Eg/2kT) parameter
increases. With regard to relative magnitudes, the exponential term increases much more rapidly
than the preexponential one, such that the electrical conductivity of an intrinsic semiconductor
increases with rising temperature. Thus, this temperature-dependence of conductivity is just the
opposite of that for metals, as outline in the previous paragraph.
The temperature behavior for metals is best explained by consulting Equation (18.8)
σ = n e μe
As the temperature rises, n will remain virtually constant, whereas the mobility (μe) will decrease,
because the thermal scattering of free electrons will become more efficient. Since |e| is independent
of temperature, the net result will be diminishment in the magnitude of σ.
For an intrinsic semiconductor, Equation (18.15) describes the conductivity; i.e.,
(
σ = n e μe + μh
) = p e (μe
+ μh
)
Both n and p increase dramatically with rising temperature (Figure 18.15), since more thermal
energy becomes available for valence band-conduction band electron excitations. The magnitudes
of μe and μh will diminish somewhat with increasing temperature (per the upper curves of Figures
478
18.18a and 18.18b), as a consequence of the thermal scattering of electrons and holes. However,
this reduction of μe and μh will be overwhelmed by the increase in n and p, with the net result is that
σ increases with temperature.
18.40 According to Figure 18.16, as dopant level is increased, the position of the horizontal &quot;Extrinsic
Region&quot; line moves upward. Thus, the point at which the intrinsic region becomes dominant moves
horizontally to higher temperatures.
18.41 This problems asks that we determine the room-temperature electrical conductivity of silicon that
has been doped with 1023 m-3 of arsenic atoms. Inasmuch as As is a group VA element in the
periodic table (Figure 2.6) it acts as a donor in silicon. Thus, this material is n-type extrinsic, and it
is necessary to use Equation (18.16), with n = 1023 m-3 since at room temperature all of the As
donor impurities are ionized. The electron mobility, from Figure 18.17 at an impurity concentration of
1023 m-3, is 0.065 m2/V-s. Therefore, the conductivity is equal to
(
23
σ = n e μe = 10
−3
m
)(1.6 x 10 −16 C)(0.065 m 2 / V − s)= 1040 (Ω − m)−1
18.42 Here we are asked to calculate the room-temperature electrical conductivity of silicon that has
been doped with 2 x 1024 m-3 of boron atoms. Inasmuch as B is a group IIIA element in the periodic
Thus, this material is p-type extrinsic, and it is
24
necessary to use Equation (18.17), with p = 2 x 10 m-3 since at room temperature all of the B
table (Figure 2.6) it acts as an acceptor in silicon.
acceptor impurities are ionized. The hole mobility, from Figure 18.17 at an impurity concentration of
2 x 1024 m-3, is 0.0065 m2/V-s. Therefore, the conductivity is equal to
(
24
σ = n e μe = 2 x 10
−3
m
)(1.6 x 10−16 C)(0.0065 m 2 / V − s)= 2080 (Ω − m) −1
18.43 In this problem we are to estimate the electrical conductivity, at 75&deg;C, of silicon that has been
doped with 1022 m-3 of phosphorous atoms. Inasmuch as P is a group VA element in the periodic
table (Figure 2.6) it acts as a donor in silicon. Thus, this material is n-type extrinsic, and it is
necessary to use Equation (18.16); n in this expression is 1022 m-3 since at 75&deg;C all of the P donor
impurities are ionized. The electron mobility is determined using Figure 18.18a. From the 1022 m-3
impurity concentration curve and at 75&deg;C (348 K), μe = 0.08 m2/V-s. Therefore, the conductivity is
equal to
(
22
σ = n e μe = 10
−3
m
)(1.6 x 10 −16 C)(0.08 m2 / V − s)= 128 (Ω − m)−1
479
18.44 In this problem we are to estimate the electrical conductivity, at 135&deg;C, of silicon that has been
doped with 1024 m-3 of aluminum atoms. Inasmuch as Al is a group IIIA element in the periodic
table (Figure 2.6) it acts as an acceptor in silicon. Thus, this material is p-type extrinsic, and it is
necessary to use Equation (18.17); p in this expression is 1024 m-3 since at 135&deg;C all of the Al
acceptor impurities are ionized. The hole mobility is determined using Figure 18.18b. From the
1024 m-3 impurity concentration curve and at 135&deg;C (408 K,) μh = 0.007 m2/V-s. Therefore, the
conductivity is equal to
(
24
σ = n e μh = 10
m
−3
)(1.6 x 10−16 C )(0.007 m2 / V − s)= 1120 (Ω − m) −1
18.45 We are asked in this problem to determine the electrical conductivity for the nonstoichiometric
Fe(1 - x)O, given that x = 0.060 and that the hole mobility is 1.0 x 10-5 m2/V-s. It is first necessary to
compute the number of vacancies per cubic meter for this material. For this determination let us use
as our basis 10 unit cells. For the sodium chloride crystal structure (Figure 12.2) there are four
cations and four anions per unit cell. Thus, in ten unit cells of FeO there will normally be forty O2and forty Fe2+ ions. However, when x = 0.06, (0.06)(40) = 2.4 of the Fe2+ sites will be vacant.
(Furthermore, there will be 4.8 Fe3+ ions in these ten unit cells inasmuch as two Fe3+ ions are
created for every vacancy). Therefore, each unit cell will, on the average contain 0.24 vacancies.
Now, the number of vacancies per cubic meter is just the number of vacancies per unit cell divided
by the unit cell volume; this volume is just the unit cell edge length (0.437 nm) cubed. Thus
# vacancies
m3
=
0.24 vacancies / unit cell
(0.437 x 10−9 m)
3
= 2.88 x 10
27
3
vacancies/m
Inasmuch as it is assumed that the vacancies are saturated, the number of holes (p) is also 2.88 x
1027 m-3. It is now possible, using Equation (18.17), to compute the electrical conductivity of this
material:
σ = p e μh
(
27
= 2.88 x 10
-3
m
)(1.602 x 10-19 C)(1.0 x 10-5 m2 /V - s) = 4600 (Ω - m)-1
480
18.46W
(a) This portion of the problem calls for us to determine the electron mobility for some
hypothetical metal having an electrical resistivity of 3.3 x 10-8 (Ω-m), given that the specimen
thickness is 15 mm, and that when Ix = 25 A and Bz = 0.95 tesla a VH of –2.4 x 10-7 V is produced.
It is first necessary to convert resistivity to conductivity (Equation 18.4). Thus
σ=
1
1
=
= 3.0 x 107 (Ω - m)-1
−
ρ
3.3 x10 8 (Ω − m)
The electron mobility may be determined using Equation (18.3bW);
and upon incorporation of
Equation (18.1W), we have
μ e = RH σ
=
VH d σ
I B
x z
)[
(
]
⎛ − 2.4 x 10−7 V ⎞ 15 x 10 −3 m 3.0 x 107 (Ω − m) −1
⎝
⎠
=
(25 A)(0.95 tesla)
= 0.0045 m2 /V - s
(b) Now we are to calculate the number of free electrons per cubic meter. From Equation (18.8) we
have
n =
σ
e μe
7
=
3.0 x 10 (Ω - m)
−1
(1.602 x 10 −19 C)(0.0045
)
m2 / V - s
= 4.17 x 1028 m-3
18.47W In this problem we are asked to determine the magnetic field required to produce a Hall voltage
of –3.5 x 10-7 V, given that σ = 1.2 x 107 (Ω-m)-1, μe = 0.0050 m2/V-s, Ix = 40 A, and d = 35 mm.
Combining Equations (18.1W) and (18.3bW), and after solving for Bz, we get
481
Bz =
=
[
VH σd
I μ
x e
](
)
)
⎛ −3.5 x 10−7 V ⎞ 1.2 x 107 (Ω − m)−1 35 x 10−3 m
⎝
⎠
(
(40 A) 0.0050 m 2 / V - s
= 0.74 tesla
18.48 The explanations called for are found in Section 18.15.
18.49 The energy generated by the electron-hole annihilation reaction, Equation (18.18), is dissipated as
heat.
18.50 In an electronic circuit, a transistor may be used to 1) amplify an electrical signal, and 2) act as a
switching device in computers.
18.51 If the temperature of a p-n junction rectifier or a junction transistor is raised high enough, the
semiconducting materials will become intrinsic and the device will become inoperative. Furthermore,
diffusion of doping species from a p region to an n region and vice versa may occur, which would
18.52 The differences in operation and application for junction transistors and MOSFETs are described
in Section 18.15.
18.53 For this problem, we are given, for NaCl, the activation energy (173,000 J/mol) and preexponential
(4.0 x 10-4 m2/s) for the diffusion coefficient of Na+ and are asked to compute the mobility for a Na+
ion at 873 K.
The mobility, μNa+, may be computed using Equation (18.20);
however, this
expression also includes the diffusion coefficient DNa+, which is determined using Equation (5.8) as
⎛ Q ⎞
= D o exp ⎜ − d ⎟
Na
⎝ RT ⎠
D
(
= 4.0 x 10
-4
+
)
⎡
⎤
173,000 J / mol
2
m /s exp ⎢−
⎥
⎣ (8.31 J / mol - K)(873 K) ⎦
482
= 1.76 x 10-14 m2 /s
Now solving for μNa+ yields
μ
(
Na
+
−19
(1) 1.602 x 10
=
=
n NaeD
Na +
kT
)(
C / atom 1.76 x 10
(
−14
)
2
m /s
)
1.38 x 10 −23 J / atom - K (873 K)
= 2.34 x 10-13 m 2/V - s
18.54W We want to compute the plate spacing of a parallel-plate capacitor as the dielectric constant is
increased form 2.5 to 4.0, while maintaining the capacitance constant.
(18.6W) and (18.7W) yields
Combining Equations
εε A
C= r o
l
Now, let us use the subscripts 1 and 2 to denote the initial and final states, respectively. Since C =
1
C , then
2
ε r1ε oA
l
=
1
εr 2ε o A
l
2
And, solving for l2
l2 =
ε l
r 2 1 = (4.0)(1 mm) = 1.6 mm
2.5
r1
ε
18.55W This problem asks for us to ascertain which of the materials listed in Table 18.1W are candidates
for a parallel-plate capacitor that has dimensions of 38 mm by 65 mm, a plate separation of 1.3 mm
so as to have a minimum capacitance of 7 x 10-11 F, when an ac potential of 1000 V is applied at 1
MHz. Upon combining Equations (18.6W) and (18.7W) and solving for the dielectric constant εr we
get
483
lC
ε oA
εr =
=
(1.3 x 10 −3 m)(7 x 10 −11F)
(8.85 x 10−12 F / m)(38 x 10−3 m)(65 x 10−3 m)
= 4.16
Thus, the minimum value of εr to achieve the desired capacitance is 4.16 at 1 MHz. Of those
materials listed in the table, titanate ceramics, mica, steatite, soda-lime glass, porcelain, and phenolformaldehyde are candidates.
18.56W In this problem we are given, for a parallel-plate capacitor, its area (3225 mm2), the plate
separation (1 mm), and that a material having an εr of 3.5 is positioned between the plates.
(a) We are first asked to compute the capacitance. Combining Equations (18.6W) and (18.7W), and
solving for C yields
C =
(
−12
(3.5) 8.85 x 10
=
ε r ε oA
l
)(
2
F / m 3225 mm
)(1 m2 / 106 mm2 )
10−3 m
= 10-10 F = 100 pF
(b) Now we are asked to compute the electric field that must be applied in order that 2 x 10-8 C be
stored on each plate. First we need to solve for V in Equation (18.4W) as
V =
Q
2 x 10 −8 C
=
= 200 V
C
10−10 F
The electric field E may now be determined using Equation (18.6); thus
E =
V
200 V
5
=
= 2.0 x 10 V/m
−3
l
m
10
18.57W This explanation is found in Section 18.19W.
484
+
18.58W Shown below are the relative positions of Na and Cl ions, without and with an electric field
present.
Now,
d = r
Na +
+ r - = 0.102 nm + 0.181 nm = 0.283 nm
Cl
and
Δd = 0.05 d = (0.05)(0.283 nm) = 0.0142 nm = 1.42 x 10-11 m
From Equation (18.8W), the dipole moment, p, is just
p = q Δd
(
= 1.602 x 10
-19
)(
-11
C 1.42 x 10
)
m
= 2.26 x 10-30 C -m
18.59W (a) In order to solve for the dielectric constant in this problem, we must employ Equation
(18.12W), which includes polarization and electric field parameters; values for these parameters are
given in the problem statement. Solving for εr from this expression gives
εr =
P
+ 1
ε oE
485
=
(
1.0 x 10−6 C/ m 2
)(
8.85 x 10−12 F / m 5 x 104 V / m
)
+ 1
= 3.26
(b) The dielectric displacement may be determined using Equation (18.11W), as
D = ε oE + P
=
(8.85 x 10-12 F/m)(5 x 104 V/m) + 1.0
x 10
-6
2
C/m
= 1.44 x 10-6 C/m2
-11
2
C, A = 160 mm , l = 3.5 mm, and εr
18.60W (a) We want to solve for the voltage when Q = 3.5 x 10
= 5.0. Combining Equations (18.4W), (18.6W), and (18.7W) yields
Q
A
= ε rε o
V
l
And, solving for V
V =
=
Ql
ε rε o A
(3.5 x 10 −11 C)(3.5 x 10 −3 m)
(5.0) (8.85 x 10 −12 F/ m)(160 mm 2 )(1 m2 / 106 mm2 )
= 17.3 V
(b) For this same capacitor, if a vacuum is used
V =
=
Ql
ε oA
(3.5 x 10−11 C)(3.5 x 10−3 m)
(8.85 x 10−12 F / m)(160 x 10 −6 m2 )
486
= 86.5 V
(c) The capacitance for part (a) is just
C =
Q
3.5 x 10−11 C
-12
=
= 2.0 x 10
F
17.3 V
V
C =
Q
3.5 x 10−11 C
-13
=
= 4.0 x 10
F
86.5 V
V
And for part (b)
(d) The dielectric displacement may be computed by combining Equations (18.11W), (18.12W), and
(18.6), as
D = ε oE + ε o(εr − 1)E = ε oε rE =
=
ε εV
o r
l
(8.85 x 10−12 F / m)(5.0)(17.3 V)
3.5 x 10 −3 m
= 2.2 x 10-7 C/m2
(e) The polarization is determined using Equations (18.12W) and (18.6) as
V
P = ε o(εr − 1)
l
=
(8.85 x 10−12 F / m)(5.0 − 1)(17.3 V)
3.5 x 10−3 m
= 1.75 x 10-7 C/m2
18.61W (a) For electronic polarization, the electric field causes a net displacement of the center of the
negatively charged electron cloud relative to the positive nucleus. With ionic polarization, the cations
and anions are displaced in opposite directions as a result of the application of an electric field.
487
Orientation polarization is found in substances that possess permanent dipole moments; these
dipole moments become aligned in the direction of the electric field.
(b) Only electronic polarization is to be found in gaseous argon; being an inert gas, its atoms will
not be ionized nor possess permanent dipole moments.
Both electronic and ionic polarizations will be found in solid LiF, since it is strongly ionic. In
all probability, no permanent dipole moments will be found in this material.
Both electronic and orientation polarizations are found in liquid H2O. The H2O molecules
have permanent dipole moments that are easily oriented in the liquid state.
Only electronic polarization is to be found in solid Si; this material does not have molecules
with permanent dipole moments, nor is it an ionic material.
18.62W For this soda-lime glass, in order to determine the fraction of the dielectric constant at low
frequencies that is attributed to ionic polarization, we must determine the εr within this low-frequency
regime; such is tabulated in Table 18.1W, and at 1 MHz its value is 6.9. Thus, this fraction is just
fraction =
ε (low) − ε (high)
r
r
ε (low)
r
=
6.9 − 2.3
= 0.67
6.9
18.63W (a) This portion of the problem asks that we compute the magnitude of the dipole moment
associated with each unit cell of BaTiO3, which is illustrated in Figure 18.26. The dipole moment p
is defined by Equation (18.8W) as p = qd in which q is the magnitude of each dipole charge, and d
is the distance of separation between the charges. Each Ti4+ ion has four units of charge
associated with it, and thus q = (4)(1.602 x 10-19 C) = 6.41 x 10-19 C. Furthermore, d is the
distance the Ti4+ ion has been displaced from the center of the unit cell, which is just 0.006 nm +
0.006 nm = 0.012 nm [Figure 18.26(b)]. Hence
(
-19
p = qd = 6.41 x 10
= 7.69 x 10
(b)
)(
-9
C 0.012 x 10
-30
)
m
C-m
Now it becomes necessary to compute the maximum polarization that is possible for this
material. The maximum polarization will exist when the dipole moments of all unit cells are aligned
in the same direction. Furthermore, it is computed by dividing the value of p by the volume of each
488
unit cell, which is equal to the product of three unit cell edge lengths, as shown in Figure 18.26.
Thus
P =
=
p
VC
7.69 x 10 −30 C − m
(0.403 x 10−9 m)(0.398 x 10−9 m)(0.398 x 10 −9 m)
= 0.121 C/m
2
18.64W The ferroelectric behavior of BaTiO3 ceases above its ferroelectric Curie temperature because
the unit cell transforms from tetragonal geometry to cubic; thus, the Ti4+ is situated at the center of
the cubic unit cell, there is no charge separation, and no net dipole moment.
18.65
Yes, the physical dimensions of a piezoelectric material such as BaTiO3 change when it is
subjected to an electric field. As noted in Figure 18.27, a voltage (or electric field) is generated when
the dimensions of a piezoelectric material are altered. Thus, it would be logical to expect the reverse
effect to occur--that is, placing the material within an electric field causes its physical dimensions to
change.
Design Problems
18.D1 This problem asks that we calculate the composition of a copper-nickel alloy that has a room
-7
temperature resistivity of 2.5 x 10 Ω-m. The first thing to do is, using the 90 Cu-10 Ni resistivity
data, determine the impurity contribution, and, from this result, calculate the constant A in Equation
(18.11). Thus,
ρ total = 1.90 x 10-7 (Ω - m) = ρi + ρ t
From Table 18.1, for pure copper
ρt =
1
1
=
= 1.67 x 10-8 (Ω - m)
7
σ
6.0 x 10 ( Ω − m) −1
489
Thus, for the 90 Cu-10 Ni alloy
ρi = ρ total − ρ t = 1.90 x 10 -7 − 1.67 x 10-8
= 1.73 x 10-7 (Ω - m)
In the problem statement, the impurity (i.e., nickel) concentration is expressed in weight percent.
However, Equation (18.11) calls for concentration in atom fraction (i.e., atom percent divided by
100). Consequently, conversion from weight percent to atom fraction is necessary. (Note: we now
'
, and the weight percents of Ni and Cu by CNi
choose to denote the atom fraction of nickel as c Ni
and CCu, respectively.) Using these notations, this conversion may be accomplished by using a
modified form of Equation (4.6a) as
'
cNi
=
CNi ACu
CNiACu + CCu ANi
Here ANi and ACu denote the atomic weights of nickel and copper. Thus
'
cNi
=
(10 wt%)(63.55 g / mol)
(10 wt%)(63.55 g / mol) + (90 wt%)(58.69 g / mol)
= 0.107
Now, solving for A in Equation (18.11)
A =
ρ
i
' ⎛
' ⎞
cNi
⎜1 − cNi
⎟
⎝
⎠
−7
=
1.73 x 10 (Ω − m)
= 1.81 x 10 -6 (Ω - m)
(0.107 )(1 − 0.107 )
-7
'
Finally, it is possible to compute the c Ni
to give a room temperature resistivity of 2.5 x 10 Ω-m.
Again, we must determine ρi as
ρi = ρ total − ρ t
490
= 2.5 x 10-7 − 1.67 x 10-8 = 2.33 x 10-7 (Ω - m)
If Equation (18.11) is expanded, then
'
' 2
ρi = Ac Ni
- AcN
i
'
and, solving for c Ni
'
A&plusmn;
A 2 − 4Aρ
cNi =
i
2A
Or
1.81 x 10 −6 &plusmn;
'
cNi
=
(1.81 x 10 −6 ) − (4)(1.81 x 10 −6 )(2.33 x 10−7 )
(2) (1.81 x 10 −6 )
2
And, taking the negative root,
'
cNi
= 0.152
which is equivalent to a concentration of 15.2 at% Ni. Now, converting this composition to weight
percent Ni, requires that we use Equation (4.7a) as
CNi =
' A
CNi
Ni
C' A
Ni Ni
=
+ C' A
x 100
Cu Cu
(15.2 at%)(58.69 g / mol)
x 100
(15.2 at%)(58.69 g / mol) + (84.8 at%)(63.55 g / mol)
= 14.2 wt%
18.D2 This problem asks that we determine the electrical conductivity of an 85 wt% Cu-15 wt% Zn alloy
at -100&deg;C using information contained in Figures 18.8 and 18.28. In order to solve this problem it is
necessary to employ Equation (18.9) which is of the form
491
ρ total = ρ t + ρi
since it is assumed that the alloy is undeformed. Let us first determine the value of ρi at room
temperature (25&deg;C) which value will be independent of temperature. From Figure (18.8), at 25&deg;C
and for pure Cu, ρt(25) = 1.75 x 10-8 Ω-m. Now, since it is assumed that the curve in Figure 18.28
was generated also at room temperature, we may take ρ as ρtotal(25) at 85 wt% Cu-15 wt% Zn
which has a value of 4.7 x 10-8 Ω-m. Thus
ρi = ρ total (25) − ρ t (25)
= 4.7 x 10
-8
Ω - m - 1.75 x 10
-8
Ω - m = 2.95 x 10
-8
Ω -m
Finally, we may determine the resistivity at -100&deg;C, ρtotal(-100), by taking the resistivity of pure Cu
at -100&deg;C from Figure 18.8, which gives us ρt(-100) = 0.90 x 10-8 Ω-m. Therefore
ρ total (-100) = ρi + ρ t (-100)
= 2.95 x 10
-8
Ω - m + 0.90 x 10
-8
Ω - m = 3.85 x 10
-8
Ω -m
And, using Equation (18.4) the conductivity is calculated as
σ =
1
1
=
= 2.60 x 107 (Ω - m)-1
−
8
ρ
3.85 x 10 Ω − m
18.D3 To solve this problem, we want to consult Figures 7.14(b) and (18.9) in order to determine the Ni
concentration ranges over which the yield strength is greater than 130 MPa (19,000 psi) and the
6
-1
conductivity exceeds 4.0 x 10 (Ω-m) .
From Figure 7.14(b), a Ni concentration greater than about 23 wt% is necessary for a yield
strength in excess of 130 MPa. In Figure 18.9 is plotted the resistivity versus the Ni content. Since
-8
conductivity is the reciprocal of resistivity, the resistivity must be less than 25 x 10 Ω-m--i.e.,
1
. According to the figure, this will be the case for Ni concentrations less than 17
6
4.0 x 10 ( Ω − m)−1
wt%.
Hence, it is not possible to prepare an alloy meeting the criteria; for the stipulated yield
strength the required Ni content must be greater than 23 wt%, whereas for the required conductivity,
less than 17 wt% is necessary.
492
18.D4 First of all, those elements which, when added to silicon render it n-type, lie one group to the right
of silicon in the periodic table; these include the group VA elements (Figure 2.6)--i.e., nitrogen,
phosphorus , arsenic, and antimony.
Since this material is extrinsic and n-type, n&gt;&gt; p, and the electrical conductivity is a function
of the hole concentration according to Equation (18.16). Also, the number of free electrons is about
equal to the number of donor impurities, Nd. That is
n ~ Nd
From Equation (18.16), the conductivity is a function of both the electron concentration (n) and the
electron mobility (μe). Furthermore, the room-temperature electron mobility is dependent on impurity
concentration (Figure 18.17). One way to solve this problem is to use an iterative approach—i.e.,
assume some donor impurity concentration (which will also equal the value of n), then determine a
&quot;calculated&quot; electron mobility from Equation 18.16—i.e.,
μe =
σ
n e
and, finally, compare this mobility with the &quot;measured&quot; value from Figure 18.17, taken at the
assumed n (i.e., Nd) value.
Let us begin by assuming that Nd = 1022 m-3. Thus, the &quot;calculated&quot; mobility value is
μe =
−1
σ
200 (Ω − m)
2
=
= 0.125 m / V − s
22
−
3
−
19
n e
10 m
1.602 x 10
C
(
)(
)
From Figure 18.17, at an impurity concentration of 1022 m-3 the &quot;measured&quot; electron mobility is 0.10
m2/V-s, which is slightly lower than the &quot;calculated&quot; value.
For our next choice, let us assume a higher impurity concentration, say 1023 m-3. At this
higher concentration there will be a reduction of both &quot;calculated&quot; and &quot;measured&quot; electron
mobilities. The &quot;calculated&quot; value is just
μe =
−1
σ
200 (Ω − m)
2
=
= 0.0125 m / V − s
23
−
3
−
19
n e
10 m
1.602 x 10
C
(
)(
)
493
Whereas, Figure 18.17 yields a &quot;measured&quot; μe of 0.05 m2/V-s, which is higher than the &quot;calculated&quot;
value. Therefore, the correct impurity concentration will lie somewhere between 1022 and 1023 m-3
probably closer to the lower of these two values. At 1.3 x 1022 m-3, &quot;measured&quot; and &quot;calculated&quot; μe
values are about equal (0.095 m2/V-s).
It next becomes necessary to calculate the concentration of donor impurities in atom
percent. This computation first requires the determination of the number of silicon atoms per cubic
meter, NSi, using Equation (4.2), which is as follows
NSi =
=
'
NAρ Si
(6.023 x 1023 atoms / mol)(2.33 g / cm3 )(106 cm3 / m3 )
28.09 g / mol
= 5 x 10
(Note:
A Si
28
-3
m
'
in the above discussion, the density of silicon is represented by ρSi
in order to avoid
confusion with resistivity, which is designated by ρ.)
The concentration of donor impurities in atom percent ( C 'd ) is just the ratio of Nd and (Nd +
NSi) multiplied by 100 as
Nd
C 'd =
=
(
1.3 x 10
1.3 x 10 22 m −3
22
Nd + NSi
x 100
−3
m
) (
+ 5 x 1028 m−3
)
-5
x 100 = 2.6 x 10
at%
Now, conversion to weight percent (Cd) is possible using Equation (4.7a) as
Cd =
Cd' A d
C' A + C ' A
d d
x 100
Si Si
where Ad and ASi are the atomic weights of the donor and silicon, respectively.
Thus, the
concentration in weight percent will depend on the particular donor type. For example, for nitrogen
494
CN =
' A
CN
N
C' A
N N
=
x 100
+ C' A
Si Si
(2.6 x 10−5 at%)(14.01g / mol)
x 100
(2.6 x 10 −5 at%)(14.01 g/ mol) + (99.999974 at%)(28.09 g / mol)
= 1.3 x 10
-5
wt%
Similar calculations may be carried out for the other possible donor impurities which yield
CP = 2.87 x 10
-5
wt%
C As = 6.93 x 10 -5 wt%
CSb = 1.127 x 10
-4
wt%
18.D5 This problem asks for us to determine the temperature at which boron is to be diffused into highpurity silicon in order to achieve a room-temperature electrical conductivity of 1000 (Ω-m)-1 at a
distance 0.2 μm from the surface if the B concentration at the surface is maintained at 1.0 x 1025
m-3. It is first necessary for us to compute the hole concentration (since B is an acceptor in Si) at
this 0.2 μm location.
From Equation (18.17), the conductivity is a function of both the hole concentration (p) and
the hole mobility (μh). Furthermore, the room-temperature hole mobility is dependent on impurity
concentration (Figure 18.17). One way to solve this problem is to use an iterative approach—i.e.,
assume some boron concentration, Nb (which will also equal the value of p), then determine a
&quot;calculated&quot; hole mobility from Equation 18.17—i.e.,
μh =
σ
p e
and then compare this mobility with the &quot;measured&quot; value from Figure 18.17, taken at the assumed p
(i.e., Nb).
Let us begin by assuming that Nb = 1024 m-3. Thus, the &quot;calculated&quot; mobility value is
495
μh =
−1
σ
1000 (Ω − m)
2
=
= 0.0062 m / V − s
24
−
3
−
19
p e
10 m
1.602 x 10
C
(
)(
)
From Figure 18.17, at an impurity concentration of 1024 m-3 the &quot;measured&quot; hole mobility is 0.01
m2/V-s, which is higher than the &quot;calculated&quot; value.
For our next choice, let us assume a lower boron concentration, say 1023 m-3. At this lower
concentration there will be an increase of both &quot;calculated&quot; and &quot;measured&quot; hole mobilities. The
&quot;calculated&quot; value is just
μh =
−1
σ
1000 (Ω − m)
2
=
= 0.062 m / V − s
23
−
3
−
19
p e
10 m
1.602 x 10
C
(
)(
)
Whereas, Figure 18.17 yields a &quot;measured&quot; μh of 0.034 m2/V-s, which is lower than the &quot;calculated&quot;
value. Therefore, the correct impurity concentration will lie somewhere between 1023 and 1024 m-3.
At 4.0 x 1023 m-3, &quot;measured&quot; and &quot;calculated&quot; values are about equal (0.016 m2/V-s).
With regard to diffusion, the problem is one involving the nonsteady-state diffusion of B into
the Si, wherein we have to solve for temperature. Temperature is incorporated into the diffusion
coefficient expression given in the problem. But we must first employ the solution to Fick's second
law for constant surface composition boundary conditions, Equation (5.5); in this expression Co is
taken to be zero inasmuch as the problem stipulates that the initial boron concentration may be
neglected. Thus,
Cx − Co
⎛ x ⎞
= 1 - erf ⎜
⎟
C −C
⎝ 2 Dt ⎠
s
o
4.0 x 1023 m −3 − 0
⎛ x ⎞
⎟
= 1 − erf ⎜
1.0 x 1025 m −3 − 0
⎝ 2 Dt ⎠
which reduces to
⎛ x ⎞
0.96 = erf ⎜
⎟
⎝ 2 Dt ⎠
496
In order to solve this expression for a value
x
of it is necessary to interpolate using data in
2 Dt
Table 5.1. Thus
z
erf(z)
1.4
0.9523
z
0.9600
1.5
0.9661
z − 1.4
0.9600 − 0.9523
=
1.5 − 1.4
0.9661 − 0.9523
From which, z = 1.4558; which is to say
1.4558 =
x
2 Dt
Inasmuch as there are 3600 s/h (= t) and x = 0.2 μm (= 2 x 10-7 m) the above equation becomes
1.4558 =
2 x 10−7 m
2 (D)(3600 s)
Which gives D = 1.31 x 10-18 m2/s. However, equating this value to the expression for D given in
the problem gives
-18
D = 1.31 x 10
2
m /s = 2.4 x 10
-4
⎡
347, 000 J / mol ⎤
exp ⎢−
⎥
(8.31
J / mol - K)(T) ⎦
⎣
And, upon solving for the temperature, T = 1271 K = 998&deg;C.
18.D6 This problem asks, for the nonstoichiometric Fe(1 - x)O, given the electrical conductivity (2000
m2/V-s) and hole mobility (1.0 x 10-5 m2/V-s) that we determine the value of x. It is first necessary
to compute the number of holes per unit volume (p) using Equation (18.17). Thus
p =
σ
e μh
497
=
2000 (Ω − m) -1
(
)(
)
1.0 x 10 −5 m2 / V - s 1.602 x 10−19 C
27
= 1.25 x 10
3
holes/m
Inasmuch as it is assumed that the vacancies are saturated, the number of vacancies is also 1.25 x
1027 m-3. Next, it is possible to compute the number of vacancies per unit cell by taking the product
of the number of vacancies per cubic meter times the volume of a unit cell, which volume is just the
unit cell edge length (0.437 nm) cubed. Thus
(
)(
)
3
# vacancies
= 1.25 x 1027 m−3 0.437 x 10 −9 m = 0.10
unit cell
A unit cell for the sodium chloride structure (Figure 12.2) contains the equivalent of four cations and
four anions. Thus, if we take as a basis for this problem 10 unit cells, there will be one vacancy, 40
O2- ions, and 39 iron ions (since one of the iron sites is vacant). (It should also be noted that since
two Fe3+ ions are created for each vacancy, that of the 39 iron ions, 37 of them are Fe2+ and 2 of
them are Fe3+). In order to find the value of (1 - x) in the chemical formula, we just take the ratio of
the number of total Fe ions (39) and the number of total Fe ion sites (40). Thus
(1 − x) =
39
= 0.975
40
Or the formula for this nonstoichiometric material is Fe0.975O.
18.D7 We are asked to compare silicon and gallium arsenide semiconductors relative to properties and
applications.
The following are the characteristics and applications for Si:
1)
being an elemental
semiconductor, it is cheaper to grow in single-crystalline form; 2) because of its electron band
structure, it is best used in transistors; 3) electronic processes are relatively slow due to the low
mobilities for electrons and holes (Table 18.2).
For GaAs:
1)
it is much more expensive to produce inasmuch as it is a compound
semiconductor; 2) because of its electron band structure it is best used in light-emitting diodes and
semiconducting lasers; 3) its band gap may be altered by alloying; 4) electronic processes are
more rapid than in Si due to the greater mobilities of electrons and holes;
5) absorption of
electromagnetic radiation is greater in GaAs, and therefore, thinner layers are required for solar
cells.
498
18.D8W (a) This portion of the problem calls for us to search for possible materials to be used for a
leadframe plate in an integrated circuit package. The requirements are (1) that the material be
highly electrically conductive--i.e., an electrical conductivity of greater that 10 x 106 (Ω-m)-1 [or,
alternatively, an electrical resistivity less than 1.0 x 10-7 (Ω-m)]; (2) that it have a coefficient of
thermal expansion between 2 x 10-6 and 10 x 10-6 (&deg;C)-1; and (3) it must also be a thermal
conductor having a thermal conductivity of at least 100 W/m-K.
When a combination query is
performed on the CD-ROM for
ρe &lt; 1.0 x 10 -7 (Ω - m)
2 x 10
-6
-1
-6
(&deg;C) &lt; αl &lt; 10 x 10
(&deg;C)
-1
k &gt; 100 W/m -K
no materials are found to simultaneously satisfy all three criteria.
(b) Now we are asked to search for insulating materials to be used for the leadframe plate . The
requirements are as follows: (1) an electrical conductivity less than 10-10 (Ω-m)-1 [equivalently, an
electrical resistivity greater than 1010 (Ω-m)]; a coefficient of thermal expansion between 2 x 10-6
and 10 x 10-6 (&deg;C)-1; and (3) a thermal conductivity greater than 30 W/m-K. When a combination
query is performed on the CD-ROM for
ρe &gt; 10
10
(Ω -m)
2 x 10-6 (&deg;C)-1 &lt; αl &lt; 10 x 10-6 (&deg;C) -1
k &gt; 30 W/m -K
no materials are found to simultaneously satisfy all three criteria.
499
CHAPTER 19
THERMAL PROPERTIES
PROBLEM SOLUTIONS
19.1 The energy, E, required to raise the temperature of a given mass of material, m, is the product of
the specific heat, the mass of material, and the temperature change, ΔT, as
E = cpm(ΔT)
The ΔT is equal to 100&deg;C - 20&deg;C = 80&deg;C (= 80 K), while the mass is 2 kg, and the specific heats are
presented in Table 19.1. Thus,
E(aluminum) = (900 J/kg-K)(2 kg)(80 K) = 1.44 x 105 J
E(steel) = (486 J/kg-K)(2 kg)(80 K) = 7.78 x 104 J
E(glass) = (840 J/kg-K)(2 kg)(80 K) = 1.34 x 105 J
E(HDPE) = (1850 J/kg-K)(2 kg)(80 K) = 2.96 x 105 J
19.2 We are asked to determine the temperature to which 10 lbm of brass initially at 25&deg;C would be
raised if 65 Btu of heat is supplied. This is accomplished by utilization of a modified form of Equation
(19.1) as
ΔT =
ΔQ
mc
p
in which ΔQ is the amount of heat supplied, m is the mass of the specimen, and cp is the specific
heat. From Table 19.1, cp = 375 J/kg-K, which in Customary U.S. units is just
⎛ 2.39 x 10 −4 Btu/ lb - &deg;F ⎞
m
⎟ = 0.090 Btu/lb - &deg;F
c p = (375 J/kg - K) ⎜
m
⎜
⎟
1 J / kg - K
⎝
⎠
Thus
500
ΔT =
65 Btu
(10 lbm)(0.090 Btu/ lbm - &deg;F)
= 72.2&deg;F
and
Tf = To + ΔT = 77&deg;F + 72.2&deg;F = 149.2&deg;F (65.1&deg;C)
19.3 (a) This problem asks that we determine the heat capacities at constant pressure, Cp, for copper,
iron, gold, and nickel. All we need do is multiply the cp values in Table 19.1 by the atomic weight,
taking into account the conversion from grams to kilograms. Thus, for Cu
Cp = (386 J/kg- K)(1 kg/1000 g)(63.55 g/mol) = 24.5 J/mol- K
For Fe
Cp = (448 J/kg- K)(1 kg/1000 g)(55.85 g/mol) = 25.0 J/mol- K
For Au
Cp = (128 J/kg- K)(1 kg/1000 g)(196.97 g/mol) = 25.2 J/mol - K
For Ni
Cp = (443 J/kg- K)(1 kg/1000 g)(58.69 g/mol) = 26.0 J/mol- K
(b) These values of Cp are very close to one another because room temperature is considerably
above the Debye temperature for these metals, and, therefore, the values of Cp should be about
equal to 3R [(3)(8.31 J/mol-K) = 24.9 J/mol-K], which is indeed the case for all four of these metals.
19.4 (a) For aluminum, C at 50 K may be approximated by Equation (19.2), since this temperature is
v
significantly below the Debye temperature. The value of C at 30 K is given, and thus, we may
v
compute the constant A as
A =
C
v = 0.81 J/ mol- K = 3 x 10-5 J/mol - K 4
3
(30 K)3
T
501
Therefore, at 50 K
C v = AT
3
(
-5
= 3 x 10
J/mol -K
4
)(50 K)3 = 3.75 J/mol -K
and
c v = (3.75 J/mol- K)(1 mol/26.98 g)(1000 g/kg) = 139 J/kg - K
(b) Since 425 K is above the Debye temperature, a good approximation for Cv is
C v = 3R
= (3)(8.31 J/mol -K) = 24.9 J/mol -K
And, converting this to specific heat
c v = (24.9 J/mol- K)(1 mol/26.98 g)(1000 g/kg) = 925 J/kg - K
19.5 For copper, we want to compute the Debye temperature, θD, given the expression for A in Equation
(19.2) and the heat capacity at 10 K. First of all, let us determine the magnitude of A, as
C
v
3
T
A =
=
(0.78 J / mol - K)(1 kg /1000 g)(63.55 g / mol)
(10 K)3
-5
= 4.96 x 10
J/mol - K
As stipulated in the problem
A =
12π 4 R
5θ3
D
Or, solving for θD
502
4
⎛ 12 π 4 R ⎞
θD = ⎜⎜
⎟⎟
⎝ 5A ⎠
1/3
⎡
4
⎢ (12)(π) (8.31 J/ mol -K)
= ⎢
−5
4
⎢⎣(5) 4.96 x 10 J/ mol- K
(
⎤
⎥
⎥
⎥⎦
)
1/ 3
= 340 K
19.6 (a) The reason that Cv rises with increasing temperature at temperatures near 0 K is because, in
this temperature range, the allowed vibrational energy levels of the lattice waves are far apart
relative to the available thermal energy, and only a portion of the lattice waves may be excited. As
temperature increases, more of the lattice waves may be excited by the available thermal energy,
and, hence, the ability of the solid to absorb energy (i.e., the magnitude of the heat capacity)
increases.
(b) At temperatures far removed from 0 K, Cv becomes independent of temperature because all of
the lattice waves have been excited and the energy required to produce an incremental temperature
change is nearly constant.
19.7 The two metals from which a bimetallic strip is constructed have different coefficients of thermal
expansion. Consequently, a change in temperature will cause the strip to bend. For a thermostat
that operates a furnace, as the temperature drops below a lower limit, the bimetallic strip bends so
as to make an electrical contact, thus, turning on the furnace. With rising temperature, the strip
bends in the opposite direction, breaking the contact (and turning the furnace off) when an upperlimit temperature is exceeded.
19.8 (a) A brass lid on a glass canning jar will loosen when heated because brass has the greater
-6
-1
-6
-1
coefficient of thermal expansion [20 x 10 (&deg;C) versus approximately 9 x 10 (&deg;C) for glass,
Table 19.1].
(b) If the ring is made of tungsten instead of brass, the ring will tighten upon heating inasmuch as
the glass will expand more than tungsten. The values of αl for glass and tungsten are 9 x 10 6 (&deg;C)-1
and 4.5 x 10-6 (&deg;C)-1, respectively.
19.9 In order to determine the change in length of the aluminum wire, we must employ Equation (19.3b)
as
Δl = loα lΔT
503
[
= (10 m) 23.6 x 10
−6
(&deg;C)
](−1&deg;C − 38&deg;C)
-1
= − 9.2 x 10-3 m = − 9.2 mm (−0.36 in.)
19.10 The linear coefficient of thermal expansion for this material may be determined using Equation
(19.3b) as
αl =
Δl
0.2 x 10−3 m
=
(0.1 m)(100&deg;C − 20&deg;C)
l ΔT
o
= 25.0 x 10-6 (&deg;C)-1
19.11 The phenomenon of thermal expansion using the potential energy-versus-interatomic spacing
curve is explained in Section 19.3.
19.12 (a) In this portion of the problem we are asked to determine the density of copper at 1000&deg;C on
the basis of thermal expansion considerations. The basis for this determination will be 1 cm3 of
material at 20&deg;C, which has a mass of 8.940 g; it is assumed that this mass will remain constant
upon heating to 1000&deg;C. Let us compute the volume expansion of this cubic centimeter of copper as
it is heated to 1000&deg;C. A volume expansion expression is given in Equation (19.4)--viz.,
ΔV
= α v ΔT
Vo
or
ΔV = Voα v ΔT
Also, αv = 3αl, as stipulated in the problem. The value of αl given in Table 19.1 for copper is 17.0 x
10-6 (&deg;C)-1. Therefore, the volume, V, of this specimen of Cu at 1000&deg;C is just
(
V = Vo + ΔV = Vo 1 + α v ΔT
(
){ [
]
)
}
= 1 cm3 1 + (3) 17.0 x 10 −6 (&deg;C)−1 (1000&deg;C − 20&deg;C)
= 1.04998 cm
504
3
Thus, the density is just the 8.940 g divided by this new volume--i.e.,
ρ =
8.940 g
= 8.514 g/cm
1.04998 cm3
3
(b) Now we are asked to compute the density at 1000&deg;C taking into consideration the creation of
vacancies, which will further lower the density. This determination requires that we calculate the
number of vacancies using Equation (4.1). But it first becomes necessary to compute the number of
Cu atoms per cubic centimeter (N) using Equation (4.2). Thus,
NAρ Cu
N =
A
Cu
(6.023 x 1023 atoms / mol)(8.514 g / cm3 )
=
63.55 g / mol
= 8.07 x 10
22
3
atoms/cm
Now the total number of vacancies, Nv, [Equation (4.1)] is just
⎛ Q ⎞
Nv = N exp ⎜ − v ⎟
⎝ kT ⎠
(
22
= 8.07 x 10
3
atoms/cm
⎡
⎤
0.90 eV / atom
⎢
⎥
exp ⎢−
−5 eV / K (1273 K) ⎥
8.62
x
10
⎢⎣
⎥⎦
)
(
19
= 2.212 x 10
vacancies/cm
)
3
We want to determine the number of vacancies per unit cell, which is possible if the unit cell volume
is multiplied by Nv. The unit cell volume (VC) may be calculated using Equation (3.5) taking n = 4
inasmuch as Cu has an FCC crystal structure. Thus
VC =
nA Cu
ρ
N
Cu A
505
=
(4 atoms / unit cell)(63.55 g / mol)
(8.514 g / cm3 )(6.023 x 1023 atoms / mol)
= 4.957 x 10-23 cm3 /unit cell
Now, the number of vacancies per unit cell, nv, is just
n v = Nv VC
(
19
= 2.212 x 10
3
vacancies/cm
)(4.957 x 10-23 cm3 /unit cell)
= 0.001096 vacancies/unit cell
What is means is that instead of there being 4.0000 atoms per unit cell, there are only 4.0000 0.001096 = 3.9989 atoms per unit cell. And, finally, the density may be computed using Equation
(3.5) taking n = 3.998904
ρCu =
=
nA Cu
V N
C A
(3.998904 atoms / unit cell)(63.55 g / mol)
(4.957 x 10 −23 cm3 / unit cell)(6.023 x 1023 atoms / mol)
= 8.512 g/cm3
Thus, the influence of the vacancies is almost insignificant--their presence reduces the density by
only 0.002 g/cm3.
19.13 This problem asks that we calculate the values of cv for aluminum and iron at room temperature
using Equation (19.10), the data in Table 19.1, given that αv = 3αl, and given values of the
compressibility. From Equation (19.10)
c v = cp −
From Table 19.1
506
α 2v vo T
β
cp(Al) = 900 J/kg-K
cp(Fe) = 448 J/kg-K
αv(Al) = (3)[23.6 x 10-6 (&deg;C)-1] = 7.08 x 10-5 (&deg;C)-1
αv(Fe) = (3)[(11.8 x 10-6 (&deg;C)-1] = 3.54 x 10-5 (&deg;C)-1
The specific volume is just the reciprocal of the density; thus
v o (Al) =
⎞ ⎛ 1000 g ⎞ ⎛ 1 m ⎞ 3
1 ⎛
1
−4 3
⎟⎜
= ⎜⎜
⎟⎜
⎟ = 3.69 x 10 m / kg
ρ ⎝ 2.71 g/cm 3 ⎟⎠ ⎝ kg ⎠ ⎝ 100 cm ⎠
⎛
⎞ ⎛ 1000 g ⎞ ⎛ 1 m ⎞ 3
1
−4 3
⎟⎟ ⎜
v o (Fe) = ⎜⎜
⎟⎜
⎟ = 1.27 x 10 m / kg
3
kg
100
cm
⎠⎝
⎠
⎝ 7.87 g/cm ⎠ ⎝
Therefore,
c v (Al) = cp (Al) −
α2
v (Al) v o(Al)T
β(Al)
(
)
2
⎡7.08 x 10−5 (&deg;C) −1⎤ 3.69 x10 −4 m 3 / kg (293 K)
⎣
⎦
= 900 J/kg - K −
−11
2 −1
(N/ m )
1.77 x 10
869 J/kg-K
And
(
)
2
⎡ 3.54 x 10 −5 (&deg;C)−1⎤ 1.27 x 10 −4 m3 / kg (293 K)
⎣
⎦
c v (Fe) = 448 J/kg - K −
−12
2 −1
2.65 x 10
(N / m )
430 J/kg-K
19.14 This problem asks for us to determine the temperature to which a cylindrical rod of tungsten
15.025 mm in diameter must be heated in order for it of just fit into a 15.000 mm diameter circular
hole in a plate of 1025 steel (which, of course, is also heated), assuming that the initial temperature
is 25&deg;C. This requires the use of Equation (19.3a), which is applied to the diameters of both the rod
and hole. That is
507
d − do
f
= α l Tf − To
d
(
o
)
Solving this expression for df yields
(
)
d f = do ⎡1 + α T − T ⎤
⎣
l f
o ⎦
Now all we need do is to establish expressions for df(steel) and df(W), set them equal to one
another, and solve for Tf. According to Table 19.1, αl(steel) = 12.0 x 10-6 (&deg;C)-1 and αl(W) = 4.5 x
10-6 (&deg;C)-1. Thus
d f (steel) = df (W)
{
{
}(
}(
)
)
(15.000 mm) ⎣⎡1 + 12.0 x 10 −6(&deg;C)−1 Tf − 25&deg;C ⎤⎦
= (15.025 mm) ⎣⎡1 + 4.5 x 10 −6(&deg;C)−1 Tf − 25&deg;C ⎤⎦
Now solving for Tf gives Tf = 222.4&deg;C
19.15 On a cold day, the metal door handle feels colder than the plastic steering wheel because metal
has the higher thermal conductivity, and, therefore, conducts heat away from one's skin more
rapidly.
19.16 (a) The steady-state heat flux through the plate may be computed using Equation (19.5); the
thermal conductivity for steel, found in Table 19.1, is 51.9 W/m-K. Therefore,
q =− k
= − (51.9 W/m -K)
ΔT
Δx
(373 K − 573 K)
10 x 10 −3 m
6
2
= 1.04 x 10 W/m
(b) Let dQ/dt represent the total heat loss such that
508
dQ
= qAt
dt
where A and t are the cross-sectional area and time, respectively. Thus,
(
)(
)
dQ
= 1.04 x 106 J/s - m2 0.25 m 2 (60 s/min)(60 min/h)
dt
= 9.3 x 108 J/h (8.9 x 105 Btu/h)
(c) If soda-lime glass is used (k = 1.7 W/m-K)(Table 19.1),
dQ
ΔT
= − kAt
dt
Δx
(
= − (1.7 J/s - m -K) 0.25 m
2
⎛
⎞
K
⎟
)(3600 s/h)⎜⎝ 10−x200
−3
10 m ⎠
= 3.06 x 107 J/h (2.9 x 104 Btu/h)
(d) If the thickness of the steel is increased to 20 mm
dQ
ΔT
= − kAt
dt
Δx
⎛ − 200 K ⎞
⎟
= − (51.9 W/m - K) 0.25 m2 (3600 s/h) ⎜⎜
−3 ⎟
⎝ 20 x 10 m ⎠
(
)
= 4.7 x 108 J/h (4.5 x 105 Btu/h)
19.17 (a) Equation (19.7) is not valid for ceramic and polymeric materials since, in the development of
this expression, it is assumed that free electrons are responsible for both electrical and thermal
conduction. Such is the case for most metals. For ceramics and polymers, free electrons are the
primary contributors to the electrical conductivity.
However, free electrons do not contribute
significantly to the thermal conductivity. For ceramics, thermal conduction is primarily by means of
phonons; for polymers, the energy transfer is made by chain vibrations, translations, and rotations.
509
2
(b) Estimated room-temperature values of L, in Ω-W/(K) , for the several materials are determined
below. Electrical conductivity values were determined by taking reciprocals of the resistivities given
in Table B.9, Appendix B; thermal conductivities are taken from Table B.7 in the same appendix.
For zirconia (3 mol% Y2O3)
L =
k
=
σT
[
2.65 W / m - K
]
10−10 (Ω − m) −1 (293 K)
= 9.0 x 107 Ω - W/K 2
For synthetic diamond
L =
[
3150 W / m - K
]
66.7 ( Ω − m)−1 (293 K)
= 0.161 Ω - W/K 2
For intrinsic gallium arsenide
L =
[
45.5 W / m - K
]
10 −6 (Ω − m) −1 (293 K)
= 1.55 x 105 Ω - W/K 2
For polyethylene terephthalate (PET)
L =
[
L =
[
0.15 W / m - K
8
]
10 −12 (Ω − m) −1 (293 K)
= 5.12 x 10
Ω - W/K
2
For silicone
0.23 W / m - K
]
10 −13 (Ω − m)−1 (293 K)
= 7.8 x 10 9 Ω - W/K2
19.18 (a) The thermal conductivity of a single crystal is greater than a polycrystalline specimen of the
same material because both phonons and free electrons are scattered at grain boundaries, thus
decreasing the efficiency of thermal transport.
(b) The thermal conductivity of a plain carbon steel is greater than that for a stainless steel because
the stainless steel has a much higher concentration of alloying elements. Atoms of these alloying
elements serve as scattering centers for the free electrons that are involved in the thermal transport
process.
510
19.19 Thermal conductivities are higher for crystalline than for noncrystalline ceramics because, for
noncrystalline, phonon scattering, and thus the resistance to heat transport, is much more effective
due to the highly disordered and irregular atomic structure.
19.20 Metals are typically better thermal conductors than ceramic materials because, for metals, most of
the heat is transported by free electrons (of which there are relatively large numbers). In ceramic
materials, the primary mode of thermal conduction is via phonons, and phonons are more easily
scattered than are free electrons.
19.21 (a) Porosity decreases the thermal conductivity of ceramic and polymeric materials because the
thermal conductivity of a gas phase that occupies pore space is extremely small relative to that of
the solid material. Furthermore, contributions from gaseous convection are generally insignificant.
(b)
Increasing the degree of crystallinity of a semicrystalline polymer enhances its thermal
conductivity; the vibrations, rotations, etc. of the molecular chains are more effective modes of
thermal transport when a crystalline structure prevails.
19.22
For some ceramic materials, the thermal conductivity first decreases with rising temperature
because the scattering of lattice vibrations increases with temperature. At higher temperatures, the
thermal conductivity will increase for some ceramics that are porous because radiant heat transfer
across pores may become important, which process increases with rising temperature.
19.23 This question asks for us to decide, for each of several pairs of materials, which has the larger
thermal conductivity and why.
(a) Pure silver has a larger conductivity than sterling silver because the impurity atoms in the latter
lead to a greater degree of free electron scattering.
(b)
Polycrystalline silica has a larger conductivity than fused silica because fused silica is
noncrystalline and lattice vibrations are more effectively scattered in noncrystalline materials.
(c) The linear polyethylene has a larger conductivity than the lightly branched polyethylene because
the former will have a higher degree of crystallinity by virtue of its linear molecular structure. Since
heat transfer is accomplished by molecular chain vibrations, and the coordination of these vibrations
increases with percent crystallinity, the higher the crystallinity, the greater the thermal conductivity.
(d) The isotactic polypropylene has a larger thermal conductivity than the atactic polypropylene
because isotactic polymers have a higher degree of crystallinity. The influence of crystallinity on
conductivity is explained in part (c).
511
19.24 This problem asks that we treat a porous material as a composite wherein one of the phases is a
pore phase, and that we estimate upper and lower limits for the room-temperature thermal
conductivity of an aluminum oxide material having a 0.25 volume fraction of pores. The upper limit
of k (kupper) may be determined using Equation (16.1) with thermal conductivity substituted for the
elastic modulus, E. From Table 19.1, the value of k for Al2O3 is 39 W/m-K, while for still air in the
pore phase, k = 0.02 W/m-K. Thus
kupper = Vpk air + VAl O k Al O
2 3
2 3
= (0.25)(0.02 W/m-K) + (0.75)(39 W/m-K) = 29.3 W/m-K
For the lower limit we employ a modification of Equation (16.2) as
klower =
=
k airk Al O
2 3
V k
p Al 2O3
+V
k
Al2O 3 air
(0.02 W / m - K)(39 W / m - K)
= 0.080 W/m- K
(0.25)(39 W / m - K) + (0.75)(0.02 W / m - K)
19.25 (a) The units of D are
T
DT =
(
k(J / s - m -K)
)
ρ kg / m3 c (J / kg -K)
p
= m2 / s
(b) Values of D for the several materials are given below:
T
For aluminum
DT =
k
=
ρcp
(
247 W / m - K
)
-4
2.70 x 103 kg / m3 (900 J / kg - K)
= 1.0 x 10
For steel
DT =
(
51.9 W / m - K
)
7.9 x 10 3 kg / m3 (486 J / kg - K)
512
2
m /s
= 1.4 x 10-5 m2/s
For aluminum oxide
(
DT =
39 W / m - K
)
4.0 x 103 kg / m3 (775 J / kg - K)
= 1.26 x 10 -5 m2 /s
For soda-lime glass
(
DT =
1.7 W / m - K
)
2.5 x 103 kg / m3 (840 J / kg - K)
= 8.1 x 10-7 m2/s
For polystyrene
DT =
(
0.13 W / m - K
)
1.05 x 103 kg / m3 (1170 J / kg -K)
= 1.06 x 10-7 m2 /s
For nylon 6,6
DT =
(
0.24 W / m - K
)
1.14 x 103 kg / m3 (1670 J / kg - K)
-7
= 1.3 x 10
2
m /s
19.26 We want to show that Equation (19.8) is valid beginning with Equation (19.3). Upon examination
of Equation (19.3b),
Δl
= αl ΔT
lo
it may be noted that the term on the left-hand side is the same expression as that for the definition of
engineering strain [Equation (6.2)].
Furthermore, elastic stress and strain are related through
Hooke's law, Equation (6.5). Making appropriate substitutions and algebraic manipulations gives
Δl
σ
= ε =
= α lΔT
lo
E
Or
σ = Eα lΔT
which is the form of Equation (19.8).
513
19.27 (a) Thermal stresses may be introduced into a structure by rapid heating or cooling because
temperature gradients will be established across the cross section due to more rapid temperature
changes at the surface than within the interior; thus, the surface will expand or contract at a different
rate than the interior and since this surface expansion or contraction will be restrained by the interior,
stresses will be introduced.
(b) For cooling, the surface stresses will be tensile in nature since the interior contracts to a lesser
degree than the cooler surface.
(c) For heating, the surface stresses will be compressive in nature since the interior expands to a
lesser degree than the hotter surface.
(d) For a ceramic material, thermal shock is more likely for rapid cooling since the surface stresses
are tensile in nature which will lead to stress concentrations at surface flaws that are present. No
such stress amplification will result for compressive stresses which are established at the surface for
rapid heating.
19.28 (a) We are asked to compute the magnitude of the stress within a steel rod that is heated while its
ends are maintained rigid. To do this we employ Equation (19.8) as
(
σ = Eα l To − Tf
(
9
2
= 207 x 10 N/m
)
)[12.0 x 10−6 (&deg;C)−1](20&deg;C − 80&deg;C)
= -150 MPa (-21,600 psi)
The stress will be compressive since its sign is negative.
(b) The stress will be the same [- 150 MPa (- 21,800 psi )], since stress is independent of bar length.
(c) Upon cooling the indicated amount, the stress becomes
(
σ = Eα l To − Tf
(
9
2
= 207 x 10 N/m
)
)[12.0 x 10−6 (&deg;C)−1][(20&deg;C − (−10&deg;C)]
= +74.5 MPa (+10,800 psi)
This stress will be tensile since its sign is positive.
514
19.29 We want to heat the copper wire in order to reduce the stress level from 70 MPa to 35 MPa; in
doing so, we reduce the stress in the wire by 70 MPa - 35 MPa = 35 MPa, which stress will be a
compressive one (i.e., σ = -35 MPa). Solving for T from Equation (19.8)
f
Tf = To −
= 20&deg;C −
σ
Eα l
-35 MPa
(110 x 103 MPa)[17 x 10−6 (&deg;C) −1]
= 20&deg;C + 19&deg;C = 39&deg;C (101&deg;F)
19.30 This problem asks for us to determine the change in diameter of a cylindrical brass rod 150.00 mm
long and 10.000 mm in diameter when it is heated from 20&deg;C to 160&deg;C while its ends are maintained
rigid. There will be two contributions to the diameter increase of the rod; the first is due to thermal
expansion (which will be denoted as Δd1), while the second is from Poisson's lateral expansion as a
result of elastic deformation from stresses that are established from the inability of the rod to
elongate as it is heated (denoted as Δd2). The magnitude of Δd1 may be computed using Equation
(19.3b) as
(
Δd1 = d oαl Tf − To
)
From Table 19.1 the value of αl for brass is 20.0 x 10-6 (&deg;C)-1. Thus,
[
−6
Δd1 = (10.000 mm) 20.0 x 10
(&deg;C)
](160&deg;C − 20&deg;C)
−1
= 0.0280 mm
For Δd2, we may calculate the stress using Equation (19.8), and the resulting longitudinal
strain using Equation (6.5), and finally the lateral strain (and Δd2) using Equation (6.8). Hence
Δd2
d
o
(
νEα l To − Tf
νσ
= − νε z = −
= −
E
E
) = − να
Solving for Δd2 and realizing that ν = 0.34 (Table 6.1) yields
515
(
l To − Tf
)
(
Δd2 = − d oνα l To − Tf
[
= − (10.000 mm)(0.34) 20.0 x 10
−6
)
](20&deg;C − 160&deg;C)
−1
(&deg;C)
= 0.0095 mm
Finally, the total Δd is just Δd1 + Δd2 = 0.0280 mm + 0.0095 mm = 0.0375 mm.
19.31 This problem asks for us to determine to what temperature a cylindrical rod of nickel 120.00 mm
long and 12.000 mm in diameter must be cooled from 70&deg;C in order to have a 0.023 mm reduction in
diameter if the rod ends are maintained rigid. There will be two contributions to the diameter
decrease of the rod; the first is due to thermal contraction (which will be denoted as Δd1), while the
second is from Poisson's lateral contraction as a result of elastic deformation from stresses that are
established from the inability of the rod to contract as it is cooled (denoted as Δd2). The magnitude
of Δd1 may be computed using Equation (19.3b) as
(
Δd1 = d oαl Tf − To
)
Furthermore, for Δd2, we may calculate the stress using Equation (19.8), and the resulting
longitudinal strain from Equation (6.5), and finally the lateral strain (and Δd2) using Equation (6.8).
Thus
Δd2
d
o
(
) = − να
(
)
νEα l To − Tf
νσ
= − νε z = −
= −
E
E
Or
Δd2 = − d oνα l To − Tf
(
l To − Tf
)
The total Δd is just Δd = Δd1 + Δd2, and
(
Δd = doα l Tf − To
) + d oνα l (Tf − To ) = doα l (Tf − To )(1 + ν)
The values of ν and αl for nickel are 0.31 and 13.3 x 10-6 (&deg;C)-1, respectively (Tables 6.1 and 19.1).
Therefore,
516
[
−(0.023 mm) = (12.000 mm) 13.3 x 10
−6
](Tf − 70&deg;C)(1 + 0.31)
−1
(&deg;C)
Solving the above expression for Tf yields Tf = - 40&deg;C.
19.32 According to Equation (19.9), the thermal shock resistance of a ceramic piece may be enhanced
by increasing the fracture strength and thermal conductivity, and by decreasing the elastic modulus
and linear coefficient of thermal expansion. Of these parameters, σf and αl are the most amenable
to alteration, usually by changing the composition and/or the microstructure.
Design Problems
19.D1 For these railroad tracks, each end is allowed to expand one-half of the joint space distance, or
the track may expand a total of this distance (4.6 mm). Equation (19.3a) is used to solve for T ,
f
-6
-1
where αl for the 1025 steel is found in Table 19.1 [i.e., 12.0 x 10 (&deg;C) ]. Thus,
Tf =
=
[
Δl
+ To
α llo
4.6 x 10−3 m
]
12.0 x 10 −6 (&deg;C)−1 (11.9 m)
+ 10&deg;C
= 32.2&deg;C + 10&deg;C = 42.2&deg;C (108&deg;F)
19.D2 This is really a materials selection problem in which we must decide for which of the five metals
listed, the stress in the rod will not exceed 138 MPa (20,000 psi), when it is heated while its ends are
mounted in rigid supports. Upon examination of Equation (19.8), it may be noted that all we need do
is to compute the EαlΔT product for each of the candidate materials, and then note for which of them
the stress is less than the stipulated maximum. (The value of ΔT is just 80&deg;C.) These parameters
and their product for each of the alloys are tabulated below. (Modulus of elasticity values were taken
from Table 6.1.)
Alloy
Aluminum
Copper
αl (&deg;C)-1
E (MPa)
αlEΔT (MPa)
-6
23.6 x 10
-6
17.0 x 10
69 x 103
110 x 103
130
517
150
Brass
20.0 x 10
-6
-6
12.0 x 10
-6
4.5 x 10
1025 Steel
Tungsten
97 x 103
207 x 103
200
407 x 103
145
155
Thus, aluminum is the only suitable candidate.
19.D3 (a) This portion of the problem asks that we cite the units for the thermal shock resistance
parameter (TSR). From Equation (19.9)
TSR =
( 2 )k(W / m -K) = W / m
E(N / m2 )α (&deg;C)−1
l
σ f N/ m
(b) Now we are asked to rank soda-lime glass, fused silica, and silicon as to their thermal shock
resistance. Thus, all we need do is calculate, for each, the value of TSR using Equation (19.9).
Values of E, σf, αl, and k are found, respectively, in Tables B.2, B.4, B.6, and B.7, Appendix B.
(Note: whenever a range for a property value in these tables is cited, the average of the extremes is
used.)
For soda-lime glass
TSR =
=
σk
f
Eα
l
(69 MPa)(1.7 W / m - K)
(69 x 103 MPa)[9.0 x 10 −6 (&deg;C)−1]
= 189 W/m
For fused silica
TSR =
(104 MPa)(1.4 W / m - K)
(73 x 103 MPa)[0.4 x 10−6 (&deg;C) −1]
= 4986 W/m
And, for silicon
TSR =
(130 MPa)(141 W / m - K)
(129 x 103 MPa)[2.5 x 10−6 (&deg;C) −1]
518
= 56,800 W/m
Thus, these materials may be ranked according to their thermal shock resistance from the greatest
to the least as follows: silicon, fused silica, and soda-lime glass.
19.D4 We want to compute the maximum temperature change allowable without thermal shock for these
several ceramic materials, which temperature change is a function of the fracture strength, elastic
modulus, and linear coefficient of thermal expansion. These data and the ΔTf's are tabulated below.
Material
σf (MPa)
E (MPa)
Soda-lime glass
69
69 x 10
Borosilicate glass
69
Aluminum oxide (96%)
358
Gallium arsenide
57
70 x 10
3
3
3
303 x 10
85 x 103
519
αl (&deg;C)-1
-6
9.0 x 10
-6
3.3 x 10
-6
7.4 x 10
5.9 x 10-6
ΔTf (&deg;C)
111
300
160
114
CHAPTER 20
MAGNETIC PROPERTIES
PROBLEM SOLUTIONS
20.1 (a) We may calculate the magnetic field strength generated by this coil using Equation (20.1) as
H =
=
NI
l
(200 turns)(10 A)
= 10,000 A - turns/m
0.2 m
(b) In a vacuum, the flux density is determined from Equation (20.3). Thus,
Bo = μoH
(
= 1.257 x 10
(c)
)
-6
-2
H/m (10,000 A - turns/m) = 1.257 x 10
tesla
When a bar of titanium is positioned within the coil, we must use an expression that is a
combination of Equations (20.5) and (20.6) in order to compute the flux density given the magnetic
susceptibility. Inasmuch as χm = 1.81 x 10-4 (Table 20.2), then
(
B = μ oH + μ oM = μ oH + μ o χmH = μ oH 1 + χ m
(
= 1.257 x 10
-6
)
(
)
H/m (10,000 A - turns/m) 1 + 1.81 x 10
-4
)
≅ 1.257 x 10-2 tesla
which is essentially the same result as part (b). This is to say that the influence of the titanium bar
within the coil makes an imperceptible difference in the magnitude of the B field.
(d) The magnetization is computed from Equation (20.6):
(
-4
M = χ mH = 1.81 x 10
)(10,000 A - turns/m) = 1.81 A/m
520
20.2 (a) This portion of the problem asks that we compute the flux density in a coil of wire 0.1 m long,
having 15 turns, that carries a current of 1.0 A, and that is situated in a vacuum. Utilizing Equations
(20.1) and (20.3), and solving for Bo yields
B o = μoH =
μoNI
l
(1.257 x 10 −6 H/ m)(15 turns)(1.0 A) = 1.89 x 10-4 tesla
=
0.1 m
(b) Now we are to compute the flux density with a bar of the iron-silicon alloy, the B-H behavior for
which is shown in Figure 20.24. It is necessary to determine the value of H using Equation (20.1) as
H =
(15 turns)(1.0 A)
NI
=
= 150 A - turns/m
0.1 m
l
Using the curve in Figure 20.24, B = 1.65 tesla at H = 150 A-turns/m.
(c) Finally, we are to assume that a bar of Mo is situated within the coil, and to calculate the current
that is necessary to produce the same B field as when the iron-silicon alloy in part (b) was used.
Molybdenum is a paramagnetic material having a χm of 1.19 x 10-4 (Table 20.2). Combining
Equations (20.2), (20.4), and (20.7) we get
H =
B
B
=
μ
μo 1 + χm
(
)
And when Mo is positioned within the coil, then
H =
1.65 tesla
(
)(
1.257 x 10−6 H/ m 1 + 1.19 x 10−4
)
6
= 1.312 x 10 A - turns/m
Now, the current may be determined using Equation (20.1);
Hl
=
I =
N
(1.312 x 10 6 A - turns / m)(0.1 m) = 8750 A
15 turns
20.3 This problem asks us to show that χm and μr are related according to χm = μr - 1. We begin with
Equation (20.5) and substitute for M using Equation (20.6). Thus,
521
B = μoH + μ oM = μoH + μo χmH
But B is also defined in Equation (20.2) as
B = μH = μ oH + μ oχ mH
(
μ = μ o 1 + χm
)
If we divide both sides of this expression by μo
μ
= μr = 1 + χm
μo
or, upon rearrangement
χ m = μ r −1
20.4 For this problem, we want to convert the volume susceptibility of silver (i.e., -2.38 x 10-5) into other
systems of units.
For the mass susceptibility
χ m (kg) =
=
χ
m
ρ(kg / m3 )
− 2.38 x 10 −5
10.49 x 103 kg / m 3
= − 2.27 x 10-9
For the atomic susceptibility
χ m (a) = χ m (kg) x [atomic weight (in kg) ]
(
-9
= − 2.27 x 10
)(0.10787 kg/mol) = − 2.45 x 10-10
For the cgs-emu susceptibilities,
522
' =
χm
' (g) =
χm
−5
-6
m = − 2.38 x 10
= − 1.89 x 10
χ
4π
4π
χ'
m
ρ(g/ cm3 )
=
− 1.89 x 10 −6
10.49 g / cm3
= − 1.80 x 10-7
' (a) = χ ' (g) x atomic weight (in g)
χm
[
]
m
(
-7
= −1.80 x 10
)(107.87 g/mol) = − 1.94 x 10-5
20.5 (a) The two sources of magnetic moments for electrons are the electron's orbital motion around the
nucleus, and also, its spin.
(b) All electrons have a net magnetic moment, which arises from orbital and spin contributions.
(c) All atoms do not have a net magnetic moment. If an atom has completely filled electron shells or
subshells, there will be a cancellation of both orbital and spin magnetic moments.
20.6 (a) The magnetic permeability of this material may be determined according to Equation (20.2) as
μ =
B
0.630 tesla
=
= 1.26 x 10-6 H/m
H 5 x 10 5 A / m
(b) The magnetic susceptibility is calculated as
χm =
μ
1.26 x 10−6 H / m
−1 =
− 1
μ
1.257 x 10−6 H/ m
o
= 2.39 x 10
-3
(c) This material would display both diamagnetic and paramagnetic behavior. All materials are
-3
diamagnetic, and since χm is positive and on the order of 10 , there would also be a paramagnetic
contribution.
20.7 (a) This portion of the problem calls for us to compute the magnetic susceptibility within a bar of
some metal alloy when M = 1.2 x 106 A/m and H =200 A/m. This requires that we solve for χm from
Equation (20.6) as
523
6
M
1.2 x 10 A / m
=
= 6000
H
200 A / m
χm =
(b) In order to calculate the permeability we must employ Equations (20.4) and (20.7) as follows:
(
)
μ = μr μo = μo χ m + 1
(
= 1.257 x 10
-6
)
H/m (6000 + 1) = 7.54 x 10
-3
H/m
(c) The magnetic flux density may be determined using Equation (20.2) as
(
-3
B = μH = 7.54 x 10
)
H/m (200 A/m) = 1.51 tesla
(d) This metal alloy would exhibit ferromagnetic behavior on the basis of the value of its χm (6000),
which is considerably larger than the χm values for diamagnetic and paramagnetic materials listed in
Table 20.2.
20.8 (a) The saturation magnetization for Co may be determined in the same manner as was done for Ni
in Example Problem 20.1. Thus,
Ms = 1.72 μBN
in which μB is the Bohr magneton and N is the number of Co atoms per cubic meter. Also, there are
1.72 Bohr magnetons per Co atom. Now, N (the number of atoms per cubic meter) is related to the
density and atomic weight of Co, and Avogadro's number according to Equation (4.2) as
N =
ρCo NA
ACo
(8.90 g / cm3 )(10 2 cm /m) (6.023 x 10 23 atoms / mol)
3
=
58.93 g / mol
28
= 9.10 x 10
Therefore,
524
3
atoms/m
(
-24
Ms = (1.72 BM/atom) 9.27 x 10
)(
2
28
A -m /BM 9.10 x 10
3
atoms/m
)
6
= 1.45 x 10 A/m
(b) The saturation flux density is determined according to Equation (20.8). Thus
Bs = μoM s
(
= 1.257 x 10
-6
)(
)
6
H/m 1.45 x 10 A/m = 1.82 tesla
20.9 We want to confirm that there are 2.2 Bohr magnetons associated with each iron atom. Therefore,
'
let nB
be the number of Bohr magnetons per atom, which we will calculate. Using a modified form
of the expression for M found in Example Problem 20.1
s
Ms
n B' =
μ N
B
Now, N is just the number of atoms per cubic meter, which is the number of atoms per unit cell (two
for BCC) divided by the unit cell volume--that is,
N =
2
2
=
VC
a3
a being the BCC unit cell edge length (i.e., 0.2866 nm). Thus
'
nB =
Ms
μBN
=
Ms a
3
2μB
(1.70 x 106 A / m)⎢⎣⎡(0.2866 x 10−9 m) / unit cell⎥⎤⎦
(2 atoms / unit cell) (9.27 x 10 −24 A - m 2 / BM)
3
=
= 2.16 BM/atom
525
20.10 We are to determine the number of Bohr magnetons per atom of a hypothetical metal that has a
simple cubic crystal structure, an atomic radius of 0.125 nm, and a saturation flux density of 0.85
tesla. It becomes necessary to employ Equations (20.8) and (20.11) as follows:
Ms =
Bs
μ
o
n μ
= B B
V
C
For the simple cubic crystal structure VC = (2r)3, where r is the atomic radius. Substituting this
relationship into the above equation and solving for nB yields
nB =
μ μ
o B
−9
m)
(
= 1.14 Bohr magnetons/atom
(1.257 x 10 −6 H/ m)(9.27 x 10−24 A - m2 / BM)
3
(0.85 tesla)(8) 0.125 x 10
=
( )
B s 8r 3
20.11 Ferromagnetic materials may be permanently magnetized (whereas paramagnetic ones may not)
because of the ability of net spin magnetic moments of adjacent atoms to align with one another.
This mutual magnetic moment alignment in the same direction exists within small volume regions-domains. When a magnetic field is applied, favorably oriented domains grow at the expense of
unfavorably oriented ones, by the motion of domain walls. When the magnetic field is removed,
there remains a net magnetization by virtue of the resistance to movement of domain walls; even
after total removal of the magnetic field, the magnetization of some net domain volume will be
aligned near the direction that the external field was oriented.
For paramagnetic materials, there is no magnetic dipole coupling, and, consequently,
domains do not form.
When a magnetic field is removed, the atomic dipoles assume random
orientations, and no magnetic moment remains.
20.12 The similarities between ferromagnetic and ferrimagnetic materials are as follows:
There is a coupling interaction between magnetic moments of adjacent atoms/cations for
both material types.
Both ferromagnets and ferrimagnets form domains.
Hysteresis B-H behavior is displayed by both, and, thus, permanent magnetizations are
possible.
526
The differences between ferromagnetic and ferrimagnetic materials are as follows:
Magnetic moment coupling is parallel for ferromagnetic materials, and antiparallel for
ferrimagnetic.
Ferromagnetics, being metallic materials, are relatively good electrical conductors;
inasmuch as ferrimagnetic materials are ceramics, they are electrically insulative.
Saturation magnetizations are higher for ferromagnetic materials.
20.13 Both spinel and inverse spinel crystal structures consist of FCC close-packed stackings of anions
2(O ions). Two types of sites, tetrahedral and octahedral, exist among the anions which may be
2+
occupied by the cations. The divalent cations (e.g., Fe ) occupy tetrahedral positions for both
3+
structures. The difference lies in the occupancy for the trivalent cations (e.g., Fe ). For spinel, all
trivalent ions reside on octahedral sites; whereas, for the inverse spinel, half are positioned on
tetrahedral sites, the other half on octahedral.
20.14 Hund's rule states that the spins of the electrons of a shell will add together in such a way as to
yield the maximum magnetic moment. This means that as electrons fill a shell, the spins of the
electrons that fill the first half of the shell are all oriented in the same direction; furthermore, the
spins of the electrons that fill the last half of this same shell will all be aligned and oriented in the
opposite direction. For example, consider the iron ions in Table 20.4; from Table 2.2, the electron
configuration for the outermost shells for the Fe atom is 3d64s2. For the Fe3+ ion the outermost
shell configuration is 3d5, which means that five of the ten possible 3d states are filled with
electrons. According to Hund's rule the spins of all of these electrons are aligned, there will be no
cancellation, and therefore, there are five Bohr magnetons associated with each Fe3+ ion, as noted
in the table. For Fe2+ the configuration of the outermost shell is 3d6, which means that the spins of
five electrons are aligned in one direction, and the spin of a single electron is aligned in the opposite
direction, which cancels the magnetic moment of one of the other five; thus, this yields a net
moment of four Bohr magnetons.
For Mn2+ the electron configuration is 3d5, the same as Fe3+, and, therefore it will have the
same number of Bohr magnetons (i.e., five).
For Co2+ the electron configuration is 3d7, which means that the spins of five electrons are
in one direction, and two are in the opposite direction, which gives rise to a net moment of three Bohr
magnetons.
For Ni2+ the electron configuration is 3d8 which means that the spins of five electrons are in
one direction, and three are in the opposite direction, which gives rise to a net moment of two Bohr
magnetons.
527
For Cu2+ the electron configuration is 3d9 which means that the spins of five electrons are
in one direction, and four are in the opposite direction, which gives rise to a net moment of one Bohr
magneton.
20.15 (a) The saturation magnetization of nickel ferrite is computed in the same manner as Example
Problem 20.2, and from the expression
Ms =
n μ
B B
a3
is just the number of Bohr magnetons per unit cell. The net magnetic moment arises from
B
2+
the Ni ions, of which there are eight per unit cell, each of which has a net magnetic moment of two
Bohr magnetons (Table 20.4). Thus, n is sixteen. Therefore,
B
Now, n
Ms =
(
−24
(16 BM / unit cell) 9.27 x 10
2
A − m / BM
(0.8337 x 10−9 m) / unit cell
)
3
5
= 2.56 x 10 A/m
(b) This portion of the problem calls for us to compute the saturation flux density. From Equation
(20.8)
Bs = μoM s
(
= 1.257 x 10
-6
)(
5
)
H/m 2.56 x 10 A/m = 0.32 tesla
2+
We want to compute the number of Bohr magnetons per Mn
ion in (MnFe O ) . Let n
2 48
2+
represent the number of Bohr magnetons per Mn
ion; then, using the expression given in
20.16
Example Problem 20.1, we have
Ms = nNμB
in which N is the number of Mn
2+
ions per cubic meter of material. But, from Equation (4.2)
528
NAρ
N =
A
in which A is the molecular weight of MnFe O (230.64 g/mol). Thus,
2 4
Ms =
nNAρμB
A
or
n =
Ms A
N ρμ
A
=
B
(5.6 x 10 5 A / m)(230.64 g / mol)
3
(6.023 x 1023 ions / mol)(5.0 g / m3 )(102 cm/ m) (9.27 x1 0−24 A - m 2 / BM)
= 4.6 Bohr magnetons/Mn2+ ion
20.17 For this problem we are given that yttrium iron garnet may be written in the form Y3cFe a2Fe d3O 12 in
which the superscripts a, c, and d represent different sites on which the Y3+ and Fe3+ ions are
located, and that the spin magnetic moments for the ions on a and c sites are oriented parallel to
one another and antiparallel to the Fe3+ ions on the d sites. We are to determine the number of
Bohr magnetons associated with each Y3+ ion given that each unit cell consists of eight formula
units, the unit cell is cubic with an edge length of 1.2376 nm, the saturation magnetization for the
material is 1.0 x 104 A/m, and that there are 5 Bohr magnetons for each Fe3+ ion.
The first thing to do is to calculate the number of Bohr magnetons per unit cell, which we will
denote nB. Solving for nB using Equation (20.11), we get
nB =
Ms VC
μB
=
Ms a
3
μB
(1.0 x 10 4 A / m)(1.2376 x 10−9 m) = 2.04 Bohr magnetons/unit cell l
3
=
9.27 x 10−24 A - m2 / BM
2.04
= 0.255 Bohr magnetons per formula unit.
8
Furthermore, for each formula unit there are two Fe3+ ions on a sites and three Fe3+ on d sites
Now, there are 8 formula units per unit cell or
which magnetic moments are aligned antiparallel. Since there are 5 Bohr magnetons associated with
529
each Fe3+ ion, the net magnetic moment contribution per formula unit from the Fe3+ ions is 5 Bohr
magnetons. This contribution is antiparallel to the contribution from the Y3+ ions, and since there
are three Y3+ ions per formula unit
No. of Bohr magnetons/Y3+ =
0.255 BM + 5 BM
= 1.75 BM
3
20.18 Repeatedly dropping a permanent magnet on the floor will cause it to become demagnetized
because the jarring will cause large numbers of magnetic dipoles to become misaligned by dipole
rotation.
20.19 For ferromagnetic materials, the saturation magnetization decreases with increasing temperature
because the atomic thermal vibrational motions counteract the coupling forces between the adjacent
atomic dipole moments, causing some magnetic dipole misalignment.
Ferromagnetic behavior
ceases above the Curie temperature because the atomic thermal vibrations are sufficiently violent so
as to completely destroy the mutual spin coupling forces.
20.20 The phenomenon of magnetic hysteresis and an explanation as to why it occurs for ferromagnetic
and ferrimagnetic materials is given in Section 20.7.
20.21 The B versus H behaviors for a ferromagnetic material at 0 K, at a temperature just below its Curie
temperature, and just above its Curie temperature are sketched schematically below.
530
At 0 K, the saturation magnetization will be a maximum, and the hysteresis loop will have the
largest area.
At a higher temperature (yet below the Curie temperature) the saturation
magnetization will decrease and the size of the hysteresis loop will diminish. Finally, above the
Curie temperature, ferromagnetic behavior ceases, and the material becomes paramagnetic, with
linear B versus H behavior; the slope of this line segment is very gentle.
20.22
A schematic sketch showing the hysteresis behavior for a ferromagnet that is gradually
demagnetized by cycling an H field that alternates direction and decreases in magnitude is shown
below.
20.23 Relative to hysteresis behavior, a hard magnetic material has a high remanence, a high coercivity,
a high saturation flux density, high hysteresis energy losses, and a low initial permeability; a soft
magnetic material, on the other hand, has a high initial permeability, a low coercivity, and low
hysteresis energy losses.
With regard to applications, hard magnetic materials are utilized for permanent magnets;
soft magnetic materials are used in devices that are subjected to alternating magnetic fields such as
transformer cores, generators, motors, and magnetic amplifier devices.
20.24 We want to determine the saturation magnetization of the 99.95 wt% Fe in Table 20.5, if it just
reaches saturation when inserted within the coil described in Problem 20.1. It is first necessary to
compute the H field within this coil using Equation (20.1) as
Hs =
NI
(200 turns)(10 A)
=
= 104 A - turns/m
0.2 m
l
531
Now, the saturation magnetization may be determined from Equation (20.5) as
Ms =
B s − μ oHs
μ
o
The value of B in Table 20.5 is 2.14 tesla; thus,
s
(
(2.14 tesla) − 1.257 x 10
Ms =
−6
)(
4
)
H/ m 10 A / m
1.257 x10 −6 H/ m
6
= 1.69 x 10 A/m
20.25 (a) The saturation flux density for the steel, the B-H behavior for which is shown in Figure 20.25,
is 1.30 tesla, the maximum B value shown on the plot.
(b) The saturation magnetization is computed from Equation (20.8) as
Ms =
=
Bs
μ
1.30 tesla
1.257 x 10 −6 H / m
o
= 1.03 x 10
6
A/m
(c) The remanence, B , is read from this plot (Figure 20.25) in the same manner as from the
r
hysteresis loop shown in Figure 20.14; its value is 0.80 tesla.
(d) The coercivity, H , is read from this plot in the same fashion as from Figure 20.14; the value is
c
80 A/m.
(e) On the basis of Tables 20.5 and 20.6, this is most likely a soft magnetic material. The saturation
flux density (1.30 tesla) lies within the range of values cited for soft materials, and the remanence
(0.80 tesla) is close to the values given in Table 20.6 for hard magnetic materials. However, the H
c
is significantly lower than for hard magnetic materials. Also, if we estimate the area within the
3
hysteresis curve, we get a value of approximately 250 J/m , which is in line with the hysteresis loss
per cycle for soft magnetic materials.
20.26 The B versus H curve for this material is shown below.
532
20.27 (a) The B-H data provided in the problem are plotted below.
(b) The first four data points are plotted below.
533
The slope of the initial portion of the curve is μi (as shown), is
μi =
(0.15 − 0) tesla
ΔB
-3
=
= 3.0 x 10 H/m
ΔH
(50 − 0) A / m
Also, the initial relative permeability [Equation (20.4)] is just
μri =
μi
μ
o
=
3.0 x 10 −3 H / m
1.257 x 10 −6 H/ m
= 2400
(c) The maximum permeability is the tangent to the B-H curve having the greatest slope; it is drawn
on the plot below, and designated as μ(max).
534
The value of μ(max) is
(1.3 − 0.3) tesla
ΔB
-3
=
= 8.70 x 10 H/m
ΔH
(160 − 45) A - m
μ(max) =
(d) The H field at which μ(max) occurs is approximately 80 A/m [as taken from the plot shown in
part (c)].
(e) We are asked for the maximum susceptibility, χ(max). From Equation (20.7)
χ (max) = μ r(max) − 1 =
=
8.70 x 10−3 H/ m
1.257 x 10 −6 H / m
μ(max)
− 1
μo
− 1 = 6920
20.28 In order to demagnetize a magnet having a coercivity of 4000 A/m, an H field of 4000 A/m must be
applied in a direction opposite to that of magnetization. According to Equation (20.1)
I =
=
Hl
N
(4000 A / m)(0.15 m)
= 6.0 A
100 turns
20.29 (a) We want to determine the magnitude of the B field within an iron-silicon alloy, the B-H
behavior for which is shown in Figure 20.24, when l = 0.20 m, N = 60 turns, and I = 0.1 A. Applying
Equation (20.1)
H =
(60 turns)(0.1 A)
NI
=
= 30 A/m
0.20 m
l
The B value from the curve corresponding to H = 30 A/m is about 1.35 tesla.
(b)
(i) The permeability at this field is just ΔB/ΔH of the tangent of the B-H curve at H = 30 A/m.
The slope of this line is
μ =
(1.6 − 1.07) tesla
ΔB
-2
=
= 1.0 x 10 H/m
ΔH
(52 − 0) A / m
535
(ii) From Equation (20.4), the relative permeability is
μr =
μ
1.0 x 10−2 H/ m
=
= 7955
μ
1.257 x 10 −6 H / m
o
(iii) Using Equation (20.7), the susceptibility is
χ m = μr − 1 = 7955 − 1 = 7954
(iv) The magnetization is determined from Equation (20.6) as
M = χ mH = (7954)(30 A/m) = 2.4 x 105 A/m
20.30
Hindering domain boundary movement will enhance the coercivity of the magnetic material,
without producing a significant alteration of the saturation flux density.
Thus, schematic B-H
behaviors with and without domain boundary obstruction are shown below.
20.31 The manner in which information is stored magnetically is discussed in Section 20.10.
20.32 (a) Given Equation (20.12) and the data in Table 20.7, we are asked to calculate the critical
magnetic fields for lead at 2.5 and 5.0 K. From the table, for Pb, TC = 7.19 K and BC(0) = 0.0803
tesla. Thus, from Equation (20.3)
HC (0) =
B C (0)
536
μ
o
=
0.0803 tesla
1.257 x 10 −6 H / m
= 6.39 x 104 A/m
Now, solving for HC(2.5) and HC(5.0) using Equation (20.12) yields
⎡
T2 ⎤
HC (T) = HC (0) ⎢1 − 2 ⎥
⎢⎣
TC ⎦⎥
2
⎡
(2.5 K) ⎤
HC (2.5) = 6.39 x 104 A / m ⎢1 −
⎥ = 5.62 x 104 A / m
⎢⎣
(7.19 K)2 ⎥⎦
(
)
2
⎡
(5.0 K) ⎤
HC (5.0) = 6.39 x 104 A / m ⎢1 −
⎥ = 3.30 x 104 A / m
2
⎢⎣
(7.19 K) ⎥⎦
(
)
(b) Now we are to determine the temperature to which mercury must be cooled in a magnetic field of
15,000 A/m in order for it to be superconductive. The value of HC(0) must first be determined using
BC(0) given in the table (i.e., 0.0411 tesla); thus from Equation (20.3)
HC (0) =
BC (0)
μo
=
0.0411 tesla
1.257 x 10−6 H/ m
= 3.27 x 104 A/m
Since TC = 4.15 K we may solve for T using Equation (20.12) as
T = TC 1 −
= (4.15 K) 1 −
20.33
HC (T)
H (0)
C
15, 000 A / m
= 3.05 K
32, 700 A / m
We are asked to determine which of the superconducting elements in Table 20.7 are
superconducting at 2 K and in a magnetic field of 40,000 A/m.
First of all, in order to be
superconductive at 2 K within any magnetic field, the critical temperature must be greater than 2 K.
Thus, aluminum, titanium, and tungsten may be eliminated upon inspection. Now, for each of lead,
mercury, and tin it is necessary, using Equation (20.12), to compute the value of HC(2); if this value
is greater than 40,000 A/m then the element will be superconductive. Hence, for Pb
537
HC (2) =
=
2⎤
B C (0) ⎡
⎢1 − T ⎥
2⎥
μ
TC
o ⎢⎣
⎦
2
⎡
(2.0 K) ⎤
⎢1 −
⎥ = 5.89 x 104 A/m
−6
2
(7.19 K) ⎥⎦
1.257 x 10 H / m ⎢⎣
0.0803 tesla
Since this value is greater than 40,000 A/m, Pb will be superconductive.
For Hg
HC (2) =
⎡
(2.0 K)2 ⎤
4
1
−
⎢
⎥ = 2.51 x 10 A/m
1.257 x 10 −6 H/ m ⎢⎣
(4.15 K)2 ⎥⎦
0.0411 tesla
Inasmuch as this value is less than 40,000 A/m, Hg will not be superconductive.
As for Sn
HC (2) =
2
⎡
(2.0 K) ⎤
⎢1 −
⎥ = 1.73 x 103 A/m
(3.72 K) 2 ⎥⎦
1.257 x 10 −6 H/ m ⎢⎣
0.0305 tesla
Therefore, Sn is not superconductive.
20.34
With increasing magnetic field, type I superconductors are completely diamagnetic and
superconductive below HC, while at HC conduction becomes normal and complete magnetic flux
penetration takes place.
On the other hand, for type II superconductors upon increasing the
magnitude of the magnetic field, the transition from the superconducting to normal conducting states
is gradual between lower-critical and upper-critical fields;
so also is magnetic flux penetration
gradual. Furthermore, type II generally have higher critical temperatures and critical magnetic fields.
20.35 The Meissner effect is a phenomenon found in superconductors wherein, in the superconducting
state, the material is diamagnetic and completely excludes any external magnetic field from its
interior. In the normal conducting state complete magnetic flux penetration of the material occurs.
20.36
The primary limitation of the new superconducting materials that have relatively high critical
temperatures is that, being ceramics, they are inherently brittle and difficult to form into useful
shapes.
538
Design Problems
20.D1 For this problem we are asked to determine the composition of a Co-Ni alloy that will yield a
saturation magnetization of 1.3 x 106 A/m. To begin, let us compute the number of Bohr magnetons
per unit cell nB from an expression that results from combining Equations (20.9) and (20.10). That is
nB =
MSVC
μ
B
in which MS is the saturation magnetization, VC is the unit cell volume, and μΒ is the magnitude of
the Bohr magneton. In Problem 3.7 it was shown for the HCP crystal structure that
(
)
⎛ c⎞
3
VC = ⎜ ⎟ 12 3 R
⎝ a⎠
where R is the atomic radius. From the inside of the front cover, the value of R for Co is given as
0.125 nm (1.25 x 10-10 m). Therefore, inasmuch as the c/a ratio for Co is 1.623, then
(
)(
)
VC = (1.623) 12 3 1.25 x 10 −10 m
-29
= 6.59 x 10
m
3
3
And, now solving for nB yields
nB =
(1.3 x 106 A / m )(6.59 x 10−29 m3 / unit cell)
9.27 x 10−24 A - m2
Bohr magneton
=
9.24 Bohr magneton
unit cell
Inasmuch as there are 1.72 and 0.60 Bohr magnetons for each of Co and Ni, and, for HCP, there are
6 equivalent atoms per unit cell, and if we represent the fraction of Ni atoms by x, then
539
nB = 9.24 Bohr magnetons/unit cell
⎛ 0.6 Bohr magnetons ⎞ ⎛ 6 x Ni atoms ⎞
⎛ 1.72 Bohr magnetons ⎞ ⎡ (6)(1 − x) Co atoms ⎤
= ⎜
⎟⎜
⎟ + ⎜
⎟⎢
⎥
Co atom
unit cell
Ni atom
⎝
⎠ ⎝ unit cell ⎠
⎝
⎠⎣
⎦
And solving for x, the fraction of Ni atoms , x = 0.161, of 16.1 at% Ni.
In order to convert this composition to weight percent, we employ Equation (4.7) as
CNi =
=
C' A
Ni Ni
'
Ni ANi + CCo A Co
&times; 100
C'
(16.1 at%)(58.69 g / mol)
&times; 100
(16.1 at%)(58.69 g / mol) + (83.9 at%)(58.93 g / mol)
= 16.0 wt%
20.D2 This problem asks that we design a cubic mixed-ferrite magnetic material that has a saturation
magnetization of 4.25 x 105 A/m. According to Example Problem 20.2 the saturation magnetization
for Fe3O4 is 5.0 x 105 A/m. In order to decrease the magnitude of Ms it is necessary to replace
some fraction of the Fe2+ with a divalent metal ion that has a smaller magnetic moment. From
Table 20.4 it may be noted that Co2+, Ni2+, and Cu2+, with 3, 2, and 1 Bohr magnetons per ion,
respectively, have fewer than the 4 Bohr magnetons/Fe2+ ion. Let us first consider Ni2+ (with 2
Bohr magnetons per ion) and employ Equation (20.11) to compute the number of Bohr magnetons
per unit cell (nB), assuming that the Ni2+ addition does not change the unit cell edge length (0.839
nm, Example Problem 20.2). Thus,
nB =
Ms a
3
μB
(4.25 x 105 A / m)(0.839 x 10−9 m) / unit cell
3
=
9.27 x 10 −24 A - m 2 / Bohr magneton
= 27.08 Bohr magnetons/unit cell
540
If we let x represent the fraction of Ni2+ that have substituted for Fe2+, then the remaining
unsubstituted Fe2+ fraction is equal to 1 - x. Furthermore, inasmuch as there are 8 divalent ions per
unit cell, we may write the following expression:
nB = 8 [2x + 4(1 − x)] = 27.08
which leads to x = 0.308. Thus, if 30.8 at% of the Fe2+ in Fe3O4 are replaced with Ni2+, the
saturation magnetization will be decreased to 4.25 x 105 A/m.
Upon going through this same procedure for Co and Cu, we find that xCo = 0.615 (or 61.5
at%) and x = 0.205 (20.5 at%) will yield the 4.25 x 105 A/m saturation magnetization.
Cu
20.D3 (a) The mechanism by which the VCR head records and plays back audio/video signals is
essentially the same as the manner by which the head on a computer storage device reads and
writes, as described in Section 20.10.
(b) Heads should be made from soft magnetic materials inasmuch as they are repeatedly
magnetized and demagnetized. Some of the requisite properties for these materials are as follows:
1) a relatively high saturation flux density (a Bs of at least 0.5 tesla); 2) a relatively high initial
permeability (at least 8000); 3) a relatively small hysteresis loop in order to keep energy losses
small; 4) a low remanence; 5) a relatively high mechanical hardness in order to resist surface
wear (a minimum Vickers hardness of 120); and 6) a moderate electrical resistivity (at least 0.6 x
10-6 Ω-m).
(c)
It is up to the student to supply three appropriate candidate materials having properties
consistent with the above requirements.
541
CHAPTER 21
OPTICAL PROPERTIES
PROBLEM SOLUTIONS
21.1 Similarities between photons and phonons are:
1) Both may be described as being wave-like in nature.
2) The energy for both is quantized.
Differences between photons and phonons are:
1) Phonons are elastic waves that exist within solid materials. Photons are electromagnetic energy
packets that may exist in solid materials, as well as in other media.
2) There is a considerable disparity between the velocities of photons and phonons. The velocity
of a photon is the same as the velocity of light in the particular medium; for a phonon, its velocity is
that of sound.
21.2 From the classical perspective, electromagnetic radiation is wave-like in character, and the possible
energies of the radiation are continuous.
From the quantum-mechanical perspective,
electromagnetic radiation is dual-like in character (being both wave-like and particle-like), and not all
energies are possible (i.e., energy is quantized).
21.3 In order to compute the frequency of a photon of orange light, we must use Equation (21.2) as
ν =
c 3 x 108 m / s
=
= 5 x 1014 s-1
λ
6 x 10−7 m
Now, for the energy computation, we employ Equation (21.3) as follows:
(
−34
)(
8
J - s 3 x 10 m / s
6.63 x 10
hc
E =
=
λ
6 x 10 −7 m
)
= 3.31 x 10-19 J (2.07 eV)
21.4 Opaque materials are impervious to light transmission; it is not possible to see through them.
Light is transmitted diffusely through translucent materials (there is some internal light
scattering). Objects are not clearly distinguishable when viewed through a translucent material.
542
Virtually all of the incident light is transmitted through transparent materials, and one can see
clearly through them.
21.5 (a) The phenomenon of electronic polarization by electromagnetic radiation is described in Section
21.4.
(b)
Two consequences of electronic polarization in transparent materials are absorption and
refraction.
21.6 (a) In ionic materials, the larger the size of the component ions the greater the degree of electronic
polarization.
(b) Upon consultation of Table 12.3 we find that the Ba2+, Ca2+, Na+, and K+ ions are all greater in
size than the Si4+ ion (0.136, 0.100, 0.102, and 0.0.138 nm, respectively, versus 0.040 nm), and,
therefore, all of these ions will increase the index of refraction when added to SiO2.
21.7 (a) The electron band structures of metals are such that empty and available electron states are
Electron excitations from filled to empty states are possible with the
absorption of electromagnetic radiation having frequencies within the visible spectrum, according to
Equation (21.6). The light energy is totally absorbed or reflected, and, since none is transmitted, the
material is opaque.
(b) Metals are transparent to high-frequency x-ray and γ-ray radiation since the energies of these
types of radiation are greater than for visible light; electron excitations corresponding to these
energies are not possible because energies for such transitions are to within an energy band gap
beyond the highest partially-filled energy band.
21.8 In order for a material to have an index of refraction less than unity, the velocity of light in the
material (v) would necessarily have to be greater than the velocity of light in a vacuum [Equation
(21.7)]. This is not possible.
-5
21.9 We want to compute the velocity of light in diamond given that εr = 5.5 and χm = -2.17 x 10 . The
velocity is determined using Equation (21.8); but first, we must calculate the values of ε and μ for
diamond. According to Equation (18.7W)
(
-12
ε = ε rε o = (5.5) 8.85 x 10
543
)
F/m = 4.87 x 10
-11
F/m
Now, combining Equations (20.4) and (20.7)
(
)
μ = μ o χm + 1
(
= 1.257 x 10
-6
)(
H/m 1 − 2.17 x 10
-5
) = 1.257 x 10-6 H/m
And, finally
1
v =
=
εμ
1
(4.87 x 10 −11 F / m)(1.257 x 10 −6 H/ m)
= 1.28 x 10
8
m/s
15
21.10W The frequencies of visible radiation are on the order of 10
Hz (Figure 21.2). At these
frequencies only electronic polarization is operable (Figure 18.8W). Thus, εr from Equation (21.10)
is the electronic contribution to εr; let us designate it as ε r' . Or, in other words
ε r' = n2
And using n values found in Table 21.1:
For fused silica
ε r' (silica) = (1.458) 2 = 2.13
And, for soda-lime glass
ε r' (glass) = (1.51)2 = 2.28
The fraction of the electronic contribution is just the ratio of ε r' and εr, εr values being taken from
Table 18.1W. Thus
εr' (silica )
ε (60 Hz)
r
=
2.13
= 0.53
4.0
544
and
ε r' (glass)
ε (60 Hz)
r
=
2.28
= 0.33
6.9
21.11W This problem asks for us, using data in Table 21.1, to estimate the dielectric constants for silica
glass, soda-lime glass, PTFE, polyethylene, and polystyrene, and then to compare these values with
those cited in Table 18.1W and briefly explain any discrepancies. From Equation (21.10)
εr = n2
Thus, for fused silica, since n = 1.458
ε r = (1.458)
2
= 2.13
Similarly, for soda-lime glass
ε r = (1.51) 2 = 2.28
And, for PTFE
ε r = (1.35) 2 = 1.82
For polyethylene
ε r = (1.51) 2 = 2.28
For polystyrene
ε r = (1.60) 2 = 2.56
When we compare the values of εr for the polymers (i.e., PTFE, PE, and PS) with those in Table
18.1W at frequencies of 1 MHz, there is reasonable agreement (i.e., 1.82 versus 2.1 for PTFE, 2.28
versus 2.3 for polyethylene, and 2.56 versus 2.6 for polystyrene). However, for fused silica and
soda-lime glass there are some significant discrepancies (i.e., 2.13 versus 3.8 for the fused silica,
and 2.28 versus 6.9 for the soda-lime glass). The reason for these discrepancies is that for these
two materials an ionic component to the dielectric constant is present at 1 MHz, but is absent at
frequencies within the visible electromagnetic spectrum, which frequencies are on the order 109
MHz (1015 Hz). These effects may be noted in Figure 18.8W.
545
21.12 Dispersion in a transparent medium is the phenomenon wherein the index of refraction varies
slightly with the wavelength of the electromagnetic radiation.
21.13 For this problem we want to compute the maximum value of ns in Equation (21.13) that will give R
= 0.050. Then we are to consult Table 21.1 in order to ascertain which of the materials listed have
indices of refraction less than this maximum value. From Equation (21.13)
0.050 =
⎡n − 1⎤
⎣ s
⎦
2
n2
s − 2n s + 1
=
2
2
n s + 2n s + 1
⎡n + 1⎤
⎣ s
⎦
or
0.95 n 2
s − 2.10 n s + 0.95 = 0
The solution of this quadratic equation is as follows:
ns =
−(− 2.10) &plusmn;
(− 2.10)2 − (4)(0.95)(0.95)
(2)(0.95)
Which leads to the following two roots:
ns(+) = 1.576
ns(-) = 0.635
Only the ns(+) solution (1.576) is physically meaningful. Thus, of the materials listed, soda-lime
glass, Pyrex glass, and polypropylene have indices of refraction less than 1.576, and would be
suitable for this application.
21.14 The thickness and dielectric constant of a thin surface coating are selected such that there is
destructive interference between the light beam that is reflected from the lens-coating interface and
the light beam that is reflected from the coating-air interface; thus, the net intensity of the total
reflected beam is very low.
21.15 The three absorption mechanisms in nonmetallic materials involve electronic polarization, electron
transitions, and scattering.
Electronic polarization is described in Section 21.4;
546
absorption by
electron transitions is discussed in Sections 21.4 and 21.7; and scattering is discussed in Section
21.10.
21.16 We want to decide whether or not Si and Ge are transparent to visible light on the basis of their
band gap energies. Table 18.2 cites 1.11 and 0.67 eV, respectively, as the E 's for these two
g
semiconductors. According to Equation (21.16b), semiconductors having band gap energies less
than about 1.8 eV are opaque to visible light. Thus, both Si and Ge fall into this category, and all
visible light is absorbed by valence-band-to-conduction-band-electron transitions across their
reasonably narrow band gaps.
21.17 This problem asks us to determine the range of visible light wavelengths over which ZnTe (E =
g
2.26 eV) is transparent. Only photons having energies of 2.26 eV or greater are absorbed by
valence-band-to-conduction-band electron transitions. Thus, photons having energies less than 2.26
eV are not absorbed; the minimum photon energy for visible light is 1.8 eV [Equation (21.16b)],
which corresponds to a wavelength of 0.7 μm. The wavelength of a photon having an energy of 2.26
eV, using Equation (21.3), is just
hc
λ =
=
E
(4.13 x 10−15 eV - s)(3 x 108 m / s)
2.26 eV
= 5.5 x 10-7 m = 0.55 μm
Thus, pure ZnTe is transparent to visible light having wavelengths between 0.55 and 0.7 μm.
21.18
The magnitude of the absorption coefficient (β in Equation 21.18) depends on the radiation
wavelength for intrinsic insulators and semiconducting materials.
This is because, for photons
hc
having energies less than the band-gap energy (or in terms of wavelength, when λ &gt;
), photon
E
g
absorption due to valence-band-to-conduction-band electron transitions are not possible, and,
therefore, the value of β will be relatively small. On the other hand, when photons having energies
hc
equal to or greater than the band gap energy (i.e., when λ ≤
) these electron transitions by the
E
g
absorption of photons will occur with the result that the magnitude of β will be relatively large.
In addition, there may be impurity levels that lie within the band gap (Section 21.7) from
which or to which electron excitations may occur with the absorption of light radiation at specific
wavelengths.
547
21.19 In this problem we are asked to calculate the fraction of nonreflected light transmitted through a 20
mm thickness of transparent material, given that the fraction transmitted through a 10 mm width is
0.90. From the fraction of nonreflected light transmitted, I T' /I o' , and using a rearranged form of
Equation (21.18), we may determine the value of β as
β = −
⎛ ' ⎞
1 ⎜ IT ⎟
ln
⎜ ' ⎟
x
⎝ Io ⎠
⎛
1 ⎞
-2
-1
= − ⎜
⎟ ln (0.90) = 1.05 x 10 mm
⎝ 10 mm ⎠
I'
Now, solving for T when x = 20 mm gives
Io'
IT'
= exp (- βx)
I'
o
(
)
= exp ⎡⎣− 1.05 x 10 −2 mm −1 (20 mm) ⎤⎦ = 0.81
21.20 The problem asks that we derive Equation (21.19), which is
IT = I o(1 − R) 2 e - βl
If we examine Figure 21.7, at the front (or left) interface, some of the incident beam having intensity
I is reflected. Since I = I R at this surface, then
o
R
o
I T' = Io − I oR = I o(1 − R)
in which I T' is the intensity of the nonreflected beam at the front surface that is transmitted.
Now there will be absorption of this transmitted beam as it passes through the solid and
transparent medium according to Equation (21.18). Just inside the back (or right) interface, the beam
has passed through a thickness l of this material (x = l) and, therefore, the intensity of the
''
transmitted beam at this point ( I T ) is just
548
I T&quot; = I 'T e
−βl
= Io (1 − R)e
- βl
Finally, a second reflection will occur at the back interface as the beam passes out of the
''
medium. The intensity of the reflected beam ( IR ) is just
- βl
IR&quot; = I &quot;T R = IoR (1 − R)e
And the intensity of the final transmitted beam (I ) becomes
T
IT = I T&quot; − IR&quot;
= I o(1 − R)e - βl − I oR(1 − R)e - βl
= I o(1 − R)2 e - βl
which is Equation (21.19).
21.21 We are asked to compute the thickness of material to yield a transmissivity of 0.75 given that T is
0.85 when l = 20 mm, n = 1.6, and for normally incident radiation. The first requirement is that we
calculate the value of β for this material using Equation (21.19); however, this necessitates that we
first compute the value of R using Equation (21.13) as
R =
=
⎡n − 1⎤
⎣ s
⎦
2
⎡n + 1⎤
⎣ s
⎦
2
(1.6 − 1)2
(1.6 + 1)2
= 5.33 x 10-2
And, from a rearranged form of Equation (21.19), we get
β =−
1
ln
l
⎡
⎤
IT
⎢
⎥
⎢⎣ I (1 − R) 2 ⎦⎥
o
549
=−
1 ⎡
T ⎤
ln ⎢
⎥
2
l
⎣(1 − R) ⎦
⎡
⎤
⎥
⎛
0.85
1 ⎞ ⎢
-3
-1
= −⎜
⎟ ln ⎢
⎥ = 2.65 x 10 mm
2
⎝ 20 mm ⎠ ⎢ 1 − 5.33 x 10−2 ⎥
⎣
⎦
(
)
Now, solving for l from Equation (21.19) when T = 0.75
l=−
⎡
⎤
1
T
ln ⎢
⎥
2
β
⎣(1 − R) ⎦
⎡
⎤
⎢
⎥
0.75
= −
ln ⎢
⎥
−
3
−
1
2
2.65 x 10 mm
⎢ 1 − 5.33 x 10−2 ⎥
⎣
⎦
1
(
)
= 67.3 mm
21.22 (a) The characteristic color of a metal is determined by the distribution of wavelengths of the
nonabsorbed light radiation that is reflected.
(b)
The characteristic color of a transparent nonmetal is determined by the distribution of
wavelengths of the nonabsorbed light radiation that is transmitted through the material.
21.23 For a transparent material that appears colorless, any absorption within its interior is the same for
all visible wavelengths. On the other hand, if there is any selective absorption of visible light (usually
by electron excitations), the material will appear colored, its color being dependent on the frequency
distribution of the transmitted light beam.
21.24 This problem calls for a calculation of the reflectivity between two quartz grains having different
orientations and different indices of refraction (1.544 and 1.553). We must employ Equation (21.12)
since the beam is normal to the grain boundary. Thus,
[n2 − n1]
2
[n2 + n1]
2
R =
550
=
(1.553 − 1.544)2
(1.553 + 1.544)2
= 8.45 x 10-6
21.25 Amorphous polymers are normally transparent because there will be no scattering of a light beam
within the material.
However, for semicrystalline polymers, visible light will be scattered at
boundaries between amorphous and crystalline regions since they have different indices of
refraction. This leads to translucency or, for extensive scattering, opacity, except for semicrystalline
polymers having very small crystallites.
21.26 (a) The phenomenon of luminescence is described in Section 21.11.
(b) The feature that distinguishes fluorescence from phosphorescence is the magnitude of the time
interval between photon absorption and reemission events. Fluorescence is for delay times less
than a second; phosphorescence occurs for longer times.
21.27 (a) The phenomenon of photoconductivity is explained in Section 21.12.
(b)
Zinc selenide, having a band gap of 2.58 eV, would be photoconductive.
In order to be
photoconductive, electrons must be excited from the valence band into the conduction band by the
absorption of light radiation. According to Equation (21.16a), the maximum band gap energy for
which there may be absorption of visible light is 3.1 eV; since the band gap energy for ZnSe is less
than this value, photoinduced valence-band-to-conduction-band electron transitions will occur.
21.28 A photographic light meter is used to measure the intensity of incident light radiation. Each photon
of incident light induces a valence-band-to-conduction band electron transition in which both
electrons and holes are produced, as depicted in Figure 21.5(a).
The magnitude of the
photoinduced current resulting from these transitions is registered, which is proportional to the
numbers of electrons and holes, and thus, the number of incident photons, or, equivalently, the
intensity of the incident light radiation.
21.29 Section 21.13 contains a description of the operation of a ruby laser.
21.30 This problem asks for the difference in energy between metastable and ground electron states for
a ruby laser. The wavelength of the radiation emitted by an electron transition from the metastable
to ground state is cited as 0.6943 μm. The difference in energy between these states, ΔE, may be
determined from using a combined form of Equations (21.6) and (21.3), as
551
ΔE = hν =
=
hc
λ
(4.13 x 10−15 eV - s)(3 x 108 m/ s)
6.943 x 10−7 m
= 1.78 eV
Design Problems
21.D1 This problem stipulates that GaAs and GaP have room-temperature band gap energies of 1.42
and 2.25 eV, respectively, that they form solid solutions in all proportions, that alloys of these two
semiconductors are used for light-emitting diodes wherein light is generated by conduction band-tovalence band electron transitions, and that the band gap of a GaAs-GaP alloy increases
approximately linearly with GaP additions (in mol%). We are asked to determine the composition of
an alloy that will emit red light having a wavelength of 0.68 μm. It first becomes necessary to
compute the band-gap energy corresponding to this wavelength of light using Equation (21.3) as
Eg =
=
hc
λ
(4.13 x 10−15 eV - s)(3 x 108 m/ s)= 1.82 eV
0.68 x 10 −6 m
Realizing that at 0 mol% GaP, Eg = 1.42 eV, while at 100 mol% GaP, Eg = 2.25 eV, it is possible to
set up the relationship
100 mol% − CGaP
100 mol% − 0 mol%
=
2.25 eV − 1.82 eV
2.25 eV − 1.42 eV
Solving for CGaP, the composition of GaP, we get CGaP = 48.2 mol%.
21.D2 Relatively high densities of digital information may be stored on the CD-R (read only) compact
disc. For example, sound (i.e., music) may be stored and subsequently reproduced virtually free of
any interference. In essence, the CD-R is a laser-optical data-storage system, wherein a continuous
laser beam functions as the playback element. The input signal is stored digitally (as optical read-
552
only memory or OROM) in the form of very small, microscopic surface pits that have been
embedded into the disc during the manufacturing process. The incident laser beam is reflected from
the surface of the disc, and modulation (i.e., variation of the phase) of this read or reflected beam is
achieved by optical interference that results from the depth of the pits.
These read-only discs consist of a substrate into which the datum pits have been replicated.
This substrate must be protected, which is accomplished by a thin and reflective layer of aluminum,
on top of which is coated an ultraviolet curable lacquer. Since the substrate is the key component of
the optical path, its properties are extremely important. Some of the substrate characteristics that
are critical are as follows: 1) it must be highly transparent; 2) it must be possible to economically
produce discs that are uniformly thick and extremely flat; 3) water absorption must be low so as to
avoid distortion; 4) high mechanical stability, good impact resistance, and high heat distortion
resistance; 5) good flow properties (while in a molten state) so as to avoid the establishment of
thermal stresses and subsequent optical nonuniformities (i.e., nonuniform birefringence); 6) the
material must be clean and defect-free in order to ensure error-free scanning; and 7) it must have a
long lifetime (on the order of 10 years).
The current material-of-choice for audio CD-Rs is a relatively low molecular weight
polycarbonate since it is the most economical material that best satisfies the above requirements.
553
CHAPTER 22
ECONOMIC, ENVIRONMENTAL, AND SOCIETAL ISSUES IN MATERIALS SCIENCE AND
ENGINEERING
PROBLEM SOLUTION
22.D1W The three materials that are used for beverage containers are glass, aluminum, and the polymer
polyethylene terephthalate (designated as PET or sometimes PETE). Currently, the most commonly
used of these three materials is the PET. Its optical clarity is excellent, it is significantly lighter than
glass, PET has high burst and impact strengths and is shatter-proof, it is inexpensive to produce,
has high gas permeation resistance, is easily fabricated (by blow-molding), and PET containers are
safer (there is no breakage as with glass and no cuts result from pull-tabs as with the Al cans).
There are virtually no incineration and landfill problems with PET, although, PET is relatively
nondegradable. On the down side, PET containers are nonrefillable, but even so, they require less
energy to produce per filled unit volume than either aluminum or glass. Also, they can be recycled.
Glass containers are refillable and recyclable, are very impermeable to the passage of
gases and liquids, and are more expensive to produce and fabricate into bottles than is PET.
However, glass bottles are nonbiodegradable and can be dangerous when they break.
Aluminum beverage containers are nonrefillable and nonbiodegradable, but recyclable, and
are also light in weight. Again, they are more expensive to produce than are PET bottles.
554
```